Variable amplitude fatigue crack growth behavior - a short overview
International Nuclear Information System (INIS)
Singh, Konjengbam Darunkumar; Parry, Matthew Roger; Sinclair, Ian
2011-01-01
A short overview concerning variable amplitude (VA) fatigue crack growth behavior is presented in this paper. The topics covered in this review encompass important issues pertaining to both single and repeated overload transients. Reviews on transient post overload effects such as plasticity induced crack closure, crack tip blunting, residual stresses, crack deflection and branching, activation of near threshold mechanisms, strain hardening are highlighted. A brief summary on experimental trends and finite element modelling of overload induced crack closure is also presented
Variable amplitude fatigue crack growth behavior - a short overview
Energy Technology Data Exchange (ETDEWEB)
Singh, Konjengbam Darunkumar [Indian Institute of Technology, Guwahati (India); Parry, Matthew Roger [Airbus Operations Ltd, Bristol (United Kingdom); Sinclair, Ian [University of Southampton, Southampton (United Kingdom)
2011-03-15
A short overview concerning variable amplitude (VA) fatigue crack growth behavior is presented in this paper. The topics covered in this review encompass important issues pertaining to both single and repeated overload transients. Reviews on transient post overload effects such as plasticity induced crack closure, crack tip blunting, residual stresses, crack deflection and branching, activation of near threshold mechanisms, strain hardening are highlighted. A brief summary on experimental trends and finite element modelling of overload induced crack closure is also presented.
Fatigue Crack Propagation Under Variable Amplitude Loading Analyses Based on Plastic Energy Approach
Directory of Open Access Journals (Sweden)
Sofiane Maachou
2014-04-01
Full Text Available Plasticity effects at the crack tip had been recognized as “motor” of crack propagation, the growth of cracks is related to the existence of a crack tip plastic zone, whose formation and intensification is accompanied by energy dissipation. In the actual state of knowledge fatigue crack propagation is modeled using crack closure concept. The fatigue crack growth behavior under constant amplitude and variable amplitude loading of the aluminum alloy 2024 T351 are analyzed using in terms energy parameters. In the case of VAL (variable amplitude loading tests, the evolution of the hysteretic energy dissipated per block is shown similar with that observed under constant amplitude loading. A linear relationship between the crack growth rate and the hysteretic energy dissipated per block is obtained at high growth rates. For lower growth rates values, the relationship between crack growth rate and hysteretic energy dissipated per block can represented by a power law. In this paper, an analysis of fatigue crack propagation under variable amplitude loading based on energetic approach is proposed.
Effects of Changing Stress Amplitude on the Rate of Fatigue-Crack Propagation in Two Aluminum Alloys
Hudson, C. Michael; Hardrath, Herbert F.
1961-01-01
A series of fatigue tests with specimens subjected to constant amplitude and two-step axial loads were conducted on 12-inch-wide sheet specimens of 2024-T3 and 7075-T6 aluminum alloy to study the effects of a change in stress level on fatigue-crack propagation. Comparison of the results of the tests in which the specimens were tested at first a high and then a low stress level with those of the constant-stress- amplitude tests indicated that crack propagation was generally delayed after the transition to the lower stress level. In the tests in which the specimens were tested at first a low and then a high stress level, crack propagation continued at the expected rate after the change in stress levels.
Fatigue Crack and Delamination Growth in Fibre Metal Laminates under Variable Amplitude Loading
Khan, S.
2013-01-01
This thesis presents the investigation into the fatigue propagation and delamination growth of Fibre Metal Laminates under variable amplitude loading. As explained in the first chapter, the motivation of the research is twofold: first, to obtain a clear understanding and detailed characterization of
Directory of Open Access Journals (Sweden)
Nirpesh Vikram
2015-12-01
Full Text Available In this study effect of strain hardening on crack closure has been examined with the help of experiments and finite element method on the side edge notched specimen of five different Aluminum alloy (3003 Al, 5052 Al, 6061 T6, 6063 T6, 6351 in mode I under constant amplitude fatigue loading with single overload using Abaqus® 6.10 which is very well accepted FEM application in research. Extended Finite Element Method Module has been used to determine effective stress intensity factor at the crack tip while propagation takes place. FEM results have given good agreement with experimental results. Regression analysis has also been done with SPSS® 16 and dependency of strain hardening coefficient on crack closure has analyzed. A generalized empirical formula has been developed based on strain hardening to calculate effective stress intensity range ratio and a modified Paris law has also been formulated for these aluminum alloy.
Fatigue Reliability under Multiple-Amplitude Loads
DEFF Research Database (Denmark)
Talreja, R.
1979-01-01
for the initial tensile strength and the fatigue life, the probability distributions for the residual tensile strength in both the crack initiation and the crack propagation stages of fatigue are determined. The method is illustrated for two-amplitude loads by means of experimental results obtained by testing...
1984-01-01
alloys (2). [--I Fig. 6. Fatigue fracture in Nitrile- butadien rubber ( NBR ). Fig. 7. The characteristic features of fatigue fracture in press moulded...in plastics and even in rubber . It follows therefore, that fatigue fractures must also occur in the mineral layers of our earth or in the rock on...effective until the weakest point yields and forms a crack. To get a feeling for this process, you can imagine that the stressed article is made of rubber
Ultrasonic sizing of fatigue cracks
International Nuclear Information System (INIS)
Burns, D.J.
1983-12-01
Surface and buried fatigue cracks in steel plates have been sized using immersion probes as transmitters-receivers, angled to produce shear waves in the steel. Sizes have been estimated by identifying the ultrasonic waves diffracted from the crack tip and by measuring the time taken for a signal to travel to and from the crack tip. The effects of compression normal to a fatigue crack and of crack front curvature are discussed. Another diffraction technique, developed by UKAEA, Harwell, is reviewed
FATIGUE CRACK PROPAGATION THROUGH AUSTEMPERED DUCTILE IRON MICROSTRUCTURE
Directory of Open Access Journals (Sweden)
Lukáš Bubenko
2010-10-01
Full Text Available Austempered ductile iron (ADI has a wide range of application, particularly for castings used in automotive and earth moving machinery industries. These components are usually subjected to variable dynamic loading that may promote initiation and propagation of fatigue cracks up to final fracture. Thus, it is important to determine the fatigue crack propagation behavior of ADI. Since fatigue crack growth rate (da/dN vs. stress intensity factor K data describe fatigue crack propagation resistance and fatigue durability of structural materials, da/dN vs. Ka curves of ADI 1050 are reported here. The threshold amplitude of stress intensity factor Kath is also determined. Finally, the influence of stress intensity factor amplitude to the character of fatigue crack propagation through the ADI microstructure is described.
Effect of residual stress induced by cold expansion on fatigue crack ...
African Journals Online (AJOL)
Fatigue life and fatigue crack growth rate are controlled by stress ratio, stress level, orientation of crack, temper-ature, residual stress, corrosion, etc. The effects of residual stress on fatigue crack growth in aluminium (Al) alloy 2024-T351 by Mode I crack were investigated by applying constant amplitude cycles based on ...
Fatigue crack growth in an aluminum alloy-fractographic study
Salam, I.; Muhammad, W.; Ejaz, N.
2016-08-01
A two-fold approach was adopted to understand the fatigue crack growth process in an Aluminum alloy; fatigue crack growth test of samples and analysis of fractured surfaces. Fatigue crack growth tests were conducted on middle tension M(T) samples prepared from an Aluminum alloy cylinder. The tests were conducted under constant amplitude loading at R ratio 0.1. The stress applied was from 20,30 and 40 per cent of the yield stress of the material. The fatigue crack growth data was recorded. After fatigue testing, the samples were subjected to detailed scanning electron microscopic (SEM) analysis. The resulting fracture surfaces were subjected to qualitative and quantitative fractographic examinations. Quantitative fracture analysis included an estimation of crack growth rate (CGR) in different regions. The effect of the microstructural features on fatigue crack growth was examined. It was observed that in stage II (crack growth region), the failure mode changes from intergranular to transgranular as the stress level increases. In the region of intergranular failure the localized brittle failure was observed and fatigue striations are difficult to reveal. However, in the region of transgranular failure the crack path is independent of the microstructural features. In this region, localized ductile failure mode was observed and well defined fatigue striations were present in the wake of fatigue crack. The effect of interaction of growing fatigue crack with microstructural features was not substantial. The final fracture (stage III) was ductile in all the cases.
International Nuclear Information System (INIS)
Lee, Shin Young; Song, Ji Ho
2000-01-01
Crack closure and growth behavior of physically short fatigue cracks under random loading are investigated by performing narrow-and wide-band random loading tests for various stress ratios. Artificially prepared two-dimensional, short through-thickness cracks are used. The closure behavior of short cracks under random loading is discussed, comparing with that of short cracks under constant-amplitude loading and also that of long cracks under random loading. Irrespective of random loading spectrum or block length, the crack opening load of short cracks is much lower under random loading than under constant-amplitude loading corresponding to the largest load cycle in a random load history, contrary to the behavior of long cracks that the crack opening load under random loading is nearly the same as or slightly higher than constant-amplitude results. This result indicates that the largest load cycle in a random load history has an effect to enhance crack opening of short cracks
Multispecimen fatigue crack propagation testing
International Nuclear Information System (INIS)
Ermi, A.M.; Bauer, R.E.; Chin, B.A.; Straalsund, J.L.
1981-01-01
Chains of miniature center-cracked-tension specimens were tested on a conventional testing machine and on a prototypic in-reactor fatigue machine as part of the fusion reactor materials alloy development program. Annealed and 20 percent cold-worked 316 stainless steel specimens were cycled under various conditions of temperature, frequency, stress ratio and chain length. Crack growth rates determined from multispecimen visual measurements and from an electrical potential technique were consistent with those obtained by conventional test methods. Results demonstrate that multispecimen chain testing is a valid method of obtaining fatigue crack propagation information for alloy development. 8 refs
Effects of Specimen Diameters on the Distribution of Corrosion Fatigue Cracks
石原, 外美; 塩澤, 和章; 宮尾, 嘉寿
1988-01-01
The distribution of corrosion fatigue cracks observed on the un-notched round specimen surface differs with specimen diameter, especially in the low stress amplitude region. At a constant fatigue life ratio, many long cracks are initiated on the larger specimen, 12 mm (diameter), in comparison with the smaller specimen, 6 mm (diameter). On the other hand, in the high stress amplitude region of corrosion fatigue and fatigue in laboratory air, the distribution of cracks during the fatigue proce...
Peridynamic model for fatigue cracking.
Energy Technology Data Exchange (ETDEWEB)
Silling, Stewart Andrew; Abe Askari (Boeing)
2014-10-01
The peridynamic theory is an extension of traditional solid mechanics in which the field equations can be applied on discontinuities, such as growing cracks. This paper proposes a bond damage model within peridynamics to treat the nucleation and growth of cracks due to cyclic loading. Bond damage occurs according to the evolution of a variable called the "remaining life" of each bond that changes over time according to the cyclic strain in the bond. It is shown that the model reproduces the main features of S-N data for typical materials and also reproduces the Paris law for fatigue crack growth. Extensions of the model account for the effects of loading spectrum, fatigue limit, and variable load ratio. A three-dimensional example illustrates the nucleation and growth of a helical fatigue crack in the torsion of an aluminum alloy rod.
Fatigue crack propagation behavior under creep conditions
International Nuclear Information System (INIS)
Ohji, Kiyotsugu; Kubo, Shiro
1991-01-01
The crack propagation behavior of the SUS 304 stainless steel under creep-fatigue conditions was reviewed. Cracks propagated either in purely time-dependent mode or in purely cycle-dependent mode, depending on loading conditions. The time-dependent crack propagation rate was correlated with modified J-integral J * and the cycle-dependent crack propagation rate was correlated with J-integral range ΔJ f . Threshold was observed in the cycle-dependent crack propagation, and below this threshold the time-dependent crack propagation appeared. The crack propagation rates were uniquely characterized by taking the effective values of J * and ΔJ f , when crack closure was observed. Change in crack propagation mode occurred reversibly and was predicted by the competitive damage model. The threshold disappeared and the cycle-dependent crack propagation continued in a subthreshold region under variable amplitude conditions, where the threshold was interposed between the maximum and minimum ΔJ f . (orig.)
Fatigue crack growth in fiber reinforced plastics
Mandell, J. F.
1979-01-01
Fatigue crack growth in fiber composites occurs by such complex modes as to frustrate efforts at developing comprehensive theories and models. Under certain loading conditions and with certain types of reinforcement, simpler modes of fatigue crack growth are observed. These modes are more amenable to modeling efforts, and the fatigue crack growth rate can be predicted in some cases. Thus, a formula for prediction of ligamented mode fatigue crack growth rate is available.
Fatigue crack Behaviour in a High Strength Tool Steel
DEFF Research Database (Denmark)
Højerslev, Christian; Carstensen, Jesper V.; Brøndsted, Povl
2002-01-01
The influence of microstructure on fatigue crack initiation and crack growth of a hardened and tempered high speed steel was investigated. The evolution of fatigue cracks was followed in four point bending at room temperature. It was found that a carbide damage zone exists above a threshold load...... value of maximally 80% of the yield strength of the steel. The size of this carbide damage zone increases with increasing load amplitude, and the zone is apparently associated with crack nucleation. On fatigue crack propagation plastic deformation of the matrix occurs in a radius of approximately 4...... microns in front of the fatigue crack tip, which is comparable with the relevant mean free carbide spacing....
Patankar, Ravindra
2003-10-01
Statistical fatigue life of a ductile alloy specimen is traditionally divided into three stages, namely, crack nucleation, small crack growth, and large crack growth. Crack nucleation and small crack growth show a wide variation and hence a big spread on cycles versus crack length graph. Relatively, large crack growth shows a lesser variation. Therefore, different models are fitted to the different stages of the fatigue evolution process, thus treating different stages as different phenomena. With these independent models, it is impossible to predict one phenomenon based on the information available about the other phenomenon. Experimentally, it is easier to carry out crack length measurements of large cracks compared to nucleating cracks and small cracks. Thus, it is easier to collect statistical data for large crack growth compared to the painstaking effort it would take to collect statistical data for crack nucleation and small crack growth. This article presents a fracture mechanics-based stochastic model of fatigue crack growth in ductile alloys that are commonly encountered in mechanical structures and machine components. The model has been validated by Ray (1998) for crack propagation by various statistical fatigue data. Based on the model, this article proposes a technique to predict statistical information of fatigue crack nucleation and small crack growth properties that uses the statistical properties of large crack growth under constant amplitude stress excitation. The statistical properties of large crack growth under constant amplitude stress excitation can be obtained via experiments.
Fatigue cracking in road pavement
Mackiewicz, P.
2018-05-01
The article presents the problem of modelling fatigue phenomena occurring in the road pavement. The example of two selected pavements shows the changes occurring under the influence of the load in different places of the pavement layers. Attention is paid to various values of longitudinal and transverse strains generated at the moment of passing the wheel on the pavement. It was found that the key element in the crack propagation analysis is the method of transferring the load to the pavement by the tire and the strain distribution in the pavement. During the passage of the wheel in the lower layers of the pavement, a complex stress state arises. Then vertical, horizontal and tangent stresses with various values appear. The numerical analyses carried out with the use of finite element methods allowed to assess the strain and stress changes occurring in the process of cracking road pavement. It has been shown that low-thickness pavements are susceptible to fatigue cracks arising "bottom to top", while pavements thicker are susceptible to "top to bottom" cracks. The analysis of the type of stress allowed to determine the cracking mechanism.
Crack propagation under conditions of low cycle fatigue
International Nuclear Information System (INIS)
Hellmann, D.
1988-01-01
A literature review is given of convenient concepts describing the mechanical behaviour of a cracked body under cyclic loading. Only the range of high growth rates is considered. However, caused by large scale yielding in this range, the application of linear elastic fracture mechanics is no longer possible. Mechanical parameters which control fatigue crack growth are a modified stress intensity factor, the J-integral, the crack tip opening displacement and a suitable strain amplitude. (orig.) With 20 figs [de
Noncontact fatigue crack evaluation using thermoelastic
Energy Technology Data Exchange (ETDEWEB)
Kim, Ji Min; An, Yun Kyu; Sohn, Hoon [KAIST, Daejeon (Korea, Republic of)
2012-12-15
This paper proposes a noncontact thermography technique for fatigue crack evaluation under a cyclic tensile loading. The proposed technique identifies and localizes an invisible fatigue crack without scanning, thus making it possible to instantaneously evaluate an incipient fatigue crack. Based on a thermoelastic theory, a new fatigue crack evaluation algorithm is proposed for the fatigue crack tip localization. The performance of the proposed algorithm is experimentally validated. To achieve this, the cyclic tensile loading is applied to a dog bone shape aluminum specimen using a universal testing machine, and the corresponding thermal responses induced by thermoelastic effects are captured by an infrared camera. The test results confirm that the fatigue crack is well identified and localized by comparing with its microscopic images.
Study on the fatigue crack initiation life under spherical contact
Energy Technology Data Exchange (ETDEWEB)
Cho, Yong Joo; Kim, Tae Wan [Busan National Univ., Busan (Korea, Republic of); Lee, Mun Ju [Samsung Electronics Co., Ltd., Suwon (Korea, Republic of)
2001-08-01
In case of contact fatigue, the accurate calculation of surface tractions and subsurface stress is essential to the prediction of crack initiation life. Surface tractions influencing shear stress amplitude have been obtained by contact analysis based on influence function. Subsurface stress has been obtained by using rectangular patch solutions. In this study, to simulate asperity contact under sliding condition, the tip of asperity was simulated by sphere and to calculate crack initiation life in the substrate, dislocation pileup theory was used.
Study on the fatigue crack initiation life under spherical contact
International Nuclear Information System (INIS)
Cho, Yong Joo; Kim, Tae Wan; Lee, Mun Ju
2001-01-01
In case of contact fatigue, the accurate calculation of surface tractions and subsurface stress is essential to the prediction of crack initiation life. Surface tractions influencing shear stress amplitude have been obtained by contact analysis based on influence function. Subsurface stress has been obtained by using rectangular patch solutions. In this study, to simulate asperity contact under sliding condition, the tip of asperity was simulated by sphere and to calculate crack initiation life in the substrate, dislocation pileup theory was used
International Nuclear Information System (INIS)
Kim, Sung Jin; Kwon, Oh Yang
2004-01-01
The fatigue crack growth behavior of a fatigue-cracked and patch-repaired AA2024-T3 plate has been monitored. It was found that the overall crack growth rate was reduced and the crack propagation into the adjacent hole was also retarded. Signals due to crack growth after patch-repair and those due to debonding of the plate-patch interface were discriminated each other by using principal component analysis. The former showed higher center frequency and lower amplitude, whereas the latter showed longer rise time, lower frequency and higher amplitude.
Growth of 2D and 3D plane cracks under thermo-mechanical loading with varying amplitudes
International Nuclear Information System (INIS)
Sbitti, Amine
2009-01-01
After a presentation of the phenomenon of thermal fatigue (in industrial applications and nuclear plants), this research thesis reports the investigation of the growth and arrest of a 2D crack under thermal fatigue (temperature and stress distribution over thickness, calculation of stress intensity factors, laws of fatigue crack growth, growth under varying amplitude), and the investigation of 3D crack growth under cyclic loading with varying amplitudes (analytic and numerical calculation of stress intensity factors, variational formulation in failure mechanics, 3D crack propagation under fatigue, use of the Aster code, use of the extended finite element method or X-FEM). The author discusses the origin and influence of the 3D crack network under thermal fatigue
Fatigue cracking on a steam generator tube
International Nuclear Information System (INIS)
Boccanfuso, M.; Lothios, J.; Thebault, Y.; Bruyere, B.; Duisabeau, L.; Herms, E.
2015-01-01
A circumferential fatigue crack was observed on a steam generator tube of the unit 2 of the Fessenheim plant. The results of destructive testing and the examination of the fracture surface show that the circumferential crack is linked to a large number of cycles with a very low stress intensity factor. Other aggravating factors like inter-granular corrosion have played a role in the initiating phase of fatigue cracking. The damage has been exacerbated by the lack of support of the tube at the level of the anti-vibration bars. (A.C.)
Study of fatigue crack propagation in magnesium alloys
International Nuclear Information System (INIS)
Yarema, S.Ya.; Zinyuk, O.D.; Ostash, O.P.; Kudryashov, V.G.; Elkin, F.M.
1981-01-01
Fatigue crack propagation in standard (MA2-1, MA8) and super light (MA21, MA18) alloys has been investigated in the whole range of load amplitude changes-from threshold to critical; the materials have been compared by cyclic crack resistance, fractographic analysis has been made. It is shown that MA2-1 alloy crack resistance is slightly lower than the resistance of the other three alloys. MA8 and MA21 alloys having similar mechanical properties almost do not differ in cyclic crack resistance as well. MA18 alloy has the highest resistance to fatigue crack propagation in the whole range of Ksub(max) changes. The presented results on cyclic crack resistance of MA21 and MA18 alloys agree with the data on statistic fracture toughness. The fractures have been also investigated using a scanning electron microscope. Fracture microrelieves of MA8 and MA21 alloys are very similar. At low crack propagation rates (v - 7 m/cycle) it develops through grains, in MA2-1 alloy fracture intergrain fracture areas can be observed. In MA8 and MA21 alloy fractures groove covered areas can be seen alonside with areas of slipping plane laminatron; their specific weight increases with #betta# decrease. Lower crack propagation rates and higher values of threshold stress intensity factors for MA8 and MA21 alloys than for MA2-1 alloy are caused by the absence of intergrain fracture
The fatigue life and fatigue crack through thickness behavior of a surface cracked plate, 2
International Nuclear Information System (INIS)
Nam, Ki-Woo; Fujibayashi, Shinpei; Ando, Kotoji; Ogura, Nobukazu.
1987-01-01
Most structures have a region where stresses concentrate, and the probability of fatigue crack initiation may be higher than in other parts. Therefore, to improve the reliability of an LBB design, it is necessary to evaluate the growth and through thickness behavior of fatigue cracks in the stress concentration part. In this paper, a fatigue crack growth test at a stress concentration region has been made on 3 % NiCrMo and HT 80 steel. Stress concentration is caused by a fillet on the plate. The main results obtained are as follows : (1) Before cracking through the plate thickness, stress concentration has a remarkable effect on the fatigue crack growth behavior and it flatens the shape of a surface crack. The crack growth behavior can be explained quantatively by using the Newman-Raju equation and the stress resolving method proposed by ASME B and P Code SecXI. (2) The da/dN-ΔK relation obtained in a stress concentration specimen shows good agreement with that obtained in a surface cracked smooth specimen. (3) It is shown that stress concentration caused by a fillet has little effect on the crack growth rate after cracking through the plate thickness. (4) By using the K value based on eq. (1), (2), particular crack growth behavior and the change in crack shape after cracking through thickness can be explained quantatively. (author)
Mechanism of electric fatigue crack growth in lead zirconate titanate
International Nuclear Information System (INIS)
Westram, Ilona; Oates, William S.; Lupascu, Doru C.; Roedel, Juergen; Lynch, Christopher S.
2007-01-01
A series of experiments was performed with through-thickness cracks in ferroelectric double cantilever beam (DCB) specimens. Cyclic electric fields of different amplitudes were applied which resulted in cyclic crack propagation perpendicular to the electric field direction. Crack propagation was observed optically and three regimes were identified: a pop-in from a notch, steady-state crack growth and a decrease of the crack growth rate with increasing cycle number. Crack growth only occurred if the applied field exceeded the coercive field strength of the material. Furthermore, the crack extended during each field reversal and the crack growth rate increased with increasing field. Based on the experimental observations, a mechanistic understanding was developed and contrasted with a nonlinear finite element analysis which quantified the stress intensity in the DCB specimens. The driving forces for crack formation at the notch and subsequent fatigue crack growth were computed based on the distribution of residual stresses due to ferroelectric switching. The finite element results are in good agreement with the experimental observations and support the proposed mechanism
International Nuclear Information System (INIS)
Akita, Koichi; Kodama, Shotaro; Misawa, Hiroshi
1994-01-01
X-ray fractography is a method of analysing the causes of accidental fracture of machine components or structures. Almost all of the previous research on this problem has been carried out using constant amplitude fatigue tests. However, the actual loads on components and structures are usually of variable amplitudes. In this study, X-ray fractography was applied to fatigue fractured surfaces produced by variable amplitude loading. Fatigue tests were carried out on Ni-Cr-Mo steel CT specimens under the conditions of repeated, two-step and multiple-step loading. Residual stresses were measured on the fatigue fractured surface by an X-ray diffraction method. The relationships between residual stress and stress intensity factor or crack propagation rate were studied. They were discussed in terms of the quantitative expressions under constant amplitude loading, proposed by the authors in previous papers. The main results obtained were as follows : (1) It was possible to estimate the crack propagation rate of the fatigue fractured surface under variable amplitude loading by using the relationship between residual stress and stress intensity factor under constant amplitude loading. (2) The compressive residual stress components on the fatigue fractured surface correspond with cyclic softening of the material rather than with compressive plastic deformation at the crack tip. (author)
Fatigue crack behaviour in mine excavator
Energy Technology Data Exchange (ETDEWEB)
Yin, Y.; Grondin, G.Y.; Elwi, A.E. [Alberta Univ., Edmonton, AB (Canada). Dept. of Civil and Environmental Engineering
2006-05-15
Fatigue cracking in excavation equipment represents a significant operating cost for oil sands operators. It is caused by high impact loads, the high frequency of load cycles, and large component sizes found in oil sands processing facilities. Monitoring and repair strategies for fatigue cracks are typically based on vendor specifications and the experience of maintenance personnel. This paper provided details of an optimized crack management program applied to a BE 395B shovel boom. The proposed crack management tool uses a chart to predict the remaining life of a corner crack in the shovel boom. Predictions are based on limited field measurements of operating loads as well as on data obtained from fatigue testing of boom material, and a finite element analysis of the shovel boom. Field and laboratory data are used along with fracture mechanics and finite element modelling to predict crack life. It was concluded that the tool will allow inspectors and planners to schedule repairs based on safe service life. The tool is applicable for any components subjected to fatigue loading. 3 refs., 21 tabs., 64 figs.
In situ fatigue-crack-propagation experiment
International Nuclear Information System (INIS)
Ermi, A.M.; Chin, B.A.
1981-01-01
An in-reactor fatigue experiment was conducted in the Oak Ridge Research Reactor to determine the effects of dynamic irradiation on fatigue crack propagation. Eight 20% cold-worked 316 stainless steel specimens were precracked to various initial crack lengths, linked together to form a chain, and inserted into a specially designed in-reactor fatigue machine. Test conditions included a maximum temperature of 460 0 C, an environment of sodium, a frequency of 1 cycle/min, and a stress ratio of 0.10. Results indicated that (1) no effects of dynamic irradiation were observed for a fluence of 1.5 x 10 21 n/cm 2 (E > 0.1 MeV); and (2) crack growth rates in elevated temperature sodium were a factor of 3 to 4 lower than in room temperature air
In-reactor fatigue crack propagation
International Nuclear Information System (INIS)
Ermi, A.M.; Mervyn, D.A.; Straalsund, J.L.
1979-08-01
An in-reactor fatigue experiment is being designed to determine the effect of dynamic irradiation on the fatigue crack propagation (FCP) behavior of candidate fusion first wall materials. This investigation has been prompted by studies which show gross differences in crack growth characteristics of creep rupture specimens testing by postirradiation versus dynamic in-reactor methods. The experiment utilizes miniature center-cracked-tension specimens developed specifically for in-reactor studies. In the test, a chain of eight specimens, precracked to various initial crack lengths, is stressed during irradiation to determine crack growth rate as a function of stress intensity. Load levels were chosen which result in small crack growth rates encompassing a regime of the crack growth curve not previously investigated during irradiation studies of FCP. The test will be conducted on 20% cold worked 316 stainless steel at a temperature of 425 0 C, in a sodium environment, and at a frequency of 1 cycle/min. Irradiation will occur in the Oak Ridge Research Reactor, resulting in a He/dpa ratio similar to that expected at the first wall in a fusion reactor. Detailed design of the experiment is presented, along with crack growth data obtained from prototypic testing of the experimental apparatus. These results are compared to data obtained under similar conditions generated by conventional test methods
International Nuclear Information System (INIS)
Taheri, Said; Julan, Emricka; Tran, Xuan-Van; Robert, Nicolas
2017-01-01
Highlights: • For crack growth analysis, weld residual stress field must be considered through its SIF in presence of a crack. • Presence of cracks of same depth proves their arrest, where equal depth is because mean stress acts only on crack opening. • Not considering amplitudes under a fatigue crack growth threshold (FCGT) does not compensate the lack of FGCT in Paris law. • Propagation rates are close for axisymmetric and circumferential semi-elliptical cracks. - Abstract: High cycle thermal crazing has been observed in some residual heat removal (RHR) systems made of 304 stainless steel in PWR nuclear plants. This paper deals with two types of analyses including logical argumentation and simulation. Crack arrest in networks is demonstrated due to the presence of two cracks of the same depth in the network. This identical depth may be proved assuming that mean stress acts only on crack opening and that cracks are fully open during the load cycle before arrest. Weld residual stresses (WRS) are obtained by an axisymmetric simulation of welding on a tube with a chamfer. Axisymmetric and 3D parametric studies of crack growth on: representative sequences for variable amplitude thermal loading, fatigue crack growth threshold (FCGT), permanent mean stress, cyclic counting methods and WRS, are performed with Code-Aster software using XFEM methodology. The following results are obtained on crack depth versus time: the effect of WRS on crack growth cannot be determined by the initial WRS field in absence of crack, but by the associated stress intensity factor. Moreover the relation between crack arrest depth and WRS is analyzed. In the absence of FCGT Paris’s law may give a significant over-estimation of crack depth even if amplitudes of loading smaller than FCGT have not been considered. Appropriate depth versus time may be obtained using different values of FCGT, but axisymmetric simulations do not really show a possibility of arrest for shallow cracks in
Energy Technology Data Exchange (ETDEWEB)
Taheri, Said, E-mail: Said.taheri@edf.fr [EDF-LAB, IMSIA, 7 Boulevard Gaspard Monge, 91120 Palaiseau Cedex (France); Julan, Emricka [EDF-LAB, AMA, 7 Boulevard Gaspard Monge, 91120 Palaiseau Cedex (France); Tran, Xuan-Van [EDF Energy R& D UK Centre/School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, Manchester M13 9PL (United Kingdom); Robert, Nicolas [EDF-DPN, UNIE, Strategic Center, Saint Denis (France)
2017-01-15
Highlights: • For crack growth analysis, weld residual stress field must be considered through its SIF in presence of a crack. • Presence of cracks of same depth proves their arrest, where equal depth is because mean stress acts only on crack opening. • Not considering amplitudes under a fatigue crack growth threshold (FCGT) does not compensate the lack of FGCT in Paris law. • Propagation rates are close for axisymmetric and circumferential semi-elliptical cracks. - Abstract: High cycle thermal crazing has been observed in some residual heat removal (RHR) systems made of 304 stainless steel in PWR nuclear plants. This paper deals with two types of analyses including logical argumentation and simulation. Crack arrest in networks is demonstrated due to the presence of two cracks of the same depth in the network. This identical depth may be proved assuming that mean stress acts only on crack opening and that cracks are fully open during the load cycle before arrest. Weld residual stresses (WRS) are obtained by an axisymmetric simulation of welding on a tube with a chamfer. Axisymmetric and 3D parametric studies of crack growth on: representative sequences for variable amplitude thermal loading, fatigue crack growth threshold (FCGT), permanent mean stress, cyclic counting methods and WRS, are performed with Code-Aster software using XFEM methodology. The following results are obtained on crack depth versus time: the effect of WRS on crack growth cannot be determined by the initial WRS field in absence of crack, but by the associated stress intensity factor. Moreover the relation between crack arrest depth and WRS is analyzed. In the absence of FCGT Paris’s law may give a significant over-estimation of crack depth even if amplitudes of loading smaller than FCGT have not been considered. Appropriate depth versus time may be obtained using different values of FCGT, but axisymmetric simulations do not really show a possibility of arrest for shallow cracks in
Simplified method of computation for fatigue crack growth
International Nuclear Information System (INIS)
Stahlberg, R.
1978-01-01
A procedure is described for drastically reducing the computation time in calculating crack growth for variable-amplitude fatigue loading when the loading sequence is periodic. By the proposed procedure, the crack growth, r, per loading is approximated as a smooth function and its reciprocal is integrated, rather than summing crack growth cycle by cycle. The savings in computation time results since only a few pointwise values of r must be computed to generate an accurate interpolation function for numerical integration. Further time savings can be achieved by selecting the stress intensity coefficient (stress intensity divided by load) as the argument of r. Once r has been obtained as a function of stress intensity coefficient for a given material, environment, and loading sequence, it applies to any configuration of cracked structure. (orig.) [de
Crack propagation at stresses below the fatigue limit.
Holden, F. C.; Hyler, W. S.; Marschall, C. W.
1967-01-01
Crack propagation for stainless steel and Ti alloy at stresses below fatigue limit, noting of alternating stress cycles crack propagation for stainless steel and Ti alloy at stresses below fatigue limit, noting role of alternating stress cycles
Subsurface metals fatigue cracking without and with crack tip
Directory of Open Access Journals (Sweden)
Andrey Shanyavskiy
2013-07-01
Full Text Available Very-High-Cycle-Fatigue regime for metals was considered and mechanisms of the subsurface crack origination were introduced. In many metals first step of crack origination takes place with specific area formation because of material pressing and rotation that directed to transition in any volume to material ultra-high-plasticity with nano-structure appearing. Then by the border of the nano-structure takes place volume rotation and fracture surface creates with spherical particles which usually named Fine-Granular-Area. In another case there takes place First-Smooth-Facet occurring in area of origin due to whirls appearing by the one of the slip systems under discussed the same stress-state conditions. Around Fine-Granular-Area or First-Smooth-Facet there plastic zone appeared and, then, subsurface cracking develops by the same manner as for through cracks. In was discussed quantum-mechanical nature of fatigue crack growth in accordance with Yang’s modulus quantization for low level of deformations. New simply equation was considered for describing subsurface cracking in metals out of Fine-Granular-Area or Fist-Smooth-Facet.
Short fatigue cracks nucleation and growth in lean duplex stainless steel LDX 2101
Energy Technology Data Exchange (ETDEWEB)
Strubbia, R., E-mail: strubbia@ifir-conicet.gov.ar [Instituto de Física Rosario – CONICET, Universidad Nacional de Rosario (Argentina); Hereñú, S.; Alvarez-Armas, I. [Instituto de Física Rosario – CONICET, Universidad Nacional de Rosario (Argentina); Krupp, U. [Faculty of Engineering and Computer Science, University of Applied Sciences Osnabrück (Germany)
2014-10-06
This work is focused on the fatigue damage of lean duplex stainless steels (LDSSs) LDX 2101. Special interest is placed on analyzing short fatigue crack behavior. In this sense, short crack initiation and growth during low cycle fatigue (LCF) and short crack nucleation during high cycle fatigue (HCF) of this LDSS have been studied. The active slip systems and their associated Schmid factors (SF) are determined using electron backscattered diffraction (EBSD). Additionally, the dislocation structure developed during cycling is observed by transmission electron microscopy (TEM). Regardless of the fatigue regime, LCF and HCF, short cracks nucleate along intrusion/extrusions in ferritic grains. Moreover, during the LCF phase boundaries decelerate short crack propagation. These results are rationalized by the hardness of the constitutive phases and the dependence of screw dislocation mobility in the ferrite phase on strain rate and stress amplitude.
Fatigue crack layer propagation in silicon-iron
Birol, Y.; Welsch, G.; Chudnovsky, A.
1986-01-01
Fatigue crack propagation in metal is almost always accompanied by plastic deformation unless conditions strongly favor brittle fracture. The analysis of the plastic zone is crucial to the understanding of crack propagation behavior as it governs the crack growth kinetics. This research was undertaken to study the fatigue crack propagation in a silicon iron alloy. Kinetic and plasticity aspects of fatigue crack propagation in the alloy were obtained, including the characterization of damage evolution.
Role of plasticity-induced crack closure in fatigue crack growth
Directory of Open Access Journals (Sweden)
Jesús Toribio
2013-07-01
Full Text Available The premature contact of crack surfaces attributable to the near-tip plastic deformations under cyclic loading, which is commonly referred to as plasticity induced crack closure (PICC, has long been focused as supposedly controlling factor of fatigue crack growth (FCG. Nevertheless, when the plane-strain near-tip constraint is approached, PICC lacks of straightforward evidence, so that its significance in FCG, and even the very existence, remain debatable. To add insights into this matter, large-deformation elastoplastic simulations of plane-strain crack under constant amplitude load cycling at different load ranges and ratios, as well as with an overload, have been performed. Modeling visualizes the Laird-Smith conceptual mechanism of FCG by plastic blunting and re-sharpening. Simulation reproduces the experimental trends of FCG concerning the roles of stress intensity factor range and overload, but PICC has never been detected. Near-tip deformation patterns discard the filling-in a crack with material stretched out of the crack plane in the wake behind the tip as supposed PICC origin. Despite the absence of closure, load-deformation curves appear bent, which raises doubts about the trustworthiness of closure assessment from the compliance variation. This demonstrates ambiguities of PICC as a supposedly intrinsic factor of FCG and, by implication, favors the stresses and strains in front of the crack tip as genuine fatigue drivers.
Fatigue crack growth in Aluminium Alloys
Van Kranenburg, C.
2010-01-01
Fatigue is a gradual process of local strength reduction. It is a phenomenon of damage accumulation at stress concentrations caused by fluctuating stresses and/or strains. In metals this results in microscopic cracks. These will start to grow under continued cyclic loading until final failure
The Growth of Small Corrosion Fatigue Cracks in Alloy 7075
Piascik, Robert S.
2015-01-01
The corrosion fatigue crack growth characteristics of small (greater than 35 micrometers) surface and corner cracks in aluminum alloy 7075 is established. The early stage of crack growth is studied by performing in situ long focal length microscope (500×) crack length measurements in laboratory air and 1% sodium chloride (NaCl) environments. To quantify the "small crack effect" in the corrosive environment, the corrosion fatigue crack propagation behavior of small cracks is compared to long through-the-thickness cracks grown under identical experimental conditions. In salt water, long crack constant K(sub max) growth rates are similar to small crack da/dN.
Fatigue crack localization using laser nonliner wave modulation spectroscopy (LNWMS)
Energy Technology Data Exchange (ETDEWEB)
Liu, Peipei; Sohn, Hoon [Dept. of Civil and Environmental Engineering, Korea Advanced Institute of Science and Technology, Daejeon (Korea, Republic of); Kundu, Tribikram [Dept. of Civil Engineering and Engineering Mechanics, University of Arizona, Tucson (United States)
2016-12-15
Nonlinear features of ultrasonic waves are more sensitive to the presence of a fatigue crack than their linear counterparts are. For this reason, the use of nonlinear ultrasonic techniques to detect a fatigue crack at its early stage has been widely investigated. Of the different proposed techniques, laser nonlinear wave modulation spectroscopy (LNWMS) is unique because a pulse laser is used to exert a single broadband input and a noncontact measurement can be performed. Broadband excitation causes a nonlinear source to exhibit modulation at multiple spectral peaks owing to interactions among various input frequency components. A feature called maximum sideband peak count difference(MSPCD), which is extracted from the spectral plot, measures the degree of crack- induced material nonlinearity. First, the ratios of spectral peaks whose amplitudes are above a moving threshold to the total number of peaks are computed for spectral signals obtained from the pristine and the current state of a target structure. Then, the difference of these ratios are computed as a function of the moving threshold. Finally, the MSPCD is defined as the maximum difference between these ratios. The basic premise is that the MSPCD will increase as the nonlinearity of the material increases. This technique has been used successfully for localizing fatigue cracks in metallic plates.
Fatigue crack localization using laser nonlinear wave modulation spectroscopy (LNWMS)
Energy Technology Data Exchange (ETDEWEB)
Liu, Peipei; Sohn, Hoon [Dept. of Civil and Environmental Engineering, Korea Advanced Institute of Science and Technology, Daejeon (Korea, Republic of); Kundu, Tribikram [Dept. of Civil Engineering and Engineering Mechanics, University of Arizona, Tucson (United States)
2014-12-15
Nonlinear features of ultrasonic waves are more sensitive to the presence of a fatigue crack than their linear counterparts are. For this reason, the use of nonlinear ultrasonic techniques to detect a fatigue crack at its early stage has been widely investigated. Of the different proposed techniques, laser nonlinear wave modulation spectroscopy (LNWMS) is unique because a pulse laser is used to exert a single broadband input and a noncontact measurement can be performed. Broadband excitation causes a nonlinear source to exhibit modulation at multiple spectral peaks owing to interactions among various input frequency components. A feature called maximum sideband peak count difference (MSPCD), which is extracted from the spectral plot, measures the degree of crack-induced material nonlinearity. First, the ratios of spectral peaks whose amplitudes are above a moving threshold to the total number of peaks are computed for spectral signals obtained from the pristine and the current state of a target structure. Then, the difference of these ratios are computed as a function of the moving threshold. Finally, the MSPCD is defined as the maximum difference between these ratios. The basic premise is that the MSPCD will increase as the nonlinearity of the material increases. This technique has been used successfully for localizing fatigue cracks in metallic plates.
Fatigue crack growth in fiber-metal laminates
Ma, YuE; Xia, ZhongChun; Xiong, XiaoFeng
2014-01-01
Fiber-metal laminates (FMLs) consist of three layers of aluminum alloy 2024-T3 and two layers of glass/epoxy prepreg, and it (it means FMLs) is laminated by Al alloy and fiber alternatively. Fatigue crack growth rates in notched fiber-metal laminates under constant amplitude fatigue loading were studied experimentally and numerically and were compared with them in monolithic 2024-T3 Al alloy plates. It is shown that the fatigue life of FMLs is about 17 times longer than monolithic 2024-T3 Al alloy plate; and crack growth rates in FMLs panels remain constant mostly even when the crack is long, unlike in the monolithic 2024-T3 Al alloy plates. The formula to calculate bridge stress profiles of FMLs was derived based on the fracture theory. A program by Matlab was developed to calculate the distribution of bridge stress in FMLs, and then fatigue growth lives were obtained. Finite element models of FMLs were built and meshed finely to analyze the stress distributions. Both results were compared with the experimental results. They agree well with each other.
Thermal fatigue cracking of austenitic stainless steels
International Nuclear Information System (INIS)
Fissolo, A.
2001-01-01
This report deals with the thermal fatigue cracking of austenitic stainless steels as AISI 316 LN and 304 L. Such damage has been clearly observed for some components used in Fast Breeder reactors (FBR) and Pressure Water Reactor (PWR). In order to investigate thermal fatigue, quasi-structural specimen have been used. In this frame, facilities enforcing temperature variations similar to those found under the operation conditions have been progressively developed. As for components, loading results from impeded dilatation. In the SPLASH facility, the purpose was to establish accurate crack initiation conditions in order to check the relevance of the usual component design methodology. The tested specimen is continuously heated by the passage of an electrical DC current, and submitted to cyclic thermal down shock (up to 1000 deg C/s) by means of periodical spraying of water on two opposite specimen faces. The number of cycles to crack initiation N i is deduced from periodic examinations of the quenched surfaces, by means of optical microscopy. It is considered that initiation occurs when at least one 50μm to 150□m long crack is observed. Additional SPLASH tests were performed for N >> N i , with a view to investigate the evolution of a surface multiple cracking network with the number of cycles N. The CYTHIA test was mainly developed for the purpose of assessing crack growth dynamics of one isolated crack in thermal fatigue conditions. Specimens consist of thick walled tubes with a 1 mm circular groove is spark-machined at the specimen centre. During the test, the external wall of the tube is periodically heated by using a HF induction coil (1 MHz), while its internal wall is permanently cooled by flowing water. Total crack growth is derived from post-mortem examinations, whereby the thermal fatigue final rupture surface is oxidized at the end of the test. The specimen is broken afterwards under mechanical fatigue at room temperature. All the tests confirm that
Yang, Yang; Xiao, Li; Qu, Wenzhong; Lu, Ye
2017-11-01
Recent theoretical and experimental studies have demonstrated that a local Green's function can be retrieved from the cross-correlation of ambient noise field. This technique can be used to detect fatigue cracking in metallic structures, owing to the fact that the presence of crack can lead to a change in Green's function. This paper presents a method of structural fatigue cracking characterization method by measuring Green's function reconstruction from noise excitation and verifies the feasibility of crack detection in poor noise source distribution. Fatigue cracks usually generate nonlinear effects, in which different wave amplitudes and frequency compositions can cause different nonlinear responses. This study also undertakes analysis of the capacity of the proposed approach to identify fatigue cracking under different noise amplitudes and frequency ranges. Experimental investigations of an aluminum plate are conducted to assess the cross-correlations of received noise between sensor pairs and finally to detect the introduced fatigue crack. A damage index is proposed according to the variation between cross-correlations obtained from the pristine crack closed state and the crack opening-closure state when sufficient noise amplitude is used to generate nonlinearity. A probability distribution map of damage is calculated based on damage indices. The fatigue crack introduced in the aluminum plate is successfully identified and oriented, verifying that a fatigue crack can be detected by reconstructing Green's functions from an imperfect diffuse field in which ambient noise sources exist locally. Copyright © 2017 Elsevier B.V. All rights reserved.
Fatigue cracks in Eurofer 97 steel: Part II. Comparison of small and long fatigue crack growth
Czech Academy of Sciences Publication Activity Database
Kruml, Tomáš; Hutař, Pavel; Náhlík, Luboš; Seitl, Stanislav; Polák, Jaroslav
2011-01-01
Roč. 412, 1 (2011), s. 7-12 ISSN 0022-3115 R&D Projects: GA ČR GA106/09/1954; GA ČR GA101/09/0867 Institutional research plan: CEZ:AV0Z20410507 Keywords : ferritic-martensitic steel * long crack growth * small crack growth * crack closure Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.052, year: 2011
Nonlinear ultrasonic wave modulation for online fatigue crack detection
Sohn, Hoon; Lim, Hyung Jin; DeSimio, Martin P.; Brown, Kevin; Derriso, Mark
2014-02-01
This study presents a fatigue crack detection technique using nonlinear ultrasonic wave modulation. Ultrasonic waves at two distinctive driving frequencies are generated and corresponding ultrasonic responses are measured using permanently installed lead zirconate titanate (PZT) transducers with a potential for continuous monitoring. Here, the input signal at the lower driving frequency is often referred to as a 'pumping' signal, and the higher frequency input is referred to as a 'probing' signal. The presence of a system nonlinearity, such as a crack formation, can provide a mechanism for nonlinear wave modulation, and create spectral sidebands around the frequency of the probing signal. A signal processing technique combining linear response subtraction (LRS) and synchronous demodulation (SD) is developed specifically to extract the crack-induced spectral sidebands. The proposed crack detection method is successfully applied to identify actual fatigue cracks grown in metallic plate and complex fitting-lug specimens. Finally, the effect of pumping and probing frequencies on the amplitude of the first spectral sideband is investigated using the first sideband spectrogram (FSS) obtained by sweeping both pumping and probing signals over specified frequency ranges.
Quantitative Acoustic Emission Fatigue Crack Characterization in Structural Steel and Weld
Directory of Open Access Journals (Sweden)
Adutwum Marfo
2013-01-01
Full Text Available The fatigue crack growth characteristics of structural steel and weld connections are analyzed using quantitative acoustic emission (AE technique. This was experimentally investigated by three-point bending testing of specimens under low cycle constant amplitude loading using the wavelet packet analysis. The crack growth sequence, that is, initiation, crack propagation, and fracture, is extracted from their corresponding frequency feature bands, respectively. The results obtained proved to be superior to qualitative AE analysis and the traditional linear elastic fracture mechanics for fatigue crack characterization in structural steel and welds.
FASTRAN II - FATIGUE CRACK GROWTH STRUCTURAL ANALYSIS (UNIX VERSION)
Newman, J. C.
1994-01-01
Predictions of fatigue crack growth behavior can be made with the Fatigue Crack Growth Structural Analysis (FASTRAN II) computer program. As cyclic loads are applied to a selected crack configuration with an initial crack size, FASTRAN II predicts crack growth as a function of cyclic load history until either a desired crack size is reached or failure occurs. FASTRAN II is based on plasticity-induced crack-closure behavior of cracks in metallic materials and accounts for load-interaction effects, such as retardation and acceleration, under variable-amplitude loading. The closure model is based on the Dugdale model with modifications to allow plastically deformed material to be left along the crack surfaces as the crack grows. Plane stress and plane strain conditions, as well as conditions between these two, can be simulated in FASTRAN II by using a constraint factor on tensile yielding at the crack front to approximately account for three-dimensional stress states. FASTRAN II contains seventeen predefined crack configurations (standard laboratory fatigue crack growth rate specimens and many common crack configurations found in structures); and the user can define one additional crack configuration. The baseline crack growth rate properties (effective stress-intensity factor against crack growth rate) may be given in either equation or tabular form. For three-dimensional crack configurations, such as surface cracks or corner cracks at holes or notches, the fatigue crack growth rate properties may be different in the crack depth and crack length directions. Final failure of the cracked structure can be modelled with fracture toughness properties using either linear-elastic fracture mechanics (brittle materials), a two-parameter fracture criterion (brittle to ductile materials), or plastic collapse (extremely ductile materials). The crack configurations in FASTRAN II can be subjected to either constant-amplitude, variable-amplitude or spectrum loading. The applied
FASTRAN II - FATIGUE CRACK GROWTH STRUCTURAL ANALYSIS (IBM PC VERSION)
Newman, J. C.
1994-01-01
Predictions of fatigue crack growth behavior can be made with the Fatigue Crack Growth Structural Analysis (FASTRAN II) computer program. As cyclic loads are applied to a selected crack configuration with an initial crack size, FASTRAN II predicts crack growth as a function of cyclic load history until either a desired crack size is reached or failure occurs. FASTRAN II is based on plasticity-induced crack-closure behavior of cracks in metallic materials and accounts for load-interaction effects, such as retardation and acceleration, under variable-amplitude loading. The closure model is based on the Dugdale model with modifications to allow plastically deformed material to be left along the crack surfaces as the crack grows. Plane stress and plane strain conditions, as well as conditions between these two, can be simulated in FASTRAN II by using a constraint factor on tensile yielding at the crack front to approximately account for three-dimensional stress states. FASTRAN II contains seventeen predefined crack configurations (standard laboratory fatigue crack growth rate specimens and many common crack configurations found in structures); and the user can define one additional crack configuration. The baseline crack growth rate properties (effective stress-intensity factor against crack growth rate) may be given in either equation or tabular form. For three-dimensional crack configurations, such as surface cracks or corner cracks at holes or notches, the fatigue crack growth rate properties may be different in the crack depth and crack length directions. Final failure of the cracked structure can be modelled with fracture toughness properties using either linear-elastic fracture mechanics (brittle materials), a two-parameter fracture criterion (brittle to ductile materials), or plastic collapse (extremely ductile materials). The crack configurations in FASTRAN II can be subjected to either constant-amplitude, variable-amplitude or spectrum loading. The applied
Parametric analysis of fatigue crack growth
International Nuclear Information System (INIS)
Carden, A.E.
1975-01-01
The effect of temperature and frequency on fatigue crack growth were empirically observed and treated as a coefficient on a stress intensity factor term. The stress intensity factor term is a function of Ksub(max), Ksub(min) (or stress ratio) and a threshold K term. The apparent threshold values were selected in order to linearize the data. At 1000 0 F a constant da/dt (creep crack growth rate) is approached for cycle periods approaching 2000 s indicating a limiting and linear-inverse frequency effect. (author)
Fatigue crack growth from blunt notches
International Nuclear Information System (INIS)
Rhodes, D.
1982-01-01
A number of methods have been proposed, by which the formation and early growth of fatigue cracks at blunt notches may be predicted. In this report, four methods are compared - i.e. analysis of the crack tip plastic deformation, the cyclic contour integral, δJ, the strain in a critical volume of material, and the notch root plastic strain range. It is shown that these approaches have fundamental elements in common, and that all are compatable with linear elastic fracture mechanics. Early results from a continuing experimental programme are reported. (orig.) [de
A crack opening stress equation for fatigue crack growth
Newman, J. C., Jr.
1984-01-01
A general crack opening stress equation is presented which may be used to correlate crack growth rate data for various materials and thicknesses, under constant amplitude loading, once the proper constraint factor has been determined. The constraint factor, alpha, is a constraint on tensile yielding; the material yields when the stress is equal to the product of alpha and sigma. Delta-K (LEFM) is plotted against rate for 2024-T3 aluminum alloy specimens 2.3 mm thick at various stress ratios. Delta-K sub eff was plotted against rate for the same data with alpha = 1.8; the rates correlate well within a factor of two.
Thermographic Inspection of Fatigue Crack by Using Contact Thermal Resistance
Energy Technology Data Exchange (ETDEWEB)
Yang, Seung Yong; Kim, No Hyu [Korean University of Technology and Education, Cheonan (Korea, Republic of)
2013-04-15
Fatigue crack was detected from a temperature change around surface crack using the thermographic technique. Thermal gradient across the crack decreased very much due to thermal resistance of contact surface in the crack. Heat diffusion flow passing through the discontinuity was visualized in temperature by infrared camera to find and locate the crack. A fatigue crack specimen(SM-45C), which was prepared according to KS specification and notched in its center to initiate fatigue crack from the notch tip, was heated by halogen lamp at the end of one side to generate a heat diffusion flow in lateral direction. A abrupt jump in temperature across the fatigue crack was observed in thermographic image, by which the crack could be located and sized from temperature distribution.
Thermographic Inspection of Fatigue Crack by Using Contact Thermal Resistance
International Nuclear Information System (INIS)
Yang, Seung Yong; Kim, No Hyu
2013-01-01
Fatigue crack was detected from a temperature change around surface crack using the thermographic technique. Thermal gradient across the crack decreased very much due to thermal resistance of contact surface in the crack. Heat diffusion flow passing through the discontinuity was visualized in temperature by infrared camera to find and locate the crack. A fatigue crack specimen(SM-45C), which was prepared according to KS specification and notched in its center to initiate fatigue crack from the notch tip, was heated by halogen lamp at the end of one side to generate a heat diffusion flow in lateral direction. A abrupt jump in temperature across the fatigue crack was observed in thermographic image, by which the crack could be located and sized from temperature distribution.
Study on durability of welded bellows. Fatigue life of bellows with crack in welded bead
International Nuclear Information System (INIS)
Hirata, Osamu; Okada, Ken; Yanagisawa, Takasi; Nakajima, Akira.
1994-01-01
Reports of study for welded bellows with cracks have apparently not been published to date. The purpose of this investigation is to understand the relationship between the state of stress of welded bellows with micro cracks and the fatigue life. Stresses of welded bellows with cracks were calculated for several different crack lengths by finite element method (FEM), and lives of bellows with cracks were examined by fatigue test. The fatigue life, i.e. the number of cycles to failure was arranged against the remaining wall thickness measured after test instead of the crack length. As a result, it was found that there is a regular relationship between the stress amplitude of peak stress calculated by FEM and the fatigue life of bellows. And then, it was shown that the life of bellows becomes longer than the life estimated using a theoretical S-N curve calculated by Manson's method. Stress intensity factor range (ΔK) and crack propagation rate (da/dN) were also calculated using the results of stress analysis by FEM and fatigue test. The relationship between ΔK and da/dN obtained was almost coincident with the earlier result of fatigue crack growth test of Inconel 718 in the region of da/dN > 1.5x10 -6 mm/cycle, and the propriety of the present results was confirmed. (author)
Variable amplitude fatigue, modelling and testing
International Nuclear Information System (INIS)
Svensson, Thomas.
1993-01-01
Problems related to metal fatigue modelling and testing are here treated in four different papers. In the first paper different views of the subject are summarised in a literature survey. In the second paper a new model for fatigue life is investigated. Experimental results are established which are promising for further development of the mode. In the third paper a method is presented that generates a stochastic process, suitable to fatigue testing. The process is designed in order to resemble certain fatigue related features in service life processes. In the fourth paper fatigue problems in transport vibrations are treated
Fatigue crack growth retardation in spot heated mild steel sheet
Indian Academy of Sciences (India)
A fatigue crack can be effectively retarded by heating a spot near the crack tip under nil remote stress condition. The subcritical spot heating at a proper position modifies the crack growth behaviour in a way, more or less, similar to specimen subjected to overload spike. It is observed that the extent of crack growth retardation ...
Investigation of the fatigue crack opening under low cyclic loading
International Nuclear Information System (INIS)
Daunys, M.; Taraskevicius, A.
2003-01-01
Low cycle loading crack opening under various load levels were investigated. Analytical method of the fatigue crack opening investigation was described using relations of crack surface displacements. Calculated results of the crack surface displacement were compared with the experimental results. (author)
Fatigue crack growth and fracture behavior of bainitic rail steels.
2011-09-01
"The microstructuremechanical properties relationships, fracture toughness, fatigue crack growth and fracture surface morphology of J6 bainitic, manganese, and pearlitic rail steels were studied. Microstructuremechanical properties correlation ...
Fatigue strength depending on position of cracks for weldments
International Nuclear Information System (INIS)
Lee, Hae Woo; Park, Won Jo
2006-01-01
This is a study of fatigue strength of weld deposits with transverse cracks in plate up to 50 mm thick. It is concerned with the fatigue properties of welds already with transverse cracks. A previous study of transverse crack occurrence, location and microstructure in accordance with welding conditions was published in the Welding Journal (Lee et al., 1998). A fatigue crack develops as a result of stress concentration and extends with each load cycle until fatigue occurs, or until the cyclic loads are transferred to redundant members. The fatigue performance of a member is more dependent on the localized state of stress than the static strength of the base metal or the weld metal. Fatigue specimens were machined to have transverse cracks located on the surface and inside the specimen. Evaluation of fatigue strength depending on location of transverse cracks was then performed. When transverse cracks were propagated in a quarter-or half-circle shape, the specimen broke at low cycle in the presence of a surface crack. However, when the crack was inside the specimen, it propagated in a circular or elliptical shape and the specimen showed high fatigue strength, enough to reach the fatigue limit within tolerance of design stresses
Fatigue crack closure in submicron-thick freestanding copper films
International Nuclear Information System (INIS)
Kondo, Toshiyuki; Ishii, Takaki; Hirakata, Hiroyuki; Minoshima, Kohji
2015-01-01
The fatigue crack closure in approximately 500-nm-thick freestanding copper films were investigated by in situ field emission scanning electron microscope (FESEM) observations of the fatigue crack opening/closing behavior at three stress ratios of R=0.1, 0.5, and 0.8 in the low–K max (maximum stress intensity factor) region of K max <4.5 MPam 1/2 . The direct observation of fatigue cracks clarified that crack closure occurred at R=0.1 and 0.5, while the fatigue crack was always open at R=0.8. Changes in the gage distance across the fatigue crack during a fatigue cycle were measured from the FESEM images, and the crack opening stress intensity factor K op was evaluated on the basis of the stress intensity factor K vs. the gage distance relationship. The effective stress intensity factor range ΔK eff =K max −K op was then evaluated. The R-dependence of the da/dN vs. ΔK eff relationship was smaller than that of the da/dN vs. ΔK relationship. This suggests that ΔK eff is a dominating parameter rather than ΔK in the fatigue crack propagation in the films. This paper is the first report on the presence of the fatigue crack closure in submicron-thick freestanding metallic films
The assessment of creep-fatigue initiation and crack growth
International Nuclear Information System (INIS)
Priest, R.H.; Miller, D.A.
1991-01-01
An outline of Nuclear Electric's Assessment Procedure for the High Temperature Response of Structures ('R5') for creep-fatigue initiation and crack growth is given. A unified approach is adopted for both regimes. For initiation, total damage is described in terms of separate creep and fatigue components. Ductility exhaustion is used for estimating creep damage whilst continuous cycling endurance data are used to evaluate the fatigue damage term. Evidence supporting this approach is given through the successful prediction of creep-fatigue endurances for a range of materials, cycle types, dwell period times, etc. Creep-fatigue crack growth is similarly described in terms of separated creep and fatigue components. Crack growth rates for each component are characterised in terms of fracture mechanics parameters. It is shown that creep crack growth rates can be rationalised on a ductility basis. Creep-fatigue interactions are accommodated in the cyclic growth component through the use of materials coefficients which depend on dwell time. (orig.)
Fatigue crack nucleation of type 316LN stainless steel
International Nuclear Information System (INIS)
Kim, Dae Whan; Kim, Woo Gon; Hong, Jun Hwa; Ryu, Woo Seog
2000-01-01
Low Cycle Fatigue (LCF) life decreases drastically with increasing temperature but increases with the addition of nitrogen at room and high temperatures. The effect of nitrogen on LCF life may be related to crack nucleation at high temperatures in austenitic stainless steel because the fraction of crack nucleation in LCF life is about 40%. The influence of nitrogen on the crack nucleation of LCF in type 316LN stainless steel is investigated by observations of crack population and crack depth after testing at 40% of fatigue life. Nitrogen increases the number of cycles to nucleate microcracks of 100 μm but decreases the crack population
Detection and closure measurement of short fatigue crack initiated at notch root
International Nuclear Information System (INIS)
Lee, Jong-Hyung; Kobayashi, Hideo
1985-01-01
Short fatigue cracks initiated at the notch root were successfully detected at a fairly high accuracy by the ultrasonic amplitude calibration method for the notched compact specimens of an A508-3 steel. Crack closure measurements by the ultrasonic and back-face strain compliance methods were also performed. Crack growth characteristics at the notch root are similar to those of delyed retardation caused by a single peak overload. Also, transitional behavior from short cracks to long cracks was interpreted in terms of effective stress intensity ΔKsub(eff). The relation between crack growth rate da/dN and ΔKsub(eff) for short cracks shows a fairly good agreement with those for long cracks. (author)
Fatigue life assessment under multiaxial variable amplitude loading
International Nuclear Information System (INIS)
Morilhat, P.; Kenmeugne, B.; Vidal-Salle, E.; Robert, J.L.
1996-06-01
A variable amplitude multiaxial fatigue life prediction method is presented in this paper. It is based on a stress as input data are the stress tensor histories which may be calculated by FEM analysis or measured directly on the structure during the service loading. The different steps of he method are first presented then its experimental validation is realized for log and finite fatigue lives through biaxial variable amplitude loading tests using cruciform steel samples. (authors). 9 refs., 7 figs
Stress corrosion and corrosion fatigue crack growth monitoring in metals
International Nuclear Information System (INIS)
Senadheera, T.; Shipilov, S.A.
2003-01-01
Environmentally assisted cracking (including stress corrosion cracking and corrosion fatigue) is one of the major causes for materials failure in a wide variety of industries. It is extremely important to understand the mechanism(s) of environmentally assisted crack propagation in structural materials so as to choose correctly from among the various possibilities-alloying elements, heat treatment of steels, parameters of cathodic protection, and inhibitors-to prevent in-service failures due to stress corrosion cracking and corrosion fatigue. An important step towards understanding the mechanism of environmentally assisted crack propagation is designing a testing machine for crack growth monitoring and that simultaneously provides measurement of electrochemical parameters. In the present paper, a direct current (DC) potential drop method for monitoring crack propagation in metals and a testing machine that uses this method and allows for measuring electrochemical parameters during stress corrosion and corrosion fatigue crack growth are described. (author)
Stochastic modeling of thermal fatigue crack growth
Radu, Vasile
2015-01-01
The book describes a systematic stochastic modeling approach for assessing thermal-fatigue crack-growth in mixing tees, based on the power spectral density of temperature fluctuation at the inner pipe surface. It shows the development of a frequency-temperature response function in the framework of single-input, single-output (SISO) methodology from random noise/signal theory under sinusoidal input. The frequency response of stress intensity factor (SIF) is obtained by a polynomial fitting procedure of thermal stress profiles at various instants of time. The method, which takes into account the variability of material properties, and has been implemented in a real-world application, estimates the probabilities of failure by considering a limit state function and Monte Carlo analysis, which are based on the proposed stochastic model. Written in a comprehensive and accessible style, this book presents a new and effective method for assessing thermal fatigue crack, and it is intended as a concise and practice-or...
Mechanism of crack initiation and crack growth under thermal and mechanical fatigue loading
International Nuclear Information System (INIS)
Utz, S.; Soppa, E.; Silcher, H.; Kohler, C.
2013-01-01
The present contribution is focused on the experimental investigations and numerical simulations of the deformation behaviour and crack development in the austenitic stainless steel X6CrNiNb18-10 under thermal and mechanical cyclic loading in HCF and LCF regimes. The main objective of this research is the understanding of the basic mechanisms of fatigue damage and the development of simulation methods, which can be applied further in safety evaluations of nuclear power plant components. In this context the modelling of crack initiation and crack growth inside the material structure induced by varying thermal or mechanical loads are of particular interest. The mechanisms of crack initiation depend among other things on the type of loading, microstructure, material properties and temperature. The Nb-stabilized austenitic stainless steel in the solution-annealed condition was chosen for the investigations. Experiments with two kinds of cyclic loading - pure thermal and pure mechanical - were carried out and simulated. The fatigue behaviour of the steel X6CrNiNb18-10 under thermal loading was studied within the framework of the joint research project [4]. Interrupted thermal cyclic tests in the temperature range of 150 C to 300 C combined with non-destructive residual stress measurements (XRD) and various microscopic investigations, e.g. in SEM (Scanning Electron Microscope), were used to study the effects of thermal cyclic loading on the material. This thermal cyclic loading leads to thermal induced stresses and strains. As a result intrusions and extrusions appear inside the grains (at the surface), at which microcracks arise and evolve to a dominant crack. Finally, these microcracks cause a continuous and significant decrease of residual stresses. The fatigue behaviour of the steel X6CrNiNb18-10 under mechanical loading at room temperature was studied within the framework of the research project [5], [8]. With a combination of interrupted LCF tests and EBSD
Mechanism of crack initiation and crack growth under thermal and mechanical fatigue loading
Energy Technology Data Exchange (ETDEWEB)
Utz, S.; Soppa, E.; Silcher, H.; Kohler, C. [Stuttgart Univ. (Germany). Materials Testing Inst.
2013-07-01
The present contribution is focused on the experimental investigations and numerical simulations of the deformation behaviour and crack development in the austenitic stainless steel X6CrNiNb18-10 under thermal and mechanical cyclic loading in HCF and LCF regimes. The main objective of this research is the understanding of the basic mechanisms of fatigue damage and the development of simulation methods, which can be applied further in safety evaluations of nuclear power plant components. In this context the modelling of crack initiation and crack growth inside the material structure induced by varying thermal or mechanical loads are of particular interest. The mechanisms of crack initiation depend among other things on the type of loading, microstructure, material properties and temperature. The Nb-stabilized austenitic stainless steel in the solution-annealed condition was chosen for the investigations. Experiments with two kinds of cyclic loading - pure thermal and pure mechanical - were carried out and simulated. The fatigue behaviour of the steel X6CrNiNb18-10 under thermal loading was studied within the framework of the joint research project [4]. Interrupted thermal cyclic tests in the temperature range of 150 C to 300 C combined with non-destructive residual stress measurements (XRD) and various microscopic investigations, e.g. in SEM (Scanning Electron Microscope), were used to study the effects of thermal cyclic loading on the material. This thermal cyclic loading leads to thermal induced stresses and strains. As a result intrusions and extrusions appear inside the grains (at the surface), at which microcracks arise and evolve to a dominant crack. Finally, these microcracks cause a continuous and significant decrease of residual stresses. The fatigue behaviour of the steel X6CrNiNb18-10 under mechanical loading at room temperature was studied within the framework of the research project [5], [8]. With a combination of interrupted LCF tests and EBSD
Fatigue crack growth in additive manufactured products
Directory of Open Access Journals (Sweden)
A. Riemer
2015-10-01
Full Text Available Additive Manufacturing (AM is a new innovative technique that allows the direct fabrication of complex, individual, delicate and high-strength products, based on their 3D data. Selective Laser Melting (SLM is one of the AM processes that generates metallic components layer by layer using powder-bed technique. The irradiation and consequent melting of metallic powder is realised by the laser source. Employing SLM, especially complex and individual products, such as implants or aerospace parts, are well suited for economic production in small batches. The first important issue in this work was to analyse the fatigue crack growth (FCG in titanium alloy Ti-6-4 and stainless steel 316L processed by SLM. As a first step, stress intensity range decreasing tests were performed on SLM samples in their “as-built” condition. The next step was to adopt measures for optimisation of fatigue crack growth performance of SLM parts. For this purpose various heat treatments such as stress relief annealing and hot isostatic pressing (HIP were applied to the CT specimens. Finally, the strong impact of heat treatment on the residual lifetime was demonstrated by numerical fatigue crack growth simulations. For this purpose, the hip joint implant consisting of Ti-6-4 and processed by SLM was taken into account. It was found that residual stresses have a strong influence on the crack growth in Ti-6-4, while the influence of the micro-pores on the threshold values remains low. In contrast the results for 316L show that its fracturemechanical behaviour is not affected by residual stresses, whereas the microstructural features lead to modification in the da/dN-K-data. The second fundamental aim of this work was to demonstrate the possibilities of the SLM process. For that reason, the individually tailored bicycle crank was optimised regarding its weight and local stresses and finally manufactured using the SLM system. The iterative optimisation procedure was based on
Fatigue crack threshold relevant to stress ratio, crack wake and loading histories
International Nuclear Information System (INIS)
Okazaki, Masakazu; Iwasaki, Akira; Kasahara, Naoto
2013-01-01
Fatigue crack propagation behavior was investigated in a low alloy steel which experienced several kind of loading histories. Both the effects of stress ratio, test temperature on the fatigue crack threshold, and the change in the threshold depending on the thermo-mechanical loading histories, were experimentally investigated. It was shown that the thermo-mechanical loading history left its effect along the prior fatigue crack wake resulting in the change of fatigue crack threshold. Some discussions are made on how this type of loading history effect should be treated from engineering point of view. (author)
Continuum damage mechanics method for fatigue growth of surface cracks
International Nuclear Information System (INIS)
Feng Xiqiao; He Shuyan
1997-01-01
With the background of leak-before-break (LBB) analysis of pressurized vessels and pipes in nuclear plants, the fatigue growth problem of either circumferential or longitudinal semi-elliptical surface cracks subjected to cyclic loading is studied by using a continuum damage mechanics method. The fatigue damage is described by a scalar damage variable. From the damage evolution equation at the crack tip, a crack growth equation similar to famous Paris' formula is derived, which shows the physical meaning of Paris' formula. Thereby, a continuum damage mechanics approach is developed to analyze the configuration evolution of surface cracks during fatigue growth
Nonlinear ultrasonic fatigue crack detection using a single piezoelectric transducer
An, Yun-Kyu; Lee, Dong Jun
2016-04-01
This paper proposes a new nonlinear ultrasonic technique for fatigue crack detection using a single piezoelectric transducer (PZT). The proposed technique identifies a fatigue crack using linear (α) and nonlinear (β) parameters obtained from only a single PZT mounted on a target structure. Based on the different physical characteristics of α and β, a fatigue crack-induced feature is able to be effectively isolated from the inherent nonlinearity of a target structure and data acquisition system. The proposed technique requires much simpler test setup and less processing costs than the existing nonlinear ultrasonic techniques, but fast and powerful. To validate the proposed technique, a real fatigue crack is created in an aluminum plate, and then false positive and negative tests are carried out under varying temperature conditions. The experimental results reveal that the fatigue crack is successfully detected, and no positive false alarm is indicated.
Miniature specimen technology for postirradiation fatigue crack growth testing
International Nuclear Information System (INIS)
Mervyn, D.A.; Ermi, A.M.
1979-01-01
Current magnetic fusion reactor design concepts require that the fatigue behavior of candidate first wall materials be characterized. Fatigue crack growth may, in fact, be the design limiting factor in these cyclic reactor concepts given the inevitable presence of crack-like flaws in fabricated sheet structures. Miniature specimen technology has been developed to provide the large data base necessary to characterize irradiation effects on the fatigue crack growth behavior. An electrical potential method of measuring crack growth rates is employed on miniature center-cracked-tension specimens (1.27 cm x 2.54 cm x 0.061 cm). Results of a baseline study on 20% cold-worked 316 stainless steel, which was tested in an in-cell prototypic fatigue machine, are presented. The miniature fatigue machine is designed for low cost, on-line, real time testing of irradiated fusion candidate alloys. It will enable large scale characterization and development of candidate first wall alloys
The fatigue life and fatigue-crack-through-thickness behavior of a surface-cracked plate, 3
International Nuclear Information System (INIS)
Nam, Ki-Woo; Matsui, Kentaro; Ando, Kotoji; Ogura, Nobukazu
1989-01-01
The LBB (leak-before-break) design is one of the most important subjects for the evaluation and the assurance of safety in pressure vessels, piping systems, LNG carriers and various other structures. In the LBB design, it is necessary to evaluate precisely the lifetime of steel plate. Furthermore, the change in crack shape that occurs during the propagation after through thickness is of paramount importance. For this reason, in a previous report, the authors proposed a simplified evaluation model for the stress intensity factor after cracking through thickness. Using this model, the crack propagation behavior, crack-opening displacement and crack shape change of surface-cracked smooth specimens and surface-cracked specimens with a stress concentration were evaluated quantitatively. The present study was also done to investigate the fatigue crack propagation behavior of surface cracks subjected to combined tensile and bending stress. Estimation of fatigue crack growth was done using the Newman-Raju formula before through thickness, and using formula (7) and (8) after through thickness. Crack length a r at just through thickness increases with increasing a bending stress. Calculated fatigue crack shape showed very good agreement with experimental one. It was also found that particular crack growth behavior and change in crack shape after cracking through thickness can be explained quantitatively using the K value based on Eqs. (7) and (8). (author)
Fatigue crack propagation and delamination growth in Glare
Alderliesten, R.C.
2005-01-01
Fibre Metal Laminate Glare consists of thin aluminium layers bonded together with pre-impregnated glass fibre layers and shows an excellent fatigue crack growth behaviour compared to monolithic aluminium. The fibres are insensitive to the occurring fatigue loads and remain intact while the fatigue
Energy Technology Data Exchange (ETDEWEB)
Ranganathan, Narayanaswami; Leroy, Rene; Tougui, Abdellah [Laboratoire de Mecanique et Rheologie, Universite Francois Rabelais de Tours, Polytech Tours, Departement Mecanique et Conception de Systemes, Tours (France)
2009-09-15
Methods to estimate fatigue crack initiation life at a notch tip are compared. The methods used determine the strain amplitudes at the notch tip using Neuber's or Glinka's approximation. In conventional approaches, equivalent-damage levels are determined, using appropriate strain-life relationships coupled with damage-summation models. In the short-crack approach, a crack-like defect is assumed to exist at the notch tip. It is shown that the short-crack concept can be successfully applied to predict crack-initiation behavior at a notch. Model predictions are compared with carefully designed experiments. It is shown that model predictions are very close to experimentally measured lives under an aircraft-wing loading spectrum. (Abstract Copyright [2009], Wiley Periodicals, Inc.)
Wu, X. R.; Newman, J. C.; Zhao, W.; Swain, M. H.; Ding, C. F.; Phillips, E. P.
1998-01-01
The small crack effect was investigated in two high-strength aluminium alloys: 7075-T6 bare and LC9cs clad alloy. Both experimental and analytical investigations were conducted to study crack initiation and growth of small cracks. In the experimental program, fatigue tests, small crack and large crack tests A,ere conducted under constant amplitude and Mini-TWIST spectrum loading conditions. A pronounced small crack effect was observed in both materials, especially for the negative stress ratios. For all loading conditions, most of the fatigue life of the SENT specimens was shown to be crack propagation from initial material defects or from the cladding layer. In the analysis program, three-dimensional finite element and A weight function methods were used to determine stress intensity factors and to develop SIF equations for surface and corner cracks at the notch in the SENT specimens. A plastisity-induced crack-closure model was used to correlate small and large crack data, and to make fatigue life predictions, Predicted crack-growth rates and fatigue lives agreed well with experiments. A total fatigue life prediction method for the aluminum alloys was developed and demonstrated using the crack-closure model.
Growth behavior of fatigue cracks in ultrafine grained Cu smooth specimens with a small hole
Directory of Open Access Journals (Sweden)
Masahiro Goto
2015-10-01
Full Text Available In order to study the growth mechanism of fatigue cracks in ultrafine grained copper, stresscontrolled fatigue tests of round-bar specimens with a small blind hole as a crack starter were conducted. The hole was drilled on the surface where an intersection between the shear plane of the final ECAP processing and the specimen surface makes an angle of 45° or 90° with respect to the loading axis. At a low stress ( a = 90 MPa, the direction of crack paths was nearly perpendicular to the loading direction regardless of the location of the hole. Profile of crack face was examined, showing the aspect ratio (b/a of b/a = 0.82. At a high stress ( a = 240 MPa, although the growth directions inclined 45° and 90° to the loading-axis were observed depending on the location of the drilling hole, crack faces in these cracks were extended along one set of maximum shear stress planes, corresponding to the final ECAP shear plane. The value of aspect ratios was b/a = 0.38 and 1.10 for the cracks with 45° and 90° inclined path directions, respectively. The role of deformation mode at the crack tip areas on crack growth behavior were discussed in terms of the mixed-mode stress intensity factor. The crack path formation at high stress amplitudes was affected by the in-plane shear-mode deformation at the crack tip.
Effects of mechanical strain amplitude on the isothermal fatigue behavior of H13
Zeng, Yan; Zuo, Peng-peng; Wu, Xiao-chun; Xia, Shu-wen
2017-09-01
Isothermal fatigue (IF) tests were performed on H13 tool steel subjected to three different mechanical strain amplitudes at a constant temperature to determine the effects of mechanical strain amplitude on the microstructure of the steel samples. The samples' extent of damage after IF tests was compared by observation of their cracks and calculation of their damage parameters. Optical microscopy (OM) and scanning electron microscopy (SEM) were used to observe the microstructure of the samples. Cracks were observed to initiate at the surface because the strains and stresses there were the largest during thermal cycling. Mechanical strain accelerated the damage and softening of the steel. A larger mechanical strain caused greater deformation of the steel, which made the precipitated carbides easier to gather and grow along the deformation direction, possibly resulting in softening of the material or the initiation of cracks.
Thermally induced high frequency random amplitude fatigue damage at sharp notches
International Nuclear Information System (INIS)
Lewis, M.W.J.
1992-01-01
Experiments have been performed using the SUPERSOMITE facility to investigate the initiation and growth of fatigue cracks at the tips of sharp surface notches subjected to random thermally-induced stress. The experimental situation is complex involving plasticity, random amplitude loading and heat transfer medium/surface coupling. Crack initiation and growth prediction have been considered using the Creager and Neuber methods to compute the strain ranges in the vicinity of the notch root. Good agreement has been obtained between the experimental results and theoretical predictions. The paper reports the results of the analysis of the notch behavior
AE characteristic for monitoring of fatigue crack in steel bridge members
Yoon, Dong-Jin; Jung, Juong-Chae; Park, Philip; Lee, Seung-Seok
2000-06-01
Acoustic emission technique was employed for the monitoring of crack activity in both steel bridge members and laboratory specimen. Laboratory experiment was carried out to identify AE characteristics of fatigue cracks for compact tension specimen. The relationship between a stress intensity factor and AE signals activity as well as conventional AE parameter analysis was discussed. A field test was also conducted on a railway bridge, which contain several fatigue cracks. Crack activities were investigated while in service with strain measurement. From the results, in the laboratory tests, the features of three parameters such as the length of crack growth, the AE energy, and the cumulative AE events, showed the almost same trend in their increase as the number of fatigue cycle increased. From the comparisons of peak amplitude and AE energy with stress intensity factor, it was verified that the higher stress intensity factors generated AE signals with higher peak amplitude and a large number of AE counts. In the field test, real crack propagation signals were captured and the crack activity was verified in two cases.
Predominantly elastic crack growth under combined creep-fatigue cycling
International Nuclear Information System (INIS)
Lloyd, G.J.
1979-01-01
A rationalization of the various observed effects of combined creep-fatigue cycling upon predominantly elastic fatigue-crack propagation in austenitic steel is presented. Existing and new evidence is used to show two main groups of behaviour: (i) material and cycling conditions which lead to modest increases (6-8 times) in the rate of crack growth are associated with relaxation-induced changes in the material deformation characteristics, and (ii) material and cycling conditions severe enough to generate internal fracture damage lead to significant (up to a factor of 30) increases in crack growth rate when compared with fast-cycling crack propagation rates at the same temperature. A working hypothesis is presented to show that the boundary between the two groups occurs when the scale of the nucleated creep damage is of the same magnitude as the crack tip opening displacement. This leads to the possibility of unstable crack advance. Creep crack growth rates are shown to provide an upper bound to creep-fatigue crack growth rates when crack advance is unstable. If the deformation properties only are affected by the creep-fatigue cycling then creep crack growth rates provide a lower bound. The role of intergranular oxygen corrosion in very low frequency crack growth tests is also briefly discussed. (author)
Crack growth prediction for low-cycle fatigue regime
International Nuclear Information System (INIS)
Kamaya, Masayuki
2017-01-01
The objective of this study is to show a crack growth prediction procedure for the low-cycle fatigue regime. First, fatigue crack growth tests using Type 316 stainless steel specimens at room temperature were reviewed. It was seen that the crack growth rates correlated well with the equivalent stress intensify factor, which was derived using strain range instead of stress range. Furthermore, the effective equivalent stress intensify factor derived using the effective strain range exhibited excellent correlation with the crack growth rates obtained under various specimen geometries and loading conditions including high and low-cycle regimens. The obtained crack growth rates were also compared with the growth rate prescribed in the fitness-for-service code of the Japan Society of Mechanical Engineers (JSME). The test results agreed with the growth rate of JSME code. Finally, the procedure for predicting the low-cycle fatigue crack growth was shown. Although the JSME code is aimed at predicting fatigue crack growth for the so-called small scale yielding condition (high-cycle fatigue regime), the material constants determined for the high-cycle fatigue regime can be used even for the low-cycle fatigue regime. (author)
Crack closure in near-threshold fatigue crack propagation in railway axle steel EA4T
Czech Academy of Sciences Publication Activity Database
Pokorný, Pavel; Vojtek, Tomáš; Náhlík, Luboš; Hutař, Pavel
2017-01-01
Roč. 185, NOV (2017), s. 2-19 ISSN 0013-7944 R&D Projects: GA MŠk(CZ) LQ1601 Institutional support: RVO:68081723 Keywords : Fatigue crack propagation * crack closure * EA4T * Railway axle Subject RIV: JL - Materials Fatigue, Friction Mechanics OBOR OECD: Audio engineering , reliability analysis Impact factor: 2.151, year: 2016
Noncontact measurement of guided ultrasonic wave scattering for fatigue crack characterization
Fromme, P.
2013-04-01
Fatigue cracks can develop in aerospace structures at locations of stress concentration such as fasteners. For the safe operation of the aircraft fatigue cracks need to be detected before reaching a critical length. Guided ultrasonic waves offer an efficient method for the detection and characterization of fatigue cracks in large aerospace structures. Noncontact excitation of guided waves was achieved using electromagnetic acoustic transducers (EMAT). The transducers were developed for the specific excitation of the A0 Lamb mode. Based on the induced eddy currents in the plate a simple theoretical model was developed and reasonably good agreement with the measurements was achieved. However, the detection sensitivity for fatigue cracks depends on the location and orientation of the crack relative to the measurement locations. Crack-like defects have a directionality pattern of the scattered field depending on the angle of the incident wave relative to the defect orientation and on the ratio of the characteristic defect size to wavelength. The detailed angular dependency of the guided wave field scattered at crack-like defects in plate structures has been measured using a noncontact laser interferometer. Good agreement with 3D Finite Element simulation predictions was achieved for machined part-through and through-thickness notches. The amplitude of the scattered wave was quantified for a variation of angle of the incident wave relative to the defect orientation and the defect depth. These results provide the basis for the defect characterization in aerospace structures using guided wave sensors.
Suppression of Fatigue Crack Propagation of Duralumin by Cavitation Peening
Directory of Open Access Journals (Sweden)
Hitoshi Soyama
2015-08-01
Full Text Available It was demonstrated in the present paper that cavitation peening which is one of the mechanical surface modification technique can suppress fatigue crack propagation in duralumin. The impacts produced when cavitation bubble collapses can be utilised for the mechanical surface modification technique in the same way as laser peening and shot peening, which is called “cavitation peening”. Cavitation peening employing a cavitating jet in water was used to treat the specimen made of duralumin Japanese Industrial Standards JIS A2017-T3. After introducing a notch, fatigue test was conducted by a load-controlled plate bending fatigue tester, which has been originally developed. The fatigue crack propagation behavior was evaluated and the relationship between the fatigue crack propagation rate versus stress intensity factor range was obtained. From the results, the fatigue crack propagation rate was drastically reduced by cavitation peening and the fatigue life of duralumin plate was extended 4.2 times by cavitation peening. In addition, the fatigue crack propagation can be suppressed by 88% in the stable crack propagation stage by cavitation peening.
International Nuclear Information System (INIS)
Iida, Satoshi; Abe, Shigeki; Nakamura, Takao; Kamaya, Masayuki
2014-01-01
For preventing nuclear power plant (NPP) accidents, NPPs are required to ensure system safety in long term safe operation under aging degradation. Now, fatigue accumulation is one of major ageing phenomena and are evaluated to ensure safety by design fatigue curve that are based on the results of uniaxial fatigue tests. On the other hand, thermal stress that occurs in piping of actual components is not uniaxial but equi-biaxial. For accurate evaluation, it is required to conform real circumstance. In this study, membranous pressure fatigue test was conducted to simulated equi-biaxial stress. Crack initiation and crack growth were examined by replica investigation. Calculation result of equivalent stress intensity factor shows crack growth under equi-biaxial stress is faster than under uniaxial stress. It is concluded that equi-biaxial fatigue behavior should be considered in the evaluation of fatigue crack initiation and crack growth. (author)
Dislocation structures around crack tips of fatigued polycrystalline copper
International Nuclear Information System (INIS)
Kaneko, Yoshihisa; Ishikawa, Masao; Hashimoto, Satoshi
2005-01-01
Dislocation structures near fatigue cracks of polycrystalline copper specimens were analyzed using the electron channelling contrast imaging (ECCI) technique. Prior to the ECCI observations, optical microscopy was conducted to classify the fatigue crack morphologies into several kinds. It was found that the dislocation structures were correlated with the slip morphologies observed using the optical microscope. The cell structure almost corresponded to the severely deformed plastic zone where the individual slip bands could not be identified. The labyrinth dislocation structure was detected at the double-slip region. Ladder-like dislocation structure was detected ahead of the Stage I type fatigue crack. Hence, it can be said that the persistent slip band (PSB) was a favorable crack path. However, the microscopic route of the crack growth was not along the PSB but along the cell structure, which was developed locally in the vicinity of the crack tip
Directory of Open Access Journals (Sweden)
Elenice Maria Rodrigues
2005-09-01
Full Text Available Aluminum-lithium alloys are candidate materials for many aerospace applications because of their high specific strength and elastic modulus. These alloys have several unique characteristics such as excellent fatigue crack growth resistance when compared with that of the conventional 2000 and 7000 series alloys. In this study, fatigue crack propagation behavior has been examined in a commercial thin plate of Al-Li-Cu-Mg alloy (8090, with specific emphasis at the fatigue threshold. The results are compared with those of the traditional Al-Cu-Mg alloy (2024. Fatigue crack closure is used to explain the different behavior of the compared alloys.
Nanoscale and submicron fatigue crack growth in nickel microbeams
International Nuclear Information System (INIS)
Yang, Y.; Yao, N.; Imasogie, B.; Soboyejo, W.O.
2007-01-01
This paper presents a novel edge-notched microbeam technique for the study of short fatigue crack growth. The technique is used to study submicron and nanoscale fatigue in LIGA Ni thin films with columnar microstructures. The edge-notched microbeams were fabricated within LIGA Ni thin films, using focused ion beam (FIB) techniques. The microbeams were then cyclically deformed to failure at a stress ratio of 0.1. Different slip-band structures were observed below the nanoscale notches. Cyclic deformation resulted in the formation of primary slip bands below the notch. Subsequent crack growth then occurred by the unzipping of fatigue cracks along intersecting slip bands. The effects of the primary slip bands were idealized using dislocation-based models. These were used to estimate the intrinsic fatigue threshold and the fatigue endurance limit. The estimates from the model are shown to be consistent with experimental data from prior stress-life experiments and current/prior fatigue threshold estimates
Environmental effects of high temperature sodium of fatigue crack characteristics
International Nuclear Information System (INIS)
Abe, Hideaki; Takahashi, Kazuo; Ozawa, Kazumasa; Takahashi, Yukio
2004-01-01
In order to study fatigue crack growth characteristics in the components used in liquid sodium, fatigue tests were carried out at 550degC. This is near the system temperature used for sodium coolant in fast breeder reactors (FBRs). The factors influencing fatigue lifetime in sodium compared with that in air were investigated by observation of surface cracks in 316FR steel. Furthermore, the effects of sodium environment on fatigue were investigated based on examining the results of thermal striping tests, etc., obtained up to now. The results of the fatigue tests show that many micro cracks in the shearing direction were produced by the mid-lifetime, and micro cracks connected quickly after that. This is because an oxidation film was not formed, since sodium is of a reductive nature, and strain of the material surface tends to distribute equally. During crack progression there is no oxide formed on broken surfaces. Therefore re-combination between broken surfaces takes place, and crack progression rate falls. Furthermore, in non-propagating crack, the wedge effect by oxide between broken surfaces at the time of compression is small. Therefore, the crack closure angle is small, compression strain generated in the crack tip becomes large, and the crack cannot stop easily. As mentioned above, the main sodium influence on the fatigue characteristics are because of its reductive nature. In summary, in sodium environment, it is hard to form a crack and to get it to grow. Once started, however, it is hard to stop the crack in sodium compared with in the case of the air. (author)
Ductile cast irons: microstructure influence on fatigue crack propagation resistance
Directory of Open Access Journals (Sweden)
Mauro Cavallini
2010-07-01
Full Text Available Microstructure influence on fatigue crack propagation resistance in five different ductile cast irons (DCI was investigated. Four ferrite/pearlite volume fractions were considered, performing fatigue crack propagation tests according to ASTM E647 standard (R equals to 0.1, 0.5 and 0.75, respectively. Results were compared with an austempered DCI. Damaging micromechanisms were investigated according to the following procedures: - “traditional” Scanning Electron Microscope (SEM fracture surfaces analysis; - SEM fracture surface analysis with 3D quantitative analysis; - SEM longitudinal crack profile analysis - Light Optical Microscope (LOM transversal crack profile analysis;
Influence of a gaseous atmosphere on fatigue crack propagation
International Nuclear Information System (INIS)
Henaff, G.
2002-01-01
The paper presents a review of the current knowledge on the influence of gaseous atmospheres, and primarily ambient air, on fatigue crack propagation in metallic alloys. Experimental evidence of the effect of exposure to ambient air or any moist environment on fatigue crack propagation in steels is first proposed. The different interacting processes are analyzed so as to clearly uncouple the influence of the various factors on crack growth resistance. Two distinct mechanisms are identified: the adsorption of vapour molecules and hydrogen assisted fracture at crack tip. (author)
On the transition of short cracks into long fatigue cracks in reactor pressure vessel steels
Directory of Open Access Journals (Sweden)
Singh Rajwinder
2018-01-01
Full Text Available Short fatigue cracks, having dimension less than 1 mm, propagate at much faster rates (da/dN even at lower stress intensity factor range (da/dN as compared to the threshold stress intensity factor range obtained from long fatigue crack growth studies. These short cracks originate at the sub-grain level and some of them ultimately transit into critical long cracks over time. Therefore, designing the components subjected to fatigue loading merely on the long crack growth data and neglecting the short crack growth behavior can overestimate the component’s life. This aspect of short fatigue cracks become even more critical for materials used for safety critical applications such as reactor pressure vessel (RPV steel in nuclear plants. In this work, the transition behaviour of short fatigue crack gowth into long fatigue crack is studied in SA508 Grade 3 Class I low alloy steel used in RPVs. In-situ characterization of initiation, propagation and transition of short fatigue cracks is performed using fatigue stage for Scanning Electron Microscope (SEM in addition to digital microscopes fitted over a servo-hydraulic fatigue machine and correlated with the microtructural information obtained using electron backscatter diffraction (EBSD. SA508 steel having an upper bainitic microstructure have several microstructural interfaces such as phase and grain boundaries that play a significant role in controlling the short fatigue crack propagation. Specially designed and prepared short fatigue specimens (eletro-polished with varying initial crack lengths of the order of tens of microns are used in this study. The transition of such short initial cracks into long cracks is then tracked to give detailed insight into the role of each phase and phase/grain boundary with an objective of establishing Kitagawa-Takahashi diagram for the given RPV steel. The behavior of the transited long cracks is then compared with the crack propagation behavior obtained using
DEFF Research Database (Denmark)
Martakos, G.; Andreasen, J. H.; Berggreen, Christian
2017-01-01
A novel crack arresting device has been implemented in sandwich panels and tested using a special rig to apply out-of-plane loading on the sandwich panel face-sheets. Fatigue crack propagation was induced in the face-core interface of the sandwich panels which met the crack arrester. The effect o...
On fatigue crack growth in ductile materials by crack-tip blunting
DEFF Research Database (Denmark)
Tvergaard, Viggo
2004-01-01
One of the basic mechanisms for fatigue crack growth in ductile metals is that depending on crack-tip blunting under tensile loads and re-sharpening of the crack-tip during unloading. In a standard numerical analysis accounting for finite strains it is not possible to follow this process during...
Fatigue crack propagation in aluminum-lithium alloys
Rao, K. T. V.; Ritchie, R. O.; Piascik, R. S.; Gangloff, R. P.
1989-01-01
The principal mechanisms which govern the fatigue crack propagation resistance of aluminum-lithium alloys are investigated, with emphasis on their behavior in controlled gaseous and aqueous environments. Extensive data describe the growth kinetics of fatigue cracks in ingot metallurgy Al-Li alloys 2090, 2091, 8090, and 8091 and in powder metallurgy alloys exposed to moist air. Results are compared with data for traditional aluminum alloys 2024, 2124, 2618, 7075, and 7150. Crack growth is found to be dominated by shielding from tortuous crack paths and resultant asperity wedging. Beneficial shielding is minimized for small cracks, for high stress ratios, and for certain loading spectra. While water vapor and aqueous chloride environments enhance crack propagation, Al-Li-Cu alloys behave similarly to 2000-series aluminum alloys. Cracking in water vapor is controlled by hydrogen embrittlement, with surface films having little influence on cyclic plasticity.
Very high cycle fatigue crack initiation in electroplated Ni films under extreme stress gradients
International Nuclear Information System (INIS)
Baumert, E.K.; Pierron, O.N.
2012-01-01
A characterization technique based on kilohertz micro-resonators is presented to investigate the very high cycle fatigue behavior of 20 μm thick electroplated Ni films with a columnar microstructure (grain diameter less than 2 μm). The films exhibit superior fatigue resistance due to the extreme stress gradients at the surface. The effects of stress amplitude and environment on the formation of fatigue extrusions and micro-cracks are discussed based on scanning electron microscopy and the tracking of the specimens’ resonant frequency.
International Nuclear Information System (INIS)
Kim, Sung Jin; Kwon, Oh Yang; Jang, Yong Joon
2007-01-01
The fatigue crack growth behavior of a cracked and patch-repaired Ah2024-T3 panel has been monitored by acoustic emission(AE). The overall crack growth rate was reduced The crack propagation into the adjacent hole was also retarded by introducing the patch repair. AE signals due to crack growth after the patch repair and those due to debonding of the plate-patch interface were discriminated by using the principal component analysis. The former showed high center frequency and low amplitude, whereas the latter showed long rise tine, low frequency and high amplitude. This type of AE signal recognition method could be effective for the prediction of fatigue crack growth behavior in the patch-repaired structures with the aid of AE source location
Yang, Yi; Ng, Ching-Tai; Kotousov, Andrei; Sohn, Hoon; Lim, Hyung Jin
2018-01-01
This paper presents experimental and theoretical analyses of the second harmonic generation due to non-linear interaction of Lamb waves with a fatigue crack. Three-dimensional (3D) finite element (FE) simulations and experimental studies are carried out to provide physical insight into the mechanism of second harmonic generation. The results demonstrate that the 3D FE simulations can provide a reasonable prediction on the second harmonic generated due to the contact nonlinearity at the fatigue crack. The effect of the wave modes on the second harmonic generation is also investigated in detail. It is found that the magnitude of the second harmonic induced by the interaction of the fundamental symmetric mode (S0) of Lamb wave with the fatigue crack is much higher than that by the fundamental anti-symmetric mode (A0) of Lamb wave. In addition, a series of parametric studies using 3D FE simulations are conducted to investigate the effect of the fatigue crack length to incident wave wavelength ratio, and the influence of the excitation frequency on the second harmonic generation. The outcomes show that the magnitude and directivity pattern of the generated second harmonic depend on the fatigue crack length to incident wave wavelength ratio as well as the ratio of S0 to A0 incident Lamb wave amplitude. In summary, the findings of this study can further advance the use of second harmonic generation in damage detection.
Numerical analysis for prediction of fatigue crack opening level
International Nuclear Information System (INIS)
Choi, Hyeon Chang
2004-01-01
Finite Element Analysis (FEA) is the most popular numerical method to simulate plasticity-induced fatigue crack closure and can predict fatigue crack closure behavior. Finite element analysis under plane stress state using 4-node isoparametric elements is performed to investigate the detailed closure behavior of fatigue cracks and the numerical results are compared with experimental results. The mesh of constant size elements on the crack surface can not correctly predict the opening level for fatigue crack as shown in the previous works. The crack opening behavior for the size mesh with a linear change shows almost flat stress level after a crack tip has passed by the monotonic plastic zone. The prediction of crack opening level presents a good agreement with published experimental data regardless of stress ratios, which are using the mesh of the elements that are in proportion to the reversed plastic zone size considering the opening stress intensity factors. Numerical interpolation results of finite element analysis can precisely predict the crack opening level. This method shows a good agreement with the experimental data regardless of the stress ratios and kinds of materials
Fatigue failure and cracking in high mast poles.
2012-03-01
This report presents the findings of a comprehensive research project to investigate the fatigue : cracking and failure of galvanized high mast illumination poles (HMIP). Ultrasonic inspection of : poles throughout the state has revealed the presence...
Cyclic inelastic deformation aspects of fatigue-crack-growth analysis
Energy Technology Data Exchange (ETDEWEB)
Leis, B.N.; Zahoor, A.
1980-01-01
This paper concentrates on a J-integral analysis of fatigue crack growth. Data on cyclic plasticity are analyzed showing that there are limitations to the usefulness of the deformation theory in applications to cyclic plasticity. 56 refs.
Fatigue crack propagation under elastic plastic medium at elevated temperature
International Nuclear Information System (INIS)
Asada, Y.; Yuuki, R.; Sakon, T.; Sunamoto, D.; Tokimasa, K.; Makino, Y.; Kitagawa, M; Shingai, K.
1980-01-01
The purposes of the present study are to establish the testing method to obtain compatible data on the low cycle fatigue crack propagation at elevated temperature, and to investigate the parameter controlling the crack propagation rate. In the present study, the preliminary experiments have been carried out on low cycle fatigue crack propagation behaviour in type 304 stainless steel in air at 550 0 C, using two types of specimen with a through thickness notch. Both strain controlled and stress controlled fatigue tests have been done under a fully reversed strain or stress cycling. The data obtained are correlated with some fracture mechanics parameters and are discussed with the appropriate parameter for evaluating the low cycle fatigue crack propagation behaviour at elevated temperature. (author)
Fatigue Crack Propagation Simulation in Plane Stress Constraint
DEFF Research Database (Denmark)
Ricardo, Luiz Carlos Hernandes; Spinelli, Dirceu
2010-01-01
Nowadays, structural and materials engineers develop structures and materials properties using finite element method. This work presents a numerical determination of fatigue crack opening and closure stress intensity factors of a C(T) specimen. Two different standard variable spectrum loadings...... are utilized, Mini-Falstaff and Wisper. The effects in two-dimensional (2D) small scale yielding models of fatigue crack growth were studied considering plane stress constraint....
Fatigue crack shape prediction based on vertex singularity
Czech Academy of Sciences Publication Activity Database
Hutař, Pavel; Náhlík, Luboš
2008-01-01
Roč. 2, č. 1 (2008), s. 45-52 ISSN 1802-680X R&D Projects: GA ČR GA101/08/1623; GA ČR GP106/06/P239 Institutional research plan: CEZ:AV0Z20410507 Keywords : 3D vertex singularity * crack shape * fatigue crack propagation Subject RIV: JL - Materials Fatigue, Friction Mechanics
Continuous fatigue crack monitoring of bridges: Long-Term Electrochemical Fatigue Sensor (LTEFS)
Moshier, Monty A.; Nelson, Levi; Brinkerhoff, Ryan; Miceli, Marybeth
2016-04-01
Fatigue cracks in steel bridges degrade the load-carrying capacity of these structures. Fatigue damage accumulation caused by the repetitive loading of everyday truck traffic can cause small fatigue cracks initiate. Understanding the growth of these fatigue cracks is critical to the safety and reliability of our transportation infrastructure. However, modeling fatigue in bridges is difficult due to the nature of the loading and variations in connection integrity. When fatigue cracks reach critical lengths failures occur causing partial or full closures, emergency repairs, and even full structural failure. Given the aging US highway and the trend towards asset management and life extension, the need for reliable, cost effective sensors and monitoring technologies to alert bridge owners when fatigue cracks are growing is higher than ever. In this study, an innovative Long-Term Electrochemical Fatigue Sensor (LTEFS) has been developed and introduced to meet the growing NDT marketplace demand for sensors that have the ability to continuously monitor fatigue cracks. The performance of the LTEFS has been studied in the laboratory and in the field. Data was collected using machined specimens with different lengths of naturally initiated fatigue cracks, applied stress levels, applied stress ratios, and for both sinusoidal and real-life bridge spectrum type loading. The laboratory data was evaluated and used to develop an empirically based algorithm used for crack detection. Additionally, beta-tests on a real bridge structure has been completed. These studies have conclusively demonstrated that LTEFS holds great potential for long-term monitoring of fatigue cracks in steel structures
Fatigue crack growth behavior under cyclic thermal transient stress
International Nuclear Information System (INIS)
Ueda, Masahiro; Kano, Takashi; Yoshitoshi, Atsushi.
1986-01-01
Thermal fatigue tests were performed using straight pipe specimens subjected to cyclic thermal shocks of liquid sodium, and crack growth behaviors were estimated using striation patterns observed clearly on any crack surface. Crack growth rate under cyclic thermal strain reaches the maximum at one depth, and after that it decreases gradually with crack depth. The peak location of crack growth rate becomes deeper by superposition of constant primary stress. Parallel cracks co-existing in the neighborhood move the peak to shallower location and decrease the maximum crack growth rate. The equivalent stress intensity factor range calculated by Walker's formula is successfully applied to the case of negative stress ratio. Fatigue crack growth rate under cyclic thermal strain agreed well with that under the constant temperature equal to the maximum value in the thermal cycle. Simplified methods for calculating the stress intensity factor and the crack interference factor have been developed. Crack growth behavior under thermal fatigue could be well predicted using numerical analysis results. (author)
Fatigue crack growth behavior under cyclic transient thermal stress
International Nuclear Information System (INIS)
Ueda, Masahiro; Kano, Takashi; Yoshitoshi, Atsushi.
1987-01-01
Thermal fatigue tests were performed using straight pipe specimens subjected to cyclic thermal shocks of liquid sodium, and crack growth behaviors were estimated using striation patterns observed clearly on any crack surface. Crack growth rate under cyclic thermal strain reaches the maximum at one depth, and after that it decreases gradually with crack depth. The peak location of crack growth rate becomes deeper by superposition of constant primary stress. Parallel cracks co-existing in the neighborhood move the peak to shallower location and decrease the maximum crack growth rate. The equivalent stress intensity factor range calculated by Walker's formula is successfully applied to the case of negative stress ratio. Fatigue crack growth rate under cyclic thermal strain agreed well with that under the constant temperature equal to the maximum value in the thermal cycle. Simplified methods for calculating the stress intensity factor and the crack interference factor have been developed. Crack growth behavior under thermal fatigue could be well predicted using numerical analysis results. (author)
Biaxial fatigue crack propagation behavior of perfluorosulfonic-acid membranes
Lin, Qiang; Shi, Shouwen; Wang, Lei; Chen, Xu; Chen, Gang
2018-04-01
Perfluorosulfonic-acid membranes have long been used as the typical electrolyte for polymer-electrolyte fuel cells, which not only transport proton and water but also serve as barriers to prevent reactants mixing. However, too often the structural integrity of perfluorosulfonic-acid membranes is impaired by membrane thinning or cracks/pinholes formation induced by mechanical and chemical degradations. Despite the increasing number of studies that report crack formation, such as crack size and shape, the underlying mechanism and driving forces have not been well explored. In this paper, the fatigue crack propagation behaviors of Nafion membranes subjected to biaxial loading conditions have been investigated. In particular, the fatigue crack growth rates of flat cracks in responses to different loading conditions are compared, and the impact of transverse stress on fatigue crack growth rate is clarified. In addition, the crack paths for slant cracks under both uniaxial and biaxial loading conditions are discussed, which are similar in geometry to those found after accelerated stress testing of fuel cells. The directions of initial crack propagation are calculated theoretically and compared with experimental observations, which are in good agreement. The findings reported here lays the foundation for understanding of mechanical failure of membranes.
Analysis of Fatigue Crack Growth in Ship Structural Details
Directory of Open Access Journals (Sweden)
Leheta Heba W.
2016-04-01
Full Text Available Fatigue failure avoidance is a goal that can be achieved only if the fatigue design is an integral part of the original design program. The purpose of fatigue design is to ensure that the structure has adequate fatigue life. Calculated fatigue life can form the basis for meaningful and efficient inspection programs during fabrication and throughout the life of the ship. The main objective of this paper is to develop an add-on program for the analysis of fatigue crack growth in ship structural details. The developed program will be an add-on script in a pre-existing package. A crack propagation in a tanker side connection is analyzed by using the developed program based on linear elastic fracture mechanics (LEFM and finite element method (FEM. The basic idea of the developed application is that a finite element model of this side connection will be first analyzed by using ABAQUS and from the results of this analysis the location of the highest stresses will be revealed. At this location, an initial crack will be introduced to the finite element model and from the results of the new crack model the direction of the crack propagation and the values of the stress intensity factors, will be known. By using the calculated direction of propagation a new segment will be added to the crack and then the model is analyzed again. The last step will be repeated until the calculated stress intensity factors reach the critical value.
Fatigue crack growth in welded joints in seawater
Energy Technology Data Exchange (ETDEWEB)
Lambert, S.B.
1988-01-01
A pipe-to-plate specimen has been developed to study the influence of seawater on the fatigue behaviour of welded tubular joints. DC potential drop techniques have been used to detect fatigue crack initiation, and to monitor the subsequent growth of fatigue cracks. Results for three specimens, tested in air are compared with similar data for tubular and T-plate joints. These comparisons indicate that the pipe/plate is a reasonable model of a tubular joint. Testing was performed on a further six specimens in artificial seawater; two each with free corrosion, optimum cathodic protection, and cathodic overprotection. Fatigue life reduction factors compared with corresponding tests in air were 1.8 and 2.8 for free corrosion, 1.7 and 1.1 with cathodic protection, and 4.2 and 3.3 with cathodic over-protection. These fatigue life reduction factors were comparable to results on T-plate specimens, and were strongly dependent on crack shape development. Linear elastic fracture mechanics techniques appear suitable for the calculation of fatigue crack propagation life. Three approximate solution techniques for crack tip stress intensity factors show reasonable agreement with experimentally derived values. It is recommended that forcing functions be used to model crack aspect ratio development in welded joints. Such forcing functions are influenced by the initial stress distribution and the environment. 207 refs., 192 figs., 22 tabs.
Probabilistic modeling of crack networks in thermal fatigue
International Nuclear Information System (INIS)
Malesys, N.
2007-11-01
Thermal superficial crack networks have been detected in mixing zone of cooling system in nuclear power plants. Numerous experimental works have already been led to characterize initiation and propagation of these cracks. The random aspect of initiation led to propose a probabilistic model for the formation and propagation of crack networks in thermal fatigue. In a first part, uniaxial mechanical test were performed on smooth and slightly notched specimens in order to characterize the initiation of multiple cracks, their arrest due to obscuration and the coalescence phenomenon by recovery of amplification stress zones. In a second time, the probabilistic model was established under two assumptions: the continuous cracks initiation on surface, described by a Poisson point process law with threshold, and the shielding phenomenon which prohibits the initiation or the propagation of a crack if this one is in the relaxation stress zone of another existing crack. The crack propagation is assumed to follow a Paris' law based on the computation of stress intensity factors at the top and the bottom of crack. The evolution of multiaxial cracks on the surface can be followed thanks to three quantities: the shielding probability, comparable to a damage variable of the structure, the initiated crack density, representing the total number of cracks per unit surface which can be compared to experimental observations, and the propagating crack density, representing the number per unit surface of active cracks in the network. The crack sizes distribution is also computed by the model allowing an easier comparison with experimental results. (author)
Miniaturized fatigue crack growth specimen technology and results
International Nuclear Information System (INIS)
Puigh, R.J.; Bauer, R.E.; Ermi, A.M.; Chin, B.A.
1981-01-01
The miniature fatigue crack propagation technology has been extended to in-cell fabrication of irradiated specimens. Baseline testing of selected titanium alloys has been performed at 25 0 C in air. At relatively small values for the stress intensity factor, ΔK, the crack growth rates for all titanium alloys investigated are within a factor of three. The crack growth rates for these titanium alloys are a factor of three greater than the crack growth rates of either 316SS (20% CW) or HT-9. Each of the titanium alloys has observable crack propagation for stress intensity factors as small as 4.2 MPa√m
Mechanism of Fatigue Crack Growth of Bridge Steel Structures
Directory of Open Access Journals (Sweden)
Zhu H.
2016-12-01
Full Text Available This study was carried out on the background of Sutong Bridge project based on fracture mechanics, aiming at analyzing the growth mechanism of fatigue cracks of a bridge under the load of vehicles. Stress intensity factor (SIF can be calculated by various methods. Three steel plates with different kinds of cracks were taken as the samples in this study. With the combination of finite element analysis software ABAQUS and the J integral method, SIF values of the samples were calculated. After that, the extended finite element method in the simulation of fatigue crack growth was introduced, and the simulation of crack growth paths under different external loads was analyzed. At last, we took a partial model from the Sutong Bridge and supposed its two dangerous parts already had fine cracks; then simulative vehicle load was added onto the U-rib to predict crack growth paths using the extended finite element method.
Fatigue-crack propagation behavior of Inconel 718
International Nuclear Information System (INIS)
James, L.A.
1975-09-01
The techniques of linear-elastic fracture mechanics were used to characterize the effect of several variables (temperature, environment, cyclic frequency, stress ratio, and heat-treatment variations) upon the fatigue-crack growth behavior of Inconel 718 base metal and weldments. Relevant crack growth data on this alloy from other laboratories is also presented. (33 fig, 39 references)
Renovation techniques for fatigue cracked orthotropic steel bridge decks
de Jong, F.B.P.
2007-01-01
This dissertation presents the research into renovation techniques for orthotropic steel bridge decks. These techniques are needed to solve fatigue problems in the decks of these bridges, as several fatigue cracks have been detected in the deck structure of these bridges the last decade. A
Fatigue-crack growth behavior in dissimilar metal weldments
International Nuclear Information System (INIS)
James, L.A.
1977-03-01
The techniques of linear-elastic fracture mechanics were used to characterize fatigue-crack propagation behavior in three dissimilar metal weldments at test temperatures of 800 0 F (427 0 C) and 1000 0 F (538 0 C). The weldments studied included Inconel 718/Type 316, all using Inconel 82 as the filler metal. In general, fatigue-crack growth rates in the weldments were equal to, or less than, those observed in the base metals. Crack deviation from the expected path perpendicular to the loading axis was noted in some cases, and is discussed
Fatigue crack growth thresholds measurements in structural materials
International Nuclear Information System (INIS)
Lindstroem, R.; Lidar, P.; Rosborg, B.
1999-05-01
Fatigue crack growth thresholds and da/dN-data at low Δk I -values ( 1/2 ) have been determined for type 304 stainless steel, nickel-base weld metal Alloy 182, nickel-base metal Alloy 600, and low-alloy steel in air at ambient temperature and in high-temperature water and steam. The stainless alloys have been tested in water with 0.2 ppm O 2 at 288 deg C and the low-alloy steel in steam at 286 deg C. The fatigue crack growth threshold was defined as the ΔK I -value resulting in a crack growth rate of 10 -7 mm per cycle. The measured fatigue crack growth thresholds (at frequencies from 0.5 to 20 Hz) are quite similar independent of the material and the environment. A relatively inexpensive and time-saving method for measuring fatigue crack growth thresholds, and fatigue crack growth rates at low ΔK I -values, has been used in the tests. The method is a ΔK I -decreasing test with constant K I Max
Fatigue crack growth in austenitic stainless steel piping
International Nuclear Information System (INIS)
Bethmont, M.; Cheissoux, J.L.; Lebey, J.
1981-04-01
The study presented in this paper is being carried out with a view to substantiating the calculations of the fatigue crack growth in pipes made of 316 L stainless steel. The results obtained may be applied to P.W.R. primary piping. It is divided into two parts. First, fatigue tests (cyclic pressure) are carried out under hot and cold conditions with straight pipes machined with notches of various dimensions. The crack propagation and the fatigue crack growth rate are measured here. Second, calculations are made in order to interpret experimental results. From elastic calculations the stress intensity factor is assessed to predict the crack growth rate. The results obtained until now and presented in this paper relate to longitudinal notches
Standard test method for creep-fatigue crack growth testing
American Society for Testing and Materials. Philadelphia
2010-01-01
1.1 This test method covers the determination of creep-fatigue crack growth properties of nominally homogeneous materials by use of pre-cracked compact type, C(T), test specimens subjected to uniaxial cyclic forces. It concerns fatigue cycling with sufficiently long loading/unloading rates or hold-times, or both, to cause creep deformation at the crack tip and the creep deformation be responsible for enhanced crack growth per loading cycle. It is intended as a guide for creep-fatigue testing performed in support of such activities as materials research and development, mechanical design, process and quality control, product performance, and failure analysis. Therefore, this method requires testing of at least two specimens that yield overlapping crack growth rate data. The cyclic conditions responsible for creep-fatigue deformation and enhanced crack growth vary with material and with temperature for a given material. The effects of environment such as time-dependent oxidation in enhancing the crack growth ra...
Crack retardation by load reduction during fatigue crack propagation
International Nuclear Information System (INIS)
Kim, Hyun Soo; Nam, Ki Woo; Ahn, Seok Hwan; Do, Jae Yoon
2003-01-01
Fracture life and crack retardation behavior were examined experimentally using CT specimens of aluminum alloy 5083. Crack retardation life and fracture life were a wide difference between 0.8 and 0.6 in proportion to ratio of load reduction. The wheeler model retardation parameter was used successfully to predict crack growth behavior. By using a crack propagation rule, prediction of fracture life can be evaluated quantitatively. A statistical approach based on Weibull distribution was applied to the test data to evaluate the dispersion in the retardation life and fracture life by the change of load reduction
International Nuclear Information System (INIS)
Park, H. B.; Chopra, O. K.
2000-01-01
A fracture mechanics approach for elastic-plastic materials has been used to evaluate the effects of light water reactor (LWR) coolant environments on the fatigue lives of carbon and low-alloy steels. The fatigue life of such steel, defined as the number of cycles required to form an engineering-size crack, i.e., 3-mm deep, is considered to be composed of the growth of (a) microstructurally small cracks and (b) mechanically small cracks. The growth of the latter was characterized in terms of ΔJ and crack growth rate (da/dN) data in air and LWR environments; in water, the growth rates from long crack tests had to be decreased to match the rates from fatigue S-N data. The growth of microstructurally small cracks was expressed by a modified Hobson relationship in air and by a slip dissolution/oxidation model in water. The crack length for transition from a microstructurally small crack to a mechanically small crack was based on studies on small crack growth. The estimated fatigue S-N curves show good agreement with the experimental data for these steels in air and water environments. At low strain amplitudes, the predicted lives in water can be significantly lower than the experimental values
Directory of Open Access Journals (Sweden)
Ivo Černý
2009-11-01
Full Text Available Results of an investigation of effect of shot peening on development of physically short fatigue crack in an aircraft V-95 Al-alloy, which is of a similar type as 7075 alloy, are described and discussed in the paper. The first part deals with adaptation and verification of direct current potential drop method for detection and measurement of short crack initiation and growth. The specific material and quite large dimensions of flat specimens with side necking of a low stress concentration factor had to be considered when position of electrodes was specified and the measurement method verified. The specimen type and dimensions were proposed taking account of the investigation of shot peening effects. Physically short fatigue cracks of the length from 0.2 mm to more than 3 mm, most of them between 0.8 – 1.5 mm, were prepared under high cycle fatigue loading of a constant nominal stress amplitude plus/minus 160 MPa. Specimens with existing short fatigue cracks were shot peened using two different groups of parameters. Development of crack growth after shot peening was measured and compared with crack growth in specimens without shot peening. Retardation of crack growth was significant particularly with cracks shorter than 2 mm. For the specific stress amplitude, evaluated results enable to estimate threshold length of defects, which after the application of shot peening will be reliably arrested.
International Nuclear Information System (INIS)
Westphal, T; Nijssen, R P L
2014-01-01
The effect of Constant Life Diagram (CLD) formulation on the fatigue life prediction under variable amplitude (VA) loading was investigated based on variable amplitude tests using three different load spectra representative for wind turbine loading. Next to the Wisper and WisperX spectra, the recently developed NewWisper2 spectrum was used. Based on these variable amplitude fatigue results the prediction accuracy of 4 CLD formulations is investigated. In the study a piecewise linear CLD based on the S-N curves for 9 load ratios compares favourably in terms of prediction accuracy and conservativeness. For the specific laminate used in this study Boerstra's Multislope model provides a good alternative at reduced test effort
Westphal, T.; Nijssen, R. P. L.
2014-12-01
The effect of Constant Life Diagram (CLD) formulation on the fatigue life prediction under variable amplitude (VA) loading was investigated based on variable amplitude tests using three different load spectra representative for wind turbine loading. Next to the Wisper and WisperX spectra, the recently developed NewWisper2 spectrum was used. Based on these variable amplitude fatigue results the prediction accuracy of 4 CLD formulations is investigated. In the study a piecewise linear CLD based on the S-N curves for 9 load ratios compares favourably in terms of prediction accuracy and conservativeness. For the specific laminate used in this study Boerstra's Multislope model provides a good alternative at reduced test effort.
Fatigue crack paths under the influence of changes in stiffness
Directory of Open Access Journals (Sweden)
G. Kullmer
2016-02-01
Full Text Available An important topic of the Collaborative Research Centre TRR 30 of the Deutsche Forschungsgemeinschaft (DFG is the crack growth behaviour in graded materials. In addition, the growth of cracks in the neighbourhood of regions and through regions with different material properties belongs under this topic. Due to the different material properties, regions with differing stiffness compared to the base material may arise. Regions with differing stiffness also arise from ribs, grooves or boreholes. Since secure findings on the propagation behaviour of fatigue cracks are essential for the evaluation of the safety of components and structures, the growth of cracks near changes in stiffness has to be considered, too. Depending on the way a crack penetrates the zone of influence of such a change in stiffness and depending on whether this region is more compliant or stiffer than the surrounding area the crack may grow towards or away from this region. Both cases result in curved crack paths that cannot be explained only by the global loading situation. To evaluate the influence of regions with differing stiffness on the path of fatigue cracks the paths and the stress intensity factors of cracks growing near and through regions with differing stiffness are numerically determined with the program system ADAPCRACK3D. Therefore, arrangements of changes in stiffness modelled as material inclusions with stiffness properties different from the base material or modelled as ribs and grooves are systematically varied to develop basic conclusions about the crack growth behaviour near and through changes in stiffness.
Infrared thermography study of the fatigue crack propagation
Directory of Open Access Journals (Sweden)
O.A. Plekhov
2012-07-01
Full Text Available The work is devoted to the experimental study of heat dissipation process caused by fatigue crack propagation. To investigate a spatial and time temperature evolution at the crack tip set of experiments was carried out using specimens with pre-grown centered fatigue crack. An original mathematical algorithm for experimental data treatment was developed to obtain a power of heat source caused by plastic deformation at crack tip. The algorithm includes spatial-time filtration and relative motion compensation procedures. Based on the results of mathematical data treatment, we proposed a way to estimate the values of J-integral and stress intensity factor for cracks with pronounced the plastic zone.
International Nuclear Information System (INIS)
Torii, Tashiyuki; Toi, Norihiko; Nakano, Kohji; Honda, Kazuo
1998-01-01
Using the X-ray method of stress measurement for Ti-6Al-4V alloys, the residual stress near the crack was measured for annealed (AN) and solution treated and aged (STA) titanium alloys, under the condition that the measured X-ray stress was in satisfactory agreement with the applied stress under tension. The residual stress measured in the wake of the propagating fatigue crack, σ r , was compressive, resulting in a smaller crack opening displacement, COD, than theorized. The measured σ r and COD-values let us understand the fatigue crack propagation rate da/dN in terms of the effective stress intensity factor K eff . As a result, the da/dN under the same K eff -value was smaller in the AN specimen with zigzag crack growth than in the STA specimen with straight crack growth, although the da/dN-K eff relationship under various stress amplitudes was represented by a straight line in a log-log scale separately for the AN and STA specimens. (author)
Effects of Shot-Peening and Stress Ratio on the Fatigue Crack Propagation of AL 7475-T7351 Specimens
Directory of Open Access Journals (Sweden)
Natália Ferreira
2018-03-01
Full Text Available Shot peening is an attractive technique for fatigue enhanced performance of metallic components, because it increases fatigue crack initiation life prevention and retards early crack growth. Engineering design based on fatigue crack propagation predictions applying the principles of fracture mechanics is commonly used in aluminum structures for aerospace engineering. The main purpose of present work was to analyze the effect of shot peening on the fatigue crack propagation of the 7475 aluminum alloy, under both constant amplitude loading and periodical overload blocks. The tests were performed on 4 and 8 mm thickness specimens with stress ratios of 0.05 and 0.4. The analysis of the shot-peened surface showed a small increase of the micro-hardness values due to the plastic deformations imposed by shot peening. The surface peening beneficial effect on fatigue crack growth is very limited; its main effect is more noticeable near the threshold. The specimen’s thickness only has marginal influence on the crack propagation, in opposite to the stress ratio. Periodic overload blocks of 300 cycles promotes a reduction of the fatigue crack growth rate for both intervals of 7500 and 15,000 cycles.
Fatigue crack growth behaviour of the aluminium-lithium alloy 2090
International Nuclear Information System (INIS)
Tabrett, C.P.; McKeighan, P.C.; Smith, D.J.
1993-01-01
The fatigue crack growth (FCG) behavior of the aluminum lithium (Al-Li) alloy 2090-T84 has been investigated from a series of constant amplitude FCG tests. The influence of in plane orientation (L-T, T-L+45) and sheet thickness (1.6 and 6 mm) on the FCG rates for the rolled product has been examined. In general, the T-L orientation possess superior FCG resistance for both thicknesses and the 6 mm thick sheet material showed improved FCG resistance when compared to the 1.6 mm thick material for all orientations. It is believed this trend is related to the greater roughness and larger asperities found on the fatigue crack surfaces for the 6 mm thick material. Closure corrected FCG data suggests that much of the difference between the L-T and T-L orientation for the 6 mm thick sheet arise from variations in crack closure levels. (author)
Zhang, Wei; Bao, Zhangmin; Jiang, Shan; He, Jingjing
2016-06-17
In the aerospace and aviation sectors, the damage tolerance concept has been applied widely so that the modeling analysis of fatigue crack growth has become more and more significant. Since the process of crack propagation is highly nonlinear and determined by many factors, such as applied stress, plastic zone in the crack tip, length of the crack, etc. , it is difficult to build up a general and flexible explicit function to accurately quantify this complicated relationship. Fortunately, the artificial neural network (ANN) is considered a powerful tool for establishing the nonlinear multivariate projection which shows potential in handling the fatigue crack problem. In this paper, a novel fatigue crack calculation algorithm based on a radial basis function (RBF)-ANN is proposed to study this relationship from the experimental data. In addition, a parameter called the equivalent stress intensity factor is also employed as training data to account for loading interaction effects. The testing data is then placed under constant amplitude loading with different stress ratios or overloads used for model validation. Moreover, the Forman and Wheeler equations are also adopted to compare with our proposed algorithm. The current investigation shows that the ANN-based approach can deliver a better agreement with the experimental data than the other two models, which supports that the RBF-ANN has nontrivial advantages in handling the fatigue crack growth problem. Furthermore, it implies that the proposed algorithm is possibly a sophisticated and promising method to compute fatigue crack growth in terms of loading interaction effects.
Fatigue crack propagation in self-assembling nanocomposites
Energy Technology Data Exchange (ETDEWEB)
Klingler, Andreas; Wetzel, Bernd [Institute for Composite Materials (IVW GmbH) Technical University of Kaiserslautern, 67633 Kaiserslautern (Germany)
2016-05-18
Self-assembling block-copolymers allow the easy manufacturing of nanocomposites due to the thermodynamically driven in situ formation of nanosized phases in thermosetting resins during the curing process. Complex mechanical dispersion processes can be avoided. The current study investigates the effect of a block-copolymer on the fatigue crack propagation resistance of a cycloaliphatic amine cured epoxy resin. It was found that a small amount of MAM triblock-copolymer significantly increases the resistance to fatigue crack propagation of epoxy. Crack growth rate and the Paris law exponent for fatigue-crack growth were considerably reduced from m=15.5 of the neat epoxy to m=8.1 of the nanocomposite. To identify the related reinforcing and fracture mechanisms structural analyses of the fractured surfaces were performed by scanning electron microscope. Characteristic features were identified to be deformation, debonding and fracture of the nano-phases as well as crack pinning. However, the highest resistance against fatigue crack propagation was achieved in a bi-continuous microstructure that consisted of an epoxy-rich phase with embedded submicron sized MAM inclusions, and which was surrounded by a block-copolymer-rich phase that showed rupture and plastic deformation.
Fatigue crack propagation in self-assembling nanocomposites
Klingler, Andreas; Wetzel, Bernd
2016-05-01
Self-assembling block-copolymers allow the easy manufacturing of nanocomposites due to the thermodynamically driven in situ formation of nanosized phases in thermosetting resins during the curing process. Complex mechanical dispersion processes can be avoided. The current study investigates the effect of a block-copolymer on the fatigue crack propagation resistance of a cycloaliphatic amine cured epoxy resin. It was found that a small amount of MAM triblock-copolymer significantly increases the resistance to fatigue crack propagation of epoxy. Crack growth rate and the Paris law exponent for fatigue-crack growth were considerably reduced from m=15.5 of the neat epoxy to m=8.1 of the nanocomposite. To identify the related reinforcing and fracture mechanisms structural analyses of the fractured surfaces were performed by scanning electron microscope. Characteristic features were identified to be deformation, debonding and fracture of the nano-phases as well as crack pinning. However, the highest resistance against fatigue crack propagation was achieved in a bi-continuous microstructure that consisted of an epoxy-rich phase with embedded submicron sized MAM inclusions, and which was surrounded by a block-copolymer-rich phase that showed rupture and plastic deformation.
Fatigue crack propagation in self-assembling nanocomposites
International Nuclear Information System (INIS)
Klingler, Andreas; Wetzel, Bernd
2016-01-01
Self-assembling block-copolymers allow the easy manufacturing of nanocomposites due to the thermodynamically driven in situ formation of nanosized phases in thermosetting resins during the curing process. Complex mechanical dispersion processes can be avoided. The current study investigates the effect of a block-copolymer on the fatigue crack propagation resistance of a cycloaliphatic amine cured epoxy resin. It was found that a small amount of MAM triblock-copolymer significantly increases the resistance to fatigue crack propagation of epoxy. Crack growth rate and the Paris law exponent for fatigue-crack growth were considerably reduced from m=15.5 of the neat epoxy to m=8.1 of the nanocomposite. To identify the related reinforcing and fracture mechanisms structural analyses of the fractured surfaces were performed by scanning electron microscope. Characteristic features were identified to be deformation, debonding and fracture of the nano-phases as well as crack pinning. However, the highest resistance against fatigue crack propagation was achieved in a bi-continuous microstructure that consisted of an epoxy-rich phase with embedded submicron sized MAM inclusions, and which was surrounded by a block-copolymer-rich phase that showed rupture and plastic deformation.
Fatigue cracks in Eurofer 97 steel: Part I. Nucleation and small crack growth kinetics
Czech Academy of Sciences Publication Activity Database
Kruml, Tomáš; Polák, Jaroslav
2011-01-01
Roč. 412, 1 (2011), s. 2-6 ISSN 0022-3115 R&D Projects: GA ČR GA106/09/1954; GA ČR GA101/09/0867 Institutional research plan: CEZ:AV0Z20410507 Keywords : ferritic-martensitic steel * low cycle fatigue * small crack growth * fatigue life prediction Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.052, year: 2011
Directory of Open Access Journals (Sweden)
Filippo Berto
2016-10-01
Full Text Available The torsional fatigue behaviour of circumferentially notched specimens made of austenitic stainless steel, SUS316L, and carbon steel, SGV410, characterized by different notch root radii has been recently investigated by Tanaka. In that contribution, it was observed that the total fatigue life of the austenitic stainless steel increases with increasing stress concentration factor for a given applied nominal shear stress amplitude. By using the electrical potential drop method, Tanaka observed that the crack nucleation life was reduced with increasing stress concentration, on the other hand the crack propagation life increased. The experimental fatigue results, originally expressed in terms of nominal shear stress amplitude, have been reanalysed by means of the local strain energy density (SED averaged over a control volume having radius R0 surrounding the notch tip. To exclude all extrinsic effects acting during the fatigue crack propagation phase, such as sliding contact and/or friction between fracture surfaces, crack initiation life has been considered in the present work. In the original paper, initiation life was defined in correspondence of a 0.1÷0.4-mm-deep crack. The control radius R0 for fatigue strength assessment of notched components, thought of as a material property, has been estimated by imposing the constancy of the averaged SED for both smooth and cracked specimens at NA = 2 million loading cycles
Detection and measurement of fatigue cracks in welded joints
International Nuclear Information System (INIS)
Smith, F.C.
1985-01-01
A direct current potential drop system was developed for the detection and measurement of very small fatigue cracks that grow from the toes of welds. Measurement of crack growth less than 0.01 mm and of crack growth rates less than 10 -10 m/cycle, even for cracks less than 1.0 mm deep, is made possible by using a high stability measurement apparatus and an adjustment based on initial conditions. Thus far, the measurement system has successfully examined several aspects of fatigue in welded elements. Crack growth results justified the use of a linear elastic expression for the stress intensity factor and provided an evaluation of a growth law which includes the threshold stress intensity factor. Needle peening fillet welded joints did not change the small proportion of crack initiation life to total fatigue life observed for untreated (not improved) welded joints. However, the measurement system demonstrated that needle peening retarded crack growth rates up to 1 mm depth below the weld toe
Estimation of Fatigue Crack Growth Behavior of Cracked Specimen Under Mixed-mode Loads
International Nuclear Information System (INIS)
Han, Jeong Woo; Woo, Eun Taek; Han, Seung Ho
2015-01-01
To estimate the fatigue crack propagation behavior of compact tension shear (CTS) specimen under mixed-mode loads, crack path prediction theories and Tanaka’s equation were applied. The stress intensity factor at a newly created crack tip was calculated using a finite element method via ANSYS, and the crack path and crack increment were then obtained from the crack path prediction theories, Tanaka’s equation, and the Paris’ equation, which were preprogrammed in Microsoft Excel. A new method called the finite element crack tip updating method (FECTUM) was developed. In this method, the finite element method and Microsoft Excel are used to calculate the stress intensity factors and the crack path, respectively, at the crack tip per each crack increment. The developed FECTUM was applied to simulate the fatigue crack propagation of a single-edge notched bending (SENB) specimen under eccentric three-point bending loads. The results showed that the number of cycles to failure of the specimen obtained experimentally and numerically were in good agreement within an error range of less than 3%
Estimation of Fatigue Crack Growth Behavior of Cracked Specimen Under Mixed-mode Loads
Energy Technology Data Exchange (ETDEWEB)
Han, Jeong Woo [KIMM, Daejeon (Korea, Republic of); Woo, Eun Taek; Han, Seung Ho [Dong-A University, Busan (Korea, Republic of)
2015-07-15
To estimate the fatigue crack propagation behavior of compact tension shear (CTS) specimen under mixed-mode loads, crack path prediction theories and Tanaka’s equation were applied. The stress intensity factor at a newly created crack tip was calculated using a finite element method via ANSYS, and the crack path and crack increment were then obtained from the crack path prediction theories, Tanaka’s equation, and the Paris’ equation, which were preprogrammed in Microsoft Excel. A new method called the finite element crack tip updating method (FECTUM) was developed. In this method, the finite element method and Microsoft Excel are used to calculate the stress intensity factors and the crack path, respectively, at the crack tip per each crack increment. The developed FECTUM was applied to simulate the fatigue crack propagation of a single-edge notched bending (SENB) specimen under eccentric three-point bending loads. The results showed that the number of cycles to failure of the specimen obtained experimentally and numerically were in good agreement within an error range of less than 3%.
Influence of dissolved hydrogen on the fatigue crack growth behaviour of AISI 4140 steel
Ramasagara Nagarajan, Varun
hydrogen induced failure mechanism in this material during cyclic loading. The secondary objective of this investigation was to determine the role of inclusions and their influence in affecting the fatigue crack growth rate of this material. Compact tension and tensile specimens were prepared as per ASTM E-647, E-399 and E-8 standards. The specimens were tested in three different heat treated conditions i.e. annealed (as received) as well as two austempered conditions. These specimens were precharged with hydrogen (ex situ) using cathodic charging method at a constant current density at three different time periods ranging from 150 to 250 hours before conducting fatigue crack growth tests. Mode 1 type fatigue tests were then performed in ambient atmosphere at constant amplitude using load ratio R of 0.1. The near threshold fatigue crack growth rate, fatigue threshold and the fatigue crack growth rate in the linear region were determined. Fatigue crack growth behaviour of specimens without any dissolve hydrogen were then compared with the specimens with different concentration of dissolved hydrogen. The test results show that the dissolved hydrogen concentration increases with the increase in charging time in all three heat treated conditions and the hydrogen uptake shows a strong dependence on the microstructure of the alloy. It was also observed that the microstructure has a significant influence of on the fatigue crack growth and SCC behaviour of the alloy with dissolved hydrogen. As the dissolved hydrogen concentration increases, the fatigue threshold was found to decrease and the near threshold crack growth rate increases in all three heat treated conditions showing the deleterious effect of hydrogen, but to a different extent in each condition. Current test results also indicate that the fatigue crack growth rates in the linear region increases as the dissolved hydrogen content increases in all three heat treated conditions. It is also observed that increasing the
Fatigue crack initiation and growth life prediction with statistical consideration
International Nuclear Information System (INIS)
Kwon, J.D.; Choi, S.H.; Kwak, S.G.; Chun, K.O.
1991-01-01
Life prediction or residual life prediction of structures or machines is one of the most strongly world wide needed problems as requirement in the stage of slowly developing economy which comes after rapidly and highly developing stage. For the purpose of statistical life prediction, fatigue test was conducted under the 3 stress levels, and for each stress level, 20 specimens are used. The statistical properties of the crack growth parameter m and C in the fatigue crack growth law of da/dN = C(ΔK) m , and the relationship between m and C, and the statistical distribution pattern of fatigue crack initiation, growth and fracture lives can be obtained by experimental results
Thermal fatigue crack growth analysis in a nozzle corner
International Nuclear Information System (INIS)
Blauel, J.G.; Hodulak, L.
1983-01-01
Calculations of the crack growth under local thermal shock fatigue are performed. Estimates of crack growth are based on stress distributions obtained by a finite element analysis for thermal transients in the structure without crack. Stress intensity factors are calculated using interpolation formulae derived from known basic solutions for part-through cracks under constant and linearly varying load. The crack propagation at selected parts of the crack front is calculated stepwise by integration of the Paris law with material constants C and n interpolated from test results on compact specimens at constant temperatures. Experimental results for the model vessel test MB1 at an internal pressure of 14 N/mm 2 and a temperature of 320 0 C exposed to a repeated local spraying with cold water are presented and compared to predictions
Investigation of fatigue crack growth rate of Al 5484 ultrafine grained alloy after ECAP process
Energy Technology Data Exchange (ETDEWEB)
Brynk, Tomasz; Rasinski, Marcin; Pakiela, Zbigniew; Kurzydlowski, Krzysztof J. [Faculty of Materials Science and Engineering, Warsaw University of Technology (Poland); Olejnik, Lech [Faculty of Production Engineering, Warsaw University of Technology (Poland)
2010-05-15
During the last decade equal-channel angular pressing (ECAP) has emerged as a widely used fabrication route of ultrafine-grained (UFG) metals and alloys. Enhanced mechanical properties of UFG materials produced by severe plastic deformation, with a grain size smaller than 1 {mu}m, have been reported in a large number of publications. However, the higher strength does not imply higher resistance to fatigue both high- and low-cyclic. In fact, due to reduced plasticity, higher fatigue crack propagation rates are reported for UFG materials, particularly in low-amplitude range. The aim of this work was to investigate fatigue crack propagation in samples of Al 5483 alloy subjected to ECAP treatment. Because of small dimensions of the coupons processed by ECAP, non-standard, mini-samples were used in a crack propagation tests. Two test procedures were used to estimate stress intensity factor (K). The first was based on optical measurements of crack length from images recorded during the test. The second method was based on digital image correlation (DIC), which was used to determine K value directly from displacement field near the crack tip. Comparison of these two methods is made and the relationship between the intensity of ECAP process (measured in terms of the number of ECAP passes) and fatigue crack propagation rates proposed. In addition to fatigue resistance, the results of tensile tests carried out with mini-samples are presented. Applicability of such samples in the investigations of the mechanical properties of UFG materials is discussed. (Abstract Copyright [2010], Wiley Periodicals, Inc.)
Study of regularities in propagation of thermal fatigue cracks
International Nuclear Information System (INIS)
Tachkova, N.G.; Sobolev, N.D.; Egorov, V.I.; Rostovtsev, Yu.V.; Ivanov, Yu.S.; Sirotin, V.L.
1978-01-01
Regularities in the propagation of thermal fatigue cracks in the Cr-Ni steels of the austenite class depending upon deformation conditions in the crack zone, have been considered. Thin-walled tube samples of the Kh16N40, Kh18N20 and Kh16N15 steels have been tested in the 10O reversible 400 deg C and 100 reversible 500 deg C regimes. The samples have possessed a slot-shaped stress concentrator. Stress intensity pseudocoefficient has been calculated for the correlation of experimental data. The formula for determining crack propagation rate has been obtained. The experiments permit to conclude that propagation rate of thermal fatigue cracks in the above steels depends upon the scope of plastic deformation during a cycle and stress intensity pseudocoefficient, and is determined by plastic deformation resistance during thermal cyclic loading
Equation of short fatigue crack growth law of 1Cr18Ni9Ti weld metal
International Nuclear Information System (INIS)
Zhao Yongxiang; Yang Bing; Gao Qing
2005-01-01
The method is investigated for characterizing the short fatigue crack (SFC) behaviour of 1Cr18Ni9Ti weld metal by the 'effective short fatigue crack criterion'. Three considerations are given. Firstly, the dominant effective short fatigue crack (DESFC) behaviour is a result of the interaction and evolution of the collective SFCs and, therefore, it is deemed suitable to describe their collective behaviour. Secondly, the significant character of microstructural short crack (MSC) regime and physical short crack (PSC) regime for the behaviour of SFCs indicates that it should be well exhibited in the characterization. Thirdly, the stronger irregular behaviour of SFCs indicates the single parameter of cyclic stress or strain amplitude for representing driving force of DESFC growth may be not appropriated. A new growth law for the collective SFCs is derived from a consideration of the local cyclic strain energy density driving the DESFC initiation in the initial zone and, then, driving the DESFC growth in the zones around its tips. The final form of this law is relative to the total cyclic strain energy density of remote fields, which circle the initial zone and, then, the zones around the DESFC tips. Availability has been indicated by an analysis of the test data of present material. (authors)
Fatigue crack growth rate of API X70 steel pipelines under spectrum loading
International Nuclear Information System (INIS)
Beden, S.M.; Abdullah, S.; Ariffin, A.K.
2012-01-01
Pipelines offer the most efficient way to transport bulk quantities of gas and oil, either from points of production to storage locations or from storage locations to distributed points of end use. As one of the main materials of west–east gas transmission pipes, X70 pipelines usually serve under variable amplitude loading (VAL). Base on the importance of in-service API X70 pipelines, it is important for the safe operation of this system to know its behaviour under VAL. This paper focuses on the ability of using the NASGRO model to predict the fatigue crack growth (FCG), based on investigation with the modified Wheeler model and experimental data. The results show that the NASGRO model give a fatigue life near by to that published in literatures and also showed the FCG rate response of X70 pipeline steels when exposed to VAL with different overload values. Extra modification to the NASGRO model may lead to better representing of FCG rate. Highlights: ► The assessment of fatigue crack propagation under different load histories are proposed and presented in this paper. ► Due to lack of knowledge in the related area, as yet no universal model exists. ► The output was based on both simulation and experiments. The simulation part was carried out based on the NASGRO model. ► This work focus on fatigue crack growth (FCG) and fatigue life based on the comparison with the previous work.
Thermo-Mechanical Fatigue Crack Growth of RR1000.
Pretty, Christopher John; Whitaker, Mark Thomas; Williams, Steve John
2017-01-04
Non-isothermal conditions during flight cycles have long led to the requirement for thermo-mechanical fatigue (TMF) evaluation of aerospace materials. However, the increased temperatures within the gas turbine engine have meant that the requirements for TMF testing now extend to disc alloys along with blade materials. As such, fatigue crack growth rates are required to be evaluated under non-isothermal conditions along with the development of a detailed understanding of related failure mechanisms. In the current work, a TMF crack growth testing method has been developed utilising induction heating and direct current potential drop techniques for polycrystalline nickel-based superalloys, such as RR1000. Results have shown that in-phase (IP) testing produces accelerated crack growth rates compared with out-of-phase (OOP) due to increased temperature at peak stress and therefore increased time dependent crack growth. The ordering of the crack growth rates is supported by detailed fractographic analysis which shows intergranular crack growth in IP test specimens, and transgranular crack growth in 90° OOP and 180° OOP tests. Isothermal tests have also been carried out for comparison of crack growth rates at the point of peak stress in the TMF cycles.
Thermo-Mechanical Fatigue Crack Growth of RR1000
Directory of Open Access Journals (Sweden)
Christopher John Pretty
2017-01-01
Full Text Available Non-isothermal conditions during flight cycles have long led to the requirement for thermo-mechanical fatigue (TMF evaluation of aerospace materials. However, the increased temperatures within the gas turbine engine have meant that the requirements for TMF testing now extend to disc alloys along with blade materials. As such, fatigue crack growth rates are required to be evaluated under non-isothermal conditions along with the development of a detailed understanding of related failure mechanisms. In the current work, a TMF crack growth testing method has been developed utilising induction heating and direct current potential drop techniques for polycrystalline nickel-based superalloys, such as RR1000. Results have shown that in-phase (IP testing produces accelerated crack growth rates compared with out-of-phase (OOP due to increased temperature at peak stress and therefore increased time dependent crack growth. The ordering of the crack growth rates is supported by detailed fractographic analysis which shows intergranular crack growth in IP test specimens, and transgranular crack growth in 90° OOP and 180° OOP tests. Isothermal tests have also been carried out for comparison of crack growth rates at the point of peak stress in the TMF cycles.
A model for high-cycle fatigue crack propagation
Energy Technology Data Exchange (ETDEWEB)
Balbi, Marcela Angela [Rosario National Univ. (Argentina); National Council of Scientific Research and Technology (CONICET) (Argentina)
2017-02-01
This paper deals with the prediction of high-cycle fatigue behavior for four different materials (7075-T6 alloy, Ti-6Al-4 V alloy, JIS S10C steel and 0.4 wt.-% C steel) using Chapetti's approach to estimate the fatigue crack propagation curve. In the first part of the paper, a single integral equation for studying the entire propagation process is determined using the recent results of Santus and Taylor, which consider a double regime of propagation (short and long cracks) characterized by the model of El Haddad. The second part of the paper includes a comparison of the crack propagation behavior model proposed by Navarro and de los Rios with the one mentioned in the first half of this work. The results allow us to conclude that the approach presented in this paper is a good and valid estimation of high-cycle fatigue crack propagation using a single equation to describe the entire fatigue crack regime.
Underclad cracks growth under fatigue loading in stainless steel cladding
International Nuclear Information System (INIS)
Bernard, J.L.; Bodson, F.; Doule, A.; Slama, G.; Bramat, M.; Doucet, J.P.; Maltrud, F.
1981-01-01
Hydrogen induced cracks have been found in HAZ of PWR vessel nozzles under stainless steel cladding. Fatigue tests were performed to collect a large amount of data on the possible propagation of this type of flaws. Tests were conducted in two steps. The aim of the first step was to set up the experimental equipment and to device an adequate method for following cracks during fatigue loading. Clad plates with electroerosion machined slots were used for this purpose. The second step was then undertaken with material taken out of an actual nozzle containing hydrogen induced cracks in the HAZ under stainless steel cladding or flaws simulated by electroerosion machined slots. The test loadings were comparable to in service loadings of the nozzles. Special attention was taken to get representative R ratios. Again for the sake of representativity, the tests were performed at 300 0 C (In service temperature) and the hydrotest was simulated. The main results are: It was possible to follow the whole failure process by combining non-destructive examinations during fatigue testing and fractographic observations of broken specimens. Different striation patterns, before and after air has penetrated the actual embedded cracks were observed. Numerical simulation of fatigue crack growth of actual or simulated defects were consistent with experimental data, provided mainly that defect shape, effect of R ratio and of environment were taken into account. (orig.)
Thermo-Mechanical Fatigue Crack Growth of RR1000
Christopher John Pretty; Mark Thomas Whitaker; Steve John Williams
2017-01-01
Non-isothermal conditions during flight cycles have long led to the requirement for thermo-mechanical fatigue (TMF) evaluation of aerospace materials. However, the increased temperatures within the gas turbine engine have meant that the requirements for TMF testing now extend to disc alloys along with blade materials. As such, fatigue crack growth rates are required to be evaluated under non-isothermal conditions along with the development of a detailed understanding of related failure mechan...
The effect of a free surface on fatigue crack behaviour
Czech Academy of Sciences Publication Activity Database
Hutař, Pavel; Náhlík, Luboš; Knésl, Zdeněk
2010-01-01
Roč. 32, č. 8 (2010), s. 1265-1269 ISSN 0142-1123 R&D Projects: GA ČR GA106/09/1954; GA ČR GA101/09/0867 Institutional research plan: CEZ:AV0Z20410507 Keywords : Vertex singularity * Generalized stress intenzity factor * Stress singularity * Fatigue crack * V- notch Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.799, year: 2010
Fatigue crack initiation – The role of point defects
Czech Academy of Sciences Publication Activity Database
Polák, Jaroslav; Man, Jiří
2014-01-01
Roč. 65, AUG (2014), s. 18-27 ISSN 0142-1123 R&D Projects: GA ČR(CZ) GAP108/10/2371; GA ČR(CZ) GA13-23652S Institutional support: RVO:68081723 Keywords : Fatigue crack initiation * Point defects * Persistent slip band * Intrusion * Extrusion Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.275, year: 2014
Xin, L.; Markine, V.L.; Shevtsov, I.
2015-01-01
The procedure for analysing rolling contact fatigue crack initiation and fatigue life prediction of the railway turnout crossing is developed. A three-dimensional finite element (FE) model is used to obtain stress and strain results, considering the dynamic effects of wheel-crossing rolling contact.
DEFF Research Database (Denmark)
Martakos, G.; Andreasen, J.H.; Berggreen, Christian
2017-01-01
A recently proposed face-sheet–core interface crack arresting device is implemented in sandwich beams and tested using the Sandwich Tear Test configuration. Fatigue loading conditions are applied to propagate the crack and determine the effect of the crack stopper on the fatigue growth rate and a...
Snider, H. L.; Reeder, F. L.; Dirkin, W. J.
1972-01-01
Fourteen C-130 airplane center wings, each containing service-imposed fatigue damage resulting from 4000 to 13,000 accumulated flight hours, were tested to determine their fatigue crack propagation and static residual strength characteristics. Eight wings were subjected to a two-step constant amplitude fatigue test prior to static testing. Cracks up to 30 inches long were generated in these tests. Residual static strengths of these wings ranged from 56 to 87 percent of limit load. The remaining six wings containing cracks up to 4 inches long were statically tested as received from field service. Residual static strengths of these wings ranged from 98 to 117 percent of limit load. Damage-tolerant structural design features such as fastener holes, stringers, doublers around door cutouts, and spanwise panel splices proved to be effective in retarding crack propagation.
Xin, L.; Markine, V.L.; Shevtsov, I.
2015-01-01
The procedure for analysing rolling contact fatigue crack initiation and fatigue life prediction of the railway turnout crossing is developed. A three-dimensional finite element (FE) model is used to obtain stress and strain results, considering the dynamic effects of wheel-crossing rolling contact. Material model accounting for elastic- plastic isotropic and kinematic hardening effects is adopted. The results from FE analysis are combined with J-S fatigue model that is based on critical plan...
Fatigue crack propagation behavior of stainless steel welds
Kusko, Chad S.
The fatigue crack propagation behavior of austenitic and duplex stainless steel base and weld metals has been investigated using various fatigue crack growth test procedures, ferrite measurement techniques, light optical microscopy, stereomicroscopy, scanning electron microscopy, and optical profilometry. The compliance offset method has been incorporated to measure crack closure during testing in order to determine a stress ratio at which such closure is overcome. Based on this method, an empirically determined stress ratio of 0.60 has been shown to be very successful in overcoming crack closure for all da/dN for gas metal arc and laser welds. This empirically-determined stress ratio of 0.60 has been applied to testing of stainless steel base metal and weld metal to understand the influence of microstructure. Regarding the base metal investigation, for 316L and AL6XN base metals, grain size and grain plus twin size have been shown to influence resulting crack growth behavior. The cyclic plastic zone size model has been applied to accurately model crack growth behavior for austenitic stainless steels when the average grain plus twin size is considered. Additionally, the effect of the tortuous crack paths observed for the larger grain size base metals can be explained by a literature model for crack deflection. Constant Delta K testing has been used to characterize the crack growth behavior across various regions of the gas metal arc and laser welds at the empirically determined stress ratio of 0.60. Despite an extensive range of stainless steel weld metal FN and delta-ferrite morphologies, neither delta-ferrite morphology significantly influence the room temperature crack growth behavior. However, variations in weld metal da/dN can be explained by local surface roughness resulting from large columnar grains and tortuous crack paths in the weld metal.
Fatigue crack growth analysis of a 450 PWR - lateral
International Nuclear Information System (INIS)
Taupin, P.; Flamand, F.
1988-01-01
Fatigue Crack Growth analysis of a 5 mm deep surface crack in the crotch region of a 45 0 Lateral (12 inch diameter) was performed on a 3-Loop 900 MWe PWR Plant under Normal and upset loading conditions. Stress Intensity factors were computed using the weight-function technique. The latter were obtained for a polynomial stress distribution at the corner of the lateral under contract with the Pressure Vessel Research Committee of the WRC. The study shows that after 40 years of normal operation the size of the end of life crack is limited to about 25 mm for the chosen lateral with a thickness of 300 mm
Fatigue crack closure behavior at high stress ratios
Turner, C. Christopher; Carman, C. Davis; Hillberry, Ben M.
1988-01-01
Fatigue crack delay behavior at high stress ratio caused by single peak overloads was investigated in two thicknesses of 7475-T731 aluminum alloy. Closure measurements indicated no closure occurred before or throughout the overload plastic zones following the overload. This was further substantiated by comparing the specimen compliance following the overload with the compliance of a low R ratio test when the crack was fully open. Scanning electron microscope studies revealed that crack tunneling and possibly reinitiation of the crack occurred, most likely a result of crack-tip blunting. The number of delay cycles was greater for the thinner mixed mode stress state specimen than for the thicker plane strain stress state specimen, which is similar to low R ratio test results and may be due to a larger plastic zone for the mixed mode cased.
Gates, Nicholas R.
The central objective of the research performed in this study was to be able to better understand and predict fatigue crack initiation and growth from stress concentrations subjected to complex service loading histories. As such, major areas of focus were related to the understanding and modeling of material deformation behavior, fatigue damage quantification, notch effects, cycle counting, damage accumulation, and crack growth behavior under multiaxial nominal loading conditions. To support the analytical work, a wide variety of deformation and fatigue tests were also performed using tubular and plate specimens made from 2024-T3 aluminum alloy, with and without the inclusion of a circular through-thickness hole. However, the analysis procedures implemented were meant to be general in nature, and applicable to a wide variety of materials and component geometries. As a result, experimental data from literature were also used, when appropriate, to supplement the findings of various analyses. Popular approaches currently used for multiaxial fatigue life analysis are based on the idea of computing an equivalent stress/strain quantity through the extension of static yield criteria. This equivalent stress/strain is then considered to be equal, in terms of fatigue damage, to a uniaxial loading of the same magnitude. However, it has often been shown, and was shown again in this study, that although equivalent stress- and strain-based analysis approaches may work well in certain situations, they lack a general robustness and offer little room for improvement. More advanced analysis techniques, on the other hand, provide an opportunity to more accurately account for various aspects of the fatigue failure process under both constant and variable amplitude loading conditions. As a result, such techniques were of primary interest in the investigations performed. By implementing more advanced life prediction methodologies, both the overall accuracy and the correlation of fatigue
Study of crack initiation in low-cycle fatigue of an austenitic stainless steel
International Nuclear Information System (INIS)
Mu, P.
2011-03-01
The material studied is an austenitic stainless steel, that is widely used in nuclear equipment for its very high corrosion resistance combined to good mechanical properties. Although crack initiation is proved to play an important role in fatigue, its mechanisms have not been fully understood. Some crack initiation criteria based on physical mechanisms of plastic deformation have been defined. However, these criteria are not easy to use and valid, as they need local variables at the grain scale. The present study aims at establishing a crack initiation criterion in low-cycle fatigue, which should be usable under variable amplitude loading conditions. Tension-compression fatigue tests were first carried out to characterize the mechanical behavior of the stainless steel AISI 316L. The mechanical behavior was simulated using a self-consistent model using a crystalline plastic law based on dislocation densities. The evolution of surface damage was observed during a fatigue test using an in situ optical microscopic device. Cracks were analyzed after 2000 cycles and their crystallographic characteristics calculated. As surface grains exhibit larger strain because they are less constraint by neighbor grains, a specific numerical frame is necessary to determine stress state in surface grains. A localization law specific to surface grains under cyclic loading was identified from finite element simulations. The proposed form needs an intergranular accommodation variable, on the pattern of the localization law of Cailletaud-Pilvin. Stress-strain state in surface grains was simulated. Potential indicators for crack initiation were then compared on a same experimental data base. Indicators based on the equivalent plastic strain were found to be suitable indicators of fatigue damage. (author)
Simulation of fatigue crack growth under large scale yielding conditions
Schweizer, Christoph; Seifert, Thomas; Riedel, Hermann
2010-07-01
A simple mechanism based model for fatigue crack growth assumes a linear correlation between the cyclic crack-tip opening displacement (ΔCTOD) and the crack growth increment (da/dN). The objective of this work is to compare analytical estimates of ΔCTOD with results of numerical calculations under large scale yielding conditions and to verify the physical basis of the model by comparing the predicted and the measured evolution of the crack length in a 10%-chromium-steel. The material is described by a rate independent cyclic plasticity model with power-law hardening and Masing behavior. During the tension-going part of the cycle, nodes at the crack-tip are released such that the crack growth increment corresponds approximately to the crack-tip opening. The finite element analysis performed in ABAQUS is continued for so many cycles until a stabilized value of ΔCTOD is reached. The analytical model contains an interpolation formula for the J-integral, which is generalized to account for cyclic loading and crack closure. Both simulated and estimated ΔCTOD are reasonably consistent. The predicted crack length evolution is found to be in good agreement with the behavior of microcracks observed in a 10%-chromium steel.
Fatigue-crack propagation behavior of Inconel 600
International Nuclear Information System (INIS)
James, L.A.
1976-05-01
The techniques of linear-elastic fracture mechanics were employed to characterize the effects of several parameters upon the fatigue-crack propagation behavior of Inconel 600. The parameters studied included temperature, cyclic frequency, stress ratio, thermal aging, and a limited amount of testing in a liquid sodium environment
Hybrid discrete dislocation models for fatigue crack growth
Curtin, W. A.; Deshpande, V. S.; Needleman, A.; Van der Giessen, E.; Wallin, M.
A framework for accurately modeling fatigue crack growth in ductile crystalline solids is necessarily multiscale The creation of new free surface occurs at the atomistic scale, where the material's cohesive strength is controlled by the local chemistry On the other hand, significant dissipation
The influence of microstructure on fatigue crack initiation in spheroidal graphite cast irons
International Nuclear Information System (INIS)
Starkey, M.S.; Irving, P.E.
1979-01-01
This paper reports the first stage of this work which concentrates on fatigue crack initiation with particular emphasis on the influence of microstructure. The fatigue lives of three fully ferritic and two fully pearlitic irons, each with different graphite nodule size distributions, have been determined at two strain amplitudes, 0.005 and 0.00018. The tests were carried out in fully reversed strain control on smooth cylindrical specimens in a servohydraulic testing machine. The effects of matrix structure and strength were clearly seen in that the pearlitic irons were superior at both strain levels. Nodule size on the other hand appeared to have no significant effect. The crack initiation sites in the specimens were located by interrupting the tests on detection of a 5% tensile load drop and heat tinting, before continuing. After failure, which was defined as complete separation, the fracture faces were examined on the scanning electron microscope. In the majority of the specimens the major crack origin was found to be a surface micropore with depths ranging from 50 to 250 μm. It is suggested that these micropores and not the graphite modules strongly influence the crack initiation behaviour in SG iron. These findings were confirmed by monitoring the initiation and growth of surface cracks from micropores using surface replica techniques. The influence of microstructure on the percentage of life spent in initiating and propagating a crack was thus determined. Hence the factors contributing to the fatigue behaviour of SG irons can be quantified. Their influence on predictions of cycles to crack initiation using the local approach is discussed. (orig.) 891 RW/orig. 892 RKD [de
Probabilistic and microstructural aspects of fatigue cracks initiation in Inconel 718
International Nuclear Information System (INIS)
Alexandre, F.
2004-03-01
Thermomechanical treatments have been recently developed to produce Inconel 718DA (Direct Aged). This alloy optimisation leads to an increase of the fatigue life but also the scatter. The aim of this study is on the one hand the understanding of the fatigue crack initiation mechanisms and on the other hand the modelling of the fatigue life and the scatter. An experimental study showed that the fatigue cracks were initiated from carbide particles in fine grain alloy. Interrupted tensile tests show that the particles cracking occurred at the first quarter of the fatigue cycle. Fatigue behaviour tests were also performed on various grain size 718 alloys. The last experimental part was devoted to measurements of the low cycle fatigue crack growth rates using a high focal distance microscope. For these tests, EDM micro-defects were used for the fatigue crack initiation sites. This method was also used to observe the small fatigue crack coalescence. A fatigue life model is proposed. It is based on the three fatigue crack initiation mechanisms competition: particle crack initiation on the surface, internal particle crack initiation and Stade I crack initiation. The particle fatigue crack initiation is supposed instantaneous at a critical stress level. The Tanaka and Mura model is used for analysing the Stage I crack initiation number of cycles. The fatigue crack growth rate was analysed using the Tomkins model identified on the small fatigue crack growth rate measurements. The proposed fatigue life model decomposed in three levels: a deterministic one and two probabilistic with and without crack coalescence. (author)
A short summary on finite element modelling of fatigue crack closure
Energy Technology Data Exchange (ETDEWEB)
Singh, Konjengbam Darunkumar [Indian Institute of Technology, Guwahati (India); Parry, Matthew Roger [Airbus Operations Ltd, Bristol(United Kingdom); Sinclair, Ian [University of Southampton, Southampton (United Kingdom)
2011-12-15
This paper presents a short summary pertaining to the finite element modelling of fatigue crack closure. Several key issues related to finite element modelling of fatigue crack closure are highlighted: element type, mesh refinement, stabilization of crack closure, crack-tip node release scheme, constitutive model, specimen geometry, stress-states (i.e., plane stress, plane strain), crack closure monitoring. Reviews are presented for both straight and deflected cracks.
Modelling probabilistic fatigue crack propagation rates for a mild structural steel
Correia, J.A.F.O.; de Jesus, A.M.P.; Fernández-Canteli, A.
2014-01-01
A class of fatigue crack growth models based on elastic–plastic stress–strain histories at the crack tip region and local strain-life damage models have been proposed in literature. The fatigue crack growth is regarded as a process of continuous crack initializations over successive elementary material blocks, which may be governed by smooth strain-life damage data. Some approaches account for the residual stresses developing at the crack tip in the actual crack driving force asse...
Fatigue crack growth behavior in equine cortical bone
Shelton, Debbie Renee
2001-07-01
Objectives for this research were to experimentally determine crack growth rates, da/dN, as a function of alternating stress intensity factor, DeltaK, for specimens from lateral and dorsal regions of equine third metacarpal cortical bone tissue, and to determine if the results were described by the Paris law. In one set of experiments, specimens were oriented for crack propagation in the circumferential direction with the crack plane transverse to the long axis of the bone. In the second set of experiments, specimens were oriented for radial crack growth with the crack plane parallel to the long axis of the bone. Results of fatigue tests from the latter specimens were used to evaluate the hypothesis that crack growth rates differ regionally. The final experiments were designed to determine if crack resistance was dependent on region, proportion of hooped osteons (those with circumferentially oriented collagen fibers in the outer lamellae) or number of osteons penetrated by the crack, and to address the hypothesis that hooped osteons resist invasion by cracks better than other osteonal types. The transverse crack growth data for dorsal specimens were described by the Paris law with an exponent of 10.4 and suggested a threshold stress intensity factor, DeltaKth, of 2.0 MPa·m1/2 and fracture toughness of 4.38 MPa·m 1/2. Similar results were not obtained for lateral specimens because the crack always deviated from the intended path and ran parallel to the loading direction. Crack growth for the dorsal and lateral specimens in the radial orientation was described by the Paris law with exponents of 8.7 and 10.2, respectively, and there were no regional differences in the apparent DeltaK th (0.5 MPa·m1/2) or fracture toughness (1.2 MPa·m 1/2). Crack resistance was not associated with cortical region, proportion of hooped osteons or the number of osteons penetrated by the crack. The extent to which cracks penetrate osteons was influenced by whether the collagen fiber
Ultrasonic testing of fatigue cracks under various conditions
International Nuclear Information System (INIS)
Jessop, T.J.; Cameron, A.G.B.
1983-01-01
Reliable detection of the fatigue cracks was possible under all conditions studied. Applied load affected the ultrasonic response in a variety of ways but never more than by 20dB and generally considerably less. Material variations affected the response under applied load by up to 20dB. Oxide in the crack and crack morphology affected the response by up to 9dB (12dB under load). Crack size variations and presence of water had little effect. Sizing accuracy was generally within 2mm although there was a tendency to undersize. The time of flight sizing technique gave the best accuracy if a tensile load was applied
Fatigue and environmentally assisted cracking in light water reactors
International Nuclear Information System (INIS)
Kassner, T.F.; Ruther, W.E.; Chung, H.M.; Hicks, P.D.; Hins, A.G.; Park, J.Y.; Shack, W.J.
1991-12-01
Fatigue and environmentally assisted cracking of piping, pressure vessels, and core components in light water reactors (LWRs) are important concerns as extended reactor lifetimes are envisaged. The degradation processes include intergranular stress corrosion cracking (IGSCC) of austenitic stainless steel (SS) piping in boiling water reactors (BWRs), and propagation of fatigue or SCC cracks (which initiate in sensitized SS cladding) into low-alloy ferritic steels in BWR pressure vessels. Similar cracking has also occurred in upper shell-to-transition cone girth welds in pressurized water reactor (PWR) steam generator vessels. Another concern is failure of reactor-core internal components after accumulation of relatively high fluence, which has occurred in both BWRs and PWRs. Research during the past year focused on (1) fatigue and SCC of ferritic steels used in piping and in steam generator and reactor pressure vessels, (2) role of chromate and sulfate in simulated BWR water in SCC of sensitized Type 304 SS, and (3) irradiation-assisted SCC in high- and commercial-purity Type 304 SS specimens from control-blade absorber tubes used in two operating BWRs. Failure after accumulation of relatively high fluence has been attributed to radiation-induced segregation (RIS) of elements such as Si, P, Ni, and Cr. This document provides a summary of research progress in these areas
International Nuclear Information System (INIS)
Arora, Punit; Tripathi, R.; Singh, P.K.; Bhasin, V.; Vijayan, P.K.
2016-01-01
The objective of the present study is to understand the Fatigue Crack Growth Rate (FCGR) behaviour after single over-load/ under-load event on carbon steel piping material. The tests have been carried out on standard Compact Tension (CT) specimens. The effect of different crack length to width ratio (a/W) of specimen and overload/under-load ratios on FCGR have been studied. The studies have shown significant reduction in FCG rate after overload event. The strain field has been measured using Digital Image Correlation (DIC) technique ahead of the crack tip to quantify the plastic zone size due to overload and constant amplitude load. In addition, plastic zone calculations have also been carried out using 3D finite element analyses for the prediction of post overload FCGR/ life. The predicted FCGR are in agreement with experimentally determined FCGR. (author)
Fatigue crack growth spectrum simplification: Facilitation of on-board damage prognosis systems
Adler, Matthew Adam
2009-12-01
Better lifetime predictions of systems subjected to fatigue loading are needed in support of the optimization of the costs of life-cycle engineering. In particular, the climate is especially encouraging for the development of safer aircraft. One issue is that aircraft experience complex fatigue loading and current methods for the prediction of fatigue damage accumulation rely on intensive computational tools that are not currently carried onboard during flight. These tools rely on complex models that are made more difficult by the complicated load spectra themselves. This presents an overhead burden as offline analysis must be performed at an offsite facility. This architecture is thus unable to provide online, timely information for on-board use. The direct objective of this research was to facilitate the real-time fatigue damage assessments of on-board systems with a particular emphasis on aging aircraft. To achieve the objective, the goal of this research was to simplify flight spectra. Variable-amplitude spectra, in which the load changes on a cycle-by-cycle basis, cannot readily be supported by an onboard system because the models required to predict fatigue crack growth during variable-amplitude loading are too complicated. They are too complicated because variable-amplitude fatigue crack growth analysis must be performed on a cycle-by-cycle basis as no closed-form solution exists. This makes these calculations too time-consuming and requires impractical, heavy onboard systems or offsite facilities. The hypothesis is to replace a variable-amplitude spectrum with an equivalent constant-amplitude spectrum. The advantage is a dramatic reduction in the complexity of the problem so that damage predictions can be made onboard by simple, fast calculations in real-time without the need to add additional weight to the aircraft. The intent is to reduce the computational burden and facilitate on-board projection of damage evolution and prediction for the accurate
Analysis and prediction of Multiple-Site Damage (MSD) fatigue crack growth
Dawicke, D. S.; Newman, J. C., Jr.
1992-08-01
A technique was developed to calculate the stress intensity factor for multiple interacting cracks. The analysis was verified through comparison with accepted methods of calculating stress intensity factors. The technique was incorporated into a fatigue crack growth prediction model and used to predict the fatigue crack growth life for multiple-site damage (MSD). The analysis was verified through comparison with experiments conducted on uniaxially loaded flat panels with multiple cracks. Configuration with nearly equal and unequal crack distribution were examined. The fatigue crack growth predictions agreed within 20 percent of the experimental lives for all crack configurations considered.
Analysis and prediction of Multiple-Site Damage (MSD) fatigue crack growth
Dawicke, D. S.; Newman, J. C., Jr.
1992-01-01
A technique was developed to calculate the stress intensity factor for multiple interacting cracks. The analysis was verified through comparison with accepted methods of calculating stress intensity factors. The technique was incorporated into a fatigue crack growth prediction model and used to predict the fatigue crack growth life for multiple-site damage (MSD). The analysis was verified through comparison with experiments conducted on uniaxially loaded flat panels with multiple cracks. Configuration with nearly equal and unequal crack distribution were examined. The fatigue crack growth predictions agreed within 20 percent of the experimental lives for all crack configurations considered.
Comparison of Fatigue Properties and Fatigue Crack Growth Rates of Various Implantable Metals
Okazaki, Yoshimitsu
2012-01-01
The fatigue strength, effects of a notch on the fatigue strength, and fatigue crack growth rate of Ti-15Zr-4Nb-4Ta alloy were compared with those of other implantable metals. Zr, Nb, and Ta are important alloying elements for Ti alloys for attaining superior long-term corrosion resistance and biocompatibility. The highly biocompatible Ti-15Zr-4Nb-4Ta alloy exhibited an excellent balance between strength and ductility. Its notched tensile strength was much higher than that of a smooth specimen. The strength of 20% cold-worked commercially pure (C.P.) grade 4 Ti was close to that of Ti alloy. The tension-to-tension fatigue strength of an annealed Ti-15Zr-4Nb-4Ta rod at 107 cycles was approximately 740 MPa. The fatigue strength of this alloy was much improved by aging treatment after solution treatment. The fatigue strengths of C.P. grade 4 Ti and stainless steel were markedly improved by 20% cold working. The fatigue strength of Co-Cr-Mo alloy was markedly increased by hot forging. The notch fatigue strengths of 20% cold-worked C.P. grade 4 Ti, and annealed and aged Ti-15Zr-4Nb-4Ta, and annealed Ti-6Al-4V alloys were less than those of the smooth specimens. The fatigue crack growth rate of Ti-15Zr-4Nb-4Ta was the same as that of Ti-6Al-4V. The fatigue crack growth rate in 0.9% NaCl was the same as that in air. Stainless steel and Co-Cr-Mo-Ni-Fe alloy had a larger stress-intensity factor range (ΔK) than Ti alloy.
Fatigue crack growth studies on a tee junction using ultrasonic non-destructive methods
International Nuclear Information System (INIS)
Subramanian, C.V.; Thavasimuthu, M.; Ramesh, A.S.; Jayakumar, T.; Kalyanasundaram, P.; Baldev Raj
1996-01-01
Fatigue cracks need to be detected and sized to maintain structural integrity. The significance of cracks detected in service must also be assessed. This paper describes the on-line ultrasonic testing carried out on a Tee joint subjected to fatigue loading. The initiation and growth of the cracks were monitored for every 5,000 cycles up to 40,000 cycles. The study demonstrated the use of ultrasonic testing for fatigue crack growth detection and sizing. (author)
New specimen design for studying the growth of small fatigue cracks with surface acoustic waves
London, Blair
1985-08-01
The study of small surface fatigue cracks in AISI 4140 quenched and tempered steel by a nondestructive surface acoustic wave technique is summarized. A novel cantilevered bending, plate-type fatigue specimen is described that is compatible with the acoustic method. Small cracks are initiated from a 25-μm deep surface pit produced by an electrospark machine. The importance of studying these cracks which closely approximate naturally occurring fatigue cracks is briefly discussed.
Mechanical factors affecting reliability of pressure components (fatigue, cracking)
International Nuclear Information System (INIS)
Lebey, J.; Garnier, C.; Roche, R.; Barrachin, B.
1978-01-01
The reliability of a pressure component can be seriously affected by the formation and development of cracks. The experimental studies presented in this paper are devoted to three different aspects of crack propagation phenomena which have been relatively little described. In close connection with safety analyses of PWR, the authors study the influence of the environment by carrying out fatigue tests with samples bathed in hot pressurized water. Ferritic, austenitic and Incolloy 800 steels were used and the results are presented in the form of fatigue curves in the oligocyclic region. The second part of the paper relates to crack initiation cirteria in ductile steels weakened by notches. The CT samples used make it possible to study almost all types of fracture (ductile, intermediate and brittle). The use of two criteria based on the load limit and on the toughness of the material constitutes a practical way of evaluating crack propagation conditions. A series of tests carried out on notched spherical vessels of different size shows that large vessels are relatively brittle; fast unstable fracture is observed as size increases. Crack growth rate in PWR primary circuits (3/6 steel) is studied on piping elements (0.25 scale) subjected to cyclic stress variations (285 0 C and with pressure varying between 1 and 160 bar in each cycle). By calculating the stress intensity factor, correlation with results obtained in the laboratory on CT samples is possible. (author)
International Nuclear Information System (INIS)
Fujikawa, Ryosuke; Abe, Shigeki; Nakamura, Takao; Kamaya, Masayuki
2014-01-01
Fatigue life of nuclear facilities tends to be decreased by the influence of reactor coolant, which is called environmental effect. The effect accelerates crack growth rate but the influence for crack initiation is not clarified. This study intends to discuss the environmental effect in crack initiation. The crack length and the number of cracks are measured from the investigation of fatigue test specimens in reactor coolant and air. The behavior of crack initiation is revealed from the measurement of number of cracks, crack sizes and fatigue life. From this study, environmental effect of reactor coolant is considered to influence crack initiation and increase the number of micro crack. It is also estimated that the coalescence of cracks influences the acceleration of crack growth. (author)
Probabilistic Model for Fatigue Crack Growth in Welded Bridge Details
DEFF Research Database (Denmark)
Toft, Henrik Stensgaard; Sørensen, John Dalsgaard; Yalamas, Thierry
2013-01-01
In the present paper a probabilistic model for fatigue crack growth in welded steel details in road bridges is presented. The probabilistic model takes the influence of bending stresses in the joints into account. The bending stresses can either be introduced by e.g. misalignment or redistribution...... of stresses in the structure. The fatigue stress ranges are estimated from traffic measurements and a generic bridge model. Based on the probabilistic models for the resistance and load the reliability is estimated for a typical welded steel detail. The results show that large misalignments in the joints can...
The role of extrusions and intrusions in fatigue crack initiation
Czech Academy of Sciences Publication Activity Database
Polák, Jaroslav; Mazánová, Veronika; Heczko, Milan; Petráš, Roman; Kuběna, Ivo; Casalena, L.; Man, Jiří
2017-01-01
Roč. 185, NOV (2017), s. 46-60 ISSN 0013-7944 R&D Projects: GA MŠk(CZ) LQ1601; GA MŠk LM2015069; GA ČR(CZ) GA13-23652S; GA ČR GA15-08826S Institutional support: RVO:68081723 Keywords : Extrusion * Fatigue crack initiation * Intrusion * Persistent slip marking * Stainless steel Subject RIV: JL - Materials Fatigue, Friction Mechanics OBOR OECD: Audio engineering, reliability analysis Impact factor: 2.151, year: 2016
Fatigue crack growth monitoring in multi-layered structures using guided ultrasonic waves
International Nuclear Information System (INIS)
Kostson, E; Fromme, P
2009-01-01
This contribution investigates the application of low frequency guided ultrasonic waves for monitoring fatigue crack growth at fastener holes in the 2nd layer of multi-layered plate structures, a common problem in aerospace industry. The model multi-layered structure investigated consists of two aluminum plate-strips adhesively bonded using a structural paste adhesive. Guided ultrasonic waves were excited using multiple piezoelectric discs bonded to the surface of the multi-layered structure. The wave propagation in the tensile specimen was measured using a laser interferometer and compared to numerical simulations. Thickness and width mode shapes of the excited flexural waves were identified from Semi-Analytical Finite Element (SAFE) calculations. Experiments and 3D Finite Element (FE) simulations show a change in the scattered field around fastener holes caused by a defect in the 2nd layer. The amplitude of the guided ultrasonic wave was monitored during fatigue experiments at a single point. The measured changes in the amplitude of the ultrasonic signal due to fatigue crack growth agree well with FE simulations.
Experimental evidence and physical models of fatigue crack initiation
Czech Academy of Sciences Publication Activity Database
Polák, Jaroslav; Man, Jiří
2016-01-01
Roč. 91, OCT (2016), s. 294-303 ISSN 0142-1123 R&D Projects: GA ČR(CZ) GA13-23652S; GA ČR GA13-32665S; GA MŠk(CZ) ED1.1.00/02.0068 Institutional support: RVO:68081723 Keywords : Crack initiation * Persistent slip band * Point defects * Extrusions * Intrusions Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.899, year: 2016
An analysis method for fatigue crack initiation on geometrical singularities
International Nuclear Information System (INIS)
Amzallag, C.; Bernard, J.L.; Pellissier-Tanon, A.; Vassal, J.M.
1982-05-01
For studying the significance of defects a promising point of view is to separate fatigue crack initiation and propagation. Comparing the works done on these two stages it appears that relatively few has been done on the first one. This presentation shows how this stage can be evaluated by using appropriate criteria. The validation of a criterion through experimental data obtained on actual and simulated singularities for different specimen geometries is presented
Heat affected zone and fatigue crack propagation behavior of high performance steel
International Nuclear Information System (INIS)
Choi, Sung Won; Kang, Dong Hwan; Kim, Tae Won; Lee, Jong Kwan
2009-01-01
The effect of heat affected zone in high performance steel on fatigue crack propagation behavior, which is related to the subsequent microstructure, was investigated. A modified Paris-Erdogan equation was presented for the analysis of fatigue crack propagation behavior corresponding to the heat affected zone conditions. Fatigue crack propagation tests under 0.3 stress ratio and 0.1 load frequency were conducted for both finegrained and coarse-grained heat affected zones, respectively. As shown in the results, much higher crack growth rate occurred in a relatively larger mean grain size material under the same stress intensity range of fatigue crack propagation process for the material.
Fatigue crack propagation in additively manufactured porous biomaterials.
Hedayati, R; Amin Yavari, S; Zadpoor, A A
2017-07-01
Additively manufactured porous titanium implants, in addition to preserving the excellent biocompatible properties of titanium, have very small stiffness values comparable to those of natural bones. Although usually loaded in compression, biomedical implants can also be under tensional, shear, and bending loads which leads to crack initiation and propagation in their critical points. In this study, the static and fatigue crack propagation in additively manufactured porous biomaterials with porosities between 66% and 84% is investigated using compact-tension (CT) samples. The samples were made using selective laser melting from Ti-6Al-4V and were loaded in tension (in static study) and tension-tension (in fatigue study) loadings. The results showed that displacement accumulation diagram obtained for different CT samples under cyclic loading had several similarities with the corresponding diagrams obtained for cylindrical samples under compression-compression cyclic loadings (in particular, it showed a two-stage behavior). For a load level equaling 50% of the yield load, both the CT specimens studied here and the cylindrical samples we had tested under compression-compression cyclic loading elsewhere exhibited similar fatigue lives of around 10 4 cycles. The test results also showed that for the same load level of 0.5F y , the lower density porous structures demonstrate relatively longer lives than the higher-density ones. This is because the high bending stresses in high-density porous structures gives rise to local Mode-I crack opening in the rough external surface of the struts which leads to quicker formation and propagation of the cracks. Under both the static and cyclic loading, all the samples showed crack pathways which were not parallel to but made 45 ° angles with respect to the notch direction. This is due to the fact that in the rhombic dodecahedron unit cell, the weakest struts are located in 45 ° direction with respect to the notch direction
Automated corrosion fatigue crack growth testing in pressurized water environments
International Nuclear Information System (INIS)
Ceschini, L.J.; Liaw, P.K.; Rudd, G.E.; Logsdon, W.A.
1984-01-01
This paper describes in detail a novel approach to construct a test facility for developing corrosion fatigue crack growth rate (FCGR) properties in aggressive environments. The environment studied is that of a pressurized water reactor (PWR) at 288 0 C (550 0 F) and 13.8 MPa (200 psig). To expedite data generation, each chamber was designed to accommodate two test specimens. A common water recirculation and pressurization system was employed to service two test chambers. Thus, four fatigue crack propagation rate tests could be conducted simultaneously in the pressurized water environment. The data analysis was automated to minimize the typically high labor costs associated with corrosion fatigue crack propagation testing. Verification FCGR tests conducted on an ASTM A469 rotor steel in a room temperature air environment as well as actual PWR environment FCGR tests performed on an ASTM A533 Grade B Class 2 pressure vessel steel demonstrated that the dual specimen test facility is an excellent system for developing the FCGR properties of materials in adverse environments
Fatigue crack growth behavior in niobium-hydrogen alloys
International Nuclear Information System (INIS)
Lin, M.C.C.; Salama, K.
1997-01-01
Near-threshold fatigue crack growth behavior has been investigated in niobium-hydrogen alloys. Compact tension specimens (CTS) with three hydrogen conditions are used: hydrogen-free, hydrogen in solid solution, and hydride alloy. The specimens are fatigued at a temperature of 296 K and load ratios of 0.05, 0.4, and 0.75. The results at load ratios of 0.05 and 0.4 show that the threshold stress intensity range (ΔK th ) decreases as hydrogen is added to niobium. It reaches a minimum at the critical hydrogen concentration (C cr ), where maximum embrittlement occurs. The critical hydrogen concentration is approximately equal to the solubility limit of hydrogen in niobium. As the hydrogen concentration exceeds C cr , ΔK th increases slowly as more hydrogen is added to the specimen. At load ratio 0.75, ΔK th decreases continuously as the hydrogen concentration is increased. The results provide evidence that two mechanisms are responsible for fatigue crack growth behavior in niobium-hydrogen alloys. First, embrittlement is retarded by hydride transformation--induced and plasticity-induced crack closures. Second, embrittlement is enhanced by the presence of hydrogen and hydride
Directory of Open Access Journals (Sweden)
Leonetti Davide
2018-01-01
Full Text Available Estimating and reducing uncertainty in fatigue test data analysis is a relevant task in order to assess the reliability of a structural connection with respect to fatigue. Several statistical models have been proposed in the literature with the aim of representing the stress range vs. endurance trend of fatigue test data under constant amplitude loading and the scatter in the finite and infinite life regions. In order to estimate the safety level of the connection also the uncertainty related to the amount of information available need to be estimated using the methods provided by the theory of statistic. The Bayesian analysis is employed to reduce the uncertainty due to the often small amount of test data by introducing prior information related to the parameters of the statistical model. In this work, the inference of fatigue test data belonging to cover plated steel beams is presented. The uncertainty is estimated by making use of Bayesian and frequentist methods. The 5% quantile of the fatigue life is estimated by taking into account the uncertainty related to the sample size for both a dataset containing few samples and one containing more data. The S-N curves resulting from the application of the employed methods are compared and the effect of the reduction of uncertainty in the infinite life region is quantified.
A study on the evolution of crack networks under thermal fatigue loading
International Nuclear Information System (INIS)
Kamaya, Masayuki; Taheri, Said
2008-01-01
The crack network is a typical cracking morphology caused by thermal fatigue loading. It was pointed out that the crack network appeared under relatively small temperature fluctuations and did not grow deeply. In this study, the mechanism of evolution of crack network and its influence on crack growth was examined by numerical calculation. First, the stress field near two interacting cracks was investigated. It was shown that there are stress-concentration and stress-shielding zones around interacting cracks, and that cracks can form a network under the bi-axial stress condition. Secondly, a Monte Carlo simulation was developed in order to simulate the initiation and growth of cracks under thermal fatigue loading and the evolution of the crack network. The local stress field formed by pre-existing cracks was evaluated by the body force method and its role in the initiation and growth of cracks was considered. The simulation could simulate the evolution of the crack network and change in number of cracks observed in the experiments. It was revealed that reduction in the stress intensity factor due to stress feature in the depth direction under high cycle thermal fatigue loading plays an important role in the evolution of the crack network and that mechanical interaction between cracks in the network affects initiation rather than growth of cracks. The crack network appears only when the crack growth in the depth direction is interrupted. It was concluded that the emergence of the crack network is preferable for the structural integrity of cracked components
Effect of overload on the fatigue crack propagation in metastable beta Ti-V alloys
International Nuclear Information System (INIS)
Chakrabortty, S.B.; Starke, E.A. Jr.; Lee, E.W.
1984-01-01
The effects of overload on the fatigue crack propagation behavior of two Ti-V alloys having different deformation mechanisms were studied. The results are explained in terms of residual stress effects associated with the overload and the removal of these stresses during post-overload cycling. An additional effect occurs during multiple cycle overload when the deformation structure representative of the strain amplitude is believed to form in the overload reverse plastic zone. This structure must be rearranged during cycling at Delta Kb before the baseline FCGR is reached and the process is responsible for part of the delay period. 46 references
International Nuclear Information System (INIS)
Baffie, N.; Stolarz, J.; Magnin, Th.
2000-01-01
The influence of martensitic transformation induced by cyclic straining on the mechanisms of low cycle fatigue damage in a metastable austenitic stainless steel with different grain sizes has been investigated using macroscopic measurements and microscopic observations of short crack evolutions. The amount of martensite formed during cyclic straining increases with increasing plastic strain amplitude and cumulative plastic strain but the dominant parameter is the grain size of austenite. The fine microstructure (D = 10 μm) with maximum martensite fraction of about 20% is characterised by a better fatigue resistance than the coarse one (D 40μm and only 2% of martensite) for the same plastic strain amplitude. Martensitic transformation is found to radically modify the cyclic response of the alloy and consequently the damage mechanisms. Indeed, both short crack nucleation and growth take place exclusively in the transformed regions. A mechanism of short crack propagation based on the γ→ α' transformation assisted by stress concentration at the crack tip is proposed. The indirect influence of grain boundaries in the austenite on crack propagation in the martensite is demonstrated. The better fatigue resistance of metastable alloys with fine granular structure can thus be understood. (authors)
Energy Technology Data Exchange (ETDEWEB)
Ritchie, R.O.; Lankford, J.
1986-01-01
Topics discussed in this volume include crack initiation and stage I growth, microstructure effects, crack closure, environment effects, the role of notches, analytical modeling, fracture mechanics characterization, experimental techniques, and engineering applications. Papers are presented on fatigue crack initiation along slip bands, the effect of microplastic surface deformation on the growth of small cracks, short fatigue crack behavior in relation to three-dimensional aspects and the crack closure effect, the influence of crack depth on crack electrochemistry and fatigue crack growth, and nondamaging notches in fatigue. Consideration is also given to models of small fatigue cracks, short crack theory, assessment of the growth of small flaws from residual strength data, the relevance of short crack behavior to the integrity of major rotating aero engine components, and the relevance of short fatigue crack growth data to the durability and damage tolerance analyses of aircraft.
Fatigue crack retardation of high strength steel in saltwater
International Nuclear Information System (INIS)
Tokaji, K.; Ando, Z.; Imai, T.; Kojima, T.
1983-01-01
A high strength steel was studied in 3 percent saltwater to investigate the effects of a corrosive environment and sheer thickness on fatigue crack propagation behavior following the application of a single tensile overload. Experiments were carried out under sinusoidally varying loads at a load ratio of 0 and frequency of 10 H /SUB z/ . A single tensile overload was found to cause delayed retardation, and the crack propagation rate at first increased, followed by fairly rapid decrease to a minimum value and then increased gradually to its steady-state value, just as it did in air. The overload affected zone size and the retardation cycles increased with decreasing sheet thickness, just as they did in air. However, the zone size and the cycles were larger in 3 percent saltwater than in air. Since the crack propagation rates through the overload affected zone were not affected by the test environment, the longer retardation cycles in 3 percent saltwater were attributed to an enlargement of the overload affected zone size. The crack propagation behavior following the application of a single tensile overload in 3 percent saltwater was well explained by the crack closure concept
Energy Technology Data Exchange (ETDEWEB)
Fissolo, A
2001-07-01
This report deals with the thermal fatigue cracking of austenitic stainless steels as AISI 316 LN and 304 L. Such damage has been clearly observed for some components used in Fast Breeder reactors (FBR) and Pressure Water Reactor (PWR). In order to investigate thermal fatigue, quasi-structural specimen have been used. In this frame, facilities enforcing temperature variations similar to those found under the operation conditions have been progressively developed. As for components, loading results from impeded dilatation. In the SPLASH facility, the purpose was to establish accurate crack initiation conditions in order to check the relevance of the usual component design methodology. The tested specimen is continuously heated by the passage of an electrical DC current, and submitted to cyclic thermal down shock (up to 1000 deg C/s) by means of periodical spraying of water on two opposite specimen faces. The number of cycles to crack initiation N{sub i} is deduced from periodic examinations of the quenched surfaces, by means of optical microscopy. It is considered that initiation occurs when at least one 50{mu}m to 150{open_square}m long crack is observed. Additional SPLASH tests were performed for N >> N{sub i}, with a view to investigate the evolution of a surface multiple cracking network with the number of cycles N. The CYTHIA test was mainly developed for the purpose of assessing crack growth dynamics of one isolated crack in thermal fatigue conditions. Specimens consist of thick walled tubes with a 1 mm circular groove is spark-machined at the specimen centre. During the test, the external wall of the tube is periodically heated by using a HF induction coil (1 MHz), while its internal wall is permanently cooled by flowing water. Total crack growth is derived from post-mortem examinations, whereby the thermal fatigue final rupture surface is oxidized at the end of the test. The specimen is broken afterwards under mechanical fatigue at room temperature. All the
On the influence of the environment on modeling the fatigue crack growth process
International Nuclear Information System (INIS)
Mc Evily, A.J.
1987-01-01
The effect of the environment at room and elevated temperature were considered with respect to the influence exerted on the basic mechanical aspects of the fatigue crack growth process. An experimental assessment of this influence was obtained by conducting fatigue crack growth tests both in air and vacuum and the results of such experiments are given. Topics considered include crack closure, short crack growth in notched and unnotched specimens, Mode II crack growth, and the effects of oxidation at elevated temperatures. It is shown that the basic mechanisms of fatigue crack growth can be greatly altered by the presence of oxide films at the fatigue crack tip. Modeling the mechanical aspects of the crack growth process is by itself a challenging task. In addition, the environmental considerations adds to the complexity of the modeling process. (Author)
A proposal for unification of fatigue crack growth law
Kobelev, V.
2017-05-01
In the present paper, the new fractional-differential dependences of cycles to failure for a given initial crack length upon the stress amplitude in the linear fracture approach are proposed. The anticipated unified propagation function describes the infinitesimal crack length growths per increasing number of load cycles, supposing that the load ratio remains constant over the load history. Two unification fractional-differential functions with different number of fitting parameters are proposed. An alternative, threshold formulations for the fractional-differential propagation functions are suggested. The mean stress dependence is the immediate consequence from the considered laws. The corresponding formulas for crack length over the number of cycles are derived in closed form.
Fatigue crack growth behavior of Inconel 718 produced by selective laser melting
Czech Academy of Sciences Publication Activity Database
Konečná, R.; Kunz, Ludvík; Nicoletto, G.; Bača, A.
2016-01-01
Roč. 35, č. 10 (2016), s. 31-40 ISSN 1971-8993 Institutional support: RVO:68081723 Keywords : Inconel 718 * Selective laser melting * Microstructure * Fatigue crack growth * Fractography Subject RIV: JL - Materials Fatigue, Friction Mechanics
Standard test method for measurement of fatigue crack growth rates
American Society for Testing and Materials. Philadelphia
2015-01-01
1.1 This test method covers the determination of fatigue crack growth rates from near-threshold to Kmax controlled instability. Results are expressed in terms of the crack-tip stress-intensity factor range (ΔK), defined by the theory of linear elasticity. 1.2 Several different test procedures are provided, the optimum test procedure being primarily dependent on the magnitude of the fatigue crack growth rate to be measured. 1.3 Materials that can be tested by this test method are not limited by thickness or by strength so long as specimens are of sufficient thickness to preclude buckling and of sufficient planar size to remain predominantly elastic during testing. 1.4 A range of specimen sizes with proportional planar dimensions is provided, but size is variable to be adjusted for yield strength and applied force. Specimen thickness may be varied independent of planar size. 1.5 The details of the various specimens and test configurations are shown in Annex A1-Annex A3. Specimen configurations other than t...
The Effect of Fatigue Cracks on Fastener Flexibility, Load Distribution and Fatigue Crack Growth
2012-05-01
Application of Damage Tolerance Concepts to Critical Engine Components”, “Damage Tolerance Concepts for Critical Engine Components, AGARD - CP 393”, NATO...railroad bridge [71]. The vast majority of fatigue tests during this period were of the rotating bending type [72, 73 ]. In these tests a specimen is...Experiment Station, University of Illinois, October 1921 73 . Mann, J. Y., Fatigue of Materials; An Introductory Text, Melbourne University Press, 1967
Czech Academy of Sciences Publication Activity Database
Wang, Q.; Du, Z.; Liu, X.; Kunz, Ludvík
2011-01-01
Roč. 2011, č. 682 (2011), s. 231-237 ISSN 1013-9826 Institutional research plan: CEZ:AV0Z20410507 Keywords : ultrafine-grained copper * equal channel angular pressing * fatigue * fatigue cracks Subject RIV: JL - Materials Fatigue, Friction Mechanics
Multi-cracking in uniaxial and biaxial fatigue of 304L stainless steel
International Nuclear Information System (INIS)
Rupil, J.
2012-01-01
When a mechanical part is subjected to a repeated mechanical stress, it may be damaged after a number of cycles by several cracks initiation and propagation of a main crack. This is the phenomenon of fatigue damage. The thesis deals specifically with possible damage to some components of nuclear plants due to thermal fatigue. Unlike conventional mechanical fatigue damage where a main crack breaks the part, the thermal fatigue damage usually results in the appearance of a surface crack network. Two aspects are discussed in the thesis. The first is the experimental study of fatigue multiple cracking stage also called multi-cracking. Two mechanical test campaigns with multi-cracking detection by digital image correlation were conducted. These campaigns involve uniaxial and equi-biaxial mechanical loads in tension/compression without mean stress. This work allows to monitor and to observe the evolution of different networks of cracks through mechanical solicitations. The second is the numerical simulation of the phenomenon of fatigue damage. Several types of model are used (stochastic, probabilistic, cohesive finite elements). The experimental results have led to identify a multiple crack initiation law in fatigue which is faced with the numerical results. This comparison shows the relevance of the use of an analytical probabilistic model to find statistical results on the density of cracks that can be initiated with thermal and mechanical fatigue loadings. (author) [fr
Low-cycle fatigue-cracking mechanisms in fcc crystalline materials
Zhang, P.; Qu, S.; Duan, Q. Q.; Wu, S. D.; Li, S. X.; Wang, Z. G.; Zhang, Z. F.
2011-01-01
The low-cycle fatigue (LCF) cracking behavior in various face-centered-cubic (fcc) crystalline materials, including Cu single crystals, bicrystals and polycrystals, Cu-Al and Cu-Zn alloys, ultrafine-grained (UFG) Al-Cu and Cu-Zn alloys, was systematically investigated and reviewed. In Cu single crystals, fatigue cracking always nucleates along slip bands and deformation bands. The large-angle grain boundary (GB) becomes the preferential site in bicrystals and polycrystals. In addition, fatigue cracking can also nucleate along slip bands and twin boundaries (TBs) in polycrystalline materials. However, shear bands and coarse deformation bands are observed to the preferential sites for fatigue cracking in UFG materials with a large number of GBs. Based on numerous observations on fatigue-cracking behavior, the fatigue-cracking mechanisms along slip bands, GBs, TBs, shear bands and deformation bands were systematically compared and classified into two types, i.e. shear crack and impingement crack. Finally, these fatigue-cracking behaviors are discussed in depth for a better understanding of their physical nature and the transition from intergranular to transgranular cracking in various fcc crystalline materials. These comprehensive results for fatigue damage mechanisms should significantly aid in obtaining the optimum design to further strengthen and toughen metallic materials in practice.
Two Parameter Fracture Mechanics: Fatigue Crack Behavior under Mixed Mode Conditions
Czech Academy of Sciences Publication Activity Database
Seitl, Stanislav; Knésl, Zdeněk
2008-01-01
Roč. 75, č. 3-4 (2008), s. 857-865 ISSN 0013-7944. [Crack Paths 2006. Parma, 14.09.2006-16.09.2006] R&D Projects: GA ČR GP101/04/P001 Institutional research plan: CEZ:AV0Z20410507 Keywords : Constraint * Mixed-mode loading * Fatigue crack * Crack growth * Crack path Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.713, year: 2008
Fatigue and fatigue crack growth properties of 316LN and Incoloy 908 below 10 K
International Nuclear Information System (INIS)
Nyilas, A.; Zhang, J.; Obst, B.; Ulbricht, A.
1992-01-01
The cyclic loading characteristics of Tokamak type thermonuclear machines demand study of the fatigue response of the materials used in critical components. The large superconducting magnets and their superconductors will operate under cyclic mechanical stress conditions. The present paper is biased towards the current superconductor design of the NET (Next European Torus) model coil concept. The superconductor of this coil will be a cable-in-conduit Nb 3 Sn type with an enveloped stiff external jacket structure. The wall thickness of the jacket structure is within the range of 4-5 mm. The manufacturing of the jacket lengths for several hundred meters require an appropriate joining process due to the prefabricated section pieces available only in short lengths of 5-7 meters. The recently anticipated solution favors the flash butt welding technique. The performance of the superconductors jacket will depend on the material selection and the proper structural design according to the existing low temperature structural materials data base. The wind and react Nb 3 Sn-manufacturing process must also account the materials properties after ageing. A program was set up to elucidate the fatigue-life behavior and fatigue crack growth rate (FCGR) of the selected two candidate materials. These materials were the AISI 316LN with a specified low carbon content to avoid the embrittlement after the ageing process and the Incoloy 908. The 316LN material in the as received condition was tested with respect to its fatigue-life for specimens bearing predefined flaws and cracks. The propagation of surface cracks at 12 K and at 295 K was characterized with non standard specimens. The tests were performed in a cryogenic dynamic test facility under helium gas environment between 7 K and 20 K. Using the reference growth laws obtained from these measurements the total crack propagation starting with the initial crack length of the specimen could be predicted by numerical computation
Crack Propagation in Plane Strain under Variable Amplitude Loading
DEFF Research Database (Denmark)
Ricardo, Luiz Carlos Hernandes
2010-01-01
. In this paper procedures to determine the crack opening and closure by finite elements analyses in plane strain will be presented. The objective of this paper is also provide a review of retardation models under variable spectrum loading considering plane strain constraint as well as their correlation...
Measurement of fatigue crack growth rate of reactor structural material in air based on DCPD method
International Nuclear Information System (INIS)
Du Donghai; Chen Kai; Yu Lun; Zhang Lefu; Shi Xiuqiang; Xu Xuelian
2014-01-01
The principles and details of direct current potential drop (DCPD) in monitoring the crack growth of reactor structural materials was introduced in this paper. Based on this method, the fatigue crack growth rate (CGR) of typical structural materials in nuclear power systems was measured. The effects of applied load, load ratio and loading frequency on the fatigue crack growth rate of reactor structural materials were discussed. The result shows that the fatigue crack growth rate of reactor structural materials depends on the hardness of materials, and the harder the material is, the higher the rate of crack growth is. (authors)
Modelling probabilistic fatigue crack propagation rates for a mild structural steel
Directory of Open Access Journals (Sweden)
J.A.F.O. Correia
2015-01-01
Full Text Available A class of fatigue crack growth models based on elastic–plastic stress–strain histories at the crack tip region and local strain-life damage models have been proposed in literature. The fatigue crack growth is regarded as a process of continuous crack initializations over successive elementary material blocks, which may be governed by smooth strain-life damage data. Some approaches account for the residual stresses developing at the crack tip in the actual crack driving force assessment, allowing mean stresses and loading sequential effects to be modelled. An extension of the fatigue crack propagation model originally proposed by Noroozi et al. (2005 to derive probabilistic fatigue crack propagation data is proposed, in particular concerning the derivation of probabilistic da/dN-ΔK-R fields. The elastic-plastic stresses at the vicinity of the crack tip, computed using simplified formulae, are compared with the stresses computed using an elasticplastic finite element analyses for specimens considered in the experimental program proposed to derive the fatigue crack propagation data. Using probabilistic strain-life data available for the S355 structural mild steel, probabilistic crack propagation fields are generated, for several stress ratios, and compared with experimental fatigue crack propagation data. A satisfactory agreement between the predicted probabilistic fields and experimental data is observed.
International Nuclear Information System (INIS)
Lindblom, J.; Sandstroem, R.; Linde, L.; Henderson, P.
1990-01-01
Low cycle fatigue (LCF) tests have been performed at 300 and 565 degrees C on welded joints and on microstructures to be found in or near welded joints in a low alloy ferritic steel 0.5 Cr, 0.5 Mo, 0.25 V. The difference in lifetimes between the 300 degrees C and 565 degrees C tests was small comparing the same microstructures and strain ranges, although the stress amplitude was greater at 300 degrees C. Under constant stress conditions the fatigue life depended on the fatigue life of the parent metal but under constant strain conditions the lifetime was governed by that of the bainitic structures. Strain controlled LCF tests have been performed at 750 degrees C on welded joints in the austenitic steel AISI 316 and on different parent and weld metals used in these joints. In continuously cycled samples all cracks were transgranular and initiated at the surface; hold-time samples displayed internally initiated intergranular cracking in the weld metal. Under constant strain conditions the 316 parent and weld metals exhibited similar lifetimes. When considering a constant stress situation the strength of the microsturctures decreased in the following order: Sanicro weld metal, cold deformed parent metal, undeformed parent metal and weld metal (K.A.E.)
The effects of loading history on fatigue crack growth threshold
International Nuclear Information System (INIS)
Ogawa, Takeshi; Tokaji, Keiro; Ochi, Satoshi; Kobayashi, Hideo.
1987-01-01
The effects of loading history on threshold stress intensity range (ΔK th ) were investigated in a low alloy steel SFVQ1A (A508 - 3) and a low carbon steel S10C. A single overload and multiple overloads were chosen as loading history. Crack growth and crack closure following the loading histories were measured at load ratios of 0.05 and 0.70. Threshold values were determined as a fatigue limit of preloaded specimens. The ΔK th values increased with increasing overload stress intensity factor (K h ). For a given K h value, multiple overloads produced much larger increase in ΔK th than a single overload and threshold values expressed by maximum stress intensity factor (K max,th ) were almost constant, independent of stress ratio. The results obtained were discussed in terms of crack closure behaviour, and a method was proposed to evaluate the threshold value based on plasticity-induced crack closure. (author)
Probabilistic Prognosis of Non-Planar Fatigue Crack Growth
Leser, Patrick E.; Newman, John A.; Warner, James E.; Leser, William P.; Hochhalter, Jacob D.; Yuan, Fuh-Gwo
2016-01-01
Quantifying the uncertainty in model parameters for the purpose of damage prognosis can be accomplished utilizing Bayesian inference and damage diagnosis data from sources such as non-destructive evaluation or structural health monitoring. The number of samples required to solve the Bayesian inverse problem through common sampling techniques (e.g., Markov chain Monte Carlo) renders high-fidelity finite element-based damage growth models unusable due to prohibitive computation times. However, these types of models are often the only option when attempting to model complex damage growth in real-world structures. Here, a recently developed high-fidelity crack growth model is used which, when compared to finite element-based modeling, has demonstrated reductions in computation times of three orders of magnitude through the use of surrogate models and machine learning. The model is flexible in that only the expensive computation of the crack driving forces is replaced by the surrogate models, leaving the remaining parameters accessible for uncertainty quantification. A probabilistic prognosis framework incorporating this model is developed and demonstrated for non-planar crack growth in a modified, edge-notched, aluminum tensile specimen. Predictions of remaining useful life are made over time for five updates of the damage diagnosis data, and prognostic metrics are utilized to evaluate the performance of the prognostic framework. Challenges specific to the probabilistic prognosis of non-planar fatigue crack growth are highlighted and discussed in the context of the experimental results.
Numerical Simulation of Fatigue Crack Growth in Hip Implants
Czech Academy of Sciences Publication Activity Database
Colic, K.; Sedmak, A.; Grbovic, A.; Burzić, M.; Hloch, Sergej; Sedmak, S.
2016-01-01
Roč. 149, č. 149 (2016), s. 229-235 E-ISSN 1877-7058. [International Conference on Manufacturing Engineering and Materials, ICMEM 2016. Nový Smokovec, 06.06.2016-10.06.2016] R&D Projects: GA MŠk ED2.1.00/03.0082; GA MŠk(CZ) LO1406 Institutional support: RVO:68145535 Keywords : biomedical application design * extended finite element method (XFEM) * Ti-6Al-4V alloy * stress intensity factor (SIF) * fatigue crack growth Subject RIV: JQ - Machines ; Tools http://www.sciencedirect.com/science/article/pii/S1877705816311699
Study of mathematical models for fatigue crack propagation
International Nuclear Information System (INIS)
Yarema, S.Ya.; Mel'nichok, L.S.
1982-01-01
Complex composition of mathematical models for description of experimental diagrams of fatigue fracture (EDFF) for different steels and alloys from the view point of their correspondence to experimental data is conducted. 5 simple formulas for EDFF description have been chosen from the known ones. It is revealed that the analytical expression should contain 6 parameters for the main peculiarities of typical EDFF. This conclusion agrees with the fact that the 6-parametric formula provides the best quality of experimental data approximation. It should be also noted that the necessary number of parameters coincides with the number of all the standard characteristics (main and additional) of cyclic crack resistance of materials
Fatigue Crack Growth in Bodies with Thermally Sprayed Coating
Czech Academy of Sciences Publication Activity Database
Kovářík, O.; Haušild, P.; Medřický, Jan; Tomek, L.; Siegl, J.; Mušálek, Radek; Curry, N.; Björklund, S.
2016-01-01
Roč. 25, 1-2 (2016), s. 311-320 ISSN 1059-9630. [ITSC 2015: International Thermal Spray Conference and Exposition. Long Beach, California, 11.05.2015-14.05.2015] R&D Projects: GA ČR GB14-36566G Institutional support: RVO:61389021 Keywords : Thermal barrier coating * fatigue * crack growth * digital image correlation * digital image correlation Subject RIV: JK - Corrosion ; Surface Treatment of Materials Impact factor: 1.488, year: 2016 http://link.springer.com/article/10.1007%2Fs11666-015-0329-9
Prediction of Fatigue Crack Growth in Gas Turbine Engine Blades Using Acoustic Emission.
Zhang, Zhiheng; Yang, Guoan; Hu, Kun
2018-04-25
Fatigue failure is the main type of failure that occurs in gas turbine engine blades and an online monitoring method for detecting fatigue cracks in blades is urgently needed. Therefore, in this present study, we propose the use of acoustic emission (AE) monitoring for the online identification of the blade status. Experiments on fatigue crack propagation based on the AE monitoring of gas turbine engine blades and TC11 titanium alloy plates were conducted. The relationship between the cumulative AE hits and the fatigue crack length was established, before a method of using the AE parameters to determine the crack propagation stage was proposed. A method for predicting the degree of crack propagation and residual fatigue life based on the AE energy was obtained. The results provide a new method for the online monitoring of cracks in the gas turbine engine blade.
International Nuclear Information System (INIS)
Chopra, O.K.; Shack, W.J.; Muscara, J.
2003-01-01
This paper examines the mechanism of fatigue crack initiation in austenitic stainless steels (SSs) in light water reactor (LWR) coolant environments. The effects of key material and loading variables on the fatigue lives of wrought and cast austenitic SSs in air and LWR environments have been evaluated. The influence of reactor coolant environments on the formation and growth of fatigue cracks in polished smooth SS specimens is discussed. The results indicate that the fatigue lives of these steels are decreased primarily by the effects of the environment on the growth of cracks <200 μm and, to a lesser extent, on enhanced growth rates of longer cracks. The fracture morphology in the specimens has been characterized. Exploratory fatigue tests were conducted to study the effects of surface micropits or minor differences in the surface oxide on fatigue crack initiation. (author)
Fatigue Crack Growth Behavior of Gas Metal Arc Welded AISI 409 Grade Ferritic Stainless Steel Joints
Lakshminarayanan, A. K.; Shanmugam, K.; Balasubramanian, V.
2009-10-01
The effect of filler metals such as austenitic stainless steel, ferritic stainless steel, and duplex stainless steel on fatigue crack growth behavior of the gas metal arc welded ferritic stainless steel joints was investigated. Rolled plates of 4 mm thickness were used as the base material for preparing single ‘V’ butt welded joints. Center cracked tensile specimens were prepared to evaluate fatigue crack growth behavior. Servo hydraulic controlled fatigue testing machine with a capacity of 100 kN was used to evaluate the fatigue crack growth behavior of the welded joints. From this investigation, it was found that the joints fabricated by duplex stainless steel filler metal showed superior fatigue crack growth resistance compared to the joints fabricated by austenitic and ferritic stainless steel filler metals. Higher yield strength and relatively higher toughness may be the reasons for superior fatigue performance of the joints fabricated by duplex stainless steel filler metal.
Temperature and loading frequency effects of fatigue crack growth in HDPE pipe material
International Nuclear Information System (INIS)
Merah, N.; Khan, Z.; Bazoune, A.; Saghir, F.
2006-01-01
High density polyethylene (HDPE) pipes are being extensively used for gas, water, sewage and waste water distribution systems. Laboratory tests appear to show that HDPE is more able to suppress rapid crack propagation, while remaining somehow resistant to slow crack growth failures observed in service. Procedures for estimating pipe life in service have been established by making use of fatigue crack growth (FCG) results. These procedures are concerned mainly with room temperature. Applications with some safety factor to include the temperature effect. Use of HDPE pipes in water and gas distribution in the Gulf area has seen a net increase. This study addresses the combined effects of temperature and frequency on FCG properties of commercial HDPE pipe material. FCG accelerated tests were conducted on single-etch notch (SEN) specimens in the temperature range of -10 to 70C at frequencies ranging from 0.1 to 50 Hz. The FCG tests are conducted at a stress amplitude level approximately 1/4 of room temperature yield stress and crack growth behavior was investigated using linear elastic fracture mechanics concepts. The stress intensity range delta K gave satisfactory correlation of crack, growth rate (da/dN) at the temperatures of -10, 0, 23 and 40C and at frequencies of 0.1, 1, and 50 Hz. The crack growth resistance was found to decrease with increase in test temperature and decrease growth resistance was found to decrease with increase in test temperature and decrease with frequency. For 70C no crack propagation was observed, the failure was observed to occur by collapse or generalized yielding. Fractographic analyses results are used to explain temperature and frequency effects on FCG. The effect of temperature on da/dN for HDPE material was investigated by considering the variation of mechanical properties with temperature. Master curves were developed by normalizing delta K yield stress. (author)
Fatigue crack growth in 2024-T3 aluminum under tensile and transverse shear stresses
Viz, Mark J.; Zehnder, Alan T.
1994-01-01
The influence of transverse shear stresses on the fatigue crack growth rate in thin 2024-T3 aluminum alloy sheets is investigated experimentally. The tests are performed on double-edge cracked sheets in cyclic tensile and torsional loading. This loading generates crack tip stress intensity factors in the same ratio as the values computed for a crack lying along a lap joint in a pressurized aircraft fuselage. The relevant fracture mechanics of cracks in thin plates along with the details of the geometrically nonlinear finite element analyses used for the test specimen calibration are developed and discussed. Preliminary fatigue crack growth data correlated using the fully coupled stress intensity factor calibration are presented and compared with fatigue crack growth data from pure delta K(sub I)fatigue tests.
An Analytical Model for Fatigue Life Prediction Based on Fracture Mechanics and Crack Closure
DEFF Research Database (Denmark)
Ibsø, Jan Behrend; Agerskov, Henning
1996-01-01
test specimens are compared with fatigue life predictions using a fracture mechanics approach. In the calculation of the fatigue life, the influence of the welding residual stresses and crack closure on the fatigue crack growth is considered. A description of the crack closure model for analytical...... determination of the fatigue life is included. Furthermore, the results obtained in studies of the various parameters that have an influence on the fatigue life, are given. A very good agreement between experimental and analytical results is obtained, when the crack closure model is used in determination...... of the analytical fatigue lives. Both the analytical and experimental results obtained show that the Miner rule may give quite unconservative predictions of the fatigue life for the types of stochastic loading studied....
An Analytical Model for Fatigue Life Prediction Based on Fracture Mechanics and Crack Closure
DEFF Research Database (Denmark)
Ibsø, Jan Behrend; Agerskov, Henning
1996-01-01
test specimens are compared with fatigue life predictions using a fracture mechanics approach. In the calculation of the fatigue life, the influence of the welding residual stresses and crack closure on the fatigue crack growth is considered. A description of the crack closure model for analytical...... of the analytical fatigue lives. Both the analytical and experimental results obtained show that the Miner rule may give quite unconservative predictions of the fatigue life for the types of stochastic loading studied....... determination of the fatigue life is included. Furthermore, the results obtained in studies of the various parameters that have an influence on the fatigue life, are given. A very good agreement between experimental and analytical results is obtained, when the crack closure model is used in determination...
Creep, Fatigue and Environmental Interactions and Their Effect on Crack Growth in Superalloys
Telesman, J.; Gabb, T. P.; Ghosn, L. J.; Smith, T.
2017-01-01
Complex interactions of creep/fatigue/environment control dwell fatigue crack growth (DFCG) in superalloys. Crack tip stress relaxation during dwells significantly changes the crack driving force and influence DFCG. Linear Elastic Fracture Mechanics, Kmax, parameter unsuitable for correlating DFCG behavior due to extensive visco-plastic deformation. Magnitude of remaining crack tip axial stresses controls DFCG resistance due to the brittle-intergranular nature of the crack growth process. Proposed a new empirical parameter, Ksrf, which incorporates visco-plastic evolution of the magnitude of remaining crack tip stresses. Previous work performed at 704C, extend the work to 760C.
He, Jingjing; Guan, Xuefei; Peng, Tishun; Liu, Yongming; Saxena, Abhinav; Celaya, Jose; Goebel, Kai
2013-10-01
This paper presents an experimental study of damage detection and quantification in riveted lap joints. Embedded lead zirconate titanate piezoelectric (PZT) ceramic wafer-type sensors are employed to perform in situ non-destructive evaluation (NDE) during fatigue cyclical loading. PZT wafers are used to monitor the wave reflection from the boundaries of the fatigue crack at the edge of bolt joints. The group velocity of the guided wave is calculated to select a proper time window in which the received signal contains the damage information. It is found that the fatigue crack lengths are correlated with three main features of the signal, i.e., correlation coefficient, amplitude change, and phase change. It was also observed that a single feature cannot be used to quantify the damage among different specimens since a considerable variability was observed in the response from different specimens. A multi-feature integration method based on a second-order multivariate regression analysis is proposed for the prediction of fatigue crack lengths using sensor measurements. The model parameters are obtained using training datasets from five specimens. The effectiveness of the proposed methodology is demonstrated using several lap joint specimens from different manufactures and under different loading conditions.
International Nuclear Information System (INIS)
He, Jingjing; Guan, Xuefei; Peng, Tishun; Liu, Yongming; Saxena, Abhinav; Celaya, Jose; Goebel, Kai
2013-01-01
This paper presents an experimental study of damage detection and quantification in riveted lap joints. Embedded lead zirconate titanate piezoelectric (PZT) ceramic wafer-type sensors are employed to perform in situ non-destructive evaluation (NDE) during fatigue cyclical loading. PZT wafers are used to monitor the wave reflection from the boundaries of the fatigue crack at the edge of bolt joints. The group velocity of the guided wave is calculated to select a proper time window in which the received signal contains the damage information. It is found that the fatigue crack lengths are correlated with three main features of the signal, i.e., correlation coefficient, amplitude change, and phase change. It was also observed that a single feature cannot be used to quantify the damage among different specimens since a considerable variability was observed in the response from different specimens. A multi-feature integration method based on a second-order multivariate regression analysis is proposed for the prediction of fatigue crack lengths using sensor measurements. The model parameters are obtained using training datasets from five specimens. The effectiveness of the proposed methodology is demonstrated using several lap joint specimens from different manufactures and under different loading conditions. (paper)
Thermal fatigue crack growth on a thick wall tube containing a semi elliptical circumferential crack
International Nuclear Information System (INIS)
Deschanels, H.; Wakai, T.; Lacire, M.H.; Michel, B.
2001-01-01
In order to check the ability of the simplified assessment procedure (A16 guide) to predict fatigue crack growth, a benchmark problem was conducted. This work is carried out under the project ''agreement on the Exchange of Information and Collaboration in the field of Research and Development of Fast Breeder Reactor (FBR) between Europe (EU) and Japan''. Experimental work is conducted by PNC using Air cooled Thermal transient Test Facility (ATTF). Specimen is a thick wall tube containing a semi elliptical (3-D) circumferential crack and subjected to cyclic thermal transients. The constitutive material is the 304 austenitic stainless steel type SUS304. Due to thermal shock (650 C-300 C) the stress distribution through the wall is non-linear and well approximated using a 3 rd order polynomial. When comparing computations and tests data we observe a good agreement for the crack propagation in length. In crack depth, accurate results are obtained in the first part of the test, but on the later stage of the experiment the computations slightly underestimate the propagation (deep crack). In addition, we notice the importance of good evaluation of fracture mechanics parameters for non-linear stress distribution through the wall. At present A16 guide handbook gives stress intensity factor solutions for non-linear stress distribution through the wall. (author)
Investigation into fatigue crack growth and kinetic diagrams of fatigue failure
International Nuclear Information System (INIS)
Yarema, S.Ya.
1977-01-01
Studies on fatigue failure are discussed in terms of fatigue failure kinetic diagrams (FFKD), in which the fatigue crack growth rate is plotted against the stress intensity coefficient (SIC). The physical sense of the crack growth rate and SIC is discussed and their applicability for description of the material in the destruction zone, particularly in presence of various media. Variation of experimental parameters (loading and environment) is followed by a transition period during which the results of the experiment may depend on its history, so that FFKD would remain invariant. Advantages of tests under constant experimental conditions are shown. The ways to stabilize SIC are indicated and requirements to the samples are given. As an example, the tests of disc samples made of plate materials are given, where SIC does not depend on the crack length. The question of controlling the experimental conditions such as asymmetry and shape of the loading cycle, loading frequency, fluctuations of temperature and air composition is considered. The analytical functions describing FFKD are discussed. It is shown, that in appropriate dimensionless coordinates the FFKD of different materials merge into one curve
An unsupervised learning algorithm for fatigue crack detection in waveguides
International Nuclear Information System (INIS)
Rizzo, Piervincenzo; Cammarata, Marcello; Kent Harries; Dutta, Debaditya; Sohn, Hoon
2009-01-01
Ultrasonic guided waves (UGWs) are a useful tool in structural health monitoring (SHM) applications that can benefit from built-in transduction, moderately large inspection ranges, and high sensitivity to small flaws. This paper describes an SHM method based on UGWs and outlier analysis devoted to the detection and quantification of fatigue cracks in structural waveguides. The method combines the advantages of UGWs with the outcomes of the discrete wavelet transform (DWT) to extract defect-sensitive features aimed at performing a multivariate diagnosis of damage. In particular, the DWT is exploited to generate a set of relevant wavelet coefficients to construct a uni-dimensional or multi-dimensional damage index vector. The vector is fed to an outlier analysis to detect anomalous structural states. The general framework presented in this paper is applied to the detection of fatigue cracks in a steel beam. The probing hardware consists of a National Instruments PXI platform that controls the generation and detection of the ultrasonic signals by means of piezoelectric transducers made of lead zirconate titanate. The effectiveness of the proposed approach to diagnose the presence of defects as small as a few per cent of the waveguide cross-sectional area is demonstrated
3-D analysis of fatigue crack behaviour in a shot peened steam turbine blade material
Energy Technology Data Exchange (ETDEWEB)
He, B.Y., E-mail: Binyan.he@soton.ac.uk [Engineering Materials, Faculty of Engineering and the Environment, University of Southampton, Southampton SO17 1BJ (United Kingdom); Katsamenis, O.L. [muVIS X-ray Imaging Centre, Faculty of Engineering and the Environment, University of Southampton, Southampton SO17 1BJ (United Kingdom); Mellor, B.G.; Reed, P.A.S. [Engineering Materials, Faculty of Engineering and the Environment, University of Southampton, Southampton SO17 1BJ (United Kingdom)
2015-08-26
Serial mechanical sectioning and high resolution X-ray tomography have been used to study the three-dimensional morphology of small fatigue cracks growing in a 12 Cr tempered martensitic steam turbine blade material. A range of surface conditions has been studied, namely polished and shot peened (with varying levels of intensity). In the polished (unpeened) condition, inclusions (alumina and manganese sulphide) played an important role in initiating and controlling early fatigue crack behaviour. When fatigue cracks initiated from an alumina stringer, the crack morphology was normally dominated by single stringers, which were always in the centre of the fatigue crack, indicating its primary role in initiation. Manganese sulphide inclusion groups however seemed to dominate and affect the crack path along both the surface and depth crack growth directions. The more intensely shot peened condition did not however evidence inclusion or stringer affected fatigue crack initiation or growth behaviour; sub-surface crack coalescence being clearly observed by both serial sectioning and computed tomography (CT) imaging techniques at a depth of about 150–180 μm. These sub-surface crack coalescences can be linked to both the extent of the compressive residual stress as well as the depth of the plastic deformation arising from the intense shot peening process. Shot peening appears to provide a different defect population that initiates fatigue cracks and competes with the underlying metallurgical defect populations. The most beneficial shot peening process would in this case appear to “deactivate” the original metallurgical defect population and substitute a known defect distribution from the shot peening process from which fatigue cracks grow rather slowly in the strain hardened surface layer which also contains compressive residual stresses. A benefit to fatigue life in bending, even under Low Cycle Fatigue (LCF) conditions, has been observed in these tests if a
Attema, T.; Courage, W.M.G.; Maljaars, J.; Meerveld, H. van; Paulissen, J.H.; Pijpers, R.J.M.; Slobbe, A.T.
2015-01-01
This paper presents a monitoring and modelling methodology to assess the current and future conditions of steel bridges subjected to fatigue cracking. Steel bridges are subjected to fatigue cracking as a result of fluctuating stresses caused by the crossing of heavy vehicles. Specifically for
Long fatigue crack growth in Inconel 718 produced by selective laser melting
Czech Academy of Sciences Publication Activity Database
Konečná, R.; Kunz, Ludvík; Nicoletto, G.; Bača, A.
2016-01-01
Roč. 92, NOV (2016), s. 499-506 ISSN 0142-1123. [CP 2015 - International Conference on Crack Paths /5./. Ferrara, 16.09.2015-18.09.2015] Institutional support: RVO:68081723 Keywords : Inconel 718 * Selective laser melting * Microstructure * Fatigue crack growth * Fractography Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.899, year: 2016
Effect of stress ratio and frequency on fatigue crack growth rate of ...
Indian Academy of Sciences (India)
Effect of stress ratio and frequency on the fatigue crack propagation of 2618 aluminium alloy–silicon carbide composite were investigated at ambient temperature. With the first set of specimens, the fatigue crack growth rates were studied at three frequencies of 1 Hz, 5 Hz and 10 Hz at a stress ratio of 0.1 whereas the effects ...
Effect of temperature upon the fatigue-crack propagation behavior of Inconel X-750
International Nuclear Information System (INIS)
James, L.A.
1976-05-01
The techniques of linear-elastic fracture mechanics were employed to characterize the effect of temperature upon the fatigue-crack propagation behavior of precipitation heat-treated Inconel X-750 in an air environment over the range 75-1200 0 F. In general, fatigue-crack growth rates increased with increasing test temperature
Behavior of Fatigue Crack Tip Opening in Air and Corrosive Atmosphere
Hayashi, Morihito; Toeda, Kazunori
In the study, a formula for predicting fatigue crack tip opening displacement is deduced firstly. And then, due to comparing actual crack growth rate with the deduced formula, the crack tip configuration factor is defined to figure out the crack tip opening configuration that is useful to clarify the behavior of fatigue crack tip formation apparently. Applying the concept, the crack growth of 7/3 brass and 6/4 brass is predicted from the formula, by replacing material properties such as plastic flow resistance, Young modulus, the Poisson ratio, and fatigue toughness, and fatigue test conditions such as the stress intensity factor range, the load ratio, and cycle frequency. Furthermore, the theoretically expected results are verified with the fatigue tests which were carried out on CT specimens under different load conditions of load ratio, cycle frequency, and cyclic peak load, in different environments of air or corrosive ammonia atmosphere, for various brasses. And by comparing and discussing the calculated crack growth rate with attained experimental results, the apparent configuration factor at the crack tip is determined. And through the attained factor which changes along with crack growth, the behaviors of fatigue crack tip formation under different test conditions have been found out.
International Nuclear Information System (INIS)
Ilman, M.N.; Kusmono,; Iswanto, P.T.
2013-01-01
Highlights: • FSW enables unweldable aircraft material AA2024-T3 to be welded without cracking. • FSW applied to aircraft structure is required to have superior fatigue resistance. • Transient thermal tensioning (TTT) is being developed for stress relieving in FSW. • The fatigue crack growth rates of FSW joints under TTT are studied. - Abstract: Friction stir welding (FSW) has become a serious candidate technology to join metallic fuselage panels for the next generation of civil aircrafts. However, residual stress introduced during welding which subsequently affects fatigue performance is still a major problem that needs to be paid attention. The present investigation aims to improve fatigue crack growth resistance of friction stir aluminium alloy AA2024-T3 welds using transient thermal tensioning (TTT) treatment. In this investigation, aluminium alloy AA2024-T3 plates were joined using FSW process with and without TTT. The welding parameters used including tool rotation speed (Rt) and the plate travelling speed (v) were 1450 rpm and 30 mm/min respectively. The TTT treatments were carried out by heating both sides of friction stir weld line using moving electric heaters ahead of, beside and behind the tool at a heating temperature of 200 °C. Subsequently, a sequence of tests was carried out including microstructural examination, hardness measurement, tensile test and fatigue crack growth rate (FCGR) test in combination with fractography using scanning electron microscopy (SEM). The FCGR test was carried out using a constant amplitude fatigue experiment with stress ratio (R) of 0.1 and frequency (f) of 11 Hz whereas specimens used were centre-crack tension (CCT) type with the initial crack located at the weld nugget. Results of this investigation showed that at low ΔK, typically below 9 MPa m 0.5 , the friction stir welds under TTT treatments lowered fatigue crack growth rate (da/dN) and the lowest (da/dN) was achieved as the heaters were located ahead of
The Effect of the Free Surface on the Singular Stress Field at the Fatigue Crack Front
Directory of Open Access Journals (Sweden)
Oplt Tomáš
2017-11-01
Full Text Available Description of stress singularity in the vicinity of a free surface is presented. Its presence causes the retardation of the fatigue crack growth in that region and fatigue crack is being curved. Numerical model is used to study dependence of the stress singularity exponent on Poisson’s ratio. Estimated values are compared to those already published. Experimentally measured angles of fatigue crack on SENB specimens confirm the relation between Poisson’s ratio and the angle between crack front and free surface.
Energy Technology Data Exchange (ETDEWEB)
Spaehn, R. (Technische Hochschule Darmstadt (Germany, F.R.))
1991-03-01
The corrosion fatigue behaviour of three stainless steels - ferritic (12% Cr), austenitic (type 316 Ti) and austenitic-ferritic (type 31803; Duplex stainless steel) - was studied under rotating bending moments in aqueous sulphuric acid of 30deg C. An instrumental set-up for recording the transient currents of specimens during potentiostatically controlled corrosion fatigue is described. Based on this transient current signal technique, three stages on the corrosion fatigue process can be discerned. In the incubation period, small stochastic current transients are caused by the response of the passive layer to alternating stresses and environmental conditions. The appearance of sinusoidal current signals indicates crack initiation whereas the phase angle between a fixed marker - i.e. a light barrier signal -, and the anodic amplitude represents the site of initiating cracks. Finally, the crack growth period is characterized by an increasing cell current and steadily growing sinusoidal current signals caused by the interplay of microplastic and repassivation processes at the crack tip. (orig.).
The creep-fatigue crack growth behaviour of a 1CrMoV rotor steel
International Nuclear Information System (INIS)
Priest, R.H.; Miller, D.A.; Gladwin, D.N.; Maguire, J.
1989-01-01
Crack growth rates under simultaneous creep-fatigue conditions have been quantified for a 1CrMoV rotor steel. Measured growth rates were partitioned into cyclic and hold period contributions and these characterized by the relevant fracture mechanics parameters K and C. Cyclic growth rates measured in the creep-fatigue tests were enhanced compared with pure fatigue rates. This observation is compared with the behaviour of other steels and explained by quantitative metallography. The resulting crack growth equation can be used during integrity assessments for plant components containing cracks which are subject to thermal fatigue
Non-equilibrium statistical theory about microscopic fatigue cracks of metal in magnetic field
International Nuclear Information System (INIS)
Zhao-Long, Liu; Hai-Yun, Hu; Tian-You, Fan; Xiu-San, Xing
2010-01-01
This paper develops the non-equilibrium statistical fatigue damage theory to study the statistical behaviour of micro-crack for metals in magnetic field. The one-dimensional homogeneous crack system is chosen for study. To investigate the effect caused by magnetic field on the statistical distribution of micro-crack in the system, the theoretical analysis on microcrack evolution equation, the average length of micro-crack, density distribution function of micro-crack and fatigue fracture probability have been performed. The derived results relate the changes of some quantities, such as average length, density distribution function and fatigue fracture probability, to the applied magnetic field, the magnetic and mechanical properties of metals. It gives a theoretical explanation on the change of fatigue damage due to magnetic fields observed by experiments, and presents an analytic approach on studying the fatigue damage of metal in magnetic field. (cross-disciplinary physics and related areas of science and technology)
Study on fatigue life evaluation of structural component based on crack growth criterion
International Nuclear Information System (INIS)
Shibata, Katsuyuki
1984-07-01
As one of the practical application of fracture mechanics, fatigue life evaluation method based on crack growth criterion has been diffusing in various field of technology in order to determine the rational and reliable life of structural components. The fatigue life by this method is evaluated based on the fatigue crack growth analysis from defects, while many problems, such as the influence of residual stress on the crack growth behavior, the effect of overloading, and evaluation method for multiple surface cracks, are not sufficiently solved yet. In this paper, the above problems are treated, and based on some exprimental data some simple mehtods for fatigue life evaluation are proposed regarding the above problems. Verification of the proposed methods are shown in the paper by comparing with some experimental results, and the applicability of the proposed method is also examined by the fatigue test of pipes with cracks in the inner surface. (author)
Numerical modeling of thermal fatigue cracks from the viewpoint of eddy current testing
International Nuclear Information System (INIS)
Yusa, Noritaka; Hashizume, Hidetoshi; Virkkunen, Iikka; Kemppainen, Mika
2012-01-01
This study discusses a suitable numerical modeling of a thermal fatigue crack from the viewpoint of eddy current testing. Five artificial thermal fatigue cracks, introduced into type 304L austenitic stainless steel plates with a thickness of 25 mm, are prepared; and eddy current inspections are carried out to gather signals using an absolute type pancake probe and a differential type plus point probe. Finite element simulations are then carried out to evaluate a proper numerical model of the thermal fatigue cracks. In the finite element simulations, the thermal fatigue cracks are modeled as a semi-elliptic planar region on the basis of the results of the destructive tests. The width and internal conductivity are evaluated by the simulations. The results of the simulations reveal that the thermal fatigue cracks are regarded as almost nonconductive when the internal conductivity is assumed to be uniform inside. (author)
Silitonga, S.; Maljaars, J.; Soetens, F.; Snijder, H.H.
2014-01-01
In this work, a numerical method is pursued based on a cohesive zone model (CZM). The method is aimed at simulating fatigue crack growth as well as crack growth retardation due to an overload. In this cohesive zone model, the degradation of the material strength is represented by a variation of the
Diffraction-based study of fatigue crack initiation and propagation in aerospace aluminum alloys
Gupta, Vipul K.
The crack initiation sites and microstructure-sensitive growth of small fatigue cracks are experimentally characterized in two precipitation-hardened aluminum alloys, 7075-T651 and 7050-T7451, stressed in ambient temperature moist-air (warm-humid) and -50°C dry N2 (cold-dry) environmental conditions. Backscattered electron imaging (BSE) and energy dispersive spectroscopy (EDS) of the fracture surfaces showed that Fe-Cu rich constituent particle clusters are the most common initiation sites within both alloys stressed in either environment. The crack growth within each alloy, on average, was observed to be slowed in the cold-dry environment than in the warm-humid environment, but only at longer crack lengths. Although no overwhelming effects of grain boundaries and grain orientations on small-crack growth were observed, crack growth data showed local fluctuations within individual grains. These observations are understood as crack propagation through the underlying substructure at the crack surface and frequent interaction with low/high-angle grain and subgrain boundaries, during cyclic loading, and, are further attributed to periodic changes in crack propagation path and multiple occurrences of crack-branching observed in the current study. SEM-based stereology in combination with electron backscattered diffraction (EBSD) established fatigue crack surface crystallography within the region from ˜1 to 50 mum of crack initiating particle clusters. Fatigue crack facets were parallel to a wide variety of crystallographic planes, with pole orientations distributed broadly across the irreducible stereographic triangle between the {001} and {101}-poles within both warm-humid and cold-dry environments. The results indicate environmentally affected fatigue cracking in both cases, given the similarity between the observed morphology and crystallography with that of a variety of aerospace aluminum alloys cracked in the presence of moist-air. There was no evidence of
Effect of interaction of embedded crack and free surface on remaining fatigue life
Directory of Open Access Journals (Sweden)
Genshichiro Katsumata
2016-12-01
Full Text Available Embedded crack located near free surface of a component interacts with the free surface. When the distance between the free surface and the embedded crack is short, stress at the crack tip ligament is higher than that at the other area of the cracked section. It can be easily expected that fatigue crack growth is fast, when the embedded crack locates near the free surface. To avoid catastrophic failures caused by fast fatigue crack growth at the crack tip ligament, fitness-for-service (FFS codes provide crack-to-surface proximity rules. The proximity rules are used to determine whether the cracks should be treated as embedded cracks as-is, or transformed to surface cracks. Although the concepts of the proximity rules are the same, the specific criteria and the rules to transform embedded cracks into surface cracks differ amongst FFS codes. This paper focuses on the interaction between an embedded crack and a free surface of a component as well as on its effects on the remaining fatigue lives of embedded cracks using the proximity rules provided by the FFS codes. It is shown that the remaining fatigue lives for the embedded cracks strongly depend on the crack aspect ratio and location from the component free surface. In addition, it can be said that the proximity criteria defined by the API and RSE-M codes give overly conservative remaining lives. On the contrary, the WES and AME codes always give long remaining lives and non-conservative estimations. When the crack aspect ratio is small, ASME code gives non-conservative estimation.
A conductive grating sensor for online quantitative monitoring of fatigue crack
Li, Peiyuan; Cheng, Li; Yan, Xiaojun; Jiao, Shengbo; Li, Yakun
2018-05-01
Online quantitative monitoring of crack damage due to fatigue is a critical challenge for structural health monitoring systems assessing structural safety. To achieve online quantitative monitoring of fatigue crack, a novel conductive grating sensor based on the principle of electrical potential difference is proposed. The sensor consists of equidistant grating channels to monitor the fatigue crack length and conductive bars to provide the circuit path. An online crack monitoring system is established to verify the sensor's capability. The experimental results prove that the sensor is suitable for online quantitative monitoring of fatigue crack. A finite element model for the sensor is also developed to optimize the sensitivity of crack monitoring, which is defined by the rate of sensor resistance change caused by the break of the first grating channel. Analysis of the model shows that the sensor sensitivity can be enhanced by reducing the number of grating channels and increasing their resistance and reducing the resistance of the conductive bar.
Fatigue Behavior of Long and Short Cracks in Wrought and Powder Aluminum Alloys.
1984-05-01
The effects of cyclic frequency, electrochemical potential and bulk solution composition on the kinetics of small corrosion fatigue cracks have not...threshold behavior between cast iron (co = 113 MPa) and maraging steel (co = 1906 MPa), as a function of surface roughness (to simulate crack size) (after...4130 steel the crack size effect on corrosion fatigue, Fig. 2, is predicted in part based on linear superposition of stress corrosion growth rates for
Effect of temperature upon the fatigue-crack propagation behavior of Inconel 625
International Nuclear Information System (INIS)
James, L.A.
1977-03-01
The techniques of linear-elastic fracture mechanics were employed to characterize the effect of temperature upon the fatigue-crack propagation behavior of mill-annealed Inconel 625 in an air environment over the range 75 0 - 1200 0 F (24 0 - 649 0 C). In general, fatigue-crack growth rates increased with increasing test temperature. Two different specimen sizes were employed at each test temperature, and no effects of specimen size upon crack growth were noted
Energy Technology Data Exchange (ETDEWEB)
Tomkins, B.
1975-05-01
The value of modelling the fatigue crack propagation process is discussed and current models are examined in the light of increasing knowledge of crack tip deformation. Elevated temperature fatigue is examined in detail as an area in which models could contribute significantly to engineering design. A model is developed which examines the role of time-dependent creep cavitation on the failure process in an interactive creep-fatigue situation. (auth)
Influence of Initial Inclined Surface Crack on Estimated Residual Fatigue Lifetime of Railway Axle
Czech Academy of Sciences Publication Activity Database
Náhlík, Luboš; Pokorný, Pavel; Ševčík, Martin; Hutař, Pavel
2016-01-01
Roč. 7, č. 4 (2016), č. článku 1640007. ISSN 1756-9737. [FDM 2016 - International Conference on Fracture and Damage Mechanics /15./. Alicante, 14.09.2016-16.09.2016] R&D Projects: GA MŠk LM2015069; GA MŠk(CZ) ED1.1.00/02.0068 Institutional support: RVO:68081723 Keywords : inclined crack * railway axle * residual fatigue lifetime * fatigue crack propagation Subject RIV: JL - Materials Fatigue, Friction Mechanics
Effect of Sensitization on Corrosion-Fatigue Cracking in Al 5083 Alloy
2015-01-21
immediately ahead of the fatigue precrack in 0.001 and 0.01% NaCl solutions are transgranular ductile void coalescences. This observation suggests the 9...Naval Research Laboratory Washington, DC 20375-5320 NRL/MR/6355--15-9581 Effect of Sensitization on Corrosion- Fatigue Cracking in Al 5083 Alloy...area code) b. ABSTRACT c. THIS PAGE 18. NUMBER OF PAGES 17. LIMITATION OF ABSTRACT Effect of Sensitization on Corrosion- Fatigue Cracking in Al 5083
International Nuclear Information System (INIS)
Shibata, Katsuyuki; Yokoyama, Norio; Ohba, Toshihiro; Kawamura, Takaichi; Miyazono, Shohachiro
1982-12-01
Part-through surface cracks are most frequently observed in the inspection of structural components, and it is one of the important subjects in the assessment of safety to evaluate appropriately the growth of such cracks during the service life of structural components. Due to the complexity of the stress at the front free surface, the crack growth at the surface shows a different behavior from the other part. Besides, an effect of interaction is caused in the growth of multiple surface cracks. These effects should be included in the growth analysis of surface part-through cracks. Authors have carried out a series of fatigue tests on some kinds of pipes with multiple cracks in the inner surface, and subsequently the fatigue test of flat plate specimens, made of Type 304L stainless steel, with a single or double surface cracks was carried out to study the basic characteristics in the growth of multiple surface cracks. Based on the results of the flat plate test. the correction factors for the front free surface (Cs) and interaction (Ci) of surface cracks were derived quantitatively by the following empirical expressions; Cs = 0.824. Ci = (0.227(a/b) 2 (sec(PI X/2) - 1) + 1)sup(1/m). Using these two correction factors, a procedure to predict the growth of surface cracks was developed by applying the crack growth formula to both the thickness and surface directions. Besides, the crack growth predictions based on the procedure of ASME Code Sex. XI, and the above procedure without the correction of the free surface and interactions on the crack growth behaviors were compared with the test results of flat plate specimens. The crack growth behavior predicted by the procedure described in this report showed the best agreement with the test results in respects of the crack growth life and the change in the crack shape. The criteria of the ASME Code did not agree with the test results. (author)
Thermal fatigue cracking in T-fittings of feed water systems
International Nuclear Information System (INIS)
Oesterberg, J.
1983-03-01
The existence of thermal fatigue cracks can be determined by ultrasonic methods. The depth of the cracks will be of importance for evaluation of the seriousness of the situation. Currently, no method is available for determining depth of cracks without cutting and grinding. Methods for gaining information of crack depth have been discussed with leading European materials testing institutes. More elaborate ultrasonic methods have been tested with negative results. On testing signals from crack corners flood possible signals from the crack tips. At present no reliable technique based on ultrasonics exist (in Europe, that will give information of crack depth.(P.Aa.)
Intrinsic fatigue crack propagation in aluminum-lithium alloys - The effect of gaseous environments
Piascik, Robert S.; Gangloff, Richard P.
1989-01-01
Gaseous environmental effects on intrinsic fatigue crack growth are significant for the Al-Li-Cu alloy 2090, peak aged. For both moderate Delta K-low R and low Delta K-high R regimes, crack growth rates decrease according to the environment order: purified water vapor, moist air, helium and oxygen. Gaseous environmental effects are pronounced near threshold and are not closure dominated. Here, embrittlement by low levels of H2O (ppm) supports hydrogen embrittlement and suggests that molecular transport controlled cracking, established for high Delta K-low R, is modified near threshold. Localized crack tip reaction sites or high R crack opening shape may enable the strong, environmental effect at low levels of Delta K. Similar crack growth in He and O2 eliminates the contribution of surface films to fatigue damage in alloy 2090. While 2090 and 7075 exhibit similar environmental trends, the Al-Li-Cu alloy is more resistant to intrinsic corrosion fatigue crack growth.
International Nuclear Information System (INIS)
Lee, S. G.; Kim, I. S.; Park, Y. S.; Kim, J. W.; Park, C. Y.
2001-01-01
Fatigue tests in air and in room temperature water were performed to obtain comparable data and stable crack measuring conditions. In air environment, fatigue crack growth rate was increased with increasing temperature due to an increase in crack tip oxidation rate. In room temperature water, the fatigue crack growth rate was faster than in air and crack path varied on loading conditions. In simulated light water reactor (LWR) conditions, there was little environmental effect on the fatigue crack growth rate (FCGR) at low dissolved oxygen or at high loading frequency conditions. While the FCGR was enhanced at high oxygen condition, and the enhancement of crack growth rate increased as loading frequency decreased to a critical value. In fractography, environmentally assisted cracks, such as semi-cleavage and secondary intergranular crack, were found near sulfide inclusions only at high dissolved oxygen and low loading frequency condition. The high crack growth rate was related to environmentally assisted crack. These results indicated that environmentally assisted crack could be formed by the Electrochemical effect in specific loading condition
The effect of low temperatures on the fatigue crack growth of S460 structural steel
Walters, C.L.; Alvaro, A.; Maljaars, J.
2016-01-01
The Fatigue Ductile–Brittle Transition (FDBT) is a phenomenon similar to the fracture ductile to brittle transition, in which the fracture mode of the fatigue cracks changes from ductile transgranular to cleavage and/or grain boundary separation. Fatigue at temperatures below the FDBT has a much
Multiaxial Fatigue Properties of 2A12 Aluminum Alloy Under Different Stress Amplitude Ratio Loadings
Directory of Open Access Journals (Sweden)
CHEN Ya-jun
2017-09-01
Full Text Available The multiaxial fatigue behavior of 2A12 aluminum alloy was studied with SDN100/1000 electro-hydraulic servo tension-torsion fatigue tester under different stress amplitude ratios, the fracture morphology and the fatigue loading curve were observed to study the failure mechanism. The results show that, under the one stage loading condition, the fatigue life prolongs with the stress amplitude ratio increasing. Under pure torsion loading, smooth and even area exists in the fracture surface. As the stress amplitude ratio increases, the number of scratch reduces, the fatigue striation and some special morphology such as the fishbone pattern, scale pattern and honeycomb pattern can be observed; under cumulative paths of different stress amplitude ratios, the variation of multiaxial fatigue life changes with first stage loading cycles; under cumulative paths of high-low stress amplitude ratio, the cycle hardening occurs obviously in the axial direction for the first stage high stress amplitude ratio loading and 2A12 alloy shows training effect.
International Nuclear Information System (INIS)
Okafor, A. Chukwujekwu; Singh, Navdeep; Singh, Navrag
2007-01-01
An aircraft is subjected to severe structural and aerodynamic loads during its service life. These loads can cause damage or weakening of the structure especially for aging military and civilian aircraft, thereby affecting its load carrying capabilities. Hence composite patch repairs are increasingly used to repair damaged aircraft metallic structures to restore its structural efficiency. This paper presents the results of Acoustic Emission (AE) monitoring of crack propagation in 2024-T3 Clad aluminum panels repaired with adhesively bonded octagonal, single sided boron/epoxy composite patch under tension-tension fatigue loading. Crack propagation gages were used to monitor crack initiation. The identified AE sensor features were used to train neural networks for predicting crack length. The results show that AE events are correlated with crack propagation. AE system was able to detect crack propagation even at high noise condition of 10 Hz loading; that crack propagation signals can be differentiated from matrix cracking signals that take place due to fiber breakage in the composite patch. Three back-propagation cascade feed forward networks were trained to predict crack length based on the number of fatigue cycles, AE event number, and both the Fatigue Cycles and AE events, as inputs respectively. Network using both fatigue cycles and AE event number as inputs to predict crack length gave the best results, followed by Network with fatigue cycles as input, while network with just AE events as input had a greater error
Crack growth under combined creep and fatigue conditions in alloy 800
International Nuclear Information System (INIS)
Pfaffelhuber, M.; Roedig, M.; Schubert, F.; Nickel, H.
1989-08-01
To investigate the crack growth behaviour under combined creep-fatigue loading, CT 25 mm-specimens of X10NiCrAlTi 32 20 (Alloy 800) have been tested in experiments with cyclic loadings and hold times, with static loadings and short stress rekief interrupts, with ramp type loadings and with sequences of separate fatigue and creep crack growth periods. The test temperature of 700deg C was selected because only in this temperature range this alloy provides similar amounts of crack growth under creep and fatigue conditions due to equivalent stress levels. For the estimation of crack growth under combined loading conditions a linear accumulation of increase in crack length was proved using the crack growth laws of pure creep and fatigue crack growth. Hold time and ramp loadings lead to a higher crack growth rate compared with pure creep or pure fatigue crack growth tests. In hold time experiments the crack growth rate is higher than ramp tests of the same period time. The results of hold time tests can be fairly enough predicted by linear damage accumulation rules. (orig.) [de
Effect of overloads on fatigue crack propagation rate
International Nuclear Information System (INIS)
Kogaev, V.P.; Bojtsov, B.V.; Petukhov, Yu.V
1986-01-01
An overload coefficient Q, the number of overload cycles Nsub(0), the value of the stress intensity coefficient swing of basic loading conditions ΔK are experimentally studied for their effect on the delay of the fatigue crack propagation Nsub(D) in 30KhGSNA steel. Results of the study are presented. It is shown that as a result of single overloads the value attains 60 - 10 thous. cycles. The delay Nsub(D) grows with the overload coefficient Q=Ksub(max)sup(0)/Ksub(max) and the number of the overload cycles Nsub(0). The regularity indicated is described by the equations valid within the limits of variation in Q and Nsub(0) values studied in the paper
Fatigue-crack propagation in gamma-based titanium aluminide alloys at large and small crack sizes
International Nuclear Information System (INIS)
Kruzic, J.J.; Campbell, J.P.; Ritchie, R.O.
1999-01-01
Most evaluations of the fracture and fatigue-crack propagation properties of γ+α 2 titanium aluminide alloys to date have been performed using standard large-crack samples, e.g., compact-tension specimens containing crack sizes which are on the order of tens of millimeters, i.e., large compared to microstructural dimensions. However, these alloys have been targeted for applications, such as blades in gas-turbine engines, where relevant crack sizes are much smaller ( 5 mm) and (c ≅ 25--300 microm) cracks in a γ-TiAl based alloy, of composition Ti-47Al-2Nb-2Cr-0.2B (at.%), specifically for duplex (average grain size approximately17 microm) and refined lamellar (average colony size ≅150 microm) microstructures. It is found that, whereas the lamellar microstructure displays far superior fracture toughness and fatigue-crack growth resistance in the presence of large cracks, in small-crack testing the duplex microstructure exhibits a better combination of properties. The reasons for such contrasting behavior are examined in terms of the intrinsic and extrinsic (i.e., crack bridging) contributions to cyclic crack advance
International Nuclear Information System (INIS)
Xiao Jun; Chen Luyao; Qiu Shaoyu; Chen Yong; Lin Zhenxia; Fu Zhenghong
2015-01-01
Inconel 690 (TT) is one of the key materials for tubes of steam generators for pressurized water reactors, where it is susceptible to corrosion fatigue cracking. In this paper, the corrosion fatigue cracking behavior of Inconel 690 (TT) was investigated under small scale yielding conditions, in the simulated secondary water of pressurized water reactor. It was observed that the fatigue crack growth rate was accelerated by a maximum factor up to 3 in the simulated secondary water, comparing to that in room temperature air. In addition, it was found that the accelerating effect was influenced by out-of-plane cracking of corrosion fatigue cracks and also correlated with stress intensity factor range, maximum stress intensity factor and stress ratio. (authors)
Probabilistic modeling of fatigue crack growth in Ti-6Al-4V
International Nuclear Information System (INIS)
Soboyejo, W.O.; Shen, W.; Soboyejo, A.B.O.
2001-01-01
This paper presents the results of a combined experimental and analytical study of the probabilistic nature of fatigue crack growth in Ti-6Al-4V. A simple experimental fracture mechanics framework is presented for the determination of statistical fatigue crack growth parameters from two fatigue tests. The experimental studies show that the variabilities in long fatigue crack growth rate data and the Paris coefficient are well described by the log-normal distributions. The variabilities in the Paris exponent are also shown to be well characterized by a normal distribution. The measured statistical distributions are incorporated into a probabilistic fracture mechanics framework for the estimation of material reliability. The implications of the results are discussed for the probabilistic analysis of fatigue crack growth in engineering components and structures. (orig.)
Crack initiation through vibration fatigue of small-diameter pipes
International Nuclear Information System (INIS)
Comby, R.; Thebault, Y.; Papaconstantinou, T.
2002-01-01
Socket welds are used extensively for small bore piping connections in nuclear power plant systems. Numerous fatigue-related failures occurred in the past ten years mainly on safeguard systems and continue to occur frequently, showing that corrective actions did not take into account all aspects of the problem. Destructive examination of cracked small bore piping connections allowed a better understanding of failure mechanisms and a prediction of crack initiation site depending on nozzle fittings such as run pipe and small bore pipe thickness. A three-dimensional finite element model confirmed the conclusions of the lab examinations. For thick run pipes, it was shown that the failure tend to initiate predominantly at the socket weld toe or at the root, depending on the respective thickness of coupling and small bore pipe. Some additional studies, based on RSE-M code, are in progress in order to determine the maximum stresses location. Lessons learned through these investigations led to optimise the in-service inspection scope and to define solutions to be carried out to prevent failure of ''susceptible'' small bore pipe connections. Since July 2000, a large program is in progress to select all ''susceptible'' small bore pipes in safety-related systems and to apply corrective measures such as piping modifications or system operational modifications. (authors)
Study on Characteristics of Corrosion Fatigue Crack Propagation for Austenitic Stainless Steel
International Nuclear Information System (INIS)
Lim, Uh Joh; Kim, Bu Ahn
1988-01-01
The characteristics of the corrosion fatigue cracking of both TIG weld heat affected zone and base metal for austenitic stainless steel were investigated under the environments of various specific resistance and the air. The corrosion fatigue crack initiation sensitivity was quantitatively investigated for SUS 304 weldments in the various specific resistances. Also, the characteristics of corrosion fatigue cracking for the weldments were investigated from mechanical, electrochemical, and microstructural point of view. Main results obtained are as follows: (1) The corrosion fatigue crack initiation sensitivity on the base metal and weld hea affected zone increases as the specific resistance of corrosion environment decreases, and the sensitivity of the weld heat affected zone appears increasing more than that of the base metal. (2) The corrosion potentials of various specific resistances are almost constant in initial corrosion fatigue cracking, but the corrosion potential becomes less noble promptly with the corrosion fatigue crack growth as the specific resistances decrease. (3) The corrosion fatigue crack growth of the weld heat affected zone rapid than that of the base metal, because of the softening and the less noble potential caused by welding heat cycle
The reduction in fatigue crack growth resistance of dentin with depth.
Ivancik, J; Neerchal, N K; Romberg, E; Arola, D
2011-08-01
The fatigue crack growth resistance of dentin was characterized as a function of depth from the dentino-enamel junction. Compact tension (CT) specimens were prepared from the crowns of third molars in the deep, middle, and peripheral dentin. The microstructure was quantified in terms of the average tubule dimensions and density. Fatigue cracks were grown in-plane with the tubules and characterized in terms of the initiation and growth responses. Deep dentin exhibited the lowest resistance to the initiation of fatigue crack growth, as indicated by the stress intensity threshold (ΔK(th) ≈ 0.8 MPa•m(0.5)) and the highest incremental fatigue crack growth rate (over 1000 times that in peripheral dentin). Cracks in deep dentin underwent incremental extension under cyclic stresses that were 40% lower than those required in peripheral dentin. The average fatigue crack growth rates increased significantly with tubule density, indicating the importance of microstructure on the potential for tooth fracture. Molars with deep restorations are more likely to suffer from the cracked-tooth syndrome, because of the lower fatigue crack growth resistance of deep dentin.
International Nuclear Information System (INIS)
Kamaya, Masayuki
2013-01-01
The number of cycles to failure of specimens in fatigue tests can be estimated by predicting crack growth. Under a cyclic thermal stress caused by fluctuation of fluid temperature, due to the stress gradient in the thickness direction, the estimated fatigue life differs from that estimated for mechanical fatigue tests. In this paper, the influence of crack growth under cyclic thermal loading on the fatigue life was investigated. First, the thermal stress was derived by superposing analytical solutions, and then, the stress intensity factor was obtained by the weight function method. It was shown that the thermal stress depended not on the rate of the fluid temperature change but on the rise time, and the magnitude of the stress was increased as the rise time was decreased. The stress intensity factor under the cyclic thermal stress was smaller than that under the uniform stress distribution. The change in the stress intensity factor with the crack depth did not depend on the heat transfer coefficient and only slightly depended on the rise time. The estimated fatigue life under the cyclic thermal loading could be 1.6 times longer than that under the uniform stress distribution. The critical size for the fatigue life determination was assumed to be 3 mm for fatigue test specimens of 10 mm diameter. By evaluating the critical size by structural integrity analyses, the fatigue life was increased and the effect of the critical size on the fatigue life was more pronounced for the cyclic thermal stress. (author)
International Nuclear Information System (INIS)
Kamaya, Masayuki
2013-01-01
The number of cycles to failure of specimens in fatigue tests can be estimated by predicting crack growth. Under a cyclic thermal stress caused by fluctuation of fluid temperature, due to the stress gradient in the thickness direction, the estimated fatigue life differs from that estimated for mechanical fatigue tests. In this paper, the influence of crack growth under cyclic thermal loading on the fatigue life was investigated. First, the thermal stress was derived by superposing analytical solutions, and then, the stress intensity factor was obtained by the weight function method. It was shown that the thermal stress depended not on the rate of the fluid temperature change but on the rise time, and the magnitude of the stress was increased as the rise time was decreased. The stress intensity factor under the cyclic thermal stress was smaller than that under the uniform stress distribution. The change in the stress intensity factor with the crack depth was almost the same regardless of the rise time. The estimated fatigue life under the cyclic thermal loading could be 1.6 times longer than that under the uniform stress distribution. The critical size for the fatigue life determination was assumed to be 3 mm for fatigue test specimens of 10 mm diameter. By evaluating the critical size by structural integrity analyses, the fatigue life was increased and the effect of the critical size on the fatigue life was more pronounced for the cyclic thermal stress. (author)
NASGRO(registered trademark): Fracture Mechanics and Fatigue Crack Growth Analysis Software
Forman, Royce; Shivakumar, V.; Mettu, Sambi; Beek, Joachim; Williams, Leonard; Yeh, Feng; McClung, Craig; Cardinal, Joe
2004-01-01
This viewgraph presentation describes NASGRO, which is a fracture mechanics and fatigue crack growth analysis software package that is used to reduce risk of fracture in Space Shuttles. The contents include: 1) Consequences of Fracture; 2) NASA Fracture Control Requirements; 3) NASGRO Reduces Risk; 4) NASGRO Use Inside NASA; 5) NASGRO Components: Crack Growth Module; 6) NASGRO Components:Material Property Module; 7) Typical NASGRO analysis: Crack growth or component life calculation; and 8) NASGRO Sample Application: Orbiter feedline flowliner crack analysis.
International Nuclear Information System (INIS)
Lloyd, G.J.; Wareing, J.
1979-01-01
The distinction between stable and unstable fatigue crack propagation during high temperature creep-fatigue in austenitic stainless steels is introduced. The transition from one class of behavior to the other is related to the precipitate distribution and to the nature of the prevailing crack path. It is shown by reference to new studies and examples drawn from the literature that this behavior is common to both high strain and predominantly elastic fatigue in austenitic stainless steels. The relevance of this distinction to a mechanistic approach to high temperature plant design is discussed
Influence of the non-singular stress on the crack extension and fatigue life
International Nuclear Information System (INIS)
Cheng, C.Z.; Recho, N.; Niu, Z.R.
2012-01-01
Highlights: ► BEM is combined by characteristic analysis to calculate the singular stress field. ► A new method is proposed to evaluate the full stress field at crack tip region. ► Effect of non-singular stress on the propagation direction of the fatigue crack is analyzed. ► The influence of non-singular stress on the fatigue crack life is evaluated. - Abstract: The complete elasticity stress field at a crack tip region can be presented by the sum of the singular stress and several non-singular stress terms according to the Williams asymptotic expansion theory. The non-singular stress has a non-negligible influence on the prediction of the crack extension direction and crack growth rate under the fatigue loading. A novel method combining the boundary element method and the singularity characteristic analysis is proposed here to evaluate the complete stress field at a crack tip region. In this new method, any non-singular stress term in the Williams series expansion can be evaluated according to the computational accuracy requirement. Then, a modified Paris law is introduced to predict the crack propagation under the mixed-mode loading for exploring the influence of the non-singular stress on the fatigue life duration. By comparing with the existed experimental results, the predicted crack fatigue life when the non-singular stress is taken into consideration is more accurate than the predicted ones only considering the singular stress.
Fatigue and Creep Crack Propagation behaviour of Alloy 617 in the Annealed and Aged Conditions
Energy Technology Data Exchange (ETDEWEB)
Julian K. Benz; Richard N. Wright
2013-10-01
The crack propagation behaviour of Alloy 617 was studied under various conditions. Elevated temperature fatigue and creep-fatigue crack growth experiments were conducted at 650 and 800 degrees C under constant stress intensity (triangle K) conditions and triangular or trapezoidal waveforms at various frequencies on as-received, aged, and carburized material. Environmental conditions included both laboratory air and characteristic VHTR impure helium. As-received Alloy 617 displayed an increase in the crack growth rate (da/dN) as the frequency was decreased in air which indicated a time-dependent contribution component in fatigue crack propagation. Material aged at 650°C did not display any influence on the fatigue crack growth rates nor the increasing trend of crack growth rate with decreasing frequency even though significant microstructural evolution, including y’ (Ni3Al) after short times, occurred during aging. In contrast, carburized Alloy 617 showed an increase in crack growth rates at all frequencies tested compared to the material in the standard annealed condition. Crack growth studies under quasi-constant K (i.e. creep) conditions were also completed at 650 degrees C and a stress intensity of K = 40 MPa9 (square root)m. The results indicate that crack growth is primarily intergranular and increased creep crack growth rates exist in the impure helium environment when compared to the results in laboratory air. Furthermore, the propagation rates (da/dt) continually increased for the duration of the creep crack growth either due to material aging or evolution of a crack tip creep zone. Finally, fatigue crack propagation tests at 800 degrees C on annealed Alloy 617 indicated that crack propagation rates were higher in air than impure helium at the largest frequencies and lowest stress intensities. The rates in helium, however, eventually surpass the rates in air as the frequency is reduced and the stress intensity is decreased which was not observed at 650
International Nuclear Information System (INIS)
Soppa, E.; Kohler, C.; Roos, E.; Schuler, X.
2012-01-01
The understanding of the crack initiation mechanisms and crack growth in apparently monolithic materials like X6CrNiNb18-10 stainless steel under cyclic loading requires the explicit analysis of the phenomena underlying fatigue on both atomistic and microscopic levels. The permanent delivery of mechanical energy through cyclic loading evokes changes in the microstructure that can lead to a martensitic transformation. The transformation of a metastable cubic face centered austenite and formation of a cubic body centered α'-martensite under cyclic loading at room temperature was found, both, in the experiment and in molecular dynamics simulations. The martensite nucleates prevalently at grain boundaries, triple points and at the specimen free surface and forms small (∝ 1 μm) differently oriented grains, also in the same parent austenitic grain. By a combination of interrupted low cycle fatigue tests (LCF) and electron backscatter diffraction (EBSD) measurements the martensitic transformation and subsequent fatigue crack formation were observed at the same area in the microstructure at different stages of the specimen lifetime. The EBSD measurements showed the following crack initiation scenarios: Cracks started (a) at the phase boundary between austenite and α'-martensite, (b) inside fully martensitic areas in the matrix, (c) at broken or debonded coarse NbCs. It is obvious that formation of a hard α'-martensite in a ductile and soft austenite and forming two-phase material causes a heterogeneous stress and strain distribution on the microscopic level. α'-martensite enhances locally the stress amplitude whereas in a soft austenite the plastic strain amplitude increases. Strain concentration in the austenite along the phase boundary is connected with a stress increase along the interface and can initiate fatigue crack there. Also at the crack tip, a permanent martensitic transformation occurs, so that the growth of the fatigue cracks at room temperature seems
Energy Technology Data Exchange (ETDEWEB)
Soppa, E.; Kohler, C.; Roos, E.; Schuler, X. [Stuttgart Univ. (Germany). MPA
2012-07-01
The understanding of the crack initiation mechanisms and crack growth in apparently monolithic materials like X6CrNiNb18-10 stainless steel under cyclic loading requires the explicit analysis of the phenomena underlying fatigue on both atomistic and microscopic levels. The permanent delivery of mechanical energy through cyclic loading evokes changes in the microstructure that can lead to a martensitic transformation. The transformation of a metastable cubic face centered austenite and formation of a cubic body centered α'-martensite under cyclic loading at room temperature was found, both, in the experiment and in molecular dynamics simulations. The martensite nucleates prevalently at grain boundaries, triple points and at the specimen free surface and forms small (∝ 1 μm) differently oriented grains, also in the same parent austenitic grain. By a combination of interrupted low cycle fatigue tests (LCF) and electron backscatter diffraction (EBSD) measurements the martensitic transformation and subsequent fatigue crack formation were observed at the same area in the microstructure at different stages of the specimen lifetime. The EBSD measurements showed the following crack initiation scenarios: Cracks started (a) at the phase boundary between austenite and α'-martensite, (b) inside fully martensitic areas in the matrix, (c) at broken or debonded coarse NbCs. It is obvious that formation of a hard α'-martensite in a ductile and soft austenite and forming two-phase material causes a heterogeneous stress and strain distribution on the microscopic level. α'-martensite enhances locally the stress amplitude whereas in a soft austenite the plastic strain amplitude increases. Strain concentration in the austenite along the phase boundary is connected with a stress increase along the interface and can initiate fatigue crack there. Also at the crack tip, a permanent martensitic transformation occurs, so that the growth of the fatigue cracks at room
Fatigue cracking of alloy 600 in simulated steam generator crevice environment
International Nuclear Information System (INIS)
Ogundele, G.; Lepik, O.
1998-01-01
Investigations were carried out to generate fatigue life (S-N) and near-threshold fatigue crack propagation (da/dN) data to determine the environmental influence on fatigue behavior for Alloy 600 in air, deionized water and in simulated Bruce Nuclear Generating Station 'A' crevice environments under appropriate loading conditions. In the low cycle fatigue regime, the simulated crevice environment did not affect the fatigue life of Alloy 600 under the applied loading conditions. The near-threshold fatigue crack growth rates of Alloy 600 in the simulated crevice environment were significantly lower compared to either pure water or air environments and is believed to be the result of higher crack closure in the crevice environment. (author)
Fatigue crack growth and endurance data on 9% Cr 1% Mo steels for AGR applications
International Nuclear Information System (INIS)
Priddle, E.K.
1987-01-01
Experimental investigations have been carried out on 9%Cr 1%Mo steels to examine: (1) The significance of carburisation on the fatigue endurance of plain and welded boiler tubes, and tube spacer strip; (2) the high cycle fatigue endurance of spacer strip and spacer weld metal; (3) fatigue crack growth rates in spacer strip and spacer weld metal. This report summarises the results of these investigations and where necessary compares the data to that in current data sheets. The effects of carburisation are variable depending on the structure and type of carburisation. The fatigue endurance properties of spacer strip and spacer weld metal are also similar and need not be considered separately for assessment or design purposes. Fatigue crack growth rates in spacer strip and space weld metal are similar and are influenced by both stress ratio and temperature. A design curve from a fast reactor data sheet may be used as an upper bound to these fatigue crack growth results. (author)
A comparison of fatigue crack growth in human enamel and hydroxyapatite.
Bajaj, Devendra; Nazari, Ahmad; Eidelman, Naomi; Arola, Dwayne D
2008-12-01
Cracks and craze lines are often observed in the enamel of human teeth, but they rarely cause tooth fracture. The present study evaluates fatigue crack growth in human enamel, and compares that to the fatigue response of sintered hydroxyapatite (HAp) with similar crystallinity, chemistry and density. Miniature inset compact tension (CT) specimens were prepared that embodied a small piece of enamel (N=8) or HAp (N=6). The specimens were subjected to mode I cyclic loads and the steady state crack growth responses were modeled using the Paris Law. Results showed that the fatigue crack growth exponent (m) for enamel (m=7.7+/-1.0) was similar to that for HAp (m=7.9+/-1.4), whereas the crack growth coefficient (C) for enamel (C=8.7 E-04 (mm/cycle)x(MPa m(0.5))(-m)) was significantly lower (pcrack growth in the enamel occurred primarily along the prism boundaries. In regions of decussation, the microstructure promoted microcracking, crack bridging, crack deflection and crack bifurcation. Working in concert, these mechanisms increased the crack growth resistance and resulted in a sensitivity to crack growth (m) similar to bone and lower than that of human dentin. These mechanisms of toughening were not observed in the crack growth response of the sintered HAp. While enamel is the most highly mineralized tissue of the human body, the microstructural arrangement of the prisms promotes exceptional resistance to crack growth.
Directory of Open Access Journals (Sweden)
Jakubowski Marek
2015-09-01
Full Text Available In the paper has been discussed influence of stresses on general corrosion rate and corrosion pit nucleation rate and growth , whose presence has been questioned by some authors but accepted by most of them. Influence of roughness of pit walls on fatigue life of a plate suffering pit corrosion and presence of the so called „ non-damaging” pits which never lead to initiation of fatigue crack, has been presented. Possibility of prediction of pit-to-crack transition moment by two different ways, i.e. considering a pit a stress concentrator or an equivalent crack, has been analyzed. Also, influence of statistical distribution of depth of corrosion pits as well as anticorrosion protection on fatigue and corrosion fatigue has been described.
Study of fatigue crack propagation in laminated metal composites alluminium 1100/alluminium 2024
International Nuclear Information System (INIS)
Tavares, R.I.
1984-01-01
A study has been made of fatigue crack propagation in laminated metal composites with different volume fraction of constituents. The composites were produced by hot rolling, combining 1100 and 2024 aluminum alloys in crack divider orientation. Mechanical and metallurgical properties of the composites and original alloys sheets have been evaluated. Paris type relationship, corresponding to stage II of fatigue crack propagation curves, has been determined by two different methods, wich have shown to be equivalent. A computer software in FORTRAN language was developed for all the mathematical manipulation of fatigue data including statistical analysis and graphics. (Author) [pt
Crack growth behaviour of aluminium wrought alloys in the Very High Cycle Fatigue regime
Directory of Open Access Journals (Sweden)
Bülbül Fatih
2018-01-01
Full Text Available Investigations have shown that in the regime of Very High Cycle Fatigue (VHCF “natural” crack initiation often takes place underneath the material surface leading to crack propagation without contact to atmospheric components. In order to elucidate the environmental damage contribution and its effect on the VHCF long crack propagation, fatigue experiments with alternating environment (vacuum and laboratory air were performed. An ultrasonic fatigue testing system (USFT equipped with a small vacuum chamber was applied that enables the in-situ examination of the long fatigue crack propagation at a resonance frequency of about 20 kHz by using a long distance microscope. By means of the Focused-Ion-Beam technique, micro-notches were prepared in the USFT specimens. The tests were carried out on the aluminium alloys EN-AW 6082 and 5083 in different conditions. It has been found that the atmosphere has a significant influence on the VHCF long crack propagation which manifests itself in the crack path as well as in the crack growth rates. Because of pronounced single sliding in vacuum, shear-stress-controlled crack propagation was detected whereas in laboratory air normal-stress-controlled crack propagation occurred. Furthermore, it has been proven that the secondary precipitation state of the aluminium alloy significantly influences the VHCF long crack propagation in vacuum.
On the controlling parameters for fatigue-crack threshold at low homologous temperatures
International Nuclear Information System (INIS)
Yu, W.; Gerberich, W.W.
1983-01-01
Fatigue crack propagation phenomena near the threshold stress intensity level ΔK /SUB TH/ , has been a vigorously studied topic in recent years. Near threshold the crack propagates rather slowly, thus giving enough time for various physical and chemical reactions to take place. Room air, which is the most commonly encountered environment, can still supply various ingredients such as oxygen, water vapor (and thus hydrogen) to support these reactions. Much effort had been directed toward the environmental aspects of near threshold fatigue crack growth. By conducting tests under vacuum, Suresh and coworkers found that the crack propagation rate in a 2-1/4 Cr-1Mo steel was higher in vacuum than in air. An oxide induced closure, which served to reduce the effective stress intensity at the crack tip, seems to furnish a good explanation. Neumann and coworkers proposed that during the fatigue process, extrusion-intrusion pairs can develop as a consequence of reversed slip around the crack tip when the crack was propagated near threshold stress intensity. Beevers demonstrated that fatigue fracture surfaces contact each other during unloading even under tension-tension cycling. Kanninen and Atkinson also reached the conclusion that the compressive stress acting at the crack tip due to residual plasticity can induce closure. Microstructural effects have also been cited as important factors in near threshold crack growth. It is generally accepted that coarser grains have a beneficial effect on the resistance to the near threshold crack propagation
An evaluation on fatigue crack growth in a fine-grained isotropic graphite
Energy Technology Data Exchange (ETDEWEB)
Wang Hongtao; Sun Libin [Institute of Nuclear and New Energy Technology, Tsinghua University, Beijing 100084 (China); Li Chenfeng [College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP (United Kingdom); Shi Li [Institute of Nuclear and New Energy Technology, Tsinghua University, Beijing 100084 (China); Wang Haitao, E-mail: wanght@tsinghua.edu.cn [Institute of Nuclear and New Energy Technology, Tsinghua University, Beijing 100084 (China)
2012-09-15
Highlights: Black-Right-Pointing-Pointer The propagation of micro- and macro-fatigue cracks in IG-11 graphite was studied. Black-Right-Pointing-Pointer The curves of the fatigue crack growth rate versus the SIF range show three stages. Black-Right-Pointing-Pointer The fatigue microcrack propagation is very sensitive to graphite's microstructures. Black-Right-Pointing-Pointer Graphite's microstructures have no significant impact on fatigue macrocrack growth. Black-Right-Pointing-Pointer The fatigue fracture surface indicates the fracture mechanism of the IG-11 graphite. - Abstract: The aim of this paper is to investigate the mechanism of fatigue crack propagation in IG-11 graphite, and determine the crack growth rate in relation to the stress level. Experimental studies were performed at both micro and macro scales. For fatigue microcrack propagation, single-edge-notch specimens were chosen for testing and the fatigue crack growth was measured in situ with a scanning electron microscope. For fatigue macrocrack propagation, CT specimens were used and the fatigue crack growth was measured with a high-accuracy optic microscope. Combining the two groups of experimental results, the following conclusions are derived: (1) The heterogeneous microstructures of the graphite material have significant impact on the fatigue microcrack growth, while their influence on fatigue macrocrack growth is very limited. (2) The relationship between the fatigue crack growth rate and the crack-tip stress intensity factor range can be expressed in the form of Paris formulae, which contains three stages: an initial rising part with a small slope, an abrupt rise with a very large acceleration, and a short final part with a small slope. (3) The fatigue fracture surface of the graphite material contains considerable sliding of leaf-shape graphite flakes combined with small cotton-shape plastic deformations. These sliding traces are approximately aligned at 45 Degree-Sign , showing the
An evaluation on fatigue crack growth in a fine-grained isotropic graphite
International Nuclear Information System (INIS)
Wang Hongtao; Sun Libin; Li Chenfeng; Shi Li; Wang Haitao
2012-01-01
Highlights: ► The propagation of micro- and macro-fatigue cracks in IG-11 graphite was studied. ► The curves of the fatigue crack growth rate versus the SIF range show three stages. ► The fatigue microcrack propagation is very sensitive to graphite's microstructures. ► Graphite's microstructures have no significant impact on fatigue macrocrack growth. ► The fatigue fracture surface indicates the fracture mechanism of the IG-11 graphite. - Abstract: The aim of this paper is to investigate the mechanism of fatigue crack propagation in IG-11 graphite, and determine the crack growth rate in relation to the stress level. Experimental studies were performed at both micro and macro scales. For fatigue microcrack propagation, single-edge-notch specimens were chosen for testing and the fatigue crack growth was measured in situ with a scanning electron microscope. For fatigue macrocrack propagation, CT specimens were used and the fatigue crack growth was measured with a high-accuracy optic microscope. Combining the two groups of experimental results, the following conclusions are derived: (1) The heterogeneous microstructures of the graphite material have significant impact on the fatigue microcrack growth, while their influence on fatigue macrocrack growth is very limited. (2) The relationship between the fatigue crack growth rate and the crack-tip stress intensity factor range can be expressed in the form of Paris formulae, which contains three stages: an initial rising part with a small slope, an abrupt rise with a very large acceleration, and a short final part with a small slope. (3) The fatigue fracture surface of the graphite material contains considerable sliding of leaf-shape graphite flakes combined with small cotton-shape plastic deformations. These sliding traces are approximately aligned at 45°, showing the main cause of the fatigue fracture is the shear stress. There are also a large amount of secondary cracks inside unit cells and on cell walls
DEFF Research Database (Denmark)
Manca, Marcello; Quispitupa, Amilcar; Berggreen, Christian
2012-01-01
Face/core fatigue crack growth in foam-cored sandwich composites is examined using the mixed mode bending (MMB) test method. The mixed mode loading at the debond crack tip is controlled by changing the load application point in the MMB test fixture. Sandwich specimens were manufactured using H45...... and H100 PVC foam cores and E-glass/polyester face sheets. All specimens were pre-cracked in order to define a sharp crack front. The static debond fracture toughness for each material configuration was measured at different mode-mixity phase angles. Fatigue tests were performed at 80% of the static...
Local strain in front of cracks in the case of creep fatigue
International Nuclear Information System (INIS)
Rie Kyongtschong; Olfe, J.
1993-01-01
In-situ measurements of strain fields in front of cracks were performed for high temperature Low Cycle Fatigue (LCF) with different hold times by means of a grid method. The tests were carried out on the austenitic stainless steel 304 L and the ferritic steel X22 CrMoV 12 1. Simultaneous observation of crack growth leads to a correlation between crack growth and local strain. The interaction of creep and fatigue related to strain concentration at the crackk tip and crack growth was discussed. A model is proposed which is based on the formation of cavities on grain boundaries. (orig.) [de
Determination and demarcation of fatigue crack initiation phase in rotating bending condition
International Nuclear Information System (INIS)
Pasha, R.A.; Rehman, K.; Shah, M.
2012-01-01
In engineering applications, components often experience cyclic loading and therefore, have crack initiation propagation phase. In this research work experimental demarcation of fatigue crack initiation has been investigated. Initiation phase of fatigue life of Aluminium was determined by using single and two step fatigue loading test on four point rotating bending fatigue testing machine. Experimental data is used to determine the distinction between the initiation and propagation phase. Initiation phase is determined at different stress levels. The obtained results demonstrate the effect of stress level on initiation phase and propagation phase. (author)
International Nuclear Information System (INIS)
Taira, S.; Fujino, M.; Maruyama, S.
Temperature dependence of the rate of fatigue crack propagation in steels was examined, and compared with the temperature dependence of tensile ductility. Microcracks initiate and affect the propagation behavior of the main crack at elevated temperatures. Factors found to be elucidated include initiation rate of microcracks, reduction of ductility of the material in the vicinity of the main crack tip, and relaxation of concentrated strain by multi-cracks. It was found that during a strain controlled low cycle fatigue test at 1 cpm, the rate of crack propagation is largest at the blue-brittleness temperature range (200 to 300 0 C) in a low carbon steel. On the other hand, it is largest at above 700 0 C in austenite stainless steels. The temperature dependence of the rate of fatigue crack propagation is opposite to that of tensile ductility. Microcracks formed in the vicinity of the main crack tip were calculated, by considering the strain concentration and strain cycles imposed. Then, the local fracture strain was evaluated. Good correlation was found between the rate of crack propagation and the local fracture strain. (U.S.)
Near-threshold fatigue crack behaviour in EUROFER 97 at different temperatures
Aktaa, J.; Lerch, M.
2006-07-01
The fatigue crack behaviour in EUROFER 97 was investigated at room temperature (RT), 300, 500 and 550 °C for the assessment of cracks in first wall structures built from EUROFER 97 of future fusion reactors. For this purpose, fatigue crack growth tests were performed using CT specimens with two R-ratios, R = 0.1 and R = 0.5 ( R is the load ratio with R = Fmin/ Fmax where Fmin and Fmax are the minimum and maximum applied loads within a cycle, respectively). Hence, fatigue crack threshold, fatigue crack growth behaviour in the near-threshold range and their dependences on temperature and R-ratio were determined and described using an analytical formula. The fatigue crack threshold showed a monotonous dependence on temperature which is for R = 0.5 insignificantly small. The fatigue crack growth behaviour exhibited for R = 0.1 a non-monotonous dependence on temperature which is explained by the decrease of yield stress and the increase of creep damage with increasing temperature.
Near-threshold fatigue crack behaviour in EUROFER 97 at different temperatures
International Nuclear Information System (INIS)
Aktaa, J.; Lerch, M.
2006-01-01
The fatigue crack behaviour in EUROFER 97 was investigated at room temperature (RT), 300, 500 and 550 deg. C for the assessment of cracks in first wall structures built from EUROFER 97 of future fusion reactors. For this purpose, fatigue crack growth tests were performed using CT specimens with two R-ratios, R = 0.1 and R = 0.5 (R is the load ratio with R = F min /F max where F min and F max are the minimum and maximum applied loads within a cycle, respectively). Hence, fatigue crack threshold, fatigue crack growth behaviour in the near-threshold range and their dependences on temperature and R-ratio were determined and described using an analytical formula. The fatigue crack threshold showed a monotonous dependence on temperature which is for R = 0.5 insignificantly small. The fatigue crack growth behaviour exhibited for R = 0.1 a non-monotonous dependence on temperature which is explained by the decrease of yield stress and the increase of creep damage with increasing temperature
Stage I surface crack formation in thermal fatigue: A predictive multi-scale approach
International Nuclear Information System (INIS)
Osterstock, S.; Robertson, C.; Sauzay, M.; Aubin, V.; Degallaix, S.
2010-01-01
A multi-scale numerical model is developed, predicting the formation of stage I cracks, in thermal fatigue loading conditions. The proposed approach comprises 2 distinct calculation steps. Firstly, the number of cycles to micro-crack initiation is determined, in individual grains. The adopted initiation model depends on local stress-strain conditions, relative to sub-grain plasticity, grain orientation and grain deformation incompatibilities. Secondly, 2-4 grains long surface cracks (stage I) is predicted, by accounting for micro-crack coalescence, in 3 dimensions. The method described in this paper is applied to a 500 grains aggregate, loaded in representative thermal fatigue conditions. Preliminary results provide quantitative insight regarding position, density, spacing and orientations of stage I surface cracks and subsequent formation of crack networks. The proposed method is fully deterministic, provided all grain crystallographic orientations and micro-crack linking thresholds are specified. (authors)
Effect of tensile overloads on fatigue crack growth of high strength steel wires
International Nuclear Information System (INIS)
Haag, J.; Reguly, A.; Strohaecker, T.R.
2013-01-01
Highlights: • A proof load process may be an option to increase the fatigue life of flexible pipelines. • There is possibility to produce plastic deformation at crack tip of tensile armor wires. • Controlled overloads provide effective crack growth retardation. • Crack growth retardation is also evident at higher stress ratios. - Abstract: Fatigue of the tensile armor wires is the main failure mode of flexible risers. Techniques to increase the life of these components are required to improve the processes safety on oil exploration. This work evaluates the crack growth retardation of high strength steel wires used in flexible pipelines. Fracture toughness tests were performed to establish the level of stress intensity factor wherein the wires present significant plastic deformation at the crack tip. The effect of tensile overload on fatigue behavior was assessed by fatigue crack growth testing under constant ΔK control and different overload ratios with two different load ratios. The outcomes show that the application of controlled overloads provides crack retardation and increases the fatigue life of the wires more than 31%. This behavior is also evident at stress ratio of 0.5, in spite of the crack closure effect being minimized by increasing the applied mean stress
Seo, Sukho; Choi, Gyudong; Eom, Tae Jhoun; Lee, Bokwon; Lee, Soo Yeol
2017-07-01
The eddy current responses of Electrical Discharge Machining (EDM) notches and fatigue cracks are directly compared to verify the reliability of eddy current inspection. The fatigue crack growth tests using a constant load range control mode were conducted to obtain a variety of edge crack sizes, ranging from 0.9 to 6.6 mm for Al alloy and from 0.1 to 3 mm for Ti alloy. EDM notch specimens of Al and Ti alloys were accordingly prepared in lengths similar to that of the fatigued specimen. The crack length was determined by optical microscope and scanning electron microscope. The eddy current responses between the EDM and fatigued specimens with varying notch/crack length were examined using probe sensors at (100-500) kHz and (1-2) MHz for Al and Ti alloys, respectively. The results show a significant difference in the eddy current signal between the two specimens, based on the correlation between the eddy current response and notch/crack length. This suggests that eddy current inspection using the EDM reference specimen is inaccurate in determining the precise crack size, unless the eddy current response data base is obtained from a fatigue-cracked specimen.
International Nuclear Information System (INIS)
Fremy, F.
2012-01-01
This thesis deals with fatigue crack growth in non-proportional variable amplitude mixed mode I + II + III loading conditions and analyses the effects of internal stresses stemming from the confinement of the plastic zone in small scale yielding conditions. The tests showed that there are antagonistic long-distance and short-distance effects of the loading history on fatigue crack growth. The shape of loading path, and not only the maximum and minimum values in this path, is crucial and, by comparison, the effects of contact and friction are of lesser importance. Internal stresses play a major role on the fatigue crack growth rate and on the crack path. An approach was developed to analyze the elastic-plastic behavior of a representative section of the crack front using the FEA. A model reduction technic is used to extract the relevant information from the FE results. To do so, the velocity field is partitioned into mode I, II, III elastic and plastic components, each component being characterized by an intensity factor and a fixed spatial distribution. The calculations were used to select seven loading paths in I + II and I + II + III mixed mode conditions, which all have the same amplitudes for each mode, the same maximum, minimum and average values. These paths are supposed to be equivalent in the sense of common failure criteria, but differ significantly when the elastic-plastic behavior of the material is accounted for. The results of finite element simulations and of simulations using a simplified model proposed in this thesis are both in agreement with experimental results. The approach was also used to discuss the role of mode III loading steps. Since the material behavior is nonlinear, the nominal loading direction does not coincide with the plastic flow direction. Adding a mode III loading step in a mode I+II fatigue cycle, may, in some cases, significantly modify the behaviour of the crack (crack growth rate, crack path and plastic flow). (author)
A study on fatigue crack growth behavior subjected to a single tensile overload
International Nuclear Information System (INIS)
Lee, S.Y.; Liaw, P.K.; Choo, H.; Rogge, R.B.
2011-01-01
Neutron diffraction and electric potential experiments were carried out to investigate the growth behavior of a fatigue crack subjected to a single tensile overload. The specific objectives were to (i) probe the crack tip deformation and fracture behaviors under applied loads; (ii) examine the overload-induced transient crack growth micromechanism; (iii) validate the effective stress intensity factor range based on the crack closure approach as the fatigue crack tip driving force; and (iv) establish a quantitative relationship between the crack tip driving force and crack growth behavior. Immediately after a single tensile overload was introduced and then unloaded, the crack tip became blunt and enlarged compressive residual stresses in both magnitude and zone size were observed around the crack tip. The results show that the combined contributions of the overload-induced enlarged compressive residual stresses and crack tip blunting with secondary cracks are responsible for the observed changes in the crack opening load and the resultant post-overload transient crack growth behavior.
International Nuclear Information System (INIS)
Sarajaervi, U.; Cronvall, O.
2007-03-01
Fatigue is produced by cyclic application of stresses by mechanical or thermal loading. The metal subjected to fluctuating stress will fail at stresses much lower than those required to cause fracture in a single application of load. The key parameters are the range of stress variation and the number of its occurrences. Low-cycle fatigue, usually induced by mechanical and thermal loads, is distinguished from high-cycle fatigue, mainly associated with vibration or high number of small thermal fluctuations. Numerical models describing fatigue behaviour of austenitic stainless piping steels under cyclic loading and their applicability for modelling of low-cycle-fatigue are discussed in this report. In order to describe the cyclic behaviour of the material for analysis with finite element method (FEM) based analysis code ABAQUS, the test data, i.e. stress-strain curves, have to be processed. A code to process the data all through the test duration was developed within this study. A description of this code is given also in this report. Input data for ABAQUS was obtained to describe both kinematic and isotropic hardening properties. Further, by combining the result data for various strain amplitudes a mathematic expression was be created which allows defining a parameter surface for cyclic (i.e. isotropic) hardening. Input data for any strain amplitude within the range of minimum and maximum strain amplitudes of the test data can be assessed with the help of the developed 3D stress-strain surface presentation. The modelling of the fatigue induced initiation and growth of cracks was not considered in this study. On the other hand, a considerable part of the fatigue life of nuclear power plant (NPP) piping components is spent in the phase preceding the initiation and growth of cracks. (au)
Energy Technology Data Exchange (ETDEWEB)
Sarajaervi, U.; Cronvall, O. [VTT (Finland)
2007-03-15
Fatigue is produced by cyclic application of stresses by mechanical or thermal loading. The metal subjected to fluctuating stress will fail at stresses much lower than those required to cause fracture in a single application of load. The key parameters are the range of stress variation and the number of its occurrences. Low-cycle fatigue, usually induced by mechanical and thermal loads, is distinguished from high-cycle fatigue, mainly associated with vibration or high number of small thermal fluctuations. Numerical models describing fatigue behaviour of austenitic stainless piping steels under cyclic loading and their applicability for modelling of low-cycle-fatigue are discussed in this report. In order to describe the cyclic behaviour of the material for analysis with finite element method (FEM) based analysis code ABAQUS, the test data, i.e. stress-strain curves, have to be processed. A code to process the data all through the test duration was developed within this study. A description of this code is given also in this report. Input data for ABAQUS was obtained to describe both kinematic and isotropic hardening properties. Further, by combining the result data for various strain amplitudes a mathematic expression was be created which allows defining a parameter surface for cyclic (i.e. isotropic) hardening. Input data for any strain amplitude within the range of minimum and maximum strain amplitudes of the test data can be assessed with the help of the developed 3D stress-strain surface presentation. The modelling of the fatigue induced initiation and growth of cracks was not considered in this study. On the other hand, a considerable part of the fatigue life of nuclear power plant (NPP) piping components is spent in the phase preceding the initiation and growth of cracks. (au)
International Nuclear Information System (INIS)
James, L.A.
1985-08-01
Section XI of the ASME Boiler and Pressure Vessel Code provides rules for the analysis of structures for which cracks or crack-like flaws have been discovered during inservice inspection. The Code provides rules for the analysis of both surface flaws as well as flaws that are embedded within the wall of the pressure vessel. In the case of surface flaws, the Code provides fatigue crack growth rate relationships for typical nuclear pressure vessel steels (e.g., ASTM A508-2 and A533-B) cycled in water environments typical of those in light-water reactors (LWR). However, for the case of embedded cracks, the Code provides crack growth relationships based on results from specimens that were cycled in an elevated temperature air environment. Although these latter relationships are often referred to as applying to ''inert'' environments, the results of this paper will show that an elevated temperature air environment is anything but inert, and that use of such relationships can result in overly pessimistic estimates of fatigue-crack growth lifetimes of embedded cracks. The reason, of course, is that embedded cracks grow in an environment that is probably much closer to a vacuum than an air environment
Crack Growth Behaviour of P92 Steel Under Creep-fatigue Interaction Conditions
Directory of Open Access Journals (Sweden)
JING Hong-yang
2017-05-01
Full Text Available Creep-fatigue interaction tests of P92 steel at 630℃ under stress-controlled were carried out, and the crack propagation behaviour of P92 steel was studied. The fracture mechanism of crack growth under creep-fatigue interaction and the transition points in a-N curves were analyzed based on the fracture morphology. The results show that the fracture of P92 steel under creep-fatigue interaction is creep ductile fracture and the (Ctavg parameter is employed to demonstrate the crack growth behaviour; in addition, the fracture morphology shows that the crack growth for P92 steel under creep-fatigue interaction is mainly caused by the nucleation and growth of the creep voids and micro-cracks. Furthermore, the transition point of a-lg(Ni/Nf curve corresponds to the turning point of initial crack growth changed into steady crack growth while the transition point of (da/dN-N curve exhibits the turning point of steady creep crack growth changed into the accelerated crack growth.
A test procedure for determining the influence of stress ratio on fatigue crack growth
Fitzgerald, J. H.; Wei, R. P.
1974-01-01
A test procedure is outlined by which the rate of fatigue crack growth over a range of stress ratios and stress intensities can be determined expeditiously using a small number of specimens. This procedure was developed to avoid or circumvent the effects of load interactions on fatigue crack growth, and was used to develop data on a mill annealed Ti-6Al-4V alloy plate. Experimental data suggest that the rates of fatigue crack growth among the various stress ratios may be correlated in terms of an effective stress intensity range at given values of K max. This procedure is not to be used, however, for determining the corrosion fatigue crack growth characteristics of alloys when nonsteady-state effects are significant.
Formation of thermal fatigue cracks in periodic rapid quenching of metal
Energy Technology Data Exchange (ETDEWEB)
Ots, A. [Tallinn Technical University, Thermal Engineering Department, Tallinn (Estonia)
1998-12-31
Water lancing is an effective technique for cleaning boiler heating surfaces from ash deposits by burning low-grade fuels with complicated composition of mineral matter. In water cleaning cycles of boiler`s heat transfer surfaces due to rapid quenching destruction of corrosion protective oxide film and formation of thermal fatigue cracks on the outer surface of the tube`s metal occur. The criterion of the thermal fatigue cracks` formation and their growth intensity depend on the character of temperature field in the tube`s metal outer layer. The solution of non-stationary heat conductivity equation for metal rapid quenching conditions is given. The convective heat transfer coefficients from hot metal surface to water jet were established experimentally. Thermal fatigue crack growth intensity was investigated in real boilers` heat transfer surfaces` tubes as well as in laboratory conditions. The formula for predicting thermal fatigue cracks` depth depending on the number of cleaning cycles. (orig.) 5 refs.
Probabilistic aspects of fatigue crack propagation data for zirconium-2.5 % niobium
International Nuclear Information System (INIS)
Wilkins, B.J.S.; Reich, A.R.
1976-11-01
Fatigue crack propagation data for Zr-2.5 % Nb pressure tube material at 20 and 400 deg C are presented. The practical application of these data in terms of error analysis and extrapolation errors is discussed. (author)
Formation of thermal fatigue cracks in periodic rapid quenching of metal
Energy Technology Data Exchange (ETDEWEB)
Ots, A [Tallinn Technical University, Thermal Engineering Department, Tallinn (Estonia)
1999-12-31
Water lancing is an effective technique for cleaning boiler heating surfaces from ash deposits by burning low-grade fuels with complicated composition of mineral matter. In water cleaning cycles of boiler`s heat transfer surfaces due to rapid quenching destruction of corrosion protective oxide film and formation of thermal fatigue cracks on the outer surface of the tube`s metal occur. The criterion of the thermal fatigue cracks` formation and their growth intensity depend on the character of temperature field in the tube`s metal outer layer. The solution of non-stationary heat conductivity equation for metal rapid quenching conditions is given. The convective heat transfer coefficients from hot metal surface to water jet were established experimentally. Thermal fatigue crack growth intensity was investigated in real boilers` heat transfer surfaces` tubes as well as in laboratory conditions. The formula for predicting thermal fatigue cracks` depth depending on the number of cleaning cycles. (orig.) 5 refs.
Fracture resistance and fatigue crack growth characteristics of two Al-Cu-Mg-Zr alloys
Sarkar, Bhaskar; Lisagor, W. B.
1992-01-01
The dependence of strength, fracture resistance, and fatigue crack growth rate on the aging conditions of two alloy compositions based on Al-3.7Cu-1.85Mg-0.2Mn is investigated. Mechanical properties were evaluated in two heat treatment conditions and in two orientations (longitudinal and transverse). Compact tension specimens were used to determine fatigue crack growth characteristics and fracture resistance. The aging response was monitored on coupons using hardness measurements determined with a standard Rockwell hardness tester. Fracture resistance is found to increase with increasing yield strength during artificial aging of age-hardenable 2124-Zr alloys processed by powder metallurgy techniques. Fatigue crack growth rate increases with increasing strength. It is argued that these changes are related to deformation modes of the alloys; a homogeneous deformation mode tends to increase fracture resistance and to decrease the resistance to the fatigue crack propagation rate.
Combined simulation of fatigue crack nucleation and propagation based on a damage indicator
Directory of Open Access Journals (Sweden)
M. Springer
2016-10-01
Full Text Available Fatigue considerations often distinguish between fatigue crack nucleation and fatigue crack propagation. The current work presents a modeling approach utilizing one Fatigue Damage Indicator to treat both in a unified way. The approach is implemented within the framework of the Finite Element Method. Multiaxial critical plane models with an extended damage accumulation are employed as Fatigue Indicators. Locations of fatigue crack emergence are predicted by these indicators and material degradation is utilized to model local material failure. The cyclic loading is continued on the now degraded structure and the next location prone to material failure is identified and degradation modeled. This way, fatigue crack propagation is represented by an evolving spatial zone of material failure. This propagating damage zone leads to a changing structural response of the pristine structure. By recourse to the Fatigue Damage Indicator a correlation between the number of applied load cycles and the changing structural behavior is established. Finally, the proposed approach is exemplified by cyclic bending experiments in the Low Cycle Fatigue regime
Fatigue Crack Behavior of Stainless Steel 304 by the Addition of Carbon Nanotubes
Directory of Open Access Journals (Sweden)
Rizwanulhaque Syed
2014-01-01
Full Text Available Fatigue is the main source of almost half of whole mechanical failures. This research investigated the effect on cyclic fatigue behavior of stainless steel 304 (SS304 when including carbon nanotubes (CNTs at the crack tip. The cyclic fatigue tests were conducted on compact tension (CT specimens to establish the relationship between crack growth and the number of cycles (a-N. It is found that the incorporation of a small amount of CNTs increased the fatigue life of the SS304/metal. Micrographs showed that the enhancement in fatigue life is caused by CNTs dense arrangement around the crack tip, entangled with each other, and finer grain size. Smooth bonding at the interface of the CNTs and SS304 grains is also observed.
Application of a Cycle Jump Technique for Acceleration of Fatigue Crack Growth Simulation
DEFF Research Database (Denmark)
Moslemian, Ramin; Berggreen, Christian; Karlsson, A.M.
2010-01-01
A method for accelerated simulation of fatigue crack growth in a bimaterial interface is proposed. To simulate fatigue crack growth in a bimaterial interface a routine is developed in the commercial finite element code ANSYS and a method to accelerate the simulation is implemented. The proposed m...... of the simulation show that with fair accuracy, using the cycle jump method, more than 70% reduction in computation time can be achieved....
G-control fatigue testing for cyclic crack propagation in composite structures
DEFF Research Database (Denmark)
Manca, Marcello; Berggreen, Christian; Carlsson, Leif A.
2015-01-01
This paper presents a computer controlled testing methodology called “The G-control Method” which allows cyclic crack growth testing using real-time control of the cyclic energy release rate. The advantages of using this approach are described and compared with traditional fatigue testing methods...... that the G-control method allows fatigue testing at a constant range of energy release rates leading to a constant crack propagation rate....
Fatigue crack propagation in UFG Ti grade 4 processed by severe plastic deformation
Czech Academy of Sciences Publication Activity Database
Fintová, Stanislava; Arzaghi, M.; Kuběna, Ivo; Kunz, Ludvík; Sarrazin-Baudoux, C.
2017-01-01
Roč. 98, MAY (2017), s. 187-194 ISSN 0142-1123 R&D Projects: GA MŠk(CZ) LQ1601; GA MŠk LM2015069 Institutional support: RVO:68081723 Keywords : Titanium * Fatigue * Crack growth * Crack closure * Equal channel angular processing Subject RIV: JL - Materials Fatigue, Friction Mechanics OBOR OECD: Audio engineering, reliability analysis Impact factor: 2.899, year: 2016 http://www.sciencedirect.com/science/article/pii/S014211231730035X
A Comparison of Fatigue Crack Growth in Human Enamel and Hydroxyapatite
Bajaj, Devendra; Nazari, Ahmad; Eidelman, Naomi; Arola, Dwayne
2008-01-01
Cracks and craze lines are often observed in the enamel of human teeth, but they rarely cause tooth fracture. The present study evaluates fatigue crack growth in human enamel, and compares that to the fatigue response of sintered hydroxyapatite (HAp) with similar crystallinity, chemistry and density. Miniature inset compact tension (CT) specimens were prepared that embodied a small piece of enamel (N=8) or HAp (N=6). The specimens were subjected to mode I cyclic loads and the steady state cra...
Creep and creep fatigue crack behavior of 1Cr- and 9Cr-steels
International Nuclear Information System (INIS)
Maile, K.; Klenk, A.; Schellenberg, G.; Granacher, J.; Tramer, M.
2000-01-01
A large database for creep crack initiation and propagation under constant load conditions is available on conventional power plant steels of types 1%Cr and 12%Cr. Modern plants are often used in the medium and peak load regime, thus the dominant loading situation in high temperature components is creep fatigue. For life assessment data about crack initiation and growth under creep fatigue loading are required. These characteristics can not be substituted by pure fatigue or creep crack data. Therefore, a comprehensive test programme was started to investigate the creep fatigue crack behaviour of a 1%CrMoNiV turbine rotor steel (30CrMoNiV 4 11) at 550 C and a new 9%CrMoVNb pipe steel (type P 9 1) at 600 C. DENT-specimen with 15 and 60 mm thickness as well as side grooved CT-specimen with 25 and 50 mm thickness have been tested to determine possible influences of geometry and thus to check the transferability of the data to components. The creep fatigue crack growth results of tests with dwell times between t H = 0,32h and 10 h lie in the scatterbands given by creep crack growth results. Nevertheless a higher crack growth rate under creep fatigue conditions can be stated. An increase in crack growth rate due to creep fatigue is clearly visible. Loading situations with frequencies higher than 1.10 -4 Hz should be not assessed with pure creep crack results or sufficient safety margins have to be applied. (orig.)
International Nuclear Information System (INIS)
Tao, Junhui; Hu, Shubing; Ji, Longbo
2016-01-01
In this paper, we describe experiments on welded joints of Ti-6Al-4V alloy specimens exhibiting fatigue characteristics in the base metal (BM), hot affected zone (HAZ) and fuse zone (FZ). The effect of micromorphology on crack propagation at the tip of the fatigue crack in joints formed by electron beam welding was investigated using an optical microscope, transmission electron microscope and other methodologies. The results demonstrated that the fatigue crack originated in and propagated along α/β boundaries in the BM. In the HAZ, the fatigue crack occurred at the boundary between martensite laths, and propagated through most irregular-equiaxed α phases and a few martensite laths. In the FZ, the fatigue crack originated at the boundaries between the fine crushing phases among martensite laths, and propagated along a majority of α/β boundaries and several narrow martensite laths. The electron beam welded joint of Ti-6Al-4V alloy showed instances of zigzag fatigue cracks that increased in degree from lowest in the HAZ, moderate in the FZ to greatest in the BM. Conversely, fatigue crack growth rate (FCGR) was greatest in the HAZ, less in the FZ and slowest in the BM. - Highlights: •Ti-6Al-4V welded joint exhibits different fatigue characteristics. •The fatigue crack propagates along α/β boundaries in the BM. •The fatigue crack propagates through α phases and martensite laths in the HAZ. •The fatigue crack propagates along α/β boundaries and martensite laths in the FZ. •Fatigue crack growth rate is fastest in the HAZ, less in the FZ, slowest in the BM.
Fatigue crack behavior on a Cu-Zn-Al SMA
Directory of Open Access Journals (Sweden)
V. Di Cocco
2014-10-01
Optical Microscope (LOM observations. Furthermore a fatigue crack propagation and fracture surface scanning electron microscope (SEM observations have been performed in order to evaluate the crack path and the main crack micromechanisms.
Cyclic deformation and fatigue data for Ti–6Al–4V ELI under variable amplitude loading
Directory of Open Access Journals (Sweden)
Patricio E. Carrion
2017-08-01
Full Text Available This article presents the strain-based experimental data for Ti–6Al–4V ELI under non-constant amplitude cyclic loading. Uniaxial strain-controlled fatigue experiments were conducted under three different loading conditions, including two-level block loading (i.e. high-low and low-high, periodic overload, and variable amplitude loading. Tests were performed under fully-reversed, and mean strain/stress conditions. For each test conducted, two sets of data were collected; the cyclic stress–strain response (i.e. hysteresis loops in log10 increments, and the peak and valley values of stress and strain for each cycle. Residual fatigue lives are reported for tests with two-level block loading, while for periodic overload and variable amplitude experiments, fatigue lives are reported in terms of number of blocks to failure.
Ford, Audrey C; Gramling, Hannah; Li, Samuel C; Sov, Jessica V; Srinivasan, Amrita; Pruitt, Lisa A
2018-03-01
Polycarbonate polyurethane has cartilage-like, hygroscopic, and elastomeric properties that make it an attractive material for orthopedic joint replacement application. However, little data exists on the cyclic loading and fracture behavior of polycarbonate polyurethane. This study investigates the mechanisms of fatigue crack growth in polycarbonate polyurethane with respect to time dependent effects and conditioning. We studied two commercially available polycarbonate polyurethanes, Bionate® 75D and 80A. Tension testing was performed on specimens at variable time points after being removed from hydration and variable strain rates. Fatigue crack propagation characterized three aspects of loading. Study 1 investigated the impact of continuous loading (24h/day) versus intermittent loading (8-10h/day) allowing for relaxation overnight. Study 2 evaluated the effect of frequency and study 3 examined the impact of hydration on the fatigue crack propagation in polycarbonate polyurethane. Samples loaded intermittently failed instantaneously and prematurely upon reloading while samples loaded continuously sustained longer stable cracks. Crack growth for samples tested at 2 and 5Hz was largely planar with little crack deflection. However, samples tested at 10Hz showed high degrees of crack tip deflection and multiple crack fronts. Crack growth in hydrated samples proceeded with much greater ductile crack mouth opening displacement than dry samples. An understanding of the failure mechanisms of this polymer is important to assess the long-term structural integrity of this material for use in load-bearing orthopedic implant applications. Copyright © 2018 Elsevier Ltd. All rights reserved.
The frequency effect on the fatigue crack growth rate of 304 stainless steel
International Nuclear Information System (INIS)
Shih, Y.-S.; Chen, J.-J.
1999-01-01
Under cyclic loading condition, the fatigue crack growth (FCG) rate governed by stress intensity factor and stress ratio is well known; Walker's equation, Forman's equation and Elber's equation are typical formulae to describe the fatigue crack growth rate. However, the loading frequency effect on the fatigue crack growth rate has yet to be explored. Recently, studies have focused on the loading frequency effect on some visco-elastic materials, and have provided a clearer understanding of the frequency effect on the fatigue crack growth rate. In a physical sense, knowledge about the loading frequency effect on the fatigue crack growth rate for 304 stainless steel is still lacking. James conducted a lot of experiments, and through data analysis, he concluded an evaluation equation which is based upon the experimental illustration. In this study, the physical properties of the material are used to illustrate the modification of fatigue crack growth rate, and a new formula which is based upon the modified Forman's equation, is provided. (orig.)
Resolved shear stress intensity coefficient and fatigue crack growth in large crystals
Chen, QI; Liu, Hao-Wen
1988-01-01
Fatigue crack growth in large grain Al alloy was studied. Fatigue crack growth is caused primarily by shear decohesion due to dislocation motion in the crack tip region. The crack paths in the large crystals are very irregular and zigzag. The crack planes are often inclined to the loading axis both in the inplane direction and the thickness direction. The stress intensity factors of such inclined cracks are approximated from the two dimensional finite element calculations. The plastic deformation in a large crystal is highly anisotropic, and dislocation motion in such crystals are driven by the resolved shear stress. The resolved shear stress intensity coefficient in a crack solid, RSSIC, is defined, and the coefficients for the slip systems at a crack tip are evaluated from the calculated stress intensity factors. The orientations of the crack planes are closely related to the slip planes with the high RSSIC values. If a single slip system has a much higher RSSIC than all the others, the crack will follow the slip plane, and the slip plane becomes the crack plane. If two or more slip systems have a high RSSIC, the crack plane is the result of the decohesion processes on these active slip planes.
Fatigue crack growth and life prediction under mixed-mode loading
Sajith, S.; Murthy, K. S. R. K.; Robi, P. S.
2018-04-01
Fatigue crack growth life as a function of crack length is essential for the prevention of catastrophic failures from damage tolerance perspective. In damage tolerance design approach, principles of fracture mechanics are usually applied to predict the fatigue life of structural components. Numerical prediction of crack growth versus number of cycles is essential in damage tolerance design. For cracks under mixed mode I/II loading, modified Paris law (d/a d N =C (ΔKe q ) m ) along with different equivalent stress intensity factor (ΔKeq) model is used for fatigue crack growth rate prediction. There are a large number of ΔKeq models available for the mixed mode I/II loading, the selection of proper ΔKeq model has significant impact on fatigue life prediction. In the present investigation, the performance of ΔKeq models in fatigue life prediction is compared with respect to the experimental findings as there are no guidelines/suggestions available on the selection of these models for accurate and/or conservative predictions of fatigue life. Within the limitations of availability of experimental data and currently available numerical simulation techniques, the results of present study attempt to outline models that would provide accurate and conservative life predictions. Such a study aid the numerical analysts or engineers in the proper selection of the model for numerical simulation of the fatigue life. Moreover, the present investigation also suggests a procedure to enhance the accuracy of life prediction using Paris law.
The influence of loading frequency on near-threshold fatigue crack growth
International Nuclear Information System (INIS)
Ogawa, Takeshi; Tokaji, Keiro; Ochi, Satoshi
1986-01-01
Fatigue crack growth and crack closure in the near-threshold region were investigated under different loading frequencies for three types of steel. The results show that the loading frequency influences the near-threshold characteristics in fatigue crack growth, through the different contributions of the fretting oxide induced crack closure. This behaviour is attributed to condensation of moisture between crack faces, which is influenced by the loading frequency. The formation of the fretting oxide debris promoted by the condensation of moisture becomes marked at a higher frequency. However, it is an unstable and complicating phenomenon, since the condensation is also influenced by relative humidity, test temperature and sheet thickness. Therefore, it is concluded that non-oxide controlled crack growth characteristics should be used for the life prediction of structures. (author)
Effect of temperature upon the fatigue-crack propagation behavior of Hastelloy X-280
International Nuclear Information System (INIS)
James, L.A.
1976-05-01
The techniques of linear-elastic fracture mechanics were employed to characterize the effect of temperature upon the fatigue-crack propagation behavior of Hastelloy X-280 in an air environment. Also included in this study are survey tests to determine the effects of thermal aging and stress ratio upon crack growth behavior in this alloy
Modelling of fatigue crack propagation assisted by gaseous hydrogen in metallic materials
International Nuclear Information System (INIS)
Moriconi, C.
2012-01-01
Experimental studies in a hydrogenous environment indicate that hydrogen created by surface reactions, then drained into the plastic zone, leads to a modification of deformation and damage mechanisms at the fatigue crack tip in metals, resulting in a significant decrease of crack propagation resistance. This study aims at building a model of these complex phenomena in the framework of damage mechanics, and to confront it with the results of fatigue crack propagation tests in high pressure hydrogen on a 15-5PH martensitic stainless steel. To do so, a cohesive zone model was implemented in the finite element code ABAQUS. A specific traction-separation law was developed, which is suitable for cyclic loadings, and whose parameters depend on local hydrogen concentration. Furthermore, hydrogen diffusion in the bulk material takes into account the influence of hydrostatic stress and trapping. The mechanical behaviour of the bulk material is elastic-plastic. It is shown that the model can qualitatively predict crack propagation in hydrogen under monotonous loadings; then, the model with the developed traction-separation law is tested under fatigue loading. In particular, the simulated crack propagation curves without hydrogen are compared to the experimental crack propagation curves for the 15-5PH steel in air. Finally, simulated fatigue crack propagation rates in hydrogen are compared to experimental measurements. The model's ability to assess the respective contributions of the different damage mechanisms (HELP, HEDE) in the degradation of the crack resistance of the 15-5PH steel is discussed. (author)
An investigation into the change of shape of fatigue cracks initiated at surface flaws
International Nuclear Information System (INIS)
Portch, D.J.
1979-09-01
Surface fatigue cracks found in plant can often be closely approximated in shape by a semi-ellipse. The stress intensity factor range at the deepest part of the surface crack is dependent upon a number of variables, including the crack aspect ratio. In fatigue life analysis, the aspect ratio of a propagating crack is frequently assumed to remain constant, possibly due to the complexity of estimating aspect ratio change on the basis of linear elastic fracture mechanics. This report describes the results of an experimental programme to examine the change of shape of fatigue cracks subjected to uniaxial tensile or bending stresses. The data obtained has been used to modify equations proposed by the author in a previous report to predict the change of aspect ratio of a crack propagating from a known defect. These modified equations, although not including terms to account for the effects of varying mean stress levels or material properties, generally give a good agreement with published experimental results. Crack propagation rate data obtained from the tensile fatigue tests has been used to estimate crack tip stress intensity factors. These are compared with values calculated from published solutions using both the constant geometry assumption and also the shape change equations proposed in this report. Use of these equations gives improved agreement with experiment in most cases. (author)
International Nuclear Information System (INIS)
Suzuki, Takafumi; Kasahara, Naoto
2012-01-01
In recent years, reports have increased about failure cases caused by high cycle thermal fatigue both at light water reactors and fast breeder reactors. One of the reasons of the cases is a turbulent mixing at a Tee-junction, where hot and cold temperature fluids are mixed, in a coolant system. In order to prevent thermal fatigue failures at Tee-junctions. The Japan Society of Mechanical Engineers published the guideline which is an evaluation method of high cycle thermal fatigue damage at nuclear pipes. In order to justify safety margin and make the procedure of the guideline concise, this paper proposes a new evaluation method of thermal fatigue damage with use of the 'equivalent stress amplitude.' Because this new method makes procedure of evaluation clear and concise, it will contribute to improving the guideline for thermal fatigue evaluation. (author)
Study of cyclic strain localization and fatigue crack initiation using FIB technique
Czech Academy of Sciences Publication Activity Database
Man, Jiří; Vystavěl, T.; Weidner, A.; Kuběna, Ivo; Petrenec, Martin; Kruml, Tomáš; Polák, Jaroslav
2012-01-01
Roč. 39, JUN (2012), s. 44-53 ISSN 0142-1123 R&D Projects: GA ČR GAP108/10/2371 Institutional research plan: CEZ:AV0Z20410507 Keywords : fatigue crack initiation * persistent slip band * focused ion beam (FIB) Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.976, year: 2012
Directory of Open Access Journals (Sweden)
G. Lesiuk
2015-10-01
Full Text Available The goal of the authors’ investigations was determination of the fatigue crack growth in fragments of steel structures (of the puddled steel and its cyclic behavior. Tested steel elements coming from the turn of the 19th and 20th were gained from still operating ancient steel construction (a main hall of Railway Station, bridges etc.. This work is a part of investigations devoted to the phenomenon of microstructural degradation and its potential influence on their strength properties. The analysis of the obtained results indicated that those long operating steels subject to microstructure degradation processes consisting mainly in precipitation of carbides and nitrides inside ferrite grains, precipitation of carbides at ferrite grain boundaries and degeneration of pearlite areas [1, 2]. It is worth noticing that resistance of the puddled steel to fatigue crack propagation in the normalized state was higher. The authors proposed the new kinetic equation of fatigue crack growth rate in such a steel. Thus the relationship between the kinetics of degradation processes and the fatigue crack growth rate also have been shown. It is also confirmed by the materials research of the viaduct from 1885, which has not shown any significant changes in microstructure. The non-classical kinetic fatigue fracture diagrams (KFFD based on deformation ( or energy (W approach was also considered. In conjunction with the results of low- and high-cycle fatigue and gradual loss of ductility as a consequence (due to the microstructural degradation processes - it seems to be a promising construction of the new kinetics fatigue fracture diagrams with the energy approach.
A Fatigue Crack Size Evaluation Method Based on Lamb Wave Simulation and Limited Experimental Data
Directory of Open Access Journals (Sweden)
Jingjing He
2017-09-01
Full Text Available This paper presents a systematic and general method for Lamb wave-based crack size quantification using finite element simulations and Bayesian updating. The method consists of construction of a baseline quantification model using finite element simulation data and Bayesian updating with limited Lamb wave data from target structure. The baseline model correlates two proposed damage sensitive features, namely the normalized amplitude and phase change, with the crack length through a response surface model. The two damage sensitive features are extracted from the first received S0 mode wave package. The model parameters of the baseline model are estimated using finite element simulation data. To account for uncertainties from numerical modeling, geometry, material and manufacturing between the baseline model and the target model, Bayesian method is employed to update the baseline model with a few measurements acquired from the actual target structure. A rigorous validation is made using in-situ fatigue testing and Lamb wave data from coupon specimens and realistic lap-joint components. The effectiveness and accuracy of the proposed method is demonstrated under different loading and damage conditions.
Initiation and propagation of fatigue cracks in cast IN713LC superalloy
Czech Academy of Sciences Publication Activity Database
Kunz, Ludvík; Lukáš, Petr; Konečná, R.
2010-01-01
Roč. 77, č. 11 (2010), s. 2008-2015 ISSN 0013-7944 R&D Projects: GA MPO FT-TA4/023; GA AV ČR 1QS200410502 Institutional research plan: CEZ:AV0Z20410507 Keywords : IN 713LC * high temperature fatigue * crystallographic fatigue crack initiation * mean stress effect Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.571, year: 2010
Fatigue crack growth in mode II of adhesively joined composites
DEFF Research Database (Denmark)
Biel, Anders; Toftegaard, Helmuth Langmaack
2017-01-01
, experiments are performed to derive material data for a crack propagation in shear i.e. in mode II. The shear loading of the crack is achieved by use of double cantilever beam specimens loaded with uneven bending moments. The experiments are performed under a constant cyclic displacement. An initial mode I...... loading is used to make the crack start in the adhesive. The crack length is measured using a load synchronized camera. Due to the shear loading the crack deviates from the adhesive layer into the laminate. A stable crack propagation is detected in the laminate. No influence have been detected due...... to an increasing crack length. It is also observed that the crack is trapped in the laminate; if the loading is changed to mode I the crack continues to propagate in the laminate....
International Nuclear Information System (INIS)
Wooldridge, A.B.
1980-01-01
The influence of compressive stress on the reflection and transmission of ultrasound has been investigated for fatigue cracks. An examination has been made of the shear wave corner echoes from surface breaking fatigue cracks which were grown at constant stress intensity factor to control the roughness of the faces. In this way a correlation has been established between the roughness of the surfaces and the ultrasonic response at both zero load and under stress. The effect of liquids in the cracks has also been studied and the results compared with theoretical predictions for a thin sided parallel gap. (author)
Probabilistic Modeling of the Fatigue Crack Growth Rate for Ni-base Alloy X-750
International Nuclear Information System (INIS)
Yoon, Jae Young; Nam, Hyo On; Hwang, Il Soon; Tae Hyun Lee
2012-01-01
The Bayesian inference was employed to reduce the uncertainties contained in EAC modeling parameters that have been established from experiments with Alloy X-750. Corrosion fatigue crack growth rate model(FCGR) was developed by fitting into Paris' Law of measured data from the several fatigue tests conducted either in constant load or constant ΔK mode. From fitting the data to Paris' Law, the parameters C and m of Paris' Law model were assumed to obey the Gaussian distribution. These parameters characterizing the corrosion fatigue crack growth behavior of X-750 were updated to reduce the uncertainty in the model by using the Bayesian inference method. (author)
International Nuclear Information System (INIS)
Nogami, Shuhei; Sato, Yuki; Hasegawa, Akira
2010-01-01
Crack growth behavior under low cycle fatigue in reduced activation ferritic/martensitic steel, F82H IEA-heat (Fe-8Cr-2W-0.2V-0.02Ta), was investigated to improve the fatigue life assessment method of fusion reactor structural material. Low cycle fatigue test was carried out at room temperature in air at a total strain range of 0.4-1.5% using an hourglass-type miniature fatigue specimen. The relationship between the surface crack length and life fraction was described using one equation independent of the total strain range. Therefore, the fatigue life and residual life could be estimated using the surface crack length. Moreover, the microcrack initiation life could be estimated using the total strain range if there was a one-to-one correspondence between the total strain range and number of cycles to failure. The crack growth rate could be estimated using the total strain range and surface crack length by introducing the concept of the normalized crack growth rate. (author)
Restraint of fatigue crack growth by wedge effects of fine particles
Takahashi, I; Kotani, N
2000-01-01
Presents some experimental results which demonstrate restraint of fatigue crack growth in an Al-Mg alloy by wedge effects of fine particles. Fatigue test specimens were machined from a JIS A5083P-O Al-Mg alloy plate of 5 mm thickness and an EDM starter notch was introduced to each specimen. Three kinds of fine particles were prepared as the materials to be wedged into the fatigue cracks, i.e. magnetic particles and two kinds of alumina particles having different mean particle sizes of 47.3 mu m and 15.2 mu m. Particles of each kind were suspended in an oil to form a paste, which was applied on the specimen surface covering the notch zone prior to the fatigue tests. In order to make some fracture mechanics approaches, in situ observations of fatigue cracks were performed for the two cases using a CCD microscope, with a magnification of *1000. The crack length and the crack opening displacement (COD) at the notch root, delta , were measured. The crack retardation effect continues almost through the entire lifet...
OBSERVATION OF FATIGUE CRACK PATHS IN NODULAR CAST IRON AND ADI MICROSTRUCTURES
Directory of Open Access Journals (Sweden)
Lukáš Bubenko
2009-07-01
Full Text Available When speaking about quality of construction materials, fatigue crack propagation resistance is one of the most important considered properties. That is essentially influenced by character of matrix. Here presented contribution deals with the fatigue crack propagation mode through the matrix of as-cast nodular cast iron (NCI and austempered ductile iron (ADI, whereas influence of microstructure has been considered and discussed. Experimental materials used in presented contribution were pearlitc-ferritic NCI and heat treated ADI 800. Pearlitic-ferritic NCI was used as the base for ADI production. Experiments were performed on mini round compact tension (RCT specimens using an Amsler vibrophore. Fatigue crack paths in both materials were investigated and compared. Light microscopy was used to analyze the microstructure, crack initiation and propagation within broken specimens. In both tested materials fatigue cracks always initiated at graphite-matrix interface, while graphite nodules remained generally unbroken, eventually only surface of nodules was damaged. Though, comparing two materials with different microstructures, the diversity of fatigue crack propagation modes at high deltaK and low deltaK was observed.
Huang, Peiyan; Liu, Guangwan; Guo, Xinyan; Huang, Man
2008-11-01
The experimental research on fatigue crack propagation rate of reinforced concrete (RC) beams strengthened with carbon fiber laminate (CFL) is carried out by MTS system in this paper. The experimental results show that, the main crack propagation on strengthened beam can be summarized into three phases: 1) fast propagation phase; 2) steady propagation and rest phase; 3) unsteady propagation phase. The phase 2-i.e. steady propagation and rest stage makes up about 95% of fatigue life of the strengthened beam. The propagation rate of the main crack, da/dN, in phase 2 can be described by Paris formula, and the constant C and m can be confirmed by the fatigue crack propagation experiments of the RC beams strengthened with CFL under three-point bending loads.
Degenerated graphite nodules influence on fatigue crack paths in a ferritic ductile cast iron
Directory of Open Access Journals (Sweden)
Francesco Iacoviello
2015-10-01
Full Text Available ferritic to a completely pearlitic matrix, and they are widely used for many applications (e.g. wheels, gears, crankshafts in cars, exhaust manifolds, valves, flywheels, boxes bearings, hubs, shafts, valves, flanges, pipelines .... Considering the graphite elements, their morphology can be considered as degenerated when its nodularity is too low and this can be due to different causes (e.g., a partially failed nodularization process or a wrong inoculant. In this work, a ferritic DCI with degenerated nodules was obtained by means of an annealing treatment and the fatigue crack propagation resistance was investigated by means of fatigue crack propagation tests performed according to ASTM E647, focusing on the influence of degenerated graphite nodules on the fatigue crack paths. This analysis was performed both analysing the crack path profile by means of a scanning electron microscope (SEM and by means of a SEM fracture surfaces analysis
Evaluation of creep-fatigue crack growth for large-scale FBR reactor vessel and NDE assessment
Energy Technology Data Exchange (ETDEWEB)
Joo, Young Sang; Kim, Jong Bum; Kim, Seok Hun; Yoo, Bong
2001-03-01
Creep fatigue crack growth contributes to the failure of FRB reactor vessels in high temperature condition. In the design stage of reactor vessel, crack growth evaluation is very important to ensure the structural safety and setup the in-service inspection strategy. In this study, creep-fatigue crack growth evaluation has been performed for the semi-elliptical surface cracks subjected to thermal loading. The thermal stress analysis of a large-scale FBR reactor vessel has been carried out for the load conditions. The distributions of axial, radial, hoop, and Von Mises stresses were obtained for the loading conditions. At the maximum point of the axial and hoop stress, the longitudinal and circumferential surface cracks (i.e. PTS crack, NDE short crack and shallow long crack) were postulated. Using the maximum and minimum values of stresses, the creep-fatigue crack growth of the proposed cracks was simulated. The crack growth rate of circumferential cracks becomes greater than that of longitudinal cracks. The total crack growth of the largest PTS crack is very small after 427 cycles. The structural integrity of a large-scale reactor can be maintained for the plant life. The crack depth growth of the shallow long crack is faster than that of the NDE short crack. In the ISI of the large-scale FBR reactor vessel, the ultrasonic inspection is beneficial to detect the shallow circumferential cracks.
International Nuclear Information System (INIS)
Lee, Sang Kee; Nam, Ki Woo; Kang, Chang Yong; Do, Jae Yoon
2000-01-01
On this study, the fatigue crack propagation of super duplex stainless steel is investigated in conditions of various volume fraction of austenite phase by changing heat treatment temperature. And we analysed acoustic emission signals during the fatigue test by time-frequency analysis methods. As the temperature of heat treatment increased, volume fraction of austenite decreased and coarse grain was obtained. The specimen heat treated at 1200 deg. C had longer fatigue life and slower rate of crack growth. As a result of time-frequency analyze of acoustic emission signals during fatigue test, main frequency was 200∼300 kHz having no correlation with heat treatment and crack length, and 500 kHz was obtained by dimple and separate of inclusion
Improvement of elastic-plastic fatigue crack growth evaluation method. 2. Crack opening behavior
Energy Technology Data Exchange (ETDEWEB)
Takahashi, Yukio [Central Research Inst. of Electric Power Industry, Tokyo (Japan)
2001-05-01
Evaluation of crack growth behavior under cyclic loading is often required in the structural integrity assessment of cracked components. Closing and re-opening of the crack give large influence on crack growth rate through the change of fracture mechanics parameters. Based on the finite element analysis for a center-cracked plate, dependency of crack opening ratio on applied stress range and mean stress was examined. Simple formulae for representing the results were derived for plane stress and plane strain conditions. (author)
Smart Patches for Monitoring Fatigue Crack Growth in Aircraft Structures
National Research Council Canada - National Science Library
Ihn, Jeong-Beom
2001-01-01
A built-in cost-effective diagnostic system for monitoring crack growth in aircraft structures was developed, particularly for riveted fuselage joints and cracked aircraft parts with composite bonded patches...
Separating the Influence of Environment from Stress Relaxation Effects on Dwell Fatigue Crack Growth
Telesman, Jack; Gabb, Tim; Ghosn, Louis J.
2016-01-01
Seven different microstructural variations of LSHR were produced by controlling the cooling rate and the subsequent aging and thermal exposure heat treatments. Through cyclic fatigue crack growth testing performed both in air and vacuum, it was established that four out of the seven LSHR heat treatments evaluated, possessed similar intrinsic environmental resistance to cyclic crack growth. For these four heat treatments, it was further shown that the large differences in dwell crack growth behavior which still persisted, were related to their measured stress relaxation behavior. The apparent differences in their dwell crack growth resistance were attributed to the inability of the standard linear elastic fracture mechanics (LEFM) stress intensity parameter to account for visco-plastic behavior. Crack tip stress relaxation controls the magnitude of the remaining local tensile stresses which are directly related to the measured dwell crack growth rates. It was hypothesized that the environmentally weakened grain boundary crack tip regions fail during the dwells when their strength is exceeded by the remaining local crack tip tensile stresses. It was shown that the classical creep crack growth mechanisms such as grain boundary sliding did not contribute to crack growth, but the local visco-plastic behavior still plays a very significant role by determining the crack tip tensile stress field which controls the dwell crack growth behavior. To account for the influence of the visco-plastic behavior on the crack tip stress field, an empirical modification to the LEFM stress intensity parameter, Kmax, was developed by incorporating into the formulation the remaining stress level concept as measured by simple stress relaxation tests. The newly proposed parameter, Ksrf, did an excellent job in correlating the dwell crack growth rates for the four heat treatments which were shown to have similar intrinsic environmental cyclic fatigue crack growth resistance.
Modeling time-dependent corrosion fatigue crack propagation in 7000 series aluminum alloys
Mason, Mark E.; Gangloff, Richard P.
1994-01-01
Stress corrosion cracking and corrosion fatigue experiments were conducted with the susceptible S-L orientation of AA7075-T651, immersed in acidified and inhibited NaCl solution, to provide a basis for incorporating environmental effects into fatigue crack propagation life prediction codes such as NASA FLAGRO. This environment enhances da/dN by five to ten-fold compared to fatigue in moist air. Time-based crack growth rates from quasi-static load experiments are an order of magnitude too small for accurate linear superposition prediction of da/dN for loading frequencies above 0.001 Hz. Alternate methods of establishing da/dt, based on rising-load or ripple-load-enhanced crack tip strain rate, do not increase da/dt and do not improve linear superposition. Corrosion fatigue is characterized by two regimes of frequency dependence; da/dN is proportional to f(exp -1) below 0.001 Hz and to F(exp 0) to F(exp -0.1) for higher frequencies. Da/dN increases mildly both with increasing hold-time at K(sub max) and with increasing rise-time for a range of loading waveforms. The mild time-dependence is due to cycle-time-dependent corrosion fatigue growth. This behavior is identical for S-L nd L-T crack orientations. The frequency response of environmental fatigue in several 7000 series alloys is variable and depends on undefined compositional or microstructural variables. Speculative explanations are based on the effect of Mg on occluded crack chemistry and embritting hydrogen uptake, or on variable hydrogen diffusion in the crack tip process zone. Cracking in the 7075/NaCl system is adequately described for life prediction by linear superposition for prolonged load-cycle periods, and by a time-dependent upper bound relationship between da/dN and delta K for moderate loading times.
Finite element analysis of fatigue crack closure under plane strain state
International Nuclear Information System (INIS)
Lee, Hak Joo; Kang, Jae Youn; Song, Ji Ho
2004-01-01
An elastic-plastic finite element analysis of fatigue crack closure is performed for plane strain conditions. The stabilization behavior of crack opening level and the effect of mesh size on the crack opening stress are investigated. In order to obtain a stabilized crack opening level for plane strain conditions, the crack must be advanced through approximately four times the initial monotonic plastic zone. The crack opening load tends to increase with the decrease of mesh size. The mesh size nearly equal to the theoretical plane strain cyclic plastic zone size may provide reasonable numerical results comparable with experimental crack opening data. The crack opening behavior is influenced by the crack growth increment and discontinuous opening behavior is observed. A procedure to predict the most appropriate mesh size for different stress ratio is suggested. Crack opening loads predicted by the FE analysis based on the procedure suggested resulted in good agreement with experimental ones within the error of 5 %. Effect of the distance behind the crack tip on the crack opening load determined by the ASTM compliance offset method based on the load-displacement relation and by the rotational offset method based on the load-differential displacement relation is investigated. Optimal gage location and method to determine the crack opening load is suggested
Crack closure and sequential effects in fatigue: A literature survey
Holmgren, M.
A literature survey of the phenomenon of crack closure is reported here. The state of the art is reviewed and several empirical formulas for determining the crack closure are compared with each other. Their properties, advantages and disadvantages are briefly discussed. Experimental techniques for determining the crack closure stress are presented and experimental data from the literature are reported.
National Research Council Canada - National Science Library
Chan, Kwai
2004-01-01
... of aerospace structural alloys. In this three-year program, physics-based fatigue crack initiation and growth models were developed and integrated into a probabilistic micromechanical code for treating fatigue life variability...
International Nuclear Information System (INIS)
Shirakihara, Kaori; Tanaka, Keisuke; Akiniwa, Yoshiaki; Suzuki, Yasuyoshi; Mukai, Hirokatsu
2006-01-01
Fatigue crack propagation tests of PZT specimens were performed under cyclic four-point bending with and without superposition of electric fields. The specimens were poled in the longitudinal direction (PL specimens) perpendicular to the crack plane. The crack propagation rate for the case of open circuit was faster than that for the case of short circuit. The application of a negative or positive electric field parallel to the poling direction accelerated the crack propagation rate, and the amount of acceleration was larger for the case of the negative field. The change of the crack propagation rate with crack extension can be divided into three regions. In the region I, the crack propagation rate decreases with increasing crack length, and then turn to increase in the region III. In the region II, the propagation rate is nearly constant. The mechanisms of fatigue crack propagation were correlated to domain switching near the crack tip. The grain boundary fracture was predominant in the low-rate region, while transgranular fracture became abundant on the unstable fracture surface. (author)
Factors Influencing Dwell Fatigue Cracking in Notches of Powder Metallurgy Superalloys
Gabb, T. P.; Telesman, J.; Ghosn, L.; Garg, A.; Gayda, J.
2011-01-01
The influences of heat treatment and cyclic dwells on the notch fatigue resistance of powder metallurgy disk superalloys were investigated for low solvus high refractory (LSHR) and ME3 disk alloys. Disks were processed to produce material conditions with varied microstructures and associated mechanical properties. Notched specimens were first subjected to baseline dwell fatigue cycles having a dwell at maximum load, as well as tensile, stress relaxation, creep rupture, and dwell fatigue crack growth tests at 704 C. Several material heat treatments displayed a bimodal distribution of fatigue life with the lives varying by two orders-of-magnitude, while others had more consistent fatigue lives. This response was compared to other mechanical properties, in search of correlations. The wide scatter in baseline dwell fatigue life was observed only for material conditions resistant to stress relaxation. For selected materials and conditions, additional tests were then performed with the dwells shifted in part or in total to minimum tensile load. The tests performed with dwells at minimum load exhibited lower fatigue lives than max dwell tests, and also exhibited early crack initiation and a substantial increase in the number of initiation sites. These results could be explained in part by modeling evolution of peak stresses in the notch with continued dwell fatigue cycling. Fatigue-environment interactions were determined to limit life for the fatigue cycles with dwells.
Fatigue life analysis of cracked gas receiver of emergency cut-off system in gas gathering station
Hu, Junzhi; Zhou, Jiyong; Li, Siyuan
2017-06-01
Small-scale air compressor and gas receiver are used as the driving gas of the emergency cut-off system in gas gathering station. Operation of block valve is ensured by starting and stopping compressor automatically. The frequent start-stop of compressor and the pressure fluctuation pose a threat to the service life of gas receiver, and then affect normal operation of the emergency cut-off system and security of gas gathering station. In this paper, the fatigue life of a pressure vessel with axial semi-elliptical surface crack in the inner wall is analyzed under the varying pressure by means of the theory of fracture mechanics. The influences of the amplitude of pressure fluctuation and the initial crack size on the residual life of gas receiver are discussed. It provides a basis for setting the working parameters of gas receiver of emergency cut-off system and determining the maintenance cycle.
International Nuclear Information System (INIS)
Kim, Jong Sung; Kim, Cheol; Jin, Tae Eun; Dong, P.
2004-01-01
The mesh-insensitive structural stress procedure by Dong is modified to apply to the welded joints with local thickness variation and inarguable shear/normal stresses along local discontinuity surface. In order to make use of the structural stress based K solution for fatigue correlation of welded joints, a proper crack growth model needs to be developed. There exist some significant discrepancies in inferring the slope or crack growth exponent in the conventional Paris law regime. Two-stage crack growth model was not considered since its applications are focused upon the fatigue behavior in welded joints in which the load ratio effects are considered negligible. In this paper, a two-stage crack growth law considering high mean loading is proposed and proven to be effective in unifying the so-called anomalous short crack growth data
A theoretical evaluation of the oxygen concentration in a corrosion-fatigue crack
International Nuclear Information System (INIS)
Turnbull, A.
1981-01-01
The oxygen concentration in a corrosion-fatigue crack has been evaluated theoretically by assuming that oxygen was consumed by cathodic reduction on the walls of the crack and mass transport occurred by diffusion and advection (forced convection), with the latter resulting from the sinusoidal variation of the displacement of the crack walls. By using parameters relevant to a compact tension specimen, the time-dependent distribution of the oxygen concentration in the crack was calculated as a function of ΔK (the range of the stress intensity factor), R-value (minimum load/maximum load), frequency, crack length, and electrode potential. The influence of advection was to significantly enhance the mass transport of oxygen in the crack compared with ''diffusion-only'' even at low frequencies and low ΔK. Regions in the crack were identified in which advection dominance or diffusion dominance of the mass transport of oxygen occurred
Fractal and multifractal approaches for the analysis of crack-size dependent scaling laws in fatigue
Energy Technology Data Exchange (ETDEWEB)
Paggi, Marco [Politecnico di Torino, Department of Structural Engineering and Geotechnics, Corso Duca degli Abruzzi 24, 10129 Torino (Italy)], E-mail: marco.paggi@polito.it; Carpinteri, Alberto [Politecnico di Torino, Department of Structural Engineering and Geotechnics, Corso Duca degli Abruzzi 24, 10129 Torino (Italy)
2009-05-15
The enhanced ability to detect and measure very short cracks, along with a great interest in applying fracture mechanics formulae to smaller and smaller crack sizes, has pointed out the so-called anomalous behavior of short cracks with respect to their longer counterparts. The crack-size dependencies of both the fatigue threshold and the Paris' constant C are only two notable examples of these anomalous scaling laws. In this framework, a unified theoretical model seems to be missing and the behavior of short cracks can still be considered as an open problem. In this paper, we propose a critical reexamination of the fractal models for the analysis of crack-size effects in fatigue. The limitations of each model are put into evidence and removed. At the end, a new generalized theory based on fractal geometry is proposed, which permits to consistently interpret the short crack-related anomalous scaling laws within a unified theoretical formulation. Finally, this approach is herein used to interpret relevant experimental data related to the crack-size dependence of the fatigue threshold in metals.
Fractal and multifractal approaches for the analysis of crack-size dependent scaling laws in fatigue
International Nuclear Information System (INIS)
Paggi, Marco; Carpinteri, Alberto
2009-01-01
The enhanced ability to detect and measure very short cracks, along with a great interest in applying fracture mechanics formulae to smaller and smaller crack sizes, has pointed out the so-called anomalous behavior of short cracks with respect to their longer counterparts. The crack-size dependencies of both the fatigue threshold and the Paris' constant C are only two notable examples of these anomalous scaling laws. In this framework, a unified theoretical model seems to be missing and the behavior of short cracks can still be considered as an open problem. In this paper, we propose a critical reexamination of the fractal models for the analysis of crack-size effects in fatigue. The limitations of each model are put into evidence and removed. At the end, a new generalized theory based on fractal geometry is proposed, which permits to consistently interpret the short crack-related anomalous scaling laws within a unified theoretical formulation. Finally, this approach is herein used to interpret relevant experimental data related to the crack-size dependence of the fatigue threshold in metals.
Directory of Open Access Journals (Sweden)
J A F O. Correia
2017-10-01
Full Text Available In Portugal there is a number of old metallic riveted railway and highway bridges that were erected by the end of the 19th century and beginning of the 20th century, and are still in operation, requiring inspections and remediation measures to overcome fatigue damage. Residual fatigue life predictions should be based on actual fatigue data from bridge materials which is scarce due to the material specificities. Fatigue crack propagation data of materials from representative Portuguese riveted bridges, namely the Pinh�o and Luiz I road bridges, the Viana road/railway bridge, the F�o road bridge and the Trez�i railway bridge were considered in this study. The fatigue crack growth rates were correlated using the Pariss law. Also, a statistical analysis of the pure mode I fatigue crack growth (FCG data available for the materials from the ancient riveted metallic bridges is presented. Based on this analysis, design FCG curves are proposed and compared with BS7910 standard proposal, for the Paris region, which is one important fatigue regime concerning the application of the Fracture Mechanics approaches, to predict the remnant fatigue life of structural details
International Nuclear Information System (INIS)
Zhou, Chao; Hong, Ming; Su, Zhongqing; Wang, Qiang; Cheng, Li
2013-01-01
There has been increasing interest in using the nonlinear features of acousto-ultrasonic (AU) waves to detect damage onset (e.g., micro-fatigue cracks) due to their high sensitivity to damage with small dimensions. However, most existing approaches are able to infer the existence of fatigue damage qualitatively, but fail to further ascertain its location and severity. A damage characterization approach, in conjunction with the use of an active piezoelectric sensor network, was established, capable of evaluating fatigue cracks in a quantitative manner (including the co-presence of multiple fatigue cracks, and their individual locations and severities). Fundamental investigations, using both experiment and enhanced finite element analysis dedicated to the simulation of nonlinear AU waves, were carried out to link the accumulation of nonlinearities extracted from high-order AU waves to the characteristic parameters of a fatigue crack. A probability-based diagnostic imaging algorithm was developed, facilitating an intuitive presentation of identification results in images. The approach was verified experimentally by evaluating multi-fatigue cracks near rivet holes of a fatigued aluminum plate, showing satisfactory precision in characterizing real, barely visible fatigue cracks. Compared with existing methods, this approach innovatively (i) uses permanently integrated active sensor networks, conducive to automatic and online health monitoring; (ii) characterizes fatigue cracks at a quantitative level; (iii) allows detection of multiple fatigue cracks; and (iv) visualizes identification results in intuitive images. (paper)
Fatigue crack growth from a cracked elastic particle into a ductile matrix
Groh, S.; Olarnrithinun, S.; Curtin, W. A.; Needleman, A.; Deshpande, V. S.; Van der Giessen, E.
2008-01-01
The monotonic and cyclic crack growth rate of cracks is strongly influenced by the microstructure. Here, the growth of cracks emanating from pre-cracked micron-scale elastic particles and growing into single crystals is investigated, with a focus on the effects of (i) plastic confinement due to the
Kang, T. S.; Liu, H. W.
1974-01-01
Cyclic prestress increases subsequent fatigue crack growth rate in 2024-T351 aluminum alloy. This increase in growth rate, caused by the prestress, and the increased rate, caused by temper embrittlement as observed by Ritchie and Knott (1973), cannot be explained by the crack tip blunting model alone. Each fatigue crack increment consists of two components, a brittle and a ductile component. They are controlled by the ductility of the material and its cyclic yield strength, respectively.
Measurements of fatigue crack length at elevated temperature by D. C. electrical potential method
International Nuclear Information System (INIS)
Matsumoto, Masakatsu; Yamauchi, Isamu; Kodaira, Tsuneo
1982-07-01
The direct current (d.c.) electrical potential method was used to automatically and continuously measure the crack length in cyclic crack growth test at elevated temperature. This report describes some results concerning the calibration curves, i.e. the relation between electrical potential change and amount of crack extention, using SUS 304 and 2 1/4Cr-1Mo steels. It can be concluded that the measurements of fatigue crack length is possible even at elevated temperature as well as at room temperature with the equivalent accuracy. (author)
Fatigue crack growth behavior of RAFM steel in Paris and threshold regimes at different temperatures
Energy Technology Data Exchange (ETDEWEB)
Babu, M. Nani; Sasikala, G., E-mail: gsasi@igcar.gov.in; Dutt, B. Shashank; Venugopal, S.; Bhaduri, A.K.; Jayakumar, T.
2014-04-01
Fatigue crack growth (FCG) behavior of a reduced activation ferritic martensitic (indigenous RAFM) steel has been evaluated at 300, 653 and 823 K in Paris and threshold regimes. The effect of temperature on threshold stress intensity factor range and associated crack closure mechanisms is highlighted. The FCG results were compared with those for EUROFER 97. Further, crack tip effective stress intensity factor ranges (ΔK{sub tip,eff}) have been evaluated by taking crack tip shielding into account in order to examine the effect of temperature on true intrinsic FCG behavior.
International Nuclear Information System (INIS)
Ekobori, T.; Konosu, S.; Ekobori, A.
1980-01-01
Classified are models of the crack growth mechanism, and in the framework of the fracture mechanics suggested are combined micro- and macroapproaches to interpreting the criterion of the brittle fracture and fatigue crack growth as fracture typical examples, when temporal processes are important or unimportant. Under the brittle fracture conditions the crack propagation criterion is shown to be brought with the high accuracy to a form analogous to one of the crack propagation in a linear fracture mechanics although it is expressed with micro- and macrostructures. Obtained is a good agreement between theoretical and experimental data
International Nuclear Information System (INIS)
Bertolino, G.; Sauzay, M.; Bertolino, G.; Doquet, V.
2003-01-01
An attempt to model the variability of short cracks development in high-cycle fatigue is made by coupling finite element calculations of the stresses ahead of a microcrack in a polycrystal with simulations of crack growth along slip planes based on discrete dislocations dynamics. The model predicts a large scatter in growth rates related to the roughness of the crack path. It also describes the influence of the mean grain size and the fact that overloads may suppress the endurance limit by allowing arrested cracks to cross the grain boundaries. (authors)
Accelerated Near-Threshold Fatigue Crack Growth Behavior of an Aluminum Powder Metallurgy Alloy
Piascik, Robert S.; Newman, John A.
2002-01-01
Fatigue crack growth (FCG) research conducted in the near threshold regime has identified a room temperature creep crack growth damage mechanism for a fine grain powder metallurgy (PM) aluminum alloy (8009). At very low DK, an abrupt acceleration in room temperature FCG rate occurs at high stress ratio (R = Kmin/Kmax). The near threshold accelerated FCG rates are exacerbated by increased levels of Kmax (Kmax less than 0.4 KIC). Detailed fractographic analysis correlates accelerated FCG with the formation of crack-tip process zone micro-void damage. Experimental results show that the near threshold and Kmax influenced accelerated crack growth is time and temperature dependent.
Detection and Sizing of Fatigue Cracks in Steel Welds with Advanced Eddy Current Techniques
Todorov, E. I.; Mohr, W. C.; Lozev, M. G.
2008-02-01
Butt-welded specimens were fatigued to produce cracks in the weld heat-affected zone. Advanced eddy current (AEC) techniques were used to detect and size the cracks through a coating. AEC results were compared with magnetic particle and phased-array ultrasonic techniques. Validation through destructive crack measurements was also conducted. Factors such as geometry, surface treatment, and crack tightness interfered with depth sizing. AEC inspection techniques have the potential of providing more accurate and complete sizing flaw data for manufacturing and in-service inspections.
Chen, Xingyang; Zhou, Chengshuang; Cai, Xiao; Zheng, Jinyang; Zhang, Lin
2017-10-01
The effects of external hydrogen on hydrogen transportation and distribution around the fatigue crack tip in type 304 stainless steel were investigated by using hydrogen microprint technique (HMT) and thermal desorption spectrometry. HMT results show that some silver particles induced by hydrogen release are located near the fatigue crack and more silver particles are concentrated around the crack tip, which indicates that hydrogen accumulates in the vicinity of the crack tip during the crack growth in hydrogen gas environment. Along with the crack propagation, strain-induced α' martensite forms around the crack tip and promotes hydrogen invasion into the matrix, which will cause the crack initiation and propagation at the austenite/ α' martensite interface. In addition, the hydrogen content in the vicinity of the crack tip is higher than that at the crack edge far away from the crack tip, which is related to the stress state and strain-induced α' martensite.
Crack luminescence as an innovative method for detection of fatigue damage
Directory of Open Access Journals (Sweden)
R. Makris
2018-04-01
Full Text Available Conventional non-destructive testing methods for crack detection provide just a snapshot of fatigue crack evolution at a specific location in the moment of examination. The crack luminescence coating realizes a clear visibility of the entire crack formation. The coating consists of two layers with different properties and functions. The bottom layer emits light as fluorescence under UV radiation. The top layer covers the fluorescing one and prevents the emitting of light in case of no damage at the surface. Several different experiments show that due to the sensitive coating even the early stage of crack formation can be detected. That makes crack luminescence helpful for investigating the incipient crack opening behavior. Cracks can be detected and observed during operation of a structure, making it also very interesting for continuous monitoring. Crack luminescence is a passive method and no skilled professionals are necessary to detect cracks, as for conventional methods. The luminescent light is clearly noticeable by unaided eye observations and also by standard camera equipment, which makes automated crack detection possible as well. It is expected that crack luminescence can reduce costs and time for preventive maintenance and inspection.
A Comparison Study of Machine Learning Based Algorithms for Fatigue Crack Growth Calculation.
Wang, Hongxun; Zhang, Weifang; Sun, Fuqiang; Zhang, Wei
2017-05-18
The relationships between the fatigue crack growth rate ( d a / d N ) and stress intensity factor range ( Δ K ) are not always linear even in the Paris region. The stress ratio effects on fatigue crack growth rate are diverse in different materials. However, most existing fatigue crack growth models cannot handle these nonlinearities appropriately. The machine learning method provides a flexible approach to the modeling of fatigue crack growth because of its excellent nonlinear approximation and multivariable learning ability. In this paper, a fatigue crack growth calculation method is proposed based on three different machine learning algorithms (MLAs): extreme learning machine (ELM), radial basis function network (RBFN) and genetic algorithms optimized back propagation network (GABP). The MLA based method is validated using testing data of different materials. The three MLAs are compared with each other as well as the classical two-parameter model ( K * approach). The results show that the predictions of MLAs are superior to those of K * approach in accuracy and effectiveness, and the ELM based algorithms show overall the best agreement with the experimental data out of the three MLAs, for its global optimization and extrapolation ability.
Reformed austenite transformation during fatigue crack propagation of 13%Cr-4%Ni stainless steel
Energy Technology Data Exchange (ETDEWEB)
Thibault, Denis, E-mail: thibault.denis@ireq.ca [Institut de recherche d' Hydro-Quebec (IREQ), 1800, boul. Lionel-Boulet, Varennes, Quebec, J3X 1S1 (Canada); Bocher, Philippe, E-mail: philippe.bocher@etsmtl.ca [Ecole de technologie superieure, 1100, rue Notre-Dame Ouest, Montreal, Quebec, H3C 1K3 (Canada); Thomas, Marc, E-mail: marc.thomas@etsmtl.ca [Ecole de technologie superieure, 1100, rue Notre-Dame Ouest, Montreal, Quebec, H3C 1K3 (Canada); Lanteigne, Jacques, E-mail: lanteigne.jacques@ireq.ca [Institut de recherche d' Hydro-Quebec (IREQ), 1800, boul. Lionel-Boulet, Varennes, Quebec, J3X 1S1 (Canada); Hovington, Pierre, E-mail: hovington.pierre@ireq.ca [Institut de recherche d' Hydro-Quebec (IREQ), 1800, boul. Lionel-Boulet, Varennes, Quebec, J3X 1S1 (Canada); Robichaud, Patrice, E-mail: patrice.robichaud@riotinto.com [Centre de recherche et de developpement Arvida (CRDA), 1955, boul. Mellon, Jonquiere, Quebec, G7S 4K8 (Canada)
2011-08-15
Highlights: {yields} Reformed austenite in 13%Cr-4%Ni stainless steel transforms during fatigue crack growth. {yields} Low cycle fatigue tests showed that this transformation to martensite is gradual. {yields} XRD spectrums obtained on the fracture surface and have been correlated to LCF results. - Abstract: In the as-quenched state, 13%Cr-4%Ni martensitic stainless steels are essentially 100% martensitic. However, a certain amount of austenite is formed during the tempering of this alloy. This reformed austenite is thermally stable at room temperature but can transform to martensite under stress. This transformation is known to happen during impact testing but it has never been established if it occurs during fatigue crack propagation. This study presents the results of X-ray diffraction measurements of reformed austenite before and after crack growth testing. It has been found that reformed austenite does transform to martensite at the crack tip and that this transformation occurs even at a low stress intensity factor. Low-cycle fatigue tests were conducted to verify austenite transformation under cyclic straining. It was found that reformed austenite transforms only partially during the first strain reversal but that essentially all austenite has disappeared after 100 cycles. The relation between austenite transformation under low-cycle fatigue and its transformation during crack growth is also discussed.
Liu, Peipei; Yang, Suyoung; Lim, Hyung Jin; Park, Hyung Chul; Ko, In Chang; Sohn, Hoon
2014-03-01
Fatigue crack is one of the main culprits for the failure of metallic structures. Recently, it has been shown that nonlinear wave modulation spectroscopy (NWMS) is effective in detecting nonlinear mechanisms produced by fatigue crack. In this study, an active wireless sensor node for fatigue crack detection is developed based on NWMS. Using PZT transducers attached to a target structure, ultrasonic waves at two distinctive frequencies are generated, and their modulation due to fatigue crack formation is detected using another PZT transducer. Furthermore, a reference-free NWMS algorithm is developed so that fatigue crack can be detected without relying on history data of the structure with minimal parameter adjustment by the end users. The algorithm is embedded into FPGA, and the diagnosis is transmitted to a base station using a commercial wireless communication system. The whole design of the sensor node is fulfilled in a low power working strategy. Finally, an experimental verification has been performed using aluminum plate specimens to show the feasibility of the developed active wireless NWMS sensor node.
Reformed austenite transformation during fatigue crack propagation of 13%Cr-4%Ni stainless steel
International Nuclear Information System (INIS)
Thibault, Denis; Bocher, Philippe; Thomas, Marc; Lanteigne, Jacques; Hovington, Pierre; Robichaud, Patrice
2011-01-01
Highlights: → Reformed austenite in 13%Cr-4%Ni stainless steel transforms during fatigue crack growth. → Low cycle fatigue tests showed that this transformation to martensite is gradual. → XRD spectrums obtained on the fracture surface and have been correlated to LCF results. - Abstract: In the as-quenched state, 13%Cr-4%Ni martensitic stainless steels are essentially 100% martensitic. However, a certain amount of austenite is formed during the tempering of this alloy. This reformed austenite is thermally stable at room temperature but can transform to martensite under stress. This transformation is known to happen during impact testing but it has never been established if it occurs during fatigue crack propagation. This study presents the results of X-ray diffraction measurements of reformed austenite before and after crack growth testing. It has been found that reformed austenite does transform to martensite at the crack tip and that this transformation occurs even at a low stress intensity factor. Low-cycle fatigue tests were conducted to verify austenite transformation under cyclic straining. It was found that reformed austenite transforms only partially during the first strain reversal but that essentially all austenite has disappeared after 100 cycles. The relation between austenite transformation under low-cycle fatigue and its transformation during crack growth is also discussed.
A Laser-based Ultrasonic Inspection System to Detect Micro Fatigue Cracks
International Nuclear Information System (INIS)
Park, Seung Kyu; Baik, Sung Hoon; Park, Moon Cheol; Lim, Chang Hwan; Cha, Hyung Ki
2005-01-01
on the surface. We can detect small fatigue cracks by finding the abrupt changing of the amplitude of the ultrasound and its center frequency in the SLS technique. It means that the scanning laser beam is located in the vicinity of the cracks. In this paper, we developed a stable laser-based ultrasonic inspection system using a pulse laser, a CFPI with a dynamic stabilizer and a computer. The computer is equipped with a GHz high speed A/D converter, three A/D converters, one D/A converter and one digital output port. The configured dynamic stabilizer generates the laser-based ultrasound by triggering a pulse laser at the maximum gain time by continually observing the gain of the CFPI. The computer acquires the laser-based ultrasound by using the GHz high-speed A/D converter and processes the ultrasonic signal in real time. We experimentally confirmed that the developed laser-based ultrasonic inspection system is stable and can detect cracks using the SLS technique
Effect of a new specimen size on fatigue crack growth behavior in thick-walled pressure vessels
International Nuclear Information System (INIS)
Shariati, Mahmoud; Mohammadi, Ehsan; Masoudi Nejad, Reza
2017-01-01
Fatigue crack growth in thick-walled pressure vessels is an important factor affecting their fracture. Predicting the path of fatigue crack growth in a pressure vessel is the main issue discussed in fracture mechanics. The objective of this paper is to design a new geometrical specimen in fatigue to define the behavior of semi-elliptical crack growth in thick-walled pressure vessels. In the present work, the importance of the behavior of fatigue crack in test specimen and real conditions in thick-walled pressure vessels is investigated. The results of fatigue loading on the new specimen are compared with the results of fatigue loading in a cylindrical pressure vessel and a standard specimen. Numerical and experimental methods are used to investigate the behavior of fatigue crack growth in the new specimen. For this purpose, a three-dimensional boundary element method is used for fatigue crack growth under stress field. The modified Paris model is used to estimate fatigue crack growth rates. In order to verify the numerical results, fatigue test is carried out on a couple of specimens with a new geometry made of ck45. A comparison between experimental and numerical results has shown good agreement. - Highlights: • This paper provides a new specimen to define the behavior of fatigue crack growth. • We estimate the behavior of fatigue crack growth in specimen and pressure vessel. • A 3D finite element model has been applied to estimate the fatigue life. • We compare the results of fatigue loading for cylindrical vessel and specimens. • Comparison between experimental and numerical results has shown a good agreement.
Fatigue-crack growth behavior of Type 347 stainless steels under simulated PWR water conditions
Energy Technology Data Exchange (ETDEWEB)
Hong, Seokmin; Min, Ki-Deuk; Yoon, Ji-Hyun; Kim, Min-Chul; Lee, Bong-Sang [Korea Atomic Energy Research Institute, Daejeon (Korea, Republic of)
2015-10-15
Fatigue crack growth rate (FCGR) curve of stainless steel exists in ASME code section XI, but it is still not considering the environmental effects. The longer time nuclear power plant is operated, the more the environmental degradation issues of materials pop up. There are some researches on fatigue crack growth rate of S304 and S316, but researches of FCGR of S347 used in Korea nuclear power plant are insufficient. In this study, the FCGR of S347 stainless steel was evaluated in the PWR high temperature water conditions. The FCGRs of S347 stainless steel under pressurized-water conditions were measured by using compact-tension (CT) specimens at different levels of dissolved oxygen (DO) and frequency. 1. FCGRs of SS347 were slower than that in ASME XI and environmental effect did not occur when frequency was higher than 1Hz. 2. Fatigue crack growth is accelerated by corrosion fatigue and it is more severe when frequency is slower than 0.1Hz. 3. Increase of crack tip opening time increased corrosion fatigue and it deteriorated environmental fatigue properties.
Statistical analysis of fatigue crack growth behavior for grade B cast steel
International Nuclear Information System (INIS)
Li, W.; Sakai, T.; Li, Q.; Wang, P.
2011-01-01
Tests for fatigue crack growth rate (FCGR) and crack-tip opening displacement (CTOD) were performed to clarify the fatigue crack growth behavior of a railway grade B cast steel. The threshold values of this steel with specific survival probabilities are evaluated, in which the mean value is 8.3516 MPa m 1/2 , very similar to the experimental value, about 8.7279 MPa m 1/2 . Under the conditions of plane strain and small-scale yielding, the values of fracture toughness for this steel with specific survival probabilities are converted from the corresponding critical CTOD values, in which the mean value is about 138.4256 MPa m 1/2 . In consideration of the inherent variability of crack growth rates, six statistical models are proposed to represent the probabilistic FCGR curves of this steel in entire crack propagation region from the viewpoints of statistical evaluation on the number of cycles at a given crack size and the crack growth rate at a given stress intensity factor range, stochastic characteristic of crack growth as well as statistical analysis of coefficient and exponent in FCGR power law equation. Based on the model adequacy checking, result shows that all models are basically in good agreement with test data. Although the probabilistic damage-tolerant design based on some models may involve a certain amount of risk in stable crack propagation region, they just accord with the fact that the dispersion degree of test data in this region is relatively smaller.
Directory of Open Access Journals (Sweden)
B. Vargas-Arista
2013-01-01
Full Text Available The fractography and mechanical behaviour of fatigue crack propagation in the heat-affected zone (HAZ of AISI 4140 steel welded using the shielded metal arc process was analysed. Different austenitic grain size was obtained by normalizing performed at 1200 °C for 5 and 10 hours after welding. Three point bending fatigue tests on pre-cracked specimens along the HAZ revealed that coarse grains promoted an increase in fatigue crack growth rate, hence causing a reduction in both fracture toughness and critical crack length, and a transgranular brittle final fracture with an area fraction of dimple zones connecting cleavage facets. A fractographic analysis proved that as the normalizing time increased the crack length decreased. The increase in the river patterns on the fatigue crack propagation in zone II was also evidenced and final brittle fracture because of transgranular quasicleavage was observed. Larger grains induced a deterioration of the fatigue resistance of the HAZ.
Subsurface crack initiation and propagation mechanisms in gigacycle fatigue
International Nuclear Information System (INIS)
Huang Zhiyong; Wagner, Daniele; Bathias, Claude; Paris, Paul C.
2010-01-01
In the very high cycle regime (N f > 10 7 cycles) cracks can nucleate on inclusions, 'supergrains' and pores, which leads to fish-eye propagation around the defect. The initiation from an inclusion or other defect is almost equal to the total crack growth lifetime, perhaps much more than 99% of this lifetime in many cases. Integration of the Paris law allows one to predict the number of cycles to crack initiation. A cyclic plastic zone around the crack exists, and recording the surface temperature of the sample during the test may allow one to follow crack propagation and determine the number of cycles to crack initiation. A thermo-mechanical model has been developed. In this study several fish-eyes from various materials have been observed by scanning electron microscopy, and the fractographic results analyzed as they related to the mechanical and thermo-mechanical models.
Fatigue Crack Growth Rate and Stress-Intensity Factor Corrections for Out-of-Plane Crack Growth
Forth, Scott C.; Herman, Dave J.; James, Mark A.
2003-01-01
Fatigue crack growth rate testing is performed by automated data collection systems that assume straight crack growth in the plane of symmetry and use standard polynomial solutions to compute crack length and stress-intensity factors from compliance or potential drop measurements. Visual measurements used to correct the collected data typically include only the horizontal crack length, which for cracks that propagate out-of-plane, under-estimates the crack growth rates and over-estimates the stress-intensity factors. The authors have devised an approach for correcting both the crack growth rates and stress-intensity factors based on two-dimensional mixed mode-I/II finite element analysis (FEA). The approach is used to correct out-of-plane data for 7050-T7451 and 2025-T6 aluminum alloys. Results indicate the correction process works well for high DeltaK levels but fails to capture the mixed-mode effects at DeltaK levels approaching threshold (da/dN approximately 10(exp -10) meter/cycle).
An accurate fatigue damage model for welded joints subjected to variable amplitude loading
Aeran, A.; Siriwardane, S. C.; Mikkelsen, O.; Langen, I.
2017-12-01
Researchers in the past have proposed several fatigue damage models to overcome the shortcomings of the commonly used Miner’s rule. However, requirements of material parameters or S-N curve modifications restricts their practical applications. Also, application of most of these models under variable amplitude loading conditions have not been found. To overcome these restrictions, a new fatigue damage model is proposed in this paper. The proposed model can be applied by practicing engineers using only the S-N curve given in the standard codes of practice. The model is verified with experimentally derived damage evolution curves for C 45 and 16 Mn and gives better agreement compared to previous models. The model predicted fatigue lives are also in better correlation with experimental results compared to previous models as shown in earlier published work by the authors. The proposed model is applied to welded joints subjected to variable amplitude loadings in this paper. The model given around 8% shorter fatigue lives compared to Eurocode given Miner’s rule. This shows the importance of applying accurate fatigue damage models for welded joints.
Energy Technology Data Exchange (ETDEWEB)
Briffod, Fabien, E-mail: briffod@rme.mm.t.u-tokyo.ac.jp; Shiraiwa, Takayuki; Enoki, Manabu
2017-05-17
In this study, fatigue crack initiation in pure α-iron is investigated through a microstructure-sensitive framework. At first, synthetic microstructures are modeled based on an anisotropic tessellation that accounts for the information of the grains morphology extracted from electron backscatter diffraction (EBSD) analysis. Low-cycle fatigue experiments under strain-controlled conditions are conducted in order to calibrate a crystal plasticity model and a J{sub 2} model including isotropic and kinematic hardening. A critical plane fatigue indicator parameter (FIP) based on the Tanaka-Mura model is then presented to evaluate the location and quantify the driving force for the formation of a crack. The FIP is averaged over several potential crack paths within each grain defined by the intersection between a given slip plane and the plane of the model thus accounting for both the lattice orientation and morphology of the grain. Several fatigue simulations at various stress amplitudes are conducted using a sub-modeling technique for the attribution of boundary conditions on the polycrystalline aggregate models including an elliptic defect. The influence of the microstructure attributes and stress level on the location and amplitude of the FIP are then quantified and discussed.
Fatigue crack growth monitoring: fracture mechanics and non-destructive testing requirements
International Nuclear Information System (INIS)
Williams, S.; Mudge, P.J.
1982-01-01
If a fatigue crack is found in a component in service, two options exist if plant integrity is to be maintained: first, the plant can be removed from service and repairs effected or replacements fitted; second, the growth of the crack can be monitored non-destructively until it is either considered to be too large to tolerate, in which case it must be repaired, or until a convenient down time when repair can be effected. The second option has obvious benefits for plant operators, but in such a situation it is essential that errors of the non-destructive estimate of defect size, which will undoubtedly exist, and uncertainties in the fatigue crack growth laws in operation must both be allowed for if a safe extension of service life is to be obtained; i.e. without failure by leakage or fast fracture arising from the fatigue crack. This paper analyses the accuracy required of non-destructive crack measurement techniques to permit the safe monitoring of crack growth by periodic inspection. It then demonstrates that it is possible to achieve adequate crack monitoring using conventional ultrasonic techniques. (author)
Fatigue Crack Growth Behavior of Nickel-base Superalloy Haynes 282 at 550-750 °C
Rozman, K. A.; Kruzic, J. J.; Hawk, J. A.
2015-08-01
The fatigue crack growth rates for nickel-based superalloy Haynes 282 were measured at temperatures of 550, 650, and 750 °C using compact tension specimens with a load ratio of 0.1 and cyclic loading frequencies of 25 Hz and 0.25 Hz. Increasing the temperature from 550 to 750 °C caused the fatigue crack growth rates to increase from ~20 to 60% depending upon the applied stress intensity level. The effect of reducing the applied loading frequency increased the fatigue crack growth rates from ~20 to 70%, also depending upon the applied stress intensity range. The crack path was observed to be transgranular for the temperatures and frequencies used during fatigue crack growth rate testing. At 750 °C, there were some indications of limited intergranular cracking excursions at both loading frequencies; however, the extent of intergranular crack growth was limited and the cause is not understood at this time.
Directory of Open Access Journals (Sweden)
Chao He
2017-01-01
Full Text Available Very high cycle fatigue behavior of nugget zone in AA 7075 friction stir welded joint was experimentally investigated using ultrasonic fatigue testing system (20 kHz to clarify the crack initiation mechanism. It was found that the fatigue strength of nugget zone decreased continuously even beyond 107 cycles with no traditional fatigue limits. Fatigue cracks initiated from the welding defects located at the bottom side of the friction stir weld. Moreover, a special semicircular zone could be characterized around the crack initiation site, of which the stress intensity factor approximately equaled the threshold of fatigue crack propagation rate. Finally, a simplified model was proposed to estimate the fatigue life by correlating the welding defect size and applied stress. The predicted results are in good agreement with the experimental results.
International Nuclear Information System (INIS)
Kamaya, Masayuki; Kawakubo, Masahiro
2012-01-01
In this study, the fatigue damage was assumed to be equivalent to the crack initiation and its growth, and fatigue life was assessed by predicting the crack growth. First, a low-cycle fatigue test was conducted in air at room temperature under constant cyclic strain range of 1.2%. The crack initiation and change in crack size during the test were examined by replica investigation. It was found that a crack of 41.2 μm length was initiated almost at the beginning of the test. The identified crack growth rate was shown to correlate well with the strain intensity factor, whose physical meaning was discussed in this study. The fatigue life prediction model (equation) under constant strain range was derived by integrating the crack growth equation defined using the strain intensity factor, and the predicted fatigue lives were almost identical to those obtained by low-cycle fatigue tests. The change in crack depth predicted by the equation also agreed well with the experimental results. Based on the crack growth prediction model, it was shown that the crack size would be less than 0.1 mm even when the estimated fatigue damage exceeded the critical value of the design fatigue curve, in which a twenty-fold safety margin was used for the assessment. It was revealed that the effect of component size and surface roughness, which have been investigated empirically by fatigue tests, could be reasonably explained by considering the crack initiation and growth. Furthermore, the environmental effect on the fatigue life was shown to be brought about by the acceleration of crack growth. (author)
International Nuclear Information System (INIS)
Weissenberg, Thomas
2014-03-01
Using the example of the ferritic steels 22NiMoCr3-7 and 15MnNi6-3 representative for Nuclear Power Plants experimental data for the evaluation of the influence of the light water reactor (LWR) coolant environment and postulated chloride contaminations on crack development and fatigue have been determined in order to verify and extend the basis for a reliable estimation of the residual service life of reactor components. The aim of the research project was the investigation of the environmental effects at low strain rate conditions and the determination of the fatigue life under cyclic loading at uniaxial and multiaxial stress state. The quasi-static tensile tests (Constant Extension Rate Test, CERT) were performed using 3 low strain rates, each differing by about one order of magnitude (2.5.10 -3 , 3.1.10 -4 and 2.3.10 -5 %/s). The low cycle fatigue (LCF) experiments were conducted applying alternating tensile-compression loading with strain amplitudes of 0.3, 0.5 and 0.9 % at strain rates of 0.1 and 0.01 %/s (tests in air primarily 0.1 %/s). The cyclic notched tensile tests were carried out with a nominal axial strain in the notch root of 0.5 % at a strain rate of 0.1 %/s. The experiments in each case were performed in air, high purity water and chloride containing water at a testing temperature of 240 C, the oxygen content of the liquid medium was set to 0.4 ppm (simulated boiling water reactor coolant). In the CERT experiments chloride contents of 30, 50 and 100 ppb were applied, in the LCF tests the chloride content was 50 ppb which can be regarded as an upper realistic limit for a postulated chloride contamination of the reactor coolant. All experiments in liquid environment were preceded by a pre-autoclaving phase of at least 100 h in order to allow the formation of a stable oxide layer (magnetite). The testing material 22NiMoCr3-7 was available in form of an original reactor pressure vessel shell primarily designated for the German nuclear power plant
77 K Fatigue Crack Growth Rate of Modified CF8M Stainless Steel Castings
International Nuclear Information System (INIS)
Walsh, R. P.; Toplosky, V. J.; Han, K.; Heitzenroeder, P. J.; Nelson, B. E.
2006-01-01
The National Compact Stellerator Experiment (NCSX) is the first of a new class of stellarators. The modular superconducting coils in the NCSX have complex geometry that are manufactured on cast stainless steel (modified CF8M) winding forms. Although CF8M castings have been used before at cryogenic temperature there is limited data available for their mechanical properties at low temperatures. The fatigue life behavior of the cast material is vital thus a test program to generate data on representative material has been conducted. Fatigue test specimens have been obtained from key locations within prototype winding forms to determine the 77 K fatigue crack growth rate. The testing has successfully developed a representative database that ensures confident design. The measured crack growth rates are analyzed in terms of the Paris law parameters and the crack growth properties are related to the materials microstructure
Shaari, M. S.; Akramin, M. R. M.; Ariffin, A. K.; Abdullah, S.; Kikuchi, M.
2018-02-01
The paper is presenting the fatigue crack growth (FCG) behavior of semi-elliptical surface cracks for API X65 gas pipeline using S-version FEM. A method known as global-local overlay technique was used in this study to predict the fatigue behavior that involve of two separate meshes each specifically for global (geometry) and local (crack). The pre-post program was used to model the global geometry (coarser mesh) known as FAST including the material and boundary conditions. Hence, the local crack (finer mesh) will be defined the exact location and the mesh control accordingly. The local mesh was overlaid along with the global before the numerical computation taken place to solve the engineering problem. The stress intensity factors were computed using the virtual crack closure-integral method (VCCM). The most important results is the behavior of the fatigue crack growth, which contains the crack depth (a), crack length (c) and stress intensity factors (SIF). The correlation between the fatigue crack growth and the SIF shows a good growth for the crack depth (a) and dissimilar for the crack length (c) where stunned behavior was resulted. The S-version FEM will benefiting the user due to the overlay technique where it will shorten the computation process.
Directory of Open Access Journals (Sweden)
Y. Nakai
2015-10-01
Full Text Available In rolling contact fatigue (RCF, cracks usually initiate from inclusions beneath the surface and propagate to the contact surface. In the present study, synchrotron radiation computed laminography (SRCL imaging was performed to observe flaking defects during the RCF of a high-strength steel. Specially fabricated inclusion-rich steel plate specimens were employed in the experiments. For the in situ observation of crack propagation, a compact RCF testing machine was developed, and a 4D analysis scheme was applied to the data obtained by SRCL. RCF tests were carried out near the measurement hatch of the beam line used SRCL to enable the successive observation of crack initiation and growth behaviors. Specimens before and after the occurrence of flaking were observed by SRCL, and flaking defects and cracks under the surface were successfully detected. As a result, details of the crack initiation and flaking process in RCF could be discussed. Shear-type horizontal cracks were found to initiate after the initiation and propagation of tensile-type vertical cracks along inclusions, where the face of the vertical cracks was perpendicular to the rolling direction and rolling surface. Therefore, the formation of vertical cracks is considered to affect shear-type crack formation and flaking, where the shape and length of inclusions also affect the initiation and propagation of vertical cracks.
Strength Behaviour of Fatigue Cracked Lugs (Festigkeitsverhalten von Rissbehafteten Augenstaeben),
1981-01-01
either surface cracks or corner cracks at holes. NASA TN 1)-8244 64 A.F. Grandt Stress intensity factors for some through fracked fastener holes...with Hydropuise L~ngszylinder longitudinal cylinder Druckblversorgung =pressure oil Supply Hydraulikaggregat = hydraulic control unit Fig 7.5 Plan of
Effect of laser shock processing on fatigue crack growth of duplex stainless steel
International Nuclear Information System (INIS)
Rubio-Gonzalez, C.; Felix-Martinez, C.; Gomez-Rosas, G.; Ocana, J.L.; Morales, M.; Porro, J.A.
2011-01-01
Research highlights: → LSP is an effective surface treatment to improve fatigue properties of duplex stainless steel. → Increasing pulse density, fatigue crack growth rate is reduced. → Microstructure is not affected by LSP. → Compressive residual stresses increases increasing pulse density. - Abstract: Duplex stainless steels have wide application in different fields like the ship, petrochemical and chemical industries that is due to their high strength and excellent toughness properties as well as their high corrosion resistance. In this work an investigation is performed to evaluate the effect of laser shock processing on some mechanical properties of 2205 duplex stainless steel. Laser shock processing (LSP) or laser shock peening is a new technique for strengthening metals. This process induces a compressive residual stress field which increases fatigue crack initiation life and reduces fatigue crack growth rate. A convergent lens is used to deliver 2.5 J, 8 ns laser pulses by a Q-switched Nd:YAG laser, operating at 10 Hz with infrared (1064 nm) radiation. The pulses are focused to a diameter of 1.5 mm. Effect of pulse density in the residual stress field is evaluated. Residual stress distribution as a function of depth is determined by the contour method. It is observed that the higher the pulse density the greater the compressive residual stress. Pulse densities of 900, 1600 and 2500 pul/cm 2 are used. Pre-cracked compact tension specimens were subjected to LSP process and then tested under cyclic loading with R = 0.1. Fatigue crack growth rate is determined and the effect of LSP process parameters is evaluated. In addition fracture toughness is determined in specimens with and without LSP treatment. It is observed that LSP reduces fatigue crack growth and increases fracture toughness if this steel.
3D characterization of rolling contact fatigue crack networks
DEFF Research Database (Denmark)
Jessop, Casey; Ahlström, Johan; Hammar, Lars
2016-01-01
analysis method for geometrical reconstruction, and a 3D representation of the complex crack network was achieved. This was compared with measurements on cross-sections after repeated metallographic sectioning to determine the accuracy of prediction of the geometrical reconstruction. A second squat...... was investigated by X-ray tomography after extraction of a section of the rail head. A third squat was opened by careful cutting, which gave full access to the crack faces, and the topography was measured by stylus profilometry. The high-energy X-ray, 3D reconstruction method showed accurate main crack geometry...... to the crack face. However this time-consuming method requires destruction of the specimen investigated. The X-ray tomography revealed the 3D crack network including side branches in a 10×10×30mm3 sample, and provided topographic information without completely opening the squat. Topography measurements...
Flat-Cladding Fiber Bragg Grating Sensors for Large Strain Amplitude Fatigue Tests
Directory of Open Access Journals (Sweden)
Xijia Gu
2010-08-01
Full Text Available We have successfully developed a flat-cladding fiber Bragg grating sensor for large cyclic strain amplitude tests of up to ±8,000 με. The increased contact area between the flat-cladding fiber and substrate, together with the application of a new bonding process, has significantly increased the bonding strength. In the push-pull fatigue tests of an aluminum alloy, the plastic strain amplitudes measured by three optical fiber sensors differ only by 0.43% at a cyclic strain amplitude of ±7,000 με and 1.9% at a cyclic strain amplitude of ±8,000 με. We also applied the sensor on an extruded magnesium alloy for evaluating the peculiar asymmetric hysteresis loops. The results obtained were in good agreement with those measured from the extensometer, a further validation of the sensor.
Effects of temperature on corrosion fatigue crack growth of pressure vessel steels in PWR coolant
International Nuclear Information System (INIS)
Tice, D.R.; Bramwell, I.L.; Fairbrother, H.; Worswick, D.
1994-01-01
This paper presents experimental results concerning crack propagation rates in A508-III pressure vessel steel (medium sulphur content) exposed to PWR primary water at temperatures between 130 and 290 C. The results indicate that the greatest increase in corrosion fatigue crack growth rate occurs at temperatures in the range 150 to 200 C. Under these conditions, there was a marked change in the appearance of the fracture surface, with extensive micro-branching of the crack front and occasional bifurcation of the whole crack path. In contrast, at 290 C, the fracture surface is smoother, similar to that due to inert fatigue. The implication of these observations for assessment of the pressure vessel integrity, is examined. 14 refs., 15 figs., 3 tabs
Fatigue crack growth of 316NG austenitic stainless steel welds at 325 °C
Li, Y. F.; Xiao, J.; Chen, Y.; Zhou, J.; Qiu, S. Y.; Xu, Q.
2018-02-01
316NG austenitic stainless steel is a commonly-used material for primary coolant pipes of pressurized water reactor systems. These pipes are usually joined together by automated narrow gap welding process. In this study, welds were prepared by narrow gap welding on 316NG austenitic stainless steel pipes, and its microstructure of the welds was characterized. Then, fatigue crack growth tests were conducted at 325 °C. Precipitates enriched with Mn and Si were found in the fusion zone. The fatigue crack path was out of plane and secondary cracks initiated from the precipitate/matrix interface. A moderate acceleration of crack growth was also observed at 325°Cair and water (DO = ∼10 ppb) with f = 2 Hz.
Lim, Hyung Jin; Sohn, Hoon; DeSimio, Martin P.; Brown, Kevin
2014-04-01
This study presents a reference-free fatigue crack detection technique using nonlinear ultrasonic modulation. When low frequency (LF) and high frequency (HF) inputs generated by two surface-mounted lead zirconate titanate (PZT) transducers are applied to a structure, the presence of a fatigue crack can provide a mechanism for nonlinear ultrasonic modulation and create spectral sidebands around the frequency of the HF signal. The crack-induced spectral sidebands are isolated using a combination of linear response subtraction (LRS), synchronous demodulation (SD) and continuous wavelet transform (CWT) filtering. Then, a sequential outlier analysis is performed on the extracted sidebands to identify the crack presence without referring any baseline data obtained from the intact condition of the structure. Finally, the robustness of the proposed technique is demonstrated using actual test data obtained from simple aluminum plate and complex aircraft fitting-lug specimens under varying temperature and loading variations.
International Nuclear Information System (INIS)
Wakai, T.; Horikiri, M.; Poussard, C.; Drubay, B.
2005-01-01
This paper presents the results of a benchmark on thermal fatigue crack growth evaluation for a thick-wall cylinder subjected to cyclic thermal transients. The simplified crack growth evaluation methods of both JNC in JAPAN and A16 procedures proposed by CEA in France are presented. The predictions obtained using both methods are compared with the experimental data. The JNC method, which accounts for the non-linear stress component provides predictions of crack advance in a good agreement with the experimental data. In contrast, significant differences are observed between the A16 predictions and the experimental data. The discrepancies are mainly due to the non-linear stress component which is not accounted for in the A16 method. When using the JNC stress intensity factor solution determined by finite element analysis to account for the non-linear stress component, the A16 method well predicts the thermal fatigue crack growth behavior
Fatigue crack growth of the MA12 magnesium alloy in vacuum and air
International Nuclear Information System (INIS)
Grinberg, N.M.; Serdyuk, V.A.; Zmeevets, S.G.; Ostapenko, I.Z.; Malinkina, T.I.; Kamyshkov, A.S.
1978-01-01
The growth of a crack and the failure mechanism have been examined in the specimens prepared from magnesium alloy sheets containing 2.9% Nd and 0.44% Zr,the specimens being subjected to the cyclic bending in the open air and in vacuum of 1x10 -6 mm Hg. Examination of the plastic zone around a crack was carried out by the methods of optical microscopy and X-ray structure analysis of fractures. It has been shown that when tested in vacuum, the growth rate of a fatigue crac in vacuum is essentially slower than being tested in the open air. The fatigue failure mechanism is the same in the open air and in vacuum; during the slow growing of a crack, that mechanism is essentially a brittle intragrain cleavage. The plastic zone forming around the crack is greater in vacuum than in the open air
International Nuclear Information System (INIS)
Rahimian, Mohammad.
1981-06-01
The aim of this work is to analyze, by numerical simulation the characteristics of the stresses and deformations at the bottom of cracks when plasticity is taken into account. This analysis is performed as from theoretical results laid down in the literature and makes it possible to understand the different solutions obtained from Hencky's deformation law or from the incremental theory. The role of plastic deformation is discussed in depth in the study of fatigue cracks. The problems linked to the fixed crack are studied in the first two chapters. The problems linked to the propagation of cracks are discussed in the following chapters. The fourth chapter is an application of the preceding results and knowledge to fatigue [fr
Fatigue crack growth prediction in 2xxx AA with friction stir weld HAZ properties
Directory of Open Access Journals (Sweden)
A. Tzamtzis
2016-02-01
Full Text Available An analytical model is developed to predict fatigue crack propagation rate under mode I loading in 2024 aluminum alloy with FSW HAZ material characteristics. Simulation of the HAZ local properties in parent 2024 AA was performed with overaging using specific heat treatment conditions. The model considers local cyclic hardening behavior in the HAZ to analyze crack growth. For the evaluation of the model, the analytical results have been compared with experimental fatigue crack growth on overaged 2024 alloy simulating material behavior at different positions within the HAZ. The analytical results showed that cyclic hardening at the crack tip can be used successfully with the model to predict FCG in a material at overaged condition associated with a location in the FSW HAZ.
Effects of pulse current stimulation on the thermal fatigue crack propagation behavior of CHWD steel
International Nuclear Information System (INIS)
Lin, H.Q.; Zhao, Y.G.; Gao, Z.M.; Han, L.G.
2008-01-01
The fatigue crack propagating behaviors of cast hot working die (CHWD) steel untreated and treated by an electric current in the intermediate stage of thermal fatigue were investigated in the present study. The circle/elliptical heating affected zone (HAZ) was formed ahead of the notch tip on the fatigued specimens after pulse electric current stimulation. Both SEM observation and X-ray diffraction analysis revealed that pulse electric current stimulation refined grains/subgrains in the HAZs. With the prolonging of discharging duration, the grains/subgrains decreased in size and the dislocation density and microhardness increased gradually. The grain refinement and dislocation density increase played an important role in the material strengthening, which inevitably enhanced the propagation resistance and delayed the propagation of thermal fatigue cracks. Therefore, the pulse electric current stimulation was an effective method to improve the service lifetime of die material
International Nuclear Information System (INIS)
Donati, J.R.; Keroulas, F.de; Masse, J.
1979-01-01
Two sodium mixers in the sodium heated steam generator test circuit at the EDF Renardieres centre developed leaks after approximately 7,000 hours operation under power. In both cases the investigation found cracking due to plastic fatigue caused by stresses of thermal origin. In one case the damage is explained solely by the size of the temperature oscillations; in the other case, unfavourable geometry reduced the duration of the initiation phase. Different types of cracking characteristic of thermal fatigue in sodium are presented. (author)
Fatigue crack propagation in neutron-irradiated ferritic pressure-vessel steels
International Nuclear Information System (INIS)
James, L.A.
1977-01-01
The results of a number of experiments dealing with fatigue crack propagation in irradiated reactor pressure-vessel steels are reviewed. The steels included ASTM alloys A302B, A533B, A508-2, and A543, as well as weldments in A543 steel. Fluences and irradiation conditions were generally typical of those experienced by most power reactors. In general, the effect of neutron irradiation on the fatigue crack propagation behavior of these steels was neither significantly beneficial nor significantly detrimental
The application of RBI-concept to ultrasonic measurement of fatigue cracks
Energy Technology Data Exchange (ETDEWEB)
Pitkaenen, J.; Saerkiniemi, P.; Kauppinen, P. [VTT Manufacturing Technology, Espoo (Finland)
1998-12-31
In many power plants there are problem areas, which are not included in the official inspection programs. Flaws can be induced during service due to the service conditions in components and welded joints. These can lead to failures, which cause unforeseen shutdowns during operation and unscheduled repairs have to be earned out. The basic idea of Risk Based Inspection (RBI) methodology is to include this kind of objects in the inspection program. In this presentation two possible objects for RBI are described - thermal fatigue cracking in process piping and fatigue cracking in spinning fly wheel. (orig.) 4 refs.
The application of RBI-concept to ultrasonic measurement of fatigue cracks
Energy Technology Data Exchange (ETDEWEB)
Pitkaenen, J; Saerkiniemi, P; Kauppinen, P [VTT Manufacturing Technology, Espoo (Finland)
1999-12-31
In many power plants there are problem areas, which are not included in the official inspection programs. Flaws can be induced during service due to the service conditions in components and welded joints. These can lead to failures, which cause unforeseen shutdowns during operation and unscheduled repairs have to be earned out. The basic idea of Risk Based Inspection (RBI) methodology is to include this kind of objects in the inspection program. In this presentation two possible objects for RBI are described - thermal fatigue cracking in process piping and fatigue cracking in spinning fly wheel. (orig.) 4 refs.
Ductile-phase toughening and fatigue crack growth in Nb3Al base alloys
International Nuclear Information System (INIS)
Gnanamoorthy, R.; Hanada, S.
1996-01-01
Niobium aluminide (Nb 3 Al) base intermetallic compounds exhibit good high-temperature strength and creep properties and potential for applications above 1,200 C provided their inadequately low room-temperature ductility, fracture toughness and fatigue crack growth behavior are improved. Addition of tantalum to Nb 3 Al base materials improves the high-temperature strength significantly and seems to be a potential alloying element. In the present study, room temperature fracture toughness and fatigue crack growth behavior of tantalum alloyed Nb 3 Al base alloy prepared by ingot metallurgy are investigated
Evaluation of fatigue crack growth and fracture resistance of SA350 LF2 material
International Nuclear Information System (INIS)
Singh, P.K.; Dubey, J.S.; Chakrabarty, J.K.; Vaze, K.K.; Kushwaha, H.S.
2003-01-01
The aim of the present paper is to evaluate the tensile and fracture mechanics properties of the SA350 LF2 carbon steel material used as the Header material in the primary heat transport (PHT) system piping of the Indian pressurized heavy water reactors (PHWR). Tensile, fatigue crack growth rate and fracture toughness tests have been carried out on specimens machined from the Header of the actual PHT pipes. The effect of temperature on tensile properties has been discussed. The effect of temperature and notch orientation on fracture resistance behavior of the material and fatigue crack growth rate dependence on the notch orientation and stress ratio has also been discussed. (author)
Fatigue crack initiation in hybrid boron/glass/aluminum fiber metal laminates
International Nuclear Information System (INIS)
Chang, P.-Y.; Yeh, P.-C.; Yang, J.-M.
2008-01-01
The fatigue crack initiation behavior of a high modulus and hybrid boron/glass/aluminum fiber/metal laminate (FML) was investigated experimentally and analytically. Two types of hybrid boron/glass/aluminum FMLs were fabricated and studied, which consisted of aluminum alloy sheets as the metal layers and a mixture of boron fibers and glass fibers as the composite layers. For the first type, the boron fiber/prepreg and the glass fiber/prepreg were used separately in the composite layers, and for the second type, the boron fibers and the glass fibers were mingled together to form a hybrid boron/glass/prepreg composite layer. These hybrid FMLs were consolidated using an autoclave curing process. The incorporation of the boron fibers improved the Young's modulus of the composite layer in FMLs, which in turn, would improve the fatigue crack initiation life of the Al sheet. The experimental results clearly showed that the fatigue crack initiation lives for both types of hybrid boron/glass/aluminum FMLs were superior to the monolithic aluminum alloy under the same loading condition. An analytical approach was proposed to calculate the fatigue crack initiation lives of hybrid boron/glass/aluminum FMLs based on the classical laminate theory and the small-crack theory. A good correlation was obtained between the predictions and the experimental results
International Nuclear Information System (INIS)
Jang, Changheui; Cho, Pyung-Yeon; Kim, Minu; Oh, Seung-Jin; Yang, Jun-Seog
2010-01-01
The effects of weld microstructure and residual stress distribution on the fatigue crack growth rate of stainless steel narrow gap welds were investigated. Stainless steel pipes were joined by the automated narrow gap welding process typical to nuclear piping systems. The weld fusion zone showed cellular-dendritic structures with ferrite islands in an austenitic matrix. Residual stress analysis showed large tensile stress in the inner-weld region and compressive stress in the middle of the weld. Tensile properties and the fatigue crack growth rate were measured along and across the weld thickness direction. Tensile tests showed higher strength in the weld fusion zone and the heat affected zone compared to the base metal. Within the weld fusion zone, strength was greater in the inner weld than outer weld region. Fatigue crack growth rates were several times greater in the inner weld than the outer weld region. The spatial variation of the mechanical properties is discussed in view of weld microstructure, especially dendrite orientation, and in view of the residual stress variation within the weld fusion zone. It is thought that the higher crack growth rate in the inner-weld region could be related to the large tensile residual stress despite the tortuous fatigue crack growth path.
Effect of heat treatment upon the fatigue-crack growth behavior of Alloy 718 weldments
International Nuclear Information System (INIS)
Mills, W.J.; James, L.A.
1981-05-01
The microstructural features that influenced the room and elevated temperature fatigue-crack growth behavior of as-welded, conventional heat-treated, and modified heat-treated Alloy 718 GTA weldments were studied. Electron fractographic examination of fatigue fracture surfaces revealed that operative fatigue mechanisms were dependent on microstructure, temperatures and stress intensity factor. All specimens exhibited three basic fracture surface appearances at temperatures up to 538 degrees C: crystallographic faceting at low stress intensity range (ΔK) levels, striation, formation at intermediate values, and dimples coupled with striations in the highest (ΔK) regime. At 649 degrees C, the heat-treated welds exhibited extensive intergranular cracking. Laves and δ particles in the conventional heat-treated material nucleated microvoids ahead of the advancing crack front and caused on overall acceleration in crack growth rates at intermediate and high ΔK levels. The modified heat treatment removed many of these particles from the weld zone, thereby improving its fatigue resistance. The dramatically improved fatigue properties exhibited by the as-welded material was attributed to compressive residual stresses introduced by the welding process. 19 refs., 16 figs
Short fatigue cracks growth and closure behavior in an austenitic stainless steel at 600 C and 650 C
International Nuclear Information System (INIS)
Polvora, J.P.; Laiarinandrasana, L.; Drubay, B.; Piques, R.; Martelet, B.
1995-01-01
In this work, following fatigue crack growth tests carried out at the CEN-SACLAY (AMORFIS program) by Laiarinandrasana (1994) on 316 L(N) CT specimens at 650 0 C and 600 0 C, short crack behavior of cracks emanating from machined notches is investigated. Experimental results are presented and discussions are directed to notch plasticity effect in relation with variations in crack opening stress intensity factor, K op , with crack lenght (author). 12 refs., 5 figs., 2 tab
Alam, Mohammad Shah
2005-11-01
Structural integrity is the science and technology of the margin between safety and disaster. Proper evaluation of the structural integrity and fatigue life of any structure (aircraft, ship, railways, bridges, gas and oil transmission pipelines, etc.) is important to ensure the public safety, environmental protection, and economical consideration. Catastrophic failure of any structure can be avoided if structural integrity is assessed and necessary precaution is taken appropriately. Structural integrity includes tasks in many areas, such as structural analysis, failure analysis, nondestructive testing, corrosion, fatigue and creep analysis, metallurgy and materials, fracture mechanics, fatigue life assessment, welding metallurgy, development of repairing technologies, structural monitoring and instrumentation etc. In this research fatigue life assessment of welded and weld-repaired joints is studied both in numerically and experimentally. A new approach for the simulation of fatigue crack growth in two elastic materials has been developed and specifically, the concept has been applied to butt-welded joint in a straight plate and in tubular joints. In the proposed method, the formation of new surface is represented by an interface element based on the interface potential energy. This method overcomes the limitation of crack growth at an artificial rate of one element length per cycle. In this method the crack propagates only when the applied load reaches the critical bonding strength. The predicted results compares well with experimental results. The Gas Metal Arc welding processes has been simulated to predict post-weld distortion, residual stresses and development of restraining forces in a butt-welded joint. The effect of welding defects and bi-axial interaction of a circular porosity and a solidification crack on fatigue crack propagation life of butt-welded joints has also been investigated. After a weld has been repaired, the specimen was tested in a universal
Effect of constraint on fatigue crack propagation near threshold in medium carbon steel
Czech Academy of Sciences Publication Activity Database
Hutař, Pavel; Seitl, Stanislav; Knésl, Zdeněk
2006-01-01
Roč. 37, 1-2 (2006), s. 51-57 ISSN 0927-0256 R&D Projects: GA ČR GA101/03/0331; GA ČR GP101/04/P001 Institutional research plan: CEZ:AV0Z20410507 Keywords : Fatigue crack propagation rate * Constraint * Two-parameter fracture mechanics Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.104, year: 2006
Surface profile evolution and fatigue crack initiation in Sanicro 25 steel at room temperature
Czech Academy of Sciences Publication Activity Database
Polák, Jaroslav; Petráš, Roman; Chai, G.; Škorík, Viktor
2016-01-01
Roč. 658, MAR (2016), s. 221-228 ISSN 0921-5093 R&D Projects: GA MŠk(CZ) ED1.1.00/02.0068; GA MŠk(CZ) EE2.3.30.0063; GA ČR(CZ) GA13-23652S Institutional support: RVO:68081723 Keywords : Sanicro 25 steel * Fatigue crack initiation * Persistent slip markings * Extrusions * Intrusions Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 3.094, year: 2016
AFM and SEM-FEG study on fundamental mechanisms leading to fatigue crack initiation
Czech Academy of Sciences Publication Activity Database
Man, Jiří; Valtr, M.; Petrenec, Martin; Dluhoš, J.; Kuběna, Ivo; Obrtlík, Karel; Polák, Jaroslav
2015-01-01
Roč. 76, JUL (2015), s. 11-18 ISSN 0142-1123 R&D Projects: GA ČR(CZ) GAP108/10/2371; GA MŠk(CZ) ED1.1.00/02.0068; GA ČR(CZ) GA13-23652S Institutional support: RVO:68081723 Keywords : fatigue crack initiation * 316L austenitic steel * atomic force microscopy * extrusion * intrusion Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 2.162, year: 2015
The shape of extrusions and intrusions and initiation of stage I fatigue cracks
Czech Academy of Sciences Publication Activity Database
Polák, Jaroslav; Man, Jiří; Vystavěl, T.; Petrenec, Martin
2009-01-01
Roč. 517, 1-2 (2009), s. 204-211 ISSN 0921-5093 R&D Projects: GA ČR GA106/06/1096; GA ČR GA101/07/1500 Institutional research plan: CEZ:AV0Z20410507 Keywords : Extrusion * Intrusion * Fatigue crack initiation * Stainless steel Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.901, year: 2009
Fatigue behaviour and crack growth of ferritic steel under environmental conditions
International Nuclear Information System (INIS)
Herter, K.H.; Schuler, X.; Weissenberg, T.
2012-01-01
The assessment of fatigue and cyclic crack growth behaviour of safety relevant components is of importance for the ageing management with regard to safety and reliability. For cyclic stress evaluation different codes and standards provide fatigue analysis procedures to be performed considering the various mechanical and thermal loading histories and geometric complexities of the components. For the fatigue design curves used as a limiting criteria the influence of different factors like e.g. environment, surface finish and temperature must be taken into consideration in an appropriate way. Fatigue tests were performed in the low cycle fatigue (LCF) und high cycle fatigue (HCF) regime with low alloy steels as well as with Nb- and Ti-stabilized German austenitic stainless steels in air and high temperature (HT) boiling water reactor environment to extend the state of knowledge of environmentally assisted fatigue (EAF) as it can occur in boiling water reactor (BWR) plants. Using the reactor pressure vessel (RPV) steel 22NiMoCr3-7 experimental data were developed to verify the influence of BWR coolant environment (high purity water as well as sulphate containing water with 90 ppb SO 4 at a test temperature of 240 C and an oxygen content of 400 ppb) on the fatigue life and to extend the basis for a reliable estimation of the remaining service life of reactor components. Corresponding experiments in air were performed to establish reference data to determine the environmental correction factor F en accounting for the environment. The experimental results are compared with international available mean data curves, the new design curves and on the basis of the environmental factor F en . Furthermore the behaviour of steel 22NiMoCr3-7 in oxygenated high temperature water under transient loading conditions was investigated with respect to crack initiation and cyclic crack growth. In this process the stress state of the specimen and the chemical composition of the high
Fatigue behaviour of fiberglass wind turbine blade material under variable amplitude loading
Energy Technology Data Exchange (ETDEWEB)
Delft, D R.V. Van; Winkel, G.D. de [Delft Univ. of Technology, STEVIN Lab., Delft (Netherlands); Joosse, P A [Stork Product Engineering b.v., Amsterdam (Netherlands)
1996-09-01
In the work presented here fatigue tests with the WISPER and WISPERX load sequence have been carried out and analysed. The test programme includes tests at low stress levels which results in fatigue lives of 50 millions of cycles. The results are compared with constant amplitude tests in the very high cycle range, carried out in a previous programme. The results are also compared with ECN results in the lower cycle range (on identical specimens). It appeared, that the difference between the fatigue life of the specimens tested with the WISPER and the WISPERX load sequence is larger than can be expected from the theoretical damage rates. Moreover, the slope of the S-N data differs from theoretical values obtained by using commonly applied design rules. (au)
Directory of Open Access Journals (Sweden)
Gourdin Stéphane
2014-01-01
Full Text Available Aircraft engine manufacturers have to demonstrate that handling surface anomalies in sensitive areas of discs are not critical for in-service life of a component. Currently, the models used consider anomalies as long cracks propagating from the first cycle, which introduces a certain degree of conservatism when calculating the fatigue life of surface flaws. Preliminary studies have shown that the first stages of crack propagation from surface anomalies are responsible for the conservative results. Thus, the aim of the study is to characterize the crack propagation from typical surface anomalies and to establish a new crack growth model, which can account for the micro-propagation stage. To separate the effects of the geometry of the anomalies and the residual stress state after introduction of the surface flaws, two V-type anomalies are studied: scratches and dents. Different studies have shown that the residual stresses beneath the anomalies seem to control the fatigue life of samples exhibiting scratches and dents. In order to monitor the crack micro-propagation, a direct current potential drop technique, coupled with heat tints is used during fatigue tests at elevated temperature. Thermal treatments releasing the residual stresses are also used to decouple the effect of crack morphology and residual stresses.
Comparison of fatigue crack initiation behavior in different microstructures of TC21 titanium alloy
Directory of Open Access Journals (Sweden)
Tan Changsheng
2018-01-01
Full Text Available Cyclic heterogeneous deformation, slip characteristics and crack nucleation with different microstructures, such as bimodal microstructure (BM and fine lamellar microstructure (FLM in TC21 alloy (Ti-6Al-2Sn-2Zr-3Mo-1Cr-2Nb-0.1Si, were systematically investigated and analyzed during high cycle fatigue at room temperature. The results demonstrated that the FLM microstructure possesses higher high-cycle fatigue strength than those of the BM one. For BM, the heterogeneous plastic deformation existed within the different large primary α phase, such as equiaxed primary α and primary α lath. The cracks at interfaces and slip bands easily coalesce with each other to form large cracks in BM. However, the α laths with similar morphology and size (nanosize distributed uniformly in FLM and could relatively deform homogeneously in micro-region, which delayed the initiation of the fatigue crack. Based on the electron-backscattered diffraction (EBSD analysis, it found that the strain was nonuniformly distributed in BM, however, it is relatively homogeneous in FLM. Moreover, lots of straight cracks are parallel and along single intrusions within the β grain which delays the coalescence of cracks.
Bray, G. H.; Reynolds, A. P.; Starke, E. A., Jr.
1992-01-01
In ingot metallurgy (IM) alloys, the number of delay cycles following a single tensile overload typically increases from a minimum at an intermediate baseline stress intensity range, Delta-K(B), with decreasing Delta-K(B) approaching threshold and increasing Delta-K(B) approaching unstable fracture to produce a characteristic 'U' shaped curve. Two models have been proposed to explain this behavior. One model is based on the interaction between roughness and plasticity-induced closure, while the other model only utilizes plasticity-induced closure. This article examines these models, using experimental results from constant amplitude and single overload fatigue tests performed on two powder metallurgy (PM) aluminum alloys, AL-905XL and AA 8009. The results indicate that the 'U'-shaped curve is primarily due to plasticity-induced closure, and that the plasticity-induced retardation effect is through-thickness in nature, occurring in both the surface and interior regions. However, the retardation effect is greater at the surface, because the increase in plastic strain at the crack tip and overload plastic zone size are larger in the plane-stress surface regions than in the plane-strain interior regions. These results are not entirely consistent with either of the proposed models.
Effect of helium on fatigue crack growth and life of reduced activation ferritic/martensitic steel
International Nuclear Information System (INIS)
Nogami, Shuhei; Takahashi, Manabu; Hasegawa, Akira; Yamazaki, Masanori
2013-01-01
The effects of helium on the fatigue life, micro-crack growth behavior up to final fatigue failure, and fracture mode under fatigue in the reduced activation ferritic/martensitic steel, F82H IEA-heat, were investigated by low cycle fatigue tests at room temperature in air at a total strain range of 0.6–1.5%. Significant reduction of the fatigue life due to helium implantation was observed for a total strain range of 1.0–1.5%, which might be attributable to an increase in the micro-crack propagation rate. However, the reduction of fatigue life due to helium implantation was not significant for a total strain range of 0.6–0.8%. A brittle fracture surface (an original point of micro-crack initiation) and a cleavage fracture surface were observed in the helium-implanted region of fracture surface. A striation pattern was observed in the non-implanted region. These fracture modes of the helium-implanted specimen were independent of the strain range
Fatigue crack growth behaviour of 21/4Cr1Mo steel tube at elevated temperature
International Nuclear Information System (INIS)
Bulloch, J.H.; Buchanan, L.W.
1987-01-01
The fatigue crack growth characteristics of 21/4Cr1Mo steel tube have been examined at 588 0 C over the frequency range 0.02-20 Hz and dwell time range 10-960 min. All tests were conducted under load control in laboratory air at an R-ratio of 0.5. The elevated temperature fatigue crack growth characteristics were adequately described in terms of the stress intensity range ΔKAPPA. The continuous cyclic test data exhibited a significant effect of frequency that agreed well with predicted effects using a simple mathematical model of the high temperature fatigue process. With the dwell time range of 10-100 min there was a significant dwell time effect on the critical ΔKAPPA level for creep-fatigue interactive growth. At dwell times > 100 min the dwell time effect saturates. When creep-fatigue interactive growth occurs, growth rates reside above the maximum for continuum-controlled fatigue crack growth, and exhibit a da/dN varies as ΔKAPPA 10 dependence; failure is then intergranular in nature. (author)
Directory of Open Access Journals (Sweden)
Tai-Cheng Chen
2018-03-01
Full Text Available Austenitic stainless steels are often considered candidate materials for use in hydrogen-containing environments because of their low hydrogen embrittlement susceptibility. In this study, the fatigue crack growth behavior of the solution-annealed and cold-rolled 301, 304L, and 310S austenitic stainless steels was characterized in 0.2 MPa gaseous hydrogen to evaluate the hydrogen-assisted fatigue crack growth and correlate the fatigue crack growth rates with the fracture feature or fracture surface roughness. Regardless of the testing conditions, higher fracture surface roughness could be obtained in a higher stress intensity factor (∆K range and for the counterpart cold-rolled specimen in hydrogen. The accelerated fatigue crack growth of 301 and 304L in hydrogen was accompanied by high fracture surface roughness and was associated with strain-induced martensitic transformation in the plastic zone ahead of the fatigue crack tip.
Fatigue crack growth due to overloads in plain concrete using ...
Indian Academy of Sciences (India)
cation of overload on concrete structures, acceleration in the crack growth process .... study by the same authors, Ray & Chandra Kishen (2010), they have employed the population growth ...... Institute of Technology, University of Trondheim.
Fatigue crack growth retardation in spot heated mild steel sheet
Indian Academy of Sciences (India)
Unknown
Department of Metallurgical Engineering, *Department of Applied Mechanics and Hydraulics, ... growth retardation increases with increasing level of overload as well as with ..... Suresh S 1996 Fatigue of materials (Cambridge: Cambridge.
Online fatigue crack growth monitoring with clip gauge and direct current potential drop
De Tender, Steven; Micone, Nahuel; De Waele, Wim
2016-01-01
Fatigue is a well-known failure phenomenon which has been and still is extensively studied. Often structures are designed according to the safe-life principle so no crack initiation occurs. Nowadays there is a high emphasis on cost-efficiency, and one might rather opt for a fail-safe design. Therefore a certain amount of crack growth can be allowed in structures, but then a good knowledge of stresses and related crack growth rates is needed. To this end, extensive studies are done to obtain a...
Small fatigue crack propagation in Y2O3 strengthened steels
Czech Academy of Sciences Publication Activity Database
Hutař, Pavel; Kuběna, Ivo; Ševčík, Martin; Šmíd, Miroslav; Kruml, Tomáš; Náhlík, Luboš
2014-01-01
Roč. 452, 1-3 (2014), s. 370-377 ISSN 0022-3115 R&D Projects: GA MŠk(CZ) EE2.3.30.0063; GA MŠk(CZ) ED1.1.00/02.0068; GA ČR(CZ) GP13-28685P Institutional support: RVO:68081723 Keywords : oxide dispersion strengthened steel * small fatigue crack * J-integral * fatigue life prediction Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.865, year: 2014
Fatigue crack growth behavior of a new single crystal nickel-based superalloy (CMSX-4) at 650 C
International Nuclear Information System (INIS)
Sengupta, A.; Putatunda, S.K.
1994-01-01
CMSX-4 is a recently developed rhenium containing single crystal nickel-based superalloy. This alloy has potential applications in many critical high-temperature applications such as turbine blades, rotors, nuclear reactors, etc. The fatigue crack growth rate and the fatigue threshold data of this material is extremely important for accurate life prediction, as well as failure safe design, at elevated temperatures. In this paper, the fatigue crack growth behavior of CMSX-4 has been studied at 650 C. The investigation also examined the influence of γ' precipitates (size and distribution) on the near-threshold fatigue crack growth rate and the fatigue threshold. The influence of load ratio on the fatigue crack growth rate and the fatigue threshold was also examined. Detailed fractographic studies were carried out to determine the crack growth mechanism in fatigue in the threshold region. Compact tension specimens were prepared from the single crystal nickel-based superalloy CMSX-4 with [001] orientation as the tensile loading axis direction. These specimens were given three different heat treatments to produce three different γ' precipitate sizes and distributions. Fatigue crack growth behavior of these specimens was studied at 650 C in air. The results of the present investigation indicate that the near-threshold fatigue crack growth rate decreases and that the fatigue threshold increases with an increase in the γ' precipitate size at 650 C. The fatigue threshold decreased linearly with an increase in load ratio. Fractographs at 650 C show a stage 2 type of crack growth along {100} type of crystal planes in the threshold region, and along {111} type of crystal planes in the high ΔK region
Investigations on creep and creep fatigue crack behaviour for component assessment
International Nuclear Information System (INIS)
Gengenbach, T.; Klenk, A.; Maile, K.
2004-01-01
There are various methods to assess crack initiation and crack growth behaviour of components under creep and creep fatigue loading. The programme system HT-Riss has been developed to support calculations aimed to determine the behaviour of a crack under creep or creep-fatigue loading using methods based on stress-intensity factor K (e.g. the Two-Criteria-Diagram) or C*-Integral. This paper describes the steps which have to be performed to assess crack initiation and growth of a component using this programme system. First the size of the maximum initial defect in a specimen or in a component has to be estimated and the necessary fracture mechanics parameters have to be determined. Then the time for creep crack initiation and creep crack growth is calculated. Using these values a prediction of life time and necessary inspection intervals is possible. For exemplification the crack assessment of a component-like specimen and a component is shown. (orig.)
Leak-before-break due to fatigue cracks in the cold leg piping system
International Nuclear Information System (INIS)
Mayfield, M.E.; Collier, R.P.
1984-01-01
This review paper presents the results of a deterministic assessment of the margin of safety against a large break in the cold leg piping system of pressurized water reactors. The paper focuses on the computation of leak rates resulting from fatigue cracks that penetrate the full wall thickness. Results are presented that illustrate the sensitivity of the leak rate to stress level, crack shape and crack orientation. Further, the leak rates for specific conditions are contrasted to detection levels, shutdown criteria, make-up capacity and the leak rate associated with final failure of the piping system. The results of these computations indicate that, in general, leaks far in excess of the present detection sensitivities would result at crack sizes well below the critical crack sizes for the upset loadings on the cold leg piping system
Crack growth retardation due to micro-roughness: a mechanism for overload effects in fatigue
International Nuclear Information System (INIS)
Suresh, S.
1982-01-01
A new mechanism for fatigue crack growth retardation following an overload is presented in this paper, based on a micro-roughness model. It is reasoned, with the aid of extensive experimental evidence available in the literature, that retardation following an overload is governed by the micromechanisms of near-threshold crack growth. This model is found to rationalize a number of hitherto unexplained experimental observations. Moreover, the present arguments, which suggest that plasticity-induced crack closure is not likely to be the primary mechanism for retardation following single overloads, do not exclude the role of residual stresses or blunting, but provide further mechanistic basis to account for the inconsistencies in the previous models. Additional sources of prolonged retardation, in terms of crack closure due to corrosion debris formed in moist environments, are suggested. It is pointed out that such environmental effects could play an important role in post-overload crack growth in certain alloy systems
Fractographic Observations on the Mechanism of Fatigue Crack Growth in Aluminium Alloys
Alderliesten, R. C.; Schijve, J.; Krkoska, M.
Special load histories are adopted to obtain information about the behavior of the moving crack tip during the increasing and decreasing part of a load cycle. It is associated with the crack opening and closure of the crack tip. Secondly, modern SEM techniques are applied for observations on the morphology of the fractures surfaces of a fatigue crack. Information about the cross section profiles of striations are obtained. Corresponding locations of the upper and the lower fracture surface are also explored in view of the crack extension mechanism. Most experiments are carried out on sheet specimens of aluminum alloys 2024-T3, but 7050-T7451 specimens are also tested in view of a different ductility of the two alloys.
A structural health monitoring fastener for tracking fatigue crack growth in bolted metallic joints
Rakow, Alexi Schroder
Fatigue cracks initiating at fastener hole locations in metallic components are among the most common form of airframe damage. The fastener hole site has been surveyed as the second leading initiation site for fatigue related accidents of fixed wing aircraft. Current methods for inspecting airframes for these cracks are manual, whereby inspectors rely on non-destructive inspection equipment or hand-held probes to scan over areas of a structure. Use of this equipment often demands disassembly of the vehicle to search appropriate hole locations for cracks, which elevates the complexity and cost of these maintenance inspections. Improved reliability, safety, and reduced cost of such maintenance can be realized by the permanent integration of sensors with a structure to detect this damage. Such an integrated system of sensors would form a structural health monitoring (SHM) system. In this study, an Additive, Interleaved, Multi-layer Electromagnetic (AIME) sensor was developed and integrated with the shank of a fastener to form a SHM Fastener, a new SHM technology targeted at detection of fastener hole cracks. The major advantages of the SHM Fastener are its installation, which does not require joint layer disassembly, its capability to detect inner layer cracks, and its capability to operate in a continuous autonomous mode. Two methods for fabricating the proposed SHM Fastener were studied. The first option consisted of a thin flexible printed circuit film that was bonded around a thin metallic sleeve placed around the fastener shank. The second option consisted of coating sensor materials directly to the shank of a part in an effort to increase the durability of the sensor under severe loading conditions. Both analytical and numerical models were developed to characterize the capability of the sensors and provide a design tool for the sensor layout. A diagnostic technique for crack growth monitoring was developed to complete the SHM system, which consists of the
Energy Technology Data Exchange (ETDEWEB)
Chongchong, Li [School of Materials Science and Engineering, Hebei University of Technology, Tianjin 300130 (China); National Key Lab for Remanufacturing, Academy of Armored Forces Engineering, Beijing 100072 (China); Lihong, Dong, E-mail: lihong.dong@126.com [National Key Lab for Remanufacturing, Academy of Armored Forces Engineering, Beijing 100072 (China); Haidou, Wang [National Key Lab for Remanufacturing, Academy of Armored Forces Engineering, Beijing 100072 (China); Guolu, Li [School of Materials Science and Engineering, Hebei University of Technology, Tianjin 300130 (China); Binshi, Xu [National Key Lab for Remanufacturing, Academy of Armored Forces Engineering, Beijing 100072 (China)
2016-05-01
Monitoring fatigue crack propagation behavior of ferromagnetic components is very important. In this paper, the tension–tension fatigue tests of center cracked tension (CCT) specimens were carried out; the variation regularity of both tangential and normal components of magnetic signals during fatigue process were investigated. The results showed that the initial abnormal signals which appeared at the notch were reversed after cyclic loading. The abnormal magnetic signals became more significant with the increase of fatigue cycles and reversed again after failure. The characteristic parameters, i.e., the peak value of tangential component, B{sub tp}, and maximum gradient value of normal component, K{sub m}, showed similar variation trends during the fatigue process, which can be divided into three different stages. An approximate linear relationship was found between the characteristic parameters and fatigue crack length 2a. The feasibility of predicting the fatigue crack propagation using the abnormal magnetic signals was discussed. What's more, the variation and distribution of the magnetic signals were also analyzed based on the theory of magnetic charge. - Highlights: • A novel and passive NDT method, i.e. MMMT method, is proposed. • Both tangential and normal components of magnetic signals were investigated. • The prediction of crack propagation by abnormal magnetic signals was discussed. • A linear relationship was found between the parameters and fatigue crack length 2a. • The parameters can be potentially used to evaluate the crack propagation state.
Effects of friction and high torque on fatigue crack propagation in Mode III
Nayeb-Hashemi, H.; McClintock, F. A.; Ritchie, R. O.
1982-12-01
Turbo-generator and automotive shafts are often subjected to complex histories of high torques. To provide a basis for fatigue life estimation in such components, a study of fatigue crack propagation in Mode III (anti-plane shear) for a mill-annealed AISI 4140 steel (RB88, 590 MN/m2 tensile strength) has been undertaken, using torsionally-loaded, circumferentially-notched cylindrical specimens. As demonstrated previously for higher strength AISI 4340 steel, Mode III cyclic crack growth rates (dc/dN) IIIcan be related to the alternating stress intensity factor ΔKIII for conditions of small-scale yielding. However, to describe crack propagation behavior over an extended range of crack growth rates (˜10-6 to 10-2 mm per cycle), where crack growth proceeds under elastic-plastic and full plastic conditions, no correlation between (dc/dN) III and ΔKIII is possible. Accordingly, a new parameter for torsional crack growth, termed the plastic strain intensity Γ III, is introduced and is shown to provide a unique description of Mode III crack growth behavior for a wide range of testing conditions, provided a mean load reduces friction, abrasion, and interlocking between mating fracture surfaces. The latter effect is found to be dependent upon the mode of applied loading (i.e., the presence of superimposed axial loads) and the crack length and torque level. Mechanistically, high-torque surfaces were transverse, macroscopically flat, and smeared. Lower torques showed additional axial cracks (longitudinal shear cracking) perpendicular to the main transverse surface. A micro-mechanical model for the main radi l Mode III growth, based on the premise that crack advance results from Mode II coalescence of microcracks initiated at inclusions ahead of the main crack front, is extended to high nominal stress levels, and predicts that Mode III fatigue crack propagation rates should be proportional to the range of plastic strain intensity (ΔΓIII if local Mode II growth rates are
A study on fatigue crack growth in dual phase martensitic steel in air
Indian Academy of Sciences (India)
Dual phase (DP) steel was intercritically annealed at different temperatures from fully martensitic state to achieve martensite plus ferrite, microstructures with martensite contents in the range of 32 to 76%. Fatigue crack growth (FCG) and fracture toughness tests were carried out as per ASTM standards E 647 and E 399, ...
Crack mode and life of Ti-6Al-4V under multiaxial low cycle fatigue
Directory of Open Access Journals (Sweden)
Takamoto Itoh
2015-10-01
Full Text Available This paper studies multiaxial low cycle fatigue crack mode and failure life of Ti-6Al-4V. Stress controlled fatigue tests were carried out using a hollow cylinder specimen under multiaxial loadings of λ=0, 0.4, 0.5 and 1 of which stress ratio R=0 at room temperature. λ is a principal stress ratio and is defined as λ=II/I, where I and II are principal stresses of which absolute values take the largest and middle ones, respectively. Here, the test at λ=0 is a uniaxial loading test and that at λ=1 an equi-biaxial loading test. A testing machine employed is a newly developed multiaxial fatigue testing machine which can apply push-pull and reversed torsion loadings with inner pressure onto the hollow cylinder specimen. Based on the obtained results, this study discusses evaluation of the biaxial low cycle fatigue life and crack mode. Failure life is reduced with increasing λ induced by cyclic ratcheting. The crack mode is affected by the surface condition of cut-machining and the failure life depends on the crack mode in the multiaxial loading largely.
Probabilistic evaluation of fatigue crack growth in SA 508 and SA 533 B steel
International Nuclear Information System (INIS)
Dufresne, J.; Rieunier, J.B.
1982-07-01
This paper describes the method used to select the best representative law of fatigue crack growth in view of its introduction in a probabilist computer code). A modelling of the selected law (Paris law) and the statistical distribution of the corresponding numerical coefficients are presented. Results of computation are given in the case of a PWR pressure vessel with defects in belt line weld
Small fatigue crack growth in aluminium alloy EN-AW 6082/T6
Czech Academy of Sciences Publication Activity Database
Jíša, D.; Liškutín, P.; Kruml, Tomáš; Polák, Jaroslav
2010-01-01
Roč. 32, č. 12 (2010), s. 1913-1920 ISSN 0142-1123 R&D Projects: GA ČR GA101/07/1500 Institutional research plan: CEZ:AV0Z20410507 Keywords : Aluminium alloys * small cracks * grack growth rate Subject RIV: JL - Materials Fatigue, Friction Mechanics Impact factor: 1.799, year: 2010
Effects of loading variables on fatigue-crack growth in liquid-metal environments
CSIR Research Space (South Africa)
Fernandes, PJL
1995-10-01
Full Text Available Liquid-metal-induced embrittlement (LMIE) refers to the loss of ductility in normally ductile metals and alloys when stressed while in contact with a liquid metal. In this study, the fatigue crack growth behaviour of brass in molten gallium...
Corrosion fatigue crack growth of pressure vessel welds in PWR environment
International Nuclear Information System (INIS)
Bamford, W.H.; Ceschini, L.J.; Moon, D.M.
1983-01-01
The fatigue crack growth rate behavior of several pressure vessel steel welds in PWR environment is discussed. The behavior is compared with associated heat-affected zone behavior, and with comparable base metal results. The welds show different degrees of susceptibility to the environmental influence, and this is discussed in some detail, along with fractographic observations on the tested specimens
Effects of friction and high torque on fatigue crack propagation in mode III
International Nuclear Information System (INIS)
Nayeb-Hashemi, H.; McClintock, F.A.; Ritchie, R.O.
1982-01-01
Turbo-generator and automotive shafts are often subjected to complex histories of high torques. To provide a basis for fatigue life estimation in such components, a study of fatigue crack propagation in Mode III (anti-plane shear) for a mill-annealed AISI 4140 steel (R /SUB B/ 88, 590 MN/m 2 tensile strength) has been undertaken, using torsionally-loaded, circumferentially-notched cylindrical specimens. As demonstrated previously for higher strength AISI 4340 steel, Mode III cyclic crack growth rates (dc/dN) /SUB III/ can be related to the alternating stress intensity factor ΔK /SUB III/ for conditions of small-scale yielding. However, to describe crack propagation behavior over an extended range of crack growth rates (about 10 -6 to 10 -2 mm per cycle), where crack growth proceeds under elastic-plastic and full plastic conditions, no correlation between (dc/dN) /SUB III/ and ΔK /SUB III/ is possible. Accordingly, a new parameter for torsional crack growth, termed the plastic strain intensity GAMMA /SUB III/, is introduced and is shown to provide a unique description of Mode III crack growth behavior for a wide range of testing conditions, provided a mean load reduces friction, abrasion, and interlocking between mating fracture surfaces A micro-mechanical model for the main radial Mode III growth is extended to high nominal stress levels, and predicts that Mode III fatigue crack propagation rates should be proportional to the range of plastic strain intensity (ΔGAMMA /SUB III/) if local Mode II growth rates are proportional to the displacements. Such predictions are shown to be in agreement with measured growth rates in AISI 4140 steel from 10 -6 to 10 -2 mm per cycle
Three-dimensional shape of the early stages of fatigue cracks nucleated in nodular cast iron
Energy Technology Data Exchange (ETDEWEB)
Verdu, C. [GEMPPM, UMR 5510, INSA de Lyon, 20 Avenue Albert Einstein, 69621 Villeurbanne Cedex (France)], E-mail: catherine.verdu@insa-lyon.fr; Adrien, J.; Buffiere, J.Y. [GEMPPM, UMR 5510, INSA de Lyon, 20 Avenue Albert Einstein, 69621 Villeurbanne Cedex (France)
2008-06-15
High resolution synchrotron X-ray tomography has been used to obtain three-dimensional (3D) images of the early stages of fatigue crack nucleation in a nodular cast iron. Microcracks were observed to initiate at casting defects (microshrinkage) and graphite nodules. The 3D observations have shown that the microcracks form in the material ligament comprised between the specimen surface and the defect. The probability of a defect to initiate a crack was correlated with the size of the defect and its position with respect to the surface. This correlation has been explained on the basis of local stress concentrations in the vicinity of the defect. The 3D observations of samples submitted to different fatigue cycles revealed that a large part of the fatigue life consisted in the progressive fracture of the ligament. The majority of the observed cracks stopped after this fracture process and, therefore, their size did not exceed the initiating defect size even if the crack seemed larger than the defect on the optical surface observations. Only few microcracks, nucleated on the largest defects, continued to grow with short-crack behaviour.
Nucleation and growth of fatigue cracks in magnesium alloys of different structure
International Nuclear Information System (INIS)
Grinberg, N.M.; Serdyuk, V.A.; Malinkina, T.I.; Kamyshkov, A.S.
1982-01-01
Duration of the fatigue crack nucleation and growth rate have been in a wide range of stress intensity factor variations for MA2-1, MA2-1 hp (higher purity), MA12, (T2, T6 and T8), MA15, IMB6, MA21 magnesium alloys of different composition and structural state. The threshold and criti- cal values of stress intensity factors, Ksub(th) and Ksub(fc) are determined for those alloys, and morphology of fracture is studied at different stages of crack growth. Duration of the nucleation stage of a fatigue crack, the rate and micromechanisms of its growth are found to depedend on alloying and structural state of magnesium alloys. The best crack resistance characteristics has the MA2-1 alloy, the poorest - MA12 (T2) alloy. It is stated that thermal treatment by hardening and ageing increases the resistance of the MA12 alloy to fatigue fracture and the MA2-1 alloy of higher purity gives poorer parameters of crack resistance [ru
International Nuclear Information System (INIS)
Arora, Punit; Singh, P.K.; Bhasin, Vivek; Vaze, K.K.; Pukazhendhi, D.M.; Gandhi, P.; Raghava, G.
2011-01-01
The objective of the present study is to understand the fatigue crack growth behavior in austenitic stainless steel and carbon steel pipes and pipe welds by carrying out analysis/predictions and experiments. The Paris law has been used for the prediction of fatigue crack growth life. To carry out the analysis, Paris constants have been determined for pipe (base) and pipe weld materials by using Compact Tension (CT)/Three Point Bend (TPB) specimens machined from the actual pipe/pipe weld. Analyses have been carried out to predict the fatigue crack growth life of pipes/pipe welds having part through cracks on the outer surface. In the analyses, Stress Intensity Factors (K) have been evaluated through two different schemes. The first scheme considers the 'K' evaluations at two points of the crack front i.e. maximum crack depth and crack tip at the outer surface. The second scheme accounts for the area averaged root mean square stress intensity factor (K RMS ) at deepest and surface points. In order to validate the analytical procedure/results, experiments have been carried out on full scale pipe and pipe welds with part through circumferential crack. Fatigue crack growth life evaluated using both schemes have been compared with experimental results. Use of stress intensity factor (K RMS ) evaluated using second scheme gives better fatigue crack growth life prediction compared to that of first scheme. (author)
Prediction of three-dimensional crack propagation paths taking high cycle fatigue into account
Directory of Open Access Journals (Sweden)
Guido Dhondt
2016-01-01
Full Text Available Engine components are usually subject to complex loading patterns such as mixed-mode Low Cycle Fatigue Loading due to maneuvering. In practice, this LCF Loading has to be superimposed by High Cyclic Fatigue Loading caused by vibrations. The changes brought along by HCF are twofold: first, the vibrational cycles which are superposed on the LCF mission increase the maximum loading of the mission and may alter the principal stress planes. Secondly, the HCF cycles themselves have to be evaluated on their own, assuring that no crack propagation occurs. Indeed, the vibrational frequency is usually so high that propagation leads to immediate failure. In the present paper it is explained how these two effects can be taken care of in a standard LCF crack propagation procedure. The method is illustrated by applying the Finite Element based crack propagation software CRACKTRACER3D on an engine blade.
Potential drop crack growth monitoring in high temperature biaxial fatigue tests
International Nuclear Information System (INIS)
Fitzgerald, B.P.; Krempl, E.
1993-01-01
The present work describes a procedure for monitoring crack growth in high temperature, biaxial, low cycle fatigue tests. The reversing DC potential drop equipment monitors smooth, tubular type 304 stainless steel specimens during fatigue testing. Electrical interference from an induction heater is filtered out by an analog filter and by using a long integration time. A Fourier smoothing algorithm and two spline interpolations process the large data set. The experimentally determined electrical potential drop is compared with the theoretical electrostatic potential that is found by solving Laplace's equation for an elliptical crack in a semi-infinite conducting medium. Since agreement between theory and experiment is good, the method can be used to measure crack growth to failure from the threshold of detectability
Testing machine for fatigue crack kinetic investigation in specimens under bending
International Nuclear Information System (INIS)
Panasyuk, V.V.; Ratych, L.V.; Dmytrakh, I.N.
1978-01-01
A kinematic diagram of testing mashine for the investigation of fatigue crack kinetics in prismatic specimens, subjected to pure bending is described. Suggested is a technique of choosing an optimum ratio of the parameters of ''the testing machine-specimen'' system, which provide the stabilization of the stress intensity coefficient for a certain region of crack development under hard loading. On the example of the 40KhS and 15Kh2MFA steel specimens the pliability of the machine constructed according to the described diagram and designed for the 30ONxm maximum bending moment. The results obtained can be used in designing of the testing machines for studying pure bending under hard loading and in choosing the sizes of specimens with rectangular cross sections for investigations into the kinetics of the fatigue crack
Fatigue crack tip damaging micromechanisms in a ferritic-pearlitic ductile cast iron
Directory of Open Access Journals (Sweden)
Francesco Iacoviello
2015-07-01
Full Text Available Due to the peculiar graphite elements shape, obtained by means of a chemical composition control (mainly small addition of elements like Mg, Ca or Ce, Ductile Cast Irons (DCIs are able to offer the good castability of gray irons with the high mechanical properties of irons (first of all, toughness. This interesting properties combination can be improved both by means of the chemical composition control and by means of different heat treatments(e.g. annealing, normalizing, quenching, austempering etc. In this work, fatigue crack tip damaging micromechanisms in a ferritic-pearlitic DCI were investigated by means of scanning electron microscope observations performed on a lateral surface of Compact Type (CT specimens during the fatigue crack propagation test (step by step procedure, performed according to the “load shedding procedure”. On the basis of the experimental results, different fatigue damaging micromechanisms were identified, both in the graphite nodules and in the ferritic – pearlitic matrix.
Crack growth and fracture in fiber reinforced concrete beams under static and fatigue loading
International Nuclear Information System (INIS)
Jeanfreau, J.; Arockiasamy, M.; Reddy, D.V.
1987-01-01
The paper presents the results of a two-phase experimental investigation on the fatigue and fracture of six different types of concrete: plain, 0.5%, 1.0%, 1.5%, and 2.0% steel fibers and 0.5% kevlar fibers. In the first phase the J-integral was evaluated for different types of concrete from load-displacement curves. The value shows a marked increase in the energy required to fracture concrete when fibers are added. The values did not vary substantially for different notch depths. In the second phase concrete beams were subjected to fatigue by applying a pure bending on the notch. The effect of fiber addition was examined with emphasis on the crack propagation and the increase in the fatigue strength. The crack pattern was mainly influenced by the presence, amount, and the distribution of the fibers in the concrete. (orig./HP)
Evaluation of fatigue cracks in FSW joints of industrial structural materials by laminography
International Nuclear Information System (INIS)
Sano, Yuji; Masaki, Kiyotaka; Kajiwara, Kentaro
2016-01-01
Friction stir welding (FSW) is an emerging technology for joining flat and thin metal materials and has been applied in manufacturing in aviation and automotive industries. Fatigue property is one of the most important items to be evaluated for the structural integrity of the products, and therefore, it is necessary to visualize the three-dimensional (3D) behavior of fatigue cracks propagating in the non-homogeneous and anisotropic stirred zone of FSW joints. We have applied laminography with synchrotron radiation of SPring-8 to the FSW joints of aluminum alloy as a typical structural material. The results showed that the fatigue cracks propagated in a unique way depending on the stirred material. (author)
Effect of Variable Amplitude Blocks' Ordering on the Functional Fatigue of Superelastic NiTi Wires
Soul, Hugo; Yawny, Alejandro
2017-12-01
Accumulation of superelastic cycles in NiTi uniaxial element generates changes on the stress-strain response. Basically, there is an uneven drop of martensitic transformation stress plateaus and an increase of residual strain. This evolution associated with deterioration of superelastic characteristics is referred to as "functional fatigue" and occurs due to irreversible microstructural changes taking place each time a material domain transforms. Unlike complete cycles, for which straining is continued up to elastic loading of martensite, partial cycles result in a differentiated evolution of those material portions affected by the transformation. It is then expected that the global stress-strain response would reflect the previous cycling history of the specimen. In the present work, the consequences of cycling of NiTi wires using blocks of different strain amplitudes interspersed in different sequences are analyzed. The effect of successive increasing, successive decreasing, and interleaved strain amplitudes on the evolution of the superelastic response is characterized. The feasibility of postulating a functional fatigue criterion similar to the Miner's cumulative damage law used in structural fatigue analysis is discussed. The relation of the observed stress-strain response with the transformational history of the specimen can be rationalized by considering that the stress-induced transformation proceeds via localized propagating fronts.
Energy Technology Data Exchange (ETDEWEB)
Alexandre, F
2004-03-15
Thermomechanical treatments have been recently developed to produce Inconel 718DA (Direct Aged). This alloy optimisation leads to an increase of the fatigue life but also the scatter. The aim of this study is on the one hand the understanding of the fatigue crack initiation mechanisms and on the other hand the modelling of the fatigue life and the scatter. An experimental study showed that the fatigue cracks were initiated from carbide particles in fine grain alloy. Interrupted tensile tests show that the particles cracking occurred at the first quarter of the fatigue cycle. Fatigue behaviour tests were also performed on various grain size 718 alloys. The last experimental part was devoted to measurements of the low cycle fatigue crack growth rates using a high focal distance microscope. For these tests, EDM micro-defects were used for the fatigue crack initiation sites. This method was also used to observe the small fatigue crack coalescence. A fatigue life model is proposed. It is based on the three fatigue crack initiation mechanisms competition: particle crack initiation on the surface, internal particle crack initiation and Stade I crack initiation. The particle fatigue crack initiation is supposed instantaneous at a critical stress level. The Tanaka and Mura model is used for analysing the Stage I crack initiation number of cycles. The fatigue crack growth rate was analysed using the Tomkins model identified on the small fatigue crack growth rate measurements. The proposed fatigue life model decomposed in three levels: a deterministic one and two probabilistic with and without crack coalescence. (author)
Biaxial fatigue of metals the present understanding
Schijve, Jaap
2016-01-01
Problems of fatigue under multiaxial fatigue loads have been addressed in a very large number of research publications. The present publication is primarily a survey of biaxial fatigue under constant amplitude loading on metal specimens. It starts with the physical understanding of the fatigue phenomenon under biaxial fatigue loads. Various types of proportional and non-proportional biaxial fatigue loads and biaxial stress distributions in a material are specified. Attention is paid to the fatigue limit, crack nucleation, initial micro crack growth and subsequent macro-crack in different modes of crack growth. The interference between the upper and lower surfaces of a fatigue crack is discussed. Possibilities for predictions of biaxial fatigue properties are analysed with reference to the similarity concept. The significance of the present understanding for structural design problems is considered. The book is completed with a summary of major observations.
Low temperature fatigue crack propagation in neutron irradiated Type 316 steel and weld metal
International Nuclear Information System (INIS)
Lloyd, G.J.; Walls, J.D.; Gravenor, J.
1981-02-01
The fast cycling fatigue crack propagation characteristics of Type 316 steel and weld metal have been investigated at 380 0 C after irradiation to 1.72-1.92x10 20 n/cm 2 (E>1MeV) and 2.03x10 21 n/cm 2 (E>1MeV) at the same temperature. With mill-annealed Type 316 steel, modest decreases in the rates of crack propagation were observed for both dose levels considered, whereas for cold-worked Type 316 steel irradiation to 2.03x10 21 n/cm 2 (E>1MeV) caused increases in the rate of crack propagation. For Type 316 weld metal, increases in the rate of crack propagation were observed for both dose levels considered. The diverse influences of irradiation upon fatigue crack propagation in these materials are explained by considering a simple continuum mechanics model of crack propagation together with the results of control tensile experiments made on similarly irradiated materials. (author)
Notch fatigue crack propagation - A consistent concept for calculating flawed service life
International Nuclear Information System (INIS)
Dankert, M.
1999-01-01
The research report presents a consistent concept of elastic-plastic fatigue fracture mechanics, to be used for numerical description of crack initiation and propagation behaviour within and out of notched areas of circular notched specimens for Woehler tests, two-phase fatigue tests and tests under service conditions. It is shown that a fracture-mechanics approach yields results capable of describing the load history over the whole service life of a structural member. A J-integral-related crack propagation model is derived that takes into account the crack opening and closure behaviour. The model is based on specially developed formulas, algorithms and approximation formulas required for description of crack opening and closure behaviour as well as calculation of the stress intensity factor K and the J-integral of cracks at notches. The values relating to crack opening were compared with experimental data, and those describing the stress intensity factor K and the J-integrals with 2D and 3D elastic-plastic FE calculations. Good and very good agreement of results was achieved. (orig./CB) [de
International Nuclear Information System (INIS)
Shalaby, H.M.; Begley, J.A.; Macdonald, D.D.
1989-01-01
The morphology of fatigue crack nucleation has been studied in 12%Cr stainless steel at a single stress level of 448 MN m -2 in deaerated H 2 SO 4 -Na 2 SO 4 -NaOH ([SO 4 2- ] = 0.01M and 1M) and in H 3 PO 4 -NaOH ([PO 4 3- ] = 0.01M and 1M) solutions at pH 2, 7 and 10 at 100 0 C. In sulphate solutions at pH 2, the specimen suffered overall surface attack without the initiation of microcracks. The surface attack intensified at the prior austenite grain boundaries, martensite platelet boundaries, and non-metallic inclusions. In contrast, cracks initiated transgranularly in sulphate solutions at pH 7 and 10 with the development of selective attack at crack sites at later stages in the fatigue life. This attack was ascribed to local acidification as a result of hydrolysis of corrosion products extruded from inside the cracks. Long cracks with crack branching and debonded zones were observed in all phosphate solutions, except in 0.01M phosphate solution at pH 7. In this latter environment, short intrusion-extrusion microcracks were observed. This difference in behaviour was attributed to changes in the characteristics of the passive film as influenced by the local environmental conditions, mechanical rupture by plastic deformation, and electrochemical differences at the metal surface. (author)
Fatigue of graphite/epoxy buffer strip panels with center cracks
Bigelow, C. A.
1985-01-01
The effects of fatigue loading on the behavior of graphite/epoxy panels with either S-Glass or Kevlar-49 buffer strips is studied. Buffer strip panels are fatigued and tested in tension to measure their residual strength with crack-like damage. Panels are made with 45/0/-45/90 sub 2s layup with either S-Glass or Kevlar-49 buffer strip material. The buffer strips are parallel to the loading direction and made by replacing narrow strips of the 0-degree graphite plies with strips of either 0-degree S-Glass/epoxy or Kevlar-49/epoxy on a one-for-one basis. The panels are subjected to a fatigue loading spectrum MINITWIST, the shortened version of the standardized load program for the wing lower surface of a transport aircraft. Two levels of maximum strain are used in the spectrum with three durations of the fatigue spectrum. One group of panels is preloaded prior to the application of the fatigue cycling. The preload consists of statistically loading the spectrum in tension until the crack-tip damage zone reaches the ajacent buffer strips. After fatigue loading, all specimens are statistically loaded in tension to failure to determine their residual strengths.
International Nuclear Information System (INIS)
Zhang, X.Q.; Li, H.; Yu, X.L.; Zhou, Y.; Duan, S.W.; Li, S.Z.; Huang, Z.L.; Zuo, L.S.
2015-01-01
Highlights: • LSP can greatly delay crack formation. • The micro-crack growing processes and its fracture are showed clearly. • Surface topographies and crack initiation locations are displayed. - Abstract: A series of contrasting experiments were carried out to examine the effects of laser shock processing (LSP) on fatigue properties of slot in 7075-T6 aluminum alloy plate. Both side surfaces of slot were subjected to LSP. The surface topographies were observed and the residual stresses were tested. The treated and the un-treated specimens were pulled by the fatigue cyclic loading respectively. The fatigue crack propagating processes were recorded, and the fatigue fracture microscopic morphologies were analyzed by scanning electron microscope (SEM). Experimental results and analyses show that LSP induces micro-dent on surface and squeezes the compressive residual stresses into surface layer of specimen. It can remarkably delay the micro-crack formation, and transfer the location of fatigue crack initiation from top surface to sub-surface. The spacing of fatigue striations on the treated specimen fatigue fracture obviously decreases. Therefore, the fatigue life of specimen after LSP treatment significantly increases
International Nuclear Information System (INIS)
Taheri, S.; Vincent, L.; Le-Roux, J.C.
2013-01-01
The application of Miner's rule using a loading issued from a mock-up of a RHR system (removal heat system) of PWR plant, made of 304 steel gives a very important non-conservative fatigue life in strain control when strain fatigue curve is used. This result is due to the absence of sequence effect in Miner's rule. Many non linear damage accumulation models have been proposed to get a sequence effect. Shortcomings of some non linear damage accumulation models are discussed. So Smith-Watson-Topper and Fatemi-Socie criterions with a linear damage accumulation rule are then applied to experimental data. A major issue is the need for an elastic-plastic constitutive law which is difficult to propose in the presence of high cycle secondary hardening observed in austenitic stainless steels. A conservative model for fatigue damage accumulation under variable amplitude loading is then proposed for austenitic stainless steels in strain control, which does not need a constitutive law, but takes into account plasticity through cyclic strain stress curve. The model uses a linear damage accumulation rule. This model is based on the fact that for stainless steels, pre-hardening is detrimental for fatigue life in strain control, while it is beneficial in stress control. In the presence of low mean stress, the model is approved based on a large number of tests. Moreover the model allows to explain the larger detrimental effect of a tension mean stress in strain control tests than in stress control tests. (authors)
Influence of overloads on dwell time fatigue crack growth in Inconel 718
Energy Technology Data Exchange (ETDEWEB)
Saarimäki, Jonas, E-mail: jonas.saarimaki@liu.se [Division of Engineering Materials, Department of Management and Engineering, Linköping University, SE-58183 Linköping (Sweden); Moverare, Johan [Division of Engineering Materials, Department of Management and Engineering, Linköping University, SE-58183 Linköping (Sweden); Siemens Industrial Turbomachinery AB, Materials Technology, SE-61283 Finspång (Sweden); Eriksson, Robert; Johansson, Sten [Division of Engineering Materials, Department of Management and Engineering, Linköping University, SE-58183 Linköping (Sweden)
2014-08-26
Inconel 718 is one of the most commonly used superalloys for high temperature applications in gasturbines and aeroengines and is for example used for components such as turbine discs. Turbine discs can be subjected to temperatures up to ∼700 °C towards the outer radius of the disc. During service, the discs might start to develop cracks due to fatigue and long dwell times. Additionally, temperature variations during use can lead to large thermal transients during start-up and shutdown which can lead to overload peaks in the normal dwell time cycle. In this study, tests at 550 °C with an overload prior to the start of each dwell time, have been performed. The aim of the investigation was to get a better understanding of the effects of overloads on the microstructure and crack mechanisms. The microstructure was studied using electron channelling contrast imaging (ECCI). The image analysis toolbox in Matlab was used on cross sections of the cracks to quantify: crack length, branch length, and the number of branches in each crack. It was found that the amount of crack branching increases with an increasing overload and that the branch length decreases with an increasing overload. When the higher overloads were applied, the dwell time effect was almost cancelled out. There is a strong tendency for an increased roughness of the crack path with an increasing crack growth rate.
Influence of overloads on dwell time fatigue crack growth in Inconel 718
International Nuclear Information System (INIS)
Saarimäki, Jonas; Moverare, Johan; Eriksson, Robert; Johansson, Sten
2014-01-01
Inconel 718 is one of the most commonly used superalloys for high temperature applications in gasturbines and aeroengines and is for example used for components such as turbine discs. Turbine discs can be subjected to temperatures up to ∼700 °C towards the outer radius of the disc. During service, the discs might start to develop cracks due to fatigue and long dwell times. Additionally, temperature variations during use can lead to large thermal transients during start-up and shutdown which can lead to overload peaks in the normal dwell time cycle. In this study, tests at 550 °C with an overload prior to the start of each dwell time, have been performed. The aim of the investigation was to get a better understanding of the effects of overloads on the microstructure and crack mechanisms. The microstructure was studied using electron channelling contrast imaging (ECCI). The image analysis toolbox in Matlab was used on cross sections of the cracks to quantify: crack length, branch length, and the number of branches in each crack. It was found that the amount of crack branching increases with an increasing overload and that the branch length decreases with an increasing overload. When the higher overloads were applied, the dwell time effect was almost cancelled out. There is a strong tendency for an increased roughness of the crack path with an increasing crack growth rate
Directory of Open Access Journals (Sweden)
Sun Qiaoyan
2018-01-01
Full Text Available Alpha phase exhibits equiaxed or lamellar morphologies with size from submicron to microns in an alpha-beta titanium alloy. Cyclic deformation, slip characteristics and crack nucleation during fatigue in different microstructures of TC21 alloy (Ti-6Al-2Sn-2Zr-3Mo-1Cr-2Nb-0.1Si were systematically investigated and analyzed. During low-cycle fatigue, equiaxed microstructure (EM in TC21 alloy exhibits higher strength, ductility and longer low-cycle fatigue life than those of the lamellar microstructure (LM. There are more voids in the single lamellar alpha than the equiaxed alpha grains. As a result, voids more easily link up to form crack in the lamellar alpha phase than the equiaxed alpha phase. However, during high-cycle fatigue, the fine lamellar microstructure (FLM shows higher fatigue limit than bimodal microstructure (BM. The localized plastic deformation can be induced during high-cycle fatigue. The slip bands or twins are observed in the equiaxed and lamellar alpha phases(>1micron, which tends to form strain concentration and initiate fatigue crack. The localized slip within nanoscale alpha plates is seldom observed and extrusion/intrusion dispersedly distributed on the sample surface in FLM. This indicates that FLM show super resistance to fatigue crack which bring about higher fatigue limit than BM.
Influence of fatigue crack wake length and state of stress on crack closure
Telesman, Jack; Fisher, Douglas M.
1988-01-01
The location of crack closure with respect to crack wake and specimen thickness under different loading conditions was determined. The rate of increase of K sub CL in the crack wake was found to be significantly higher for plasticity induced closure in comparison to roughness induced closure. Roughness induced closure was uniform throughout the thickness of the specimen while plasticity induced closure levels were 50 percent higher in the near surface region than in the midthickness. The influence of state of stress on low-high load interaction effects was also examined. Load interaction effects differed depending upon the state of stress and were explained in terms of delta K sub eff.
A Review of Spectral Methods for Variable Amplitude Fatigue Prediction and New Results
Larsen, Curtis E.; Irvine, Tom
2013-01-01
A comprehensive review of the available methods for estimating fatigue damage from variable amplitude loading is presented. The dependence of fatigue damage accumulation on power spectral density (psd) is investigated for random processes relevant to real structures such as in offshore or aerospace applications. Beginning with the Rayleigh (or narrow band) approximation, attempts at improved approximations or corrections to the Rayleigh approximation are examined by comparison to rainflow analysis of time histories simulated from psd functions representative of simple theoretical and real world applications. Spectral methods investigated include corrections by Wirsching and Light, Ortiz and Chen, the Dirlik formula, and the Single-Moment method, among other more recent proposed methods. Good agreement is obtained between the spectral methods and the time-domain rainflow identification for most cases, with some limitations. Guidelines are given for using the several spectral methods to increase confidence in the damage estimate.
Energy Technology Data Exchange (ETDEWEB)
Wu, Huan Chun; Yang, Bin [State Key Laboratory for Advanced Metals and Materials, University of Science and Technology Beijing, Beijing (China); Chen, Yue Feng; Chen, Xu Dong [Collaborative Innovation Center of Steel Technology, Beijing (China)
2017-06-15
The fatigue crack propagation behaviors of Z3CN20.09M duplex stainless steel (DSS) were investigated by studying oxide films of specimens tested in 290°C water and air. The results indicate that a full oxide film that consisted of oxides and hydroxides was formed in 290°C water. By contrast, only a half-baked oxide film consisting of oxides was formed in 290°C air. Both environments are able to deteriorate the elastic modulus and hardness of the oxide films, especially the 290°C water. The fatigue lives of the specimens tested in 290°C air were about twice of those tested in 290°C water at all strain amplitudes. Moreover, the crack propagation rates of the specimen tested in 290°C water were confirmed to be faster than those tested in 290°C air, which was thought to be due to the deteriorative strength of the oxide films induced by the mutual promotion of oxidation and crack propagation at the crack tip. It is noteworthy that the crack propagation can be postponed by the ferrite phase in the DSS, especially when the specimens were tested in 290°C water.
2011-09-01
detection of a fatigue crack via 3D LDV measurements, both in aluminum plates. All the referenced LDV/guided wave studies made use of PZT or similar...Figure 1a). (b) (a) (c) Figure 1: (a) Test specimen in MTS fatigue test machine, (b) hole with 5 mm crack, (c) PZT placement with...mm thick aluminum plates with a small (1.59 mm) center hole added to facilitate growth of a fatigue crack. One plate was left undamaged while the
The role of crack tip opening in corrosion fatigue for the ductile ferritic steel-water system
International Nuclear Information System (INIS)
Tomkins, B.
1977-01-01
Water vapour or a water environment can dramatically reduce the fatigue strength of structural alloys, including aluminium and steel, and this reduction can be often related to the effect of the environment on crack initiation. More recently, however, under certain circumstances, it has become clear that fatigue crack growth rates can also be increased. A limited examination of crack tip openings in ductile steels under corrosion fatigue conditions, indicates that it may be possible to develop more physically based design rules for components which operate in some aqueous environments (author)
Fatigue crack propagation: Probabilistic models and experimental evidence
International Nuclear Information System (INIS)
Lucia, A.C.; Jovanovic, A.
1987-01-01
The central aim of the LWR Primary Circuit Component Life Prediction Project, going on at JRC-Ispra, is to develop and check a 'procedure' (encompassing monitoring and inspection, data collection and analysis, prediction) allowing the quantitatives estimation of the accumulation of structural damage and of the residual lifetime. The ongoing activity matches theoretical development and experimentation, the latter being at present essentially based on a test-rig for room-temperature fatigue cycling of 1:5 scaled models of pressure vessels. During Phase I of fatigue testing of vessel R2, different pieces of information coming from material characterization, non-destructive inspection, continuous monitoring, stress analysis, have been merged and used to infere the future behaviour of the structure. The prediction of residual lifetime (cycles to failure), based on the outcomes of the ultrasonic continuous monitoring and made by means of the COVASTOL code, was in quite good agreement with experimental evidence. (orig./HP)
Parametric calculations of fatigue-crack growth in piping
International Nuclear Information System (INIS)
Simonen, F.A.; Goodrich, C.W.
1983-06-01
This study presents calculations of the growth of piping flaws produced by fatigue. Flaw growth was predicted as a function of the initial flaw size, the level and number of stress cycles, the piping material, and environmental factors. The results indicate that the present flaw acceptance standards of ASME Section XI provide a relatively consistent set of allowable flaw sizes because the predicted life of flawed piping is relatively insensitive to pipe wall thickness, flaw aspect ratio, and piping material (ferritic versus austenitic). On the other hand, the results show that flaws that are acceptable under ASME Section XI can grow at unacceptable rates if the cyclic stresses are at the maximum level permitted by the design rules of ASME Section III. However, a review of the conservatisms inherent to the ASME code rules is presented to explain the low occurrence of piping fatigue failures in service. It is concluded that decreases in the allowable flaw sizes are not justified
Effect of heat treatment upon the fatigue-crack growth behavior of Alloy 718 weldments
International Nuclear Information System (INIS)
James, L.A.; Mills, W.J.
1981-05-01
Gas-tungsten-arc weldments in Alloy 718 were studied in fatigue-crack growth test conducted at five temperatures over the range 24--649 degree C. In general, crack growth rates increased with increasing temperature, and weldments given the ''conventional'' post-weld heat-treatment generally exhibited crack growth rates that were higher than for weldments given the ''modified'' (INEL) heat-treatment. Limited testing in the as-welded condition revealed crack growth rates significantly lower than observed for the heat-treated cases, and this was attributed to residual stresses. Three different heats of filler wire were utilized, and no heat-to-heat variations were noted. 23 refs., 9 figs., 6 tabs
Effect of defect length on rolling contact fatigue crack propagation in high strength steel
Directory of Open Access Journals (Sweden)
T. Makino
2015-10-01
Full Text Available The objective of the present paper is to clarify the effect of defect length in depth direction on rolling contact fatigue (RCF crack propagation in high strength steel. RCF test and synchrotron radiation micro computed tomography (SR micro CT imaging were conducted. In the case of the defect with the 15 m diameter, flaking life decreased with increasing defect length. In a comparison of the CT image and the SEM view, the shapes of defects and the locations of the horizontal cracks were almost the same respectively. The mechanism of RCF crack propagation was discussed by finite element (FE analysis. Defects led to higher tensile residual stress than that without defects in the region where the defect exists. The shear stress range at 0.1 mm in depth on the middle line of the defect and the range of mode II stress intensity factor at the bottom of a vertical crack increased with increasing defect length.
Accelerated Threshold Fatigue Crack Growth Effect-Powder Metallurgy Aluminum Alloy
Piascik, R. S.; Newman, J. A.
2002-01-01
Fatigue crack growth (FCG) research conducted in the near threshold regime has identified a room temperature creep crack growth damage mechanism for a fine grain powder metallurgy (PM) aluminum alloy (8009). At very low (Delta) K, an abrupt acceleration in room temperature FCG rate occurs at high stress ratio (R = K(sub min)/K(sub max)). The near threshold accelerated FCG rates are exacerbated by increased levels of K(sub max) (K(sub max) = 0.4 K(sub IC)). Detailed fractographic analysis correlates accelerated FCG with the formation of crack-tip process zone micro-void damage. Experimental results show that the near threshold and K(sub max) influenced accelerated crack growth is time and temperature dependent.
Fatigue crack growth in ferritic steels as influence by elevated temperature and environment
International Nuclear Information System (INIS)
Nakamura, H.; Minakawa, K.; Murali, K.; Mc Evily, A.J.
1987-01-01
Fatigue crack growth studies have been carried out at room temperature and at 538 deg C in air as well as in vacuum in order to assess the influence of both temperature and environment on the growth process. The materials investigated were 2 1/4Cr-1Mo steel, a modified 9Cr-1Mo steel and a 9Cr-2Mo steel, as well as weldments of the 9Cr-2Mo steel. Crack opening levels were determined for all test conditions. The R-dependency of the crack growth rate could be accounted for by crack closure, both at room and elevated temperature. Closure in air at 538 deg C was due to oxidation, whereas at room temperature closure was due to microstructurally related roughness and the influence of oxygen. (Author)
Mesh sensitivity effects on fatigue crack growth by crack-tip blunting and re-sharpening
DEFF Research Database (Denmark)
Tvergaard, Viggo
2007-01-01
remeshing at several stages of the plastic deformation, with studies of the effect of overloads or compressive underloads. Recent published analyses for the first two cycles have shown folding of the crack surface in compression, leading to something that looks like striations. The influence of mesh...... refinement is used to study the possibility of this type of behaviour within the present method. Even with much refined meshes no indication of crack surface folding is found here....
Rohman, Muhamad Nur; Hidayat, Mas Irfan P.; Purniawan, Agung
2018-04-01
Neural networks (NN) have been widely used in application of fatigue life prediction. In the use of fatigue life prediction for polymeric-base composite, development of NN model is necessary with respect to the limited fatigue data and applicable to be used to predict the fatigue life under varying stress amplitudes in the different stress ratios. In the present paper, Multilayer-Perceptrons (MLP) model of neural network is developed, and Genetic Algorithm was employed to optimize the respective weights of NN for prediction of polymeric-base composite materials under variable amplitude loading. From the simulation result obtained with two different composite systems, named E-glass fabrics/epoxy (layups [(±45)/(0)2]S), and E-glass/polyester (layups [90/0/±45/0]S), NN model were trained with fatigue data from two different stress ratios, which represent limited fatigue data, can be used to predict another four and seven stress ratios respectively, with high accuracy of fatigue life prediction. The accuracy of NN prediction were quantified with the small value of mean square error (MSE). When using 33% from the total fatigue data for training, the NN model able to produce high accuracy for all stress ratios. When using less fatigue data during training (22% from the total fatigue data), the NN model still able to produce high coefficient of determination between the prediction result compared with obtained by experiment.
Examination of the SG tube fatigue cracking at Fessenheim unit no.2 of EDF
International Nuclear Information System (INIS)
Boccanfuso, M.; Lorthios, J.; Thebault, Y.; Bruyere, B.; Duisabeau, L.; Herms, E.
2015-01-01
In February 2008, a primary-to-secondary leak occurred at Fessenheim Unit No.2 on a steam generator. A circumferential fatigue crack was observed at the upper tube support plate level of the R12C62 tube although the stability ratio evaluation performed to take into account some prior international events, concluded that this tube had no risk of fluid-elastic instability. A new tube pull process was developed and performed by AREVA in 2011 just before the SG replacement. The extraction at the uppermost TSP elevation was a first occurrence in the French EDF PWR. Destructive examinations were carried out in the EDF hot laboratory of CEIDRE/Chinon in order to characterize damage mechanisms at the initiation and propagation stage. The document relates the major results of laboratory examinations leading us to exclude the fluid-elastic instability scenario as previously reported in North-Anna (1987) and Mihama (1991) tube rupture incidents. Results analysis with particular focus on the fracture surface description using Scanning Electron microscopy observations and metallurgical investigations provide new elements concerning the aggravating factors of fatigue damage. Fracture surface investigations reveal that the circumferential crack was due to high cycle fatigue with a very low stress intensity factor. Some aggravating factors like intergranular corrosion appeared to be critical for the fatigue cracking initiation stage. The deterioration was also largely promoted by the lack of tube support at the Anti-Vibration Bars
Effect of pre-deformation on the fatigue crack initiation life of X60 pipeline steel
International Nuclear Information System (INIS)
Zheng, M.; Luo, J.H.; Zhao, X.W.; Bai, Z.Q.; Wang, R.
2005-01-01
It is impossible to keep petroleum and natural gas transmission pipelines free from defects in the manufacturing, installation and servicing processes. The damage might endanger the safety of pipelines and even shorten their service life; gas or petroleum release due to defects may jeopardise the surrounding ecological environments with associated economic and life costs. Pre-tensile deformation of X60 steel is employed to experimentally simulate the influence of dents on the fatigue crack initiation life. The investigation indicates that the fatigue crack initiation life of pre-deformed X60 pipeline steel can be assessed by a previously proposed energetic approach. The threshold for crack initiation increases with the pre-deformation due to a strain hardening effect, while the fatigue resistant factor exhibits a maximum with pre-deformation owing to its special dependence on fracture strain and fracture strength. The result is expected to be beneficial to the understanding of the effect of damage on the safety of pipelines and fatigue life prediction
Fatigue-crack propagation response of two nickel-base alloys in a liquid sodium environment
International Nuclear Information System (INIS)
Mills, W.J.; James, L.A.
1979-01-01
The elevated temperature fatigue-crack propagation response of Inconel 600 and Inconel 718 was characterized within a linear-elastic fracture mechanics framework in air and low-oxygen liquid sodium environments. The crack growth rates of both nickel-base alloys tested in liquid sodium were found to be considerably lower than those obtained in air. This enhanced fatigue resistance in sodium was attributed to the very low oxygen content in the inert sodium environment. Electron fractographic examination of the Inconel 600 and Inconel 718 fatigue fracture surfaces revealed that operative crack growth mechanisms were dependent on the prevailing stress intensity level. Under low growth rate conditions, Inconel 600 and Inconel 718 fracture surfaces exhibited a faceted, crystallographic morphology in both air and sodium environments. In the higher growth rate regime, fatigue striations were observed; however, striations formed in sodium were rather ill-defined. These indistinct striations were attributed to the absence of oxygen in the liquid sodium environment. Striation spacing measurements were found to be in excellent agreement with macroscopic growth rates in both environments
Directory of Open Access Journals (Sweden)
G. M. Domínguez Almaraz
2015-10-01
Full Text Available Crack initiation and propagation have been investigated on the polymeric material ABS (Acrylonitrile Butadiene Styrene, under ultrasonic fatigue testing. Three controlled actions were implemented in order to carry out fatigue tests at very high frequency on this material of low thermal conductivity, they are: a The applying load was low to limit heat dissipation at the specimen neck section, b The dimensions of testing specimen were small (but fitting the resonance condition, in order to restraint the temperature gradient at the specimen narrow section, c Temperature at the specimen neck section was restrained by immersion in water or oil during ultrasonic fatigue testing. Experimental results are discussed on the basis of thermo-mechanical behaviour: the tail phenomenon at the initial stage of fatigue, initial shear yielding deformation, crazed development on the later stage, plastic strain on the fracture surface and the transition from low to high crack growth rate. In addition, a numerical analysis is developed to evaluate the J integral of energy dissipation and the stress intensity factor K, with the crack length
International Nuclear Information System (INIS)
Broekhoven, M.J.G.; Ruijtenbeek, M.G. van de
1975-01-01
The fracture mechanics based stress intensity factor (K-factor) concept has obtained wide-spread acceptance as a tool for quantitative analysis of both fatigue crack growth and instable fracture. The present study discusses the applicability of various simple analytical approximations by comparing results with experimental data. A semi-analytical procedure has been developed whose main characteristics are: the true stress distribution perpendicular to the crack plane for the uncracked structure is used as input data; an extended version of the Shah and Kobayashi solution for elliptical cracks, loaded on their surfaces by tractions described by fourth order double symmetrical polynomials fit through the data of previous step is used to calculate full K-factor variations along the crack fronts; several corrections, a.o. to correct for free surfaces and for a corner radius are incorporated. The experiments concern careful monitoring crack growth rates (da/dN) under uniaxial fatigue loading of precracked nozzle-on-plate models, a.o. using a closed T.V. circuit. Resulting da/dN versus crack length (a) curves are converted into K versus a curves using da/dN versus ΔK curves for the same material (ASTM A 508 C12) obtained by standard procedures. Comparison of theoretical and experimental data yields the conclusion that: simple analytical approximations as sometimes recommended in literature may largely overestimate or underestimate K-factors for nozzle corner cracks; a computer program based on the semi-analytical procedure yields results within seconds of CPU-time once the input data have been generated. These results compare well with experimental and available finite element data for the range of crack depths of practical concern
Surface crack behavior in socket weld of nuclear piping under fatigue loading condition
International Nuclear Information System (INIS)
Choi, Y.H.; Kim, J.S.; Choi, S.Y.
2005-01-01
The ASME B and PV Code Sec. III allows the socket weld for the nuclear piping in spite of the weakness on the weld integrity. Recently, the integrity of the socket weld is regarded as a safety concern in nuclear power plants because many failures and leaks have been reported in the socket weld. OPDE (OECD Piping Failure Data Exchange) database lists 108 socket weld failures among 2,399 nuclear piping failure cases during 1970 to 2001. Eleven failures in the socket weld were also reported in Korean NPPs. Many failure cases showed that the root cause of the failure is the fatigue and the gap requirement for the socket weld given in ASME Code was not satisfied. The purpose of this paper is to evaluate the fatigue crack behavior of a surface crack in the socket weld under fatigue loading condition considering the gap effect. Three-dimensional finite element analysis was performed to estimate the fatigue crack behavior of the surface crack. Three types of loading conditions such as the deflection due to vibration, the pressure transient ranging from P=0 to 15.51 MPa, and the thermal transient ranging from T=25 C to 288 C were considered. The results are as follows; 1) The socket weld is susceptible to the vibration where the vibration levels exceed the requirement in the ASME operation and maintenance (OM) Code. 2) The effect of pressure or temperature transient load on the socket weld integrity is not significant. 3) No-gap condition gives very high possibility of the crack initiation at the socket weld under vibration loading condition. 4) For the specific systems having the vibration condition to exceed the requirement in the ASME Code OM and/or the transient loading condition from P=0 and T=25 C to P=15.51 MPa and T=288 C, radiographic examination to examine the gap during the construction stage is recommended. (orig.)
Fatigue crack growth threshold of austenitic stainless steels in simulated PWR primary water
International Nuclear Information System (INIS)
Tsutsumi, Kazuya; Yamamoto, Kenji; Nitta, Yoshikazu
2007-01-01
Many studies have revealed that fatigue crack growth (FCG) rate of austenitic stainless steels is accelerated in light water reactor environment compared to that in air at room temperature. Major driving factors in the acceleration of FCG rate are stress ratio, temperature and stress rise time. Based on this knowledge, FCG curves have been developed considering these factors as parameters. However, there are few data of FCG threshold ΔK th in light water reactor environment. Hence it is necessary to clarify FCG rate under near-threshold condition for more accurate evaluation of fatigue crack growth behavior under cyclic stress with relatively low ΔK. In the present study, therefore, ΔK th was determined for austenitic stainless steels in simulated PWR primary water, and FCG behavior under near-threshold condition was revealed by collecting fatigue crack propagation data. The results are summarized as follows: No propagation of fatigue crack was found in high temperature water, and there was a definite ΔK th . Average ΔK eff,th was 4.3 MPa·m 0.5 at 325degC, 3.3 MPa·m 0.5 at 100degC, and there was no considerable reduction compared to currently known ΔK eff,th in air. Thus, it was revealed tha ambient conditions had minimal effect, on ΔK eff,th , ΔK th increases with increasing temperature and decreasing frequency. As a result of fracture surface observation, oxide-induced-crack-closure was considered to be a cause of the dependency described above. In addition, it was suggested that changes in material properties also had influence on ΔK th, since ΔK eff,th itself increased at elevated temperature. (author)
Directory of Open Access Journals (Sweden)
Jin-Feng Jiao
2018-01-01
Full Text Available The fatigue stress amplitude of the welded cross plate-hollow sphere joint (WCPHSJ in a grid structure varies due to the random loading produced by suspending cranes. A total of 14 specimens considering three different types of WCPHSJs were prepared and tested using a specially designed test rig. Four typical loading conditions, “low-high,” “high-low,” “low-high-low,” and “high-low-high,” were first considered in the tests to investigate the fatigue behavior under variable load amplitudes, followed by metallographic analyses. The experimental and metallographic analysis results provide a fundamental understanding on the fatigue fracture form and fatigue mechanism of WCPHSJs. Based on the available data from constant-amplitude fatigue tests, the variable-amplitude fatigue life of the three types of WCPHSJs was estimated using the Miner rule and Corten-Dolan theory. Since both accumulative damage theories yield virtually same damaging results, the Miner rule is hence suggested to estimate the fatigue life of WCPHSJs.
Fatigue Crack Growth Behavior of Austempered AISI 4140 Steel with Dissolved Hydrogen
Directory of Open Access Journals (Sweden)
Varun Ramasagara Nagarajan
2017-11-01
Full Text Available The focus of this investigation was to examine the influence of dissolved hydrogen on the fatigue crack growth behavior of an austempered low-alloy AISI 4140 steel. The investigation also examined the influence of dissolved hydrogen on the fatigue threshold in this material. The material was tested in two conditions, as-received (cold rolled and annealed and austempered (austenitized at 882 °C for 1 h and austempered at 332 °C for 1 h. The microstructure of the annealed specimens consisted of a mix of ferrite and fine pearlite; the microstructure of the austempered specimens was lower bainite. Tensile and Compact Tension specimens were prepared. To examine the influence of dissolved hydrogen, two subsets of the CT specimens were charged with hydrogen for three different time periods between 150 and 250 h. All of the CT samples were then subjected to fatigue crack growth tests in the threshold and linear regions at room temperature. The test results indicate that austempering resulted in significant improvement in the yield and tensile strength as well as the fracture toughness of the material. The test results also show that, in the absence of dissolved hydrogen, the crack growth rate in the threshold and linear regions was lower in austempered samples compared to the as-received (annealed samples. The fatigue threshold was also slightly greater in the austempered samples. In presence of dissolved hydrogen, the crack growth rate was dependent upon the ∆K value. In the low ∆K region (<30 MPa√m, the presence of dissolved hydrogen caused the crack growth rate to be higher in the austempered samples as compared to annealed samples. Above this value, the crack growth rate was increasingly greater in the annealed specimens when compared to the austempered specimens in presence of dissolved hydrogen. It is concluded that austempering of 4140 steel appears to provide a processing route by which the strength, hardness, and fracture toughness of
Rovinelli, Andrea; Guilhem, Yoann; Proudhon, Henry; Lebensohn, Ricardo A.; Ludwig, Wolfgang; Sangid, Michael D.
2017-06-01
Microstructurally small cracks exhibit large variability in their fatigue crack growth rate. It is accepted that the inherent variability in microstructural features is related to the uncertainty in the growth rate. However, due to (i) the lack of cycle-by-cycle experimental data, (ii) the complexity of the short crack growth phenomenon, and (iii) the incomplete physics of constitutive relationships, only empirical damage metrics have been postulated to describe the short crack driving force metric (SCDFM) at the mesoscale level. The identification of the SCDFM of polycrystalline engineering alloys is a critical need, in order to achieve more reliable fatigue life prediction and improve material design. In this work, the first steps in the development of a general probabilistic framework are presented, which uses experimental result as an input, retrieves missing experimental data through crystal plasticity (CP) simulations, and extracts correlations utilizing machine learning and Bayesian networks (BNs). More precisely, experimental results representing cycle-by-cycle data of a short crack growing through a beta-metastable titanium alloy, VST-55531, have been acquired via phase and diffraction contrast tomography. These results serve as an input for FFT-based CP simulations, which provide the micromechanical fields influenced by the presence of the crack, complementing the information available from the experiment. In order to assess the correlation between postulated SCDFM and experimental observations, the data is mined and analyzed utilizing BNs. Results show the ability of the framework to autonomously capture relevant correlations and the equivalence in the prediction capability of different postulated SCDFMs for the high cycle fatigue regime.
International Nuclear Information System (INIS)
Masaki, Kiyotaka; Ochi, Yasuo; Matsumura, Takashi; Ikarashi, Takaaki; Sano, Yuji
2010-01-01
Laser peening without protective coating (LPwC) treatment is one of surface enhancement techniques using an impact wave of high pressure plasma induced by laser pulse irradiation. High compressive residual stress was induced by the LPwC treatment on the surface of low-carbon type austenitic stainless steel SUS316L. The affected depth reached about 1mm from the surface. High cycle fatigue tests with four-points rotating bending loading were carried out to confirm the effects of the LPwC treatment on fatigue strength and surface fatigue crack propagation behaviors. The fatigue strength was remarkably improved by the LPwC treatment over the whole regime of fatigue life up to 10 8 cycles. Specimens with a pre-crack from a small artificial hole due to fatigue loading were used for the quantitative study on the effect of the LPwC treatment. The fracture mechanics investigation on the pre-cracked specimens showed that the LPwC treatment restrained the further propagation of the pre-crack if the stress intensity factor range ΔK on the crack tip was less than 7.6 MPa√m. Surface cracks preferentially propagated into the depth direction as predicted through ΔK analysis on the crack by taking account of the compressive residual stresses due to the LPwC treatment. (author)
Lu, Mingyu; Qu, Yongwei; Lu, Ye; Ye, Lin; Zhou, Limin; Su, Zhongqing
2012-04-01
An experimental study is reported in this paper demonstrating monitoring of surface-fatigue crack propagation in a welded steel angle structure using Lamb waves generated by an active piezoceramic transducer (PZT) network which was freely surface-mounted for each PZT transducer to serve as either actuator or sensor. The fatigue crack was initiated and propagated in welding zone of a steel angle structure by three-point bending fatigue tests. Instead of directly comparing changes between a series of specific signal segments such as S0 and A0 wave modes scattered from fatigue crack tips, a variety of signal statistical parameters representing five different structural status obtained from marginal spectrum in Hilbert-huang transform (HHT), indicating energy progressive distribution along time period in the frequency domain including all wave modes of one wave signal were employed to classify and distinguish different structural conditions due to fatigue crack initiation and propagation with the combination of using principal component analysis (PCA). Results show that PCA based on marginal spectrum is effective and sensitive for monitoring the growth of fatigue crack although the received signals are extremely complicated due to wave scattered from weld, multi-boundaries, notch and fatigue crack. More importantly, this method indicates good potential for identification of integrity status of complicated structures which cause uncertain wave patterns and ambiguous sensor network arrangement.
Assessment of thermal fatigue crack propagation in safety injection PWR lines
International Nuclear Information System (INIS)
Simos, N.; Reich, M.; Costantino, C.J.; Hartzman, M.
1990-01-01
Cyclic thermal stratification resulting in alternating thermal stresses in pipe cross sections has been identified as the primary cause of high cycle thermal fatigue failure. A number of piping lines in operating plants around the world, susceptible to thermal stratification, have experienced circumferential cracking as a result of high levels of alternating bending stresses. This paper addresses the mechanisms of crack initiation and crack growth and provides estimates of fatigue cycles to failure for a typical safety injection line with such cyclic load history. Utilizing a 3-D finite element analysis, the temperature profile and the corresponding thermal stress field of a complete thermal cycle in a safety injection line consisting of a horizontal pipe section and an elbow, is obtained. Since the observed cracking occurred in the region of the elbow-to-horizontal pipe weld, the analysis performed assessed (1) the impact of the level of local geometric discontinuities on the initiation of an inside surface flaw is greatest and (2) the number of thermal cycles required to drive a small surface crack through the pipe wall. 12 refs., 14 figs., 2 tabs
International Nuclear Information System (INIS)
West, S.L.; Nelson, D.Z.; Louthan, M.R. Jr.
1992-01-01
The secondary cooling water system pressure boundary of Savannah River Site reactors includes expansion joints utilizing a thin-wall bellows. While successfully used for over thirty years, an occasional replacement has been required because of the development of small, circumferential fatigue cracks in a bellows convolute. One such crack was recently shown to have initiated from a weld heat-affected zone liquation microcrack. The crack, initially open to the outer surface of the rolled and seam welded cylindrical bellows section, was closed when cold forming of the convolutes placed the outer surface in residual compression. However, the bellows was placed in tension when installed, and the tensile stresses reopened the microcrack. This five to eight grain diameter microcrack was extended by ductile fatigue processes. Initial extension was by relatively rapid propagation through the large-grained weld metal, followed by slower extension through the fine-grained base metal. A significant through-wall crack was not developed until the crack extended into the base metal on both sides of the weld. Leakage of cooling water was subsequently detected and the bellows removed and a replacement installed
System for nucleation and propagation of fatigue cracks on SE(B) specimens
Energy Technology Data Exchange (ETDEWEB)
Rocha, Nirlando Antonio; Gomes Junyor, Jose Onesimo; Reis, Emil; Vilela, Jefferson Jose, E-mail: nar@cdtn.br, E-mail: ze_onezo@hotmail.com, E-mail: emilr@cdtn.br, E-mail: jjv@cdtn.br [Centro de Desenvolvimento da Tecnologia Nuclear (CDTN/CNEN-MG), Belo Horizonte, MG (Brazil); Moura, Cassio Melo, E-mail: cassio.moura@gerdau.com.br [Gerdau S.A., Ouro Branco, MG (Brazil)
2015-07-01
The degree of safety that a structural component has against catastrophic fracture in service can be obtained from fracture mechanics parameters. The master curve could be used for integrity evaluation in pressure vessel of nuclear power plant. The pre-crack specimens are used in this evaluation. The tests based on ASTM E 8M and ASTM E 647 standards to determination of material properties related to fracture mechanics, most often performed in a servo-hydraulic drive equipment, are time consuming and costly. This paper presents the development of a system for nucleation and propagation of fatigue cracks on SE(B) specimens. The operating principle consists of a cyclic loading, concentrated in the center of the specimen, transmitted and controlled by an eccentric mechanism. The main contribution of this work is the low-cost technology in the production of fatigue pre-crack, and the possibility of performing the nucleation and propagation of the pre-crack required for obtaining the J{sub IC} and CTOD parameters. The experimental results satisfied expectations with respect to the plastic deformation in the crack tip and met the requirements of the standards. (author)
System for nucleation and propagation of fatigue cracks on SE(B) specimens
International Nuclear Information System (INIS)
Rocha, Nirlando Antonio; Gomes Junyor, Jose Onesimo; Reis, Emil; Vilela, Jefferson Jose; Moura, Cassio Melo
2015-01-01
The degree of safety that a structural component has against catastrophic fracture in service can be obtained from fracture mechanics parameters. The master curve could be used for integrity evaluation in pressure vessel of nuclear power plant. The pre-crack specimens are used in this evaluation. The tests based on ASTM E 8M and ASTM E 647 standards to determination of material properties related to fracture mechanics, most often performed in a servo-hydraulic drive equipment, are time consuming and costly. This paper presents the development of a system for nucleation and propagation of fatigue cracks on SE(B) specimens. The operating principle consists of a cyclic loading, concentrated in the center of the specimen, transmitted and controlled by an eccentric mechanism. The main contribution of this work is the low-cost technology in the production of fatigue pre-crack, and the possibility of performing the nucleation and propagation of the pre-crack required for obtaining the J IC and CTOD parameters. The experimental results satisfied expectations with respect to the plastic deformation in the crack tip and met the requirements of the standards. (author)
Numerical analysis of the influence of liquid on propagation of a rolling contact fatigue crack
Directory of Open Access Journals (Sweden)
M. Olzak
2017-10-01
Full Text Available Numerical investigations of the propagation of rolling contact fatigue crack filled by the liquid have been conducted. Two models of fluid crack interaction have been considered. In the first model called 䖓hydrostatic� the assumption of incompressible, inviscid and weightless liquid was accepted. It was also assumed that due to the wheel load the trapped liquid could not get outside the crack and its volume remained constant until the rising pressure would open up the crack mouth again. On this assumption the analysis has a steady-state character. In the second model it has been assumed that the crack is filled by the viscous, incompressible fluid and the fluid motion as well as the resulting pressure distribution can be represented by one-dimensional form of the Reynolds equation. The method for solving the problem of the coupled motion of liquid and crack faces has been developed and series of calculation were made. The method has been employed for the predicting of crack deformation in the course of wheel rolling
Fracture Toughness and Fatigue Crack Growth Behavior of As-Cast High-Entropy Alloys
Seifi, Mohsen; Li, Dongyue; Yong, Zhang; Liaw, Peter K.; Lewandowski, John J.
2015-08-01
The fracture toughness and fatigue crack growth behavior of two as-vacuum arc cast high-entropy alloys (HEAs) (Al0.2CrFeNiTi0.2 and AlCrFeNi2Cu) were determined. A microstructure examination of both HEA alloys revealed a two-phase structure consisting of body-centered cubic (bcc) and face-centered cubic (fcc) phases. The notched and fatigue precracked toughness values were in the range of those reported in the literature for two-phase alloys but significantly less than recent reports on a single phase fcc-HEA that was deformation processed. Fatigue crack growth experiments revealed high fatigue thresholds that decreased significantly with an increase in load ratio, while Paris law slopes exhibited metallic-like behavior at low R with significant increases at high R. Fracture surface examinations revealed combinations of brittle and ductile/dimpled regions at overload, with some evidence of fatigue striations in the Paris law regime.
International Nuclear Information System (INIS)
Jones, D.P.; Hoppe, R.G.; James, B.A.
1993-01-01
A series of fatigue crack growth rate tests was conducted in order to study effects of negative stress ratio on fatigue crack growth rate of low-alloy steel in air. Four-point bend specimens were used to simulate linear stress distributions typical of pressure vessel applications. This type of testing adds to knowledge on negative stress ratio effects for low-alloy steels obtained in the past from uniform tension-compression tests. Applied bending stress range was varied over twice the yield strength. Load control was used for tests for which the stress range was less than twice the yield strength and deflection control was used for the higher stress range tests. Crack geometries were both short and long fatigue cracks started at notches and tight fatigue cracks for which crack closure could occur over the full crack face. Results are presented in terms of the stress intensity factor ratio R = K MIN /K MAX . The negative R-ratio test results were correlated to an equation of the form da/dN = C[ΔK/(A-R)] n , where A, C, and n are curve fitting parameters. It was found that effects of negative R-ratio on fatigue crack growth rates for even the high stress range tests could be bounded by correlating the above equation to only positive R-ratio test results and extending the resulting equation into the negative R-ratio regime
International Nuclear Information System (INIS)
Lee, Ho Jin; Kim, Maan Won; Lee, Bong Sang
2003-12-01
Fatigue crack growth analysis plays an important role in the structural integrity assessment or the service life calculation of the nuclear power plant pipes. To obtain the material properties as a basic data to achieve an accurate crack growth analysis, a lot of tests and numerical crack growth simulations have been done for decades. The BS 7910 or the ASME Boiler and Pressure Vessel Code Section XI, generally used to evaluate crack growth behavior, were made under the based on simple stress states or at the evaluated isothermal temperature. It is well known that the ASME code could sometimes give so conservative results in some cases of which the cracked components are experiencing with cyclic thermal shock. In this report, we suggested a method for the life assessment of a crack embedded in nuclear power plant pipes under the thermal-mechanical fatigue loads. We here use the numerical method to get the temperature history for thermal- mechanical fatigue crack growth test. And then we can calculate the remaining life time of the pipe by using the fracture mechanics and the test results together. For this purpose, we constructed a thermal-mechanical fatigue crack growth testing system. We also gave a lot of review about recent researches in the experimental field of thermal-mechanical fatigue analysis
Sub-surface Fatigue Crack Growth at Alumina Inclusions in AISI 52100 Roller Bearings
DEFF Research Database (Denmark)
Cerullo, Michele
2014-01-01
Sub-surface fatigue crack growth at non metallic inclusions is studied in AISI 52100 bearing steel under typical rolling contact loads. A first 2D plane strain finite element analysis is carried out to compute the stress history in the innner race at a characteristic depth, where the Dang Van...... damage factor is highest. Subsequently the stress history is imposed as boundary conditions in a periodic unit cell model, where an alumina inclusion is embedded in a AISI 52100 matrix. Cracks are assumed to grow radially from the inclusion under cyclic loading. The growth is predicted by means...